arXiv:condmat/0601569v4 [condmat.mtrlsci] 1 Jun 2010
M. P. KASHCHENKO
THE WAVE MODEL OF MARTENSITE GROWTH FOR THE γ − α TRANSFORMATION OF IRONBASED ALLOYS
ξ1 ξ2
c~2 c~1
EKATERINBURG 2005
~c
M.P.KASHCHENKO THE WAVE MODEL OF MARTENSITE GROWTH FOR THE γ − α TRANSFORMATION OF IRONBASED ALLOYS Prof. Michael P. Kashchenko Ural State Forest Engineering University Physics Chair Sybirskyi Tract 37 620100 Ekaterinburg RUSSIA
[email protected] or
[email protected]
Ekaterinburg UIF PublishingHouse ”Nauka” Original Russian Edition 1993 English Edition 2005. Translation from Russian by J. Gerlts and U. KayserHerold
Contents Preface
8
Introduction
11
1 Basic notions on the γ−α martensitic transformation in iron based alloys 1.1 Position of the γ − α martensitic transformation in relation to other solid state structural transformations . . . . . . . . . . . . . . . . . 1.2 Characteristic features of the spontaneous γ − α martensitic transformation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Latticestability near the MS temperature and the problem of nucleation during the γ − α martensitic transformation . . . . . . . . 1.4 Solved and unresolved problems on the theoretical description of the γ − α martensitic transformation . . . . . . . . . . . . . . . . . 1.5 General physical tasks and objectives . . . . . . . . . . . . . . . . . 2 Particularities of an electronic energy spectrum as required for realization of a PhononMaser 2.1 The Hamiltonian Problem . . . . . . . . . . . . . . . . . . . . . . . 2.2 Form of a nonequilibrium addend to the electronic distribution function and definition of points separating inversely occupied states in a onedimensional electronic spectrum . . . . . . . . . . . . . . . 2.3 Definition of boundary surfaces separating inversely occupied states for a 3dimensional electronic spectrum . . . . . . . . . . . . . . . . 2.4 Limitations imposed by the equidistance relations in (1.9) . . . . . . 2.5 Potentially active pairs of electronic states in the electronicspectrum of fcc iron . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6 Summary of Chapter 2 . . . . . . . . . . . . . . . . . . . . . . . . .
15 15 18 22 28 39 49 49
50 52 58 64 73
3 Constitutive equations of the electronphonon system and the threshold wave generation conditions 77 3.1 Threshold conditions for singlemode generation . . . . . . . . . . . 77 3.2 Threshold conditions for two and threemode wave generation and characteristics of a phase transition of a radiation system . . . . . . 84 5
3.3 3.4
The lattice strain induced by the generated waves . . . . . . . . . . 91 Conclusions from Chapter 3 . . . . . . . . . . . . . . . . . . . . . . 95
4 Coordination between of the γ−α martensitic transformation temperature and the optimum wave generation temperature in ironbased alloys 99 4.1 Definition of the task . . . . . . . . . . . . . . . . . . . . . . . . . . 99 4.2 Modified electronic distributions and their derivatives in the case of a rectangular spectral density function . . . . . . . . . . . . . . . . 102 4.3 Region of T ′ , Γ ′ values with optimum conditions for phonongeneration in the case of a Lorentzshaped SDfunction . . . . . . . . . . . . . 108 4.4 Mapping of the functions MS (C) into the T ′ , Γ ′ region of optimum phonongeneration, with analysis of the electronic configurations of atoms in binary substitutional alloys . . . . . . . . . . . . . . . . . 111 4.5 Discussion of the results on substitutional alloys . . . . . . . . . . . 118 4.5.1 Determination of the parameter a0 and of electronic atomconfigurations on the basis of electrical and optical characteristics of alloying components . . . . . . . . . . . . . . . . 118 4.5.2 Effect of variations of latticeparameter and the sband width on the difference of the charge numbers ∆Z of alloying components . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 122 4.5.3 Estimation of the chemical potential differences of some γ and α  phases, for the subsystem of delectrons . . . . . . . 128 4.6 The MS (C) function for steel and degree of ionization of carbonatoms129 4.7 Summary of Chapter 4 . . . . . . . . . . . . . . . . . . . . . . . . . 131 5 Interpretation of a variety of characteristic morphological features of martensite within the notion of a phononmaser 135 5.1 Habitplanes in FeNi, FeCalloys . . . . . . . . . . . . . . . . . . . 136 5.1.1 Matching of a plane with a pair of waves . . . . . . . . . . . 136 5.1.2 Habit (225) . . . . . . . . . . . . . . . . . . . . . . . . . . . 136 5.1.3 Habit (557). Criterion for transition from habitus (557) to (225) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 139 5.1.4 Habits {15 3 10} ÷ {9 2 5} . . . . . . . . . . . . . . . . . . . 140 5.2 Grouping laws for packetmartensite crystals . . . . . . . . . . . . . 142 5.3 Effect of the magnetic state of austenite and of an externally applied magnetic field on the martensitic γ − α  transformation . . . . . . 145 5.3.1 Possible causes for the transition of habitplanes . . . . . . . 145 5.3.2 Single peak density of states (DOS) model, exchangesplitting and electronic redistribution . . . . . . . . . . . . . . . . . 147 5.3.3 Oriented latticegrowth of athermal martensite in an externally applied magnetic field . . . . . . . . . . . . . . . . . . 153 5.4 Summary of chapter 5 . . . . . . . . . . . . . . . . . . . . . . . . . 157 6
6 Wavemodel of motion for a martensitic lattice boundary 162 6.1 Coordinated propagation of a displacementwave with a switchingwave of chemical potential or temperature . . . . . . . . . . . . . . 164 6.2 Coordinated propagation of a pair of displacementwaves with the switchingwave of T (µ) . . . . . . . . . . . . . . . . . . . . . . . . . 167 6.3 Stationary wave of relative spatial deformation ε˜ during the γ − α  transformation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 170 6.3.1 ε˜  triggerswitching  wave in absence of displacementwaves 170 6.3.2 Effect of the displacementwaves on the velocity of the ε˜ switchingwave . . . . . . . . . . . . . . . . . . . . . . . . . 174 6.3.3 The ε˜  ModifiedSwitchingWave . . . . . . . . . . . . . . . 175 6.4 Summary of Chapter 6 . . . . . . . . . . . . . . . . . . . . . . . . . 179 Synopsis and outlook
183
Bibliography
193
Epilogue
213
Summary
218
7
Preface Since the early seventies, the Author and his Team have been engaged in their still ongoing task and vision of developing a comprehensive physical notion of the γ −α Martensitic Transformation (γ − α MT). The main results of their research work are published in this monograph. Shortly after an initial review and analysis of existing literature on the subject, the following initial conclusions could be drawn:  The γ−α MT is a cooperative lattice transformation proceeding under highly pronounced deviations from local equilibrium conditions;  The velocity of rapid controlled growth of αMartensite crystals is so large that only a wavemodel has the physical potential for a conclusive detailed and comprehensive explanation of the transformation and growth ;  A microscopic theory of the transformation is missing. From the very beginning, the development of a new and comprehensive growth model of a single martensite crystal was mainly guided by the following two factors: On the one hand, the realization that a substantial fraction of energy released during the martensitic transformation process is immediately being converted into the energy of cooperative lattice displacement waves, by the mechanism of stimulated emission of coherent phonons, becoming most effective in a subsystem of nonequilibrium 3d electrons, which ”jump” down to a lower energetic level at the very instant and location of the martensitic lattice transformation, and on the other hand, the formulation of a simple twowave scheme of the crystal growth control mechanism. Even though these two factors were known to the author since 1976, considerable efforts were necessary to figure out in detail the kind and sequence of events during lattice wave generation, and to consistently interpret in their entirety the observed morphological and kinetic particularities of the γ − α MT, including those of some binary alloys in a wide range of concentrations of their second component, as well as to prove experimentally a variety of postulates and predictions related to the problem. The matter described in this monograph nearly reproduces the contents of the habilitation paper of the Author at the Department of Radiating Materials Science of the Ural Polytechnical Institute (nowadays the Ural State Technical University) and at the Cathedra of Physics of the Ural Forest 8
Engineering Institute (nowadays Ural Forest Engineering State University) completed in 1986. The decision to publish this monograph was motivated, on the one hand, by several wishes expressed during the many and extensive discussions with specialists in the disciplines of Solid State Physics and PhaseTransitions, as well as with Metal and Materials scientists, and on the other hand, by the presently achieved success in the realization of theoretical and experimental research programs on αMartensite nucleation focusing on the specific aspects of the WaveGrowthModel. The results obtained from 1989 to 1991 are supposed to be worth a presentation in a single special monograph. The short survey in the final part of this monograph is to complete the notion of the γ − α MT. Here, let us only mention the most important:  It has been found that 60˚ straight line dislocations with h110i lines could act as dislocation nucleation centers (DNC) for αMartensite crystals with habit planes close to {557}  {225}, whereas 30˚ dislocations with h112i lines were acceptable candidates for the role of DNC for crystals with habits close to {259}  {3 10 15}.  Physical models have been developed for the excited premartensitic lattice condition, being typical of the state of nucleation. It was also possible to reproduce the physical conditions prevailing in the transformation wavefront, by means of picosecondlaser irradiation directed onto the surface of a Fe 31,5 Ni single crystal. The results of these investigations can be interpreted as supportive and further detailing the qualitative notion of nucleation, which had been presupposed during the development of the growth model. This is the first time that the mechanism of phonon generation during a solid state transformation has been analyzed and identified as a fundamental aspect of the γ − α transformation. Obviously, the newly developed model of spontaneous martensitic nucleation and growth is also suitable for a physical description of the reverse martensitic α − γtransformation, as well as for other transformations of the type (i.e. cubicbcc ↔ cubicfcc lattice of CuZn alloys). Moreover, the example of the γ − α MT shows that the key for comprehensive understanding of the mechanism controlling the growth of a new phase during reconstructive cooperative transformations is to reveal the dynamic characteristics of an excited lattice in the nonequilibrium system conditions developing in the frontal zone of a nonlinear transformation wave. This latter conclusion is fundamental as it includes the essence of the paradigm complementing the traditional conceptual notion of equilibrium thermodynamics. The Author hopes that this monograph will close (to some degree) the gap which previously had existed in the theory of reconstructive martensitic transformations, and will attract the attention of other scientists to the problem, and be useful to a wider audience of readers. 9
The Author wants to express his thanks and acknowledgments to all his Colleagues and Specialists who discussed this matter with him, thereby promoting the progress in research, as well as to the cooperative ”AlvoMaterialovedenie”, who sponsored the publication of this monograph.
10
Introduction Since many epochs, the production and use of steel and ferrous alloys have been of high and ever increasing importance, for almost any branch of industry and economy. Thus the development of new types of steel with prescribed combinations of the desired mechanical and physical properties, as well as economical benefits, have been the final aim of numerous and still ongoing metallurgical research projects. On the one hand, such research traditionally comprises the empirical development of highly sophisticated metallurgical production methods, like new thermomechanical methods of treatment, by making use of the most suitable phase and structural transformations and, on the other hand, has the final aim of comprehensive and fundamental theoretical understanding of the underlying phase transitions and related physical processes. In the metallurgy of steel, the spontaneous martensitic γ − α transformation plays a key role among structural transformations, as it constitutes the most important hardening process ending up in the formation of martensite. Traditionally, the spontaneous martensitic transformation (MT) is produced by quenching of the hightemperature (austenitic) phase. The spontaneous MT of ferrous alloys is intriguing and challenging from a scientific point of view. One of the most characteristic features of MT is their diffusionless transformation mechanism, by means of rapid cooperative rearrangement of the facecentered cubic (fcc) hightemperature γphase (austenite) into the body centered cubic (bcc) or bodycentered tetragonal (bct) low temperature αphase (martensite). The results of specific research focusing on martensitic transformations substantially contributed to the increase of understanding of the many relevant details of diffusionless structural transformations. However until recently, some key features of martensitic transformations, like the growth process and latticedynamics of the spontaneous transformation, remained as one of metal physics greatest intractable problems. The disclosure of the dynamical mechanisms and principles underlying the process of martensitic transformations would enlighten their intrinsic characteristics and physical nature, and can thus be regarded as one of the fundamental problems of metal physics. Till now, dynamic approach has only been (partially) developed for transformations of the distortional type, in which the lattice symmetry groups of the final and of the initial phases are mutually subordinated. In principle, the transformations of the distortional type are close to a secondorder phase transition (as a rule they exhibit weakly pronounced characteristics of firstorder transitions). Such 11
transformations are almost satisfactorily explained within the ”SoftMode” theory, which, for the most part, focuses around the ShapeMemoryEffect (SME). In contrast, the reconstructive phase transitions, to which the spontaneous γ − α MT is related, demonstrate pronounced features of the firstorder transitions, namely, considerable temperature hysteresis (between the direct and reverse transformations) and thermal and volume effects. Therefore, the ”SoftMode” theory cannot be directly applied to them. Theoretical research on the γ − α MT is mainly characterized by the parallel development of the latticegeometrical, thermodynamic and wave approaches. The few attempts to describe the martensite growth within the wave theory remained uninformative, mainly due to the poorly understood mechanisms of wave excitation and stabilization, as well as of the types of waves and their directions of propagation. On the other hand, the results of such investigations remained in the shadow of an impressive success in the interpretation of the morphology of the martensite crystals, which had mainly been achieved by means of latticegeometrical and thermodynamic investigations. At the same time it turned out more and more obvious that only the wave approach would have the full potential for a comprehensive description of the dynamical aspects of the transformation process. This circumstance determines the immediateness of development of the wave models of martensite crystal growth. The main problems of the wave theory of the α phase growth are the type of the wave process and the mechanism of energy supply that ensures their steadystate propagation. Experimental results indicate that the frontal velocity of martensitic lattice growth only weakly depends on temperature. Its speed of propagation of about ∼ 103 m/s is of the same order of magnitude as the sound velocity, presumably exceeding the velocity of longitudinal elastic waves. Supersonic growth speed, on the one hand, is a clear indication of a complicated, nonlinear character of a waveprocess and on the other hand, of its adiabatic nature, which, in combination with supercooling by about ∆T ≈ 200K below phase equilibrium temperature T0 , together with considerable heat and volumetransformation effects, must inevitably lead to a strongly pronounced nonequilibrium condition with large temperature and chemical potential gradients, in the area between the two phases and, finally, to intensive electronic flows. In accordance with the general laws of nonequilibrium thermodynamics, specific selforganizing processes and structures can in principle emerge within any kind of pronounced nonequilibrium system. In the particular case of interactions between radiation fields comprising photons or phonons with inversely occupied radiative (electronic) subsystems, such conditions may strongly support the generation of coherent waves. To achieve our final aim of determination of the mechanism controlling the cooperative atom displacements (in a microscopic frame of description) associated with the γ − α MT, it is necessary to analyze the dynamical properties of a nonequilibrium system comprising essential electronphonon interactions. The direction of research initiated by this work, being mainly related to the γ − α martensitic transformation of ferrous alloys, can essentially be formulated as follows: 12
A theoretical description of rapid growth of a martensite crystal as a selforganizing process being inherently associated with the propagation of displacement waves generated and amplified by nonequilibrium 3d electrons. Thus the aim of this work will focus on the substantiation of a wavemodel of martensite growth, which in principle should enable us to determine the basic relationships between the microscopic particularities of the electronic structure and the macroscopic (morphologic) features of the transforming systems. To achieve this goal, the following basic prerequisites will have to be met: 1. The development of a methodology for specific search and the identification of pairs of electronic states, that are potentially active for the generation of displacement waves in a local nonequilibrium medium, and an assessment of the amount of such pairs in the electronic spectrum of fcciron during the γ − α MT. 2. Definition of the threshold conditions for the generation of elastic displacement waves by nonequilibrium electrons, including an estimation of maximum wave amplitudes. 3. Substantiation of the possibility to realize the conditions required for wave generation within a wide range of temperatures and concentrations of the second component in ferrous alloys. 4. Creation of a model associating a variety of morphologic features of martensite crystals with the coordinated propagation of lattice displacement waves. 5. Investigation of the motion of the martensitic crystal interface within the concept of a coordinated propagation of a ”switchingwave” for relative volume deformation and displacement waves ensuring the onset of threshold deformation. A qualitative notion of the physical state of rapid frontal growth of martensitic lattice, as obtained from theoretical analysis, thus must at least comprise the following key features: 1. Frontal growth of martensite is controlled by quasilongitudinal lattice distortion waves fastly propagating through a γ phase; 2. The characteristics of such waves define the basic spatial and temporal scales of martensitic growth, and as a consequence the gradients of the chemical potential of electrons (and thereby also the magnitudes of the electrical field strength and current density) and of temperature in the transformation zone; 3. During martensitic lattice growth, the physical parameters of the interphase region comprise key characteristics of a highly pronounced nonequilibrium condition; 13
4. The amplitudes of lattice distortion waves are maintained owing to the process of stimulated emission of phonons by nonequilibrium 3d electrons located in the transformation zone, thereby revealing the physical nature of the real process controlling a spontaneous martensitic reaction. Detailed physical information on the various field characteristics (i.e. displacements, temperature, electrical and magnetic fields) within the nonequilibrium area in the vicinity of a growing lattice will be of fundamental importance for the design of experiments aiming at a simulation of the process of lattice nucleation of the α phase, as well as for the design of experimental devices for dynamical excitation of a premartensitic lattice condition by hypersonic frequencies in a range of ∼ 1010 s−1 , which would have to coincide with the range of frequencies of the distortion waves controlling martensite lattice growth. There exists a variety of possibilities for controlled oriented lattice growth during the γ −α  transformation of austenitic single crystals, for example by means of the combined influence of hypersound, mechanical stress and strong external magnetic fields. In particular, the effect of controlled orientation of martensitic crystal growth by means of a strong magnetic field, as predicted by the author, has experimentally been confirmed at the ”Institute of Physics of Metals ” of the Academy of Sciences of the USSR. The first chapter of this monograph includes a short review of the most important results of theoretical and experimental research on the subject of γ − α martensitic transformations. The theoretical difficulties arising at the description of a martensite nucleation and rapid growth of a martensite crystal will be discussed (in particular, the deficiencies of existing theories dealing with the wave model), also the discussion of the physical problem will be presented in detail. Contents of Chapters 2 to 6 is the absolutely original and corresponds to the objectives of the aforementioned points 1 to 5. Briefly it is presented in a synopsis. In this synopsis, the conclusions playing a major role in understanding of the dynamical sequence of processes during the γ − α martensitic transformation with a survey of results relating to a description of the martensitic nucleation process are presented. In addition, some objectives of proposed further research are outlined. In order to understand this monograph, it is essential to read Chapter 1. However, some alternatives exist for the further sequence of reading. For instance, those readers only being interested in an explanation of the morphology of the products of the γ − α MT, can immediately skip over to Chapter 5. Chapter 2 is of interest for the experts in kinetic properties of metals and alloys. In Chapter 4, specialists in phasediagrams and electronic structures of alloys can find new information related to the dependence between concentration and optimum temperature for the onset of the γ − α MT, from the point of view of the growth theory. None the less, the author recommends to read this monograph in sequence to those readers who want to thoroughly understand such a complicated process as the γ − α MT.
14
Chapter 1 Basic notions on the γ − α martensitic transformation in iron based alloys 1.1
Position of the γ − α martensitic transformation in relation to other solid state structural transformations
The proposition that the causal dependence between a structural state and physical properties of a material is fundamental for solid state physics and defines thus raising permanent interest and intensive research efforts on structural transformations (ST). From the point of view of symmetrytheory, the following two types of ST may be emphasized [1]. The transformations are related to the first type (ST1) if the spatial group of one of the phases (as a rule, the lowtemperature phase) is a subgroup of the initial phase symmetry group. They are called distortional transitions. The success of latticedynamical theories can mainly be attributed to the notion of ”SoftPhonons”. Accordingly, the frequencies of certain phonons exhibit a strong temperaturedependence and can even vanish at temperature T0 (Ms) owing to interactions in the system. At the critical point T0 , a macroscopic amount of zerofrequency phonons emerges, and the associated static rearrangements of atoms can be interpreted and visualized by the concept of SoftModes ”frozen” in initial crystal. At present, this approach for STI is well elaborated and described in detail in the literature (i.e. [1–4]). For this reason, we shall neither dwell on examples of ST1 nor on details of the mechanism of the phonons softening, only remarking here that such structural transformations may proceed as secondorder phase transitions (as a rule, the features of the firstorder phase transitions are only weakly expressed). In contrast, for the structural transformations of the second type (ST2) there is no subordination between the symmetries of the initial phase and the final 15
phase. Phase transitions from the fcc to a bcc or to a close packed hexagonal phase are the examples of the ST2 transitions. ST2 exhibits the pronounced characteristics of the firstorder phase transitions, namely, the significant thermal and volume effects and a temperature hysteresis (between the direct and reverse transformations). This type of transition is called ”reconstructive”. A separate class (ST3) of structural transitions belongs to the type ”orderdisorder”, during which the atoms occupy mainly one of the quasiequilibrium positions on temperatures below a transition temperature T0 whereas at temperatures above T0 different (not less than two) positions are occupied with the same probability. In addition to [1–4], an extensive survey of ST3 transformations is given in [5]. As to the fourth type (ST4) of structural transitions, it is possible to assign them as ”symmetricnoncommensuratecommensurate” phase transition, in which an intermediate phase features a ”superstructure” with a lattice period that is noncommensurate with the period of the parent structure (see more in detail [1, 4, 6]). The term ”Martensitic Transformation” is used as a common attribute for diffusionless structural transitions proceeding by a cooperative rearrangement of the lattice structure. With such an extensive definition, the term MT would equally apply to the above defined ST1, ST2 and ST4 transitions, with specific exclusion of such ST3 transformation, for which atomic displacements over distances comparable to the interatomic distances would be an indispensable prerequisite, typical of this transformation process. It should however be noted that the term ”Martensite” originally was used for designation of the lamellar component in the microstructure of hardened steel [7]. If the extensive definition of MT encompasses the below mentioned totality of transformation characteristics, then we would rather prefer to use term MT in a more restricted sense, i.e. only for the subset of MT relating to diffusionless transformations of the ST2 type. As mentioned in articles [8,9] it is necessary to refine the terminology. Among the reasons for the insufficient present classification of MT are, on the one hand, its incompleteness, and on the other hand, the dissimilarities between the microscopic mechanisms of structural transformations of various types, whose clarification would require an utmost differentiation of MT from the outset. And viceversa, in a latticegeometrical or thermodynamic model of MT, it would suggest itself to strive for a standardized interpretation of all the numerous classes of MT. If kinetic characteristics [10, 11] were used for the classification of diffusionless spontaneous phase transitions, and if their speed of transformation was mainly determined by the velocity of their mobile phase boundaries, then the distinguishing features of MT would be their cooperative way of lattice transformation and their large velocity of growth (with a magnitude of about the sound velocity), being practically independent on temperature. In contrast, ”normal” or polymorphic transformations are characterized by an alternative group of distinguishing features (like noncorrelated migration of atoms over the phase boundaries, as well 16
as relatively slow, thermally activated motion of phase boundaries). Due to a missing of the standardized classification it is obvious to regard the existing approaches as complementary, each of them is focused on a different set of features and aspects of a MT. Within the frame of this theoretical research work on the γ − α MT (related to fcc, bcc or bct lattice, respectively), particular attention will be paid to steel and ironbased (ferrous) alloys. Thus in this paper, the term ”Martensitic Transformation” (MT) will only be used in its more restricted meaning, if not otherwise explicitly noted. In addition to its great practical importance, the choice of the γ −α MT as a subject of research has also been guided by the large amount of already available experimental data. As contemporary well matured latticegeometrical and thermodynamical approaches are not able to provide a comprehensive notion of MT, there is an increasing need to extend them by a microscopic description, with the final aim to develop a dynamical model of the γ − α MT. Of course, the objectives of this work are more modest than the development of a complete microscopic theory of the γ − α MT. We shall formulate our objectives after a brief review of the main and well established notions on the γ − α MT in steel and ferrous alloys.
17
1.2
Characteristic features of the spontaneous γ − α martensitic transformation
There exist many monographs [10–16] and survey papers (i.e. [7, 17–19]) dealing with the history of research, as well as with basic aspects of the γ − α MT. For this reason there is no need here to dwell with history. We only would like to remark that the basis for quantitative research on the subject of γ − α MT has been founded in the twenties. In those days it had already been determined by means of Xray investigations [20] that the lowtemperature phase in steel (martensite) features a bodycentered tetragonal (bct) lattice, whereas the hightemperature phase (austenite) features a fcclattice. A bct lattice is typical of interstitial alloys (FeC, FeN), in which tetragonality increases with increasing concentration of the interstitial component, whereas a bcclattice is more typical of substitutional alloys (FeNi, FeMn). Martensitic transformations of both kinds of alloys feature similar characteristics. As for their classification, we shall preferentially follow [13] and choose the systems FeC and FeNi for a quantitative presentation. The definition of the martensitic transformation (MT) mechanism by G.W. Kurdjumov essentially postulates that a MT is a spontaneous process of lattice transformation following certain rules, one of them being that the relative migration distance of neighbor atoms does not exceed the interatomic distance of the parent lattice. An immediate conclusion from this definition is that a MT is as a phase transition without change of composition, analog to phase transitions in a onecomponent system. For 1st order transitions, the equilibriumtemperature T0 of phases [21] is determined by the HelmholtzEquation of free energy F: Fγ (T0 ) = Fα (T0 ). Thus the energy to be invested for creation of a new phaseboundary always requires a given amount of supercooling below T0 (or, conversely, of superheating above T0 , during the reverse transition). Typical measured values of the temperaturehysteresis between these two transformations are quite substantial and amount to (MS − AS ) ≃ 400 K, with similar magnitudes of supercooling and superheating, respectively: T0 − MS ≈ AS − T0 ≈ 200K. Here MS is the starting temperature of the γ − α MT and AS the starting temperature of the reverse α − γ MT . The change of specific volume also is considerable and has been assessed by different authors up to values within a range of 2 to 5%, where the larger figures of the specific volume effect (per unit weight) are more characteristic of the α phase. The specific heating effect [22] during a MT amounts to some hundreds of calories per mol, resulting in an increase of the temperature of a sample by some dozens of centigrades [22, 23]. Let us now enumerate some of the indisputable structural (morphologic) characteristics of the γ − α MT. 1. Martensite emerges in the shape of lamellae featuring a low ratio of thickness to the other of their characteristic linear dimensions, or in the shape of lenticular crystals, in the middle of which a lamella (midrib) sets off in the 18
first stage of a MT. The thickness of such lamellae varies between 10−7 and 10−6 m (i.e. from 0.1 to a few µm). 2. The habitplane of a lamellae (i.e. the phaseboundary or flat midribboundaries) has some stable orientations (depending on constitution), in relation to the crystallographic axis of the γ and αphases. In the systems FeC, FeNi, there have been observed habitplanes coming close to the {557} ÷ {111} (up to 0,6 weight% C, up to 29 % Ni), {2 2 5}  (0,6 ÷ 1,4 weight.% C), {2 5 9} ÷ {3 10 15}  (1,4 ÷ 1,8 weight.% C, 29 + 34 % Ni ). 1 3. The shape of the transformed areas changes with the emergence of a surfacerelief, the shape of which being characterized by distinct macroscopic shearparameters. This latter feature suggested the commonly used designation ”ShearTransformation” as a synonym for MT. 4. There exists an orientational relationship among the γ and the αphase, indicating parallelism (or approximate parallelism) among the densely packed phaseplanes: {111}γ k {110}α and among angles of rotation in relation to the orientation of the densely packed parallel planes. 5. Martensite crystals exhibit an ordered internal structure, and in many cases a more or less ordered relative arrangement. This way, crystals with habitplanes {557} ÷ {111} are characterized by a rather complicated lattice displacement structure. They form colonies (packets) of crystals with almost equal orientation, whereas for crystals with habitplanes {225}, {259} ÷ {3 10 15}, the formation of internal transformation twins and other crystal arrangements are more typical (more detailed in [24]). An important conclusion raised in [16] states that ” . . . In a single crystal of martensite, its habitplane incorporates a substantial aspect of an orientational relation, being closely linked to the macroscopic shear parameters or, in other words, only a single way of martensitic transformation corresponds to a given habitplane.” Any classification of the kinetic characteristics of MT should therefore clearly distinguish between microkinetics, which characterize the growth of a single lamella, and macrokinetics, which characterize the increase of the bulk amount of martensite in a sample. In terms of microkinetics, a MT can be classified as athermal, because firstly, the speed of transformation and growth of a single lamella is very large (in the order of magnitude of the speed of sound) and independent on temperature, even though the MT may occur within a wide range of temperature T  (0 ÷ 103 ) K, and secondly, because the transformed volume is determined by the emergence of 1
In the following, the crystallographic terms without notation will relate to the axis of the γparentphase (i.e. three righthand vectors along the axis of symmetry of the 4th order h001i).
19
discrete new crystals and not by the steady growth of previously existing ones. Thus the growth proceeds with almost nonexistent thermal activation, giving reason for the attribute ”athermal”. In terms of macrokinetics, it can be distinguished between isothermal and athermal MT. Isothermal MT can proceed at constant temperature, attainable by an isothermal highcapacity heat receptacle (in relation to the transforming volume), while there exists a characteristic temperature (depending on the composition of an alloy) at which the rate of increase of the macroscopic amount of martensite is utmost. If significant deviations from the optimum temperature are forced in (i.e. by rapid quenching), then isothermal MT can be suppressed. This category of macrokinetics is typical for the formation of packetmartensite. If athermal macrokinetics predominate, then the amount of martensite is determined by the degree of supercooling below MS , while isothermal stops of the quenching process would not cause any increase in the transformed volume. These characteristics are typical of the growth of crystals with habit planes {259} ÷ {3 10 15}. The extreme case of athermal growth is the ”explosive” MT, during which an appreciable fraction (some dozens of percents) of the total transformed volume is produced almost instantaneously within a short ”explosive” period. Remarkably, there have also been discovered alloys featuring both types of reaction kinetics [25]. Though, as a rule, the athermal martensite formation normally proceeds after isothermal (during the cooling process), the observation of the reverse sequence has also been reported in [26]. In spite of the crucial importance of data required for a precise determination of the speed of growth of martensite crystals, as well as of the transformation mechanism, only few experimental data with quantitative details like those shown in Table 1.1 have been published. Table 1.1. Experimental data on the speed of growth of martensite Material Fe  29,5 % Ni Fe  30 % Ni Fe  32 % Ni Fe  0,35 % C  8 % Mn Steel Type 188
Speed of growth 103 m/s 1 (1,8 ÷ 2) 0.1 1.1 0.2 6,6 (0,1 ÷ 0,2)
Source [27] [28] [23] [29] [29] [30, 31] [32]
Let us now comment the data shown in Table 1.1. Obviously, the emergence of a single martensite crystal immediately changes the electrical resistance of a sample and, in turn, triggers an electrical signal which can be registered by means of a simple oscilloscope, as reported in [27]. The speed v = l · τ −1 has been determined 20
from previously known values of the signal period τ and the grain size l. Basically in the same way, the speed v has been estimated in [28]. The different order of magnitude of the data presented in [23] can mainly be deduced from the different experimental method of determination of the signal period τ , which in this case was obtained by observation of the change in reflectivity of the sample, being caused by a dull surface relief showing up simultaneously with the MT and remaining engraved in the aftermath. Instead of a characteristic timescale τ ≈ 10−7 s, as used in [27, 28], a timescale of τ ≈ 5 · 10−6 s was used in [23], which however is not directly related to the growth of a single crystal, but to the ”explosive” bulk growth of the crystals as a whole. It has been clarified in [29] that the speed of 2 · 102 m/s only relates to the lateral speed of crystal growth, while a radial (frontal) speed of growth of an order of magnitude of 103 m/s could be confirmed. In [27], the potential coexistence of two different, superimposed stages of growth of martensite crystals has been postulated for the first time, based on signalform analysis. In another analysis of [27] by Arskij, published in [33], it was further asserted that the initially upshooting edge of the signal is caused by the rapid formation of a twodimensional crystal nucleus, in conjunction with radial growth. We note that the surface of such a nucleus represents an inhomogeneity, immediately prompting an increase in electrical resistance. Based on this assumption, it can be inferred that the observed declining signal edge, having a period 5 to 6 times as large as that of the increasing edge, can be used as a natural time gauge for lateral growth of the nucleus (bearing in mind that the specific resistance of martensite is less than that of austenite). Based on such differentiation of growth stages and on data published in [27], Lokschin [30, 31] obtained a value of 7 · 103 m/s for radial growth velocity, clearly exceeding the velocity of longitudinal sound waves in austenite. This evaluation was substantiated in [30, 31] by measurements of the propagation of detonation waves in steel. In the case where the MT was initiated by an external detonation, the speed of wave propagation was (6, 5 ÷ 6, 6) · 103 m/s. By contrast, in cases where a MT in steel was induced by a precooling, the speed of the detonation wave was remarkably lower: (4, 8 ÷ 4, 9) · 103 m/s. Assuming a measurement error of 4 % in [31], this difference can be interpreted as an indication of a large proper speed of the transformation. Even though in [28] no reason is given for a differentiation of the growth mechanism into two different stages, the observations reported in [34–36], relating to the nucleation of thin martensite lamellae being triggered by a strong magnetic field, where an initially rapid nucleation process was followed up by a significantly slower growth stage, convincingly support the assumption that a differentiation or classification of the growth mechanism is realistic. Without doubt from a methodological point of view, such nucleation and growth phenomena would be most promising for further experimental research aiming at the measurement of frontal velocity of growth, by systematic measurement and analysis of signals. And finally, it should be noted that the data reported in [32], which were obtained by evaluation of acoustic signals, only pertain to the average speed of growth of martensite crystals 21
and not to that of a single lamellae, as would be required. Thus, on the basis of experimental data, an order of magnitude of 103 m/s for radial (frontal) growth of a martensite crystal during the γ −α MT presumably would be realistic. The results of direct experiments reported in [30, 31] further support the assumption that the frontal velocity of growth is greater than the velocity of longitudinal elastic waves.
1.3
Latticestability near the MS temperature and the problem of nucleation during the γ − α martensitic transformation
The pronounced characteristics of a firstorder transition of the γ − α MT suggest to assume the separate existence of a nucleation and of a growth stage of the new phase. Thus an important question is related to the stability of the austenitic lattice at MS  temperature, being closely related to the question of the possible existence of a temperature TC at which the stability of the austenitic lattice would completely vanish. In fact, the existence of an absolute temperature TC > 0, at which a supposedly perfect lattice becomes unstable with respect to infinitesimally small fluctuations, will lead us to the conclusion that a MT is almost inevitable during the cooling process. Due to an obvious disparity indicated by the inequality MS > TC , it can be inferred for alloys with isothermal reaction kinetics, which can normally be suppressed by sufficiently rapid quenching below MS , that a distinguished TC  temperature is missing. This in turn is a clear indication of metastability (relative stability) of the parent lattice at temperatures comprising not only the T0 > T > MS region, but also the T < MS region. An important characteristic of alloys with athermal transformation kinetics, being mentioned in most relevant publications, is the independence of MS from the quenching rate, which can be interpreted as a clear indication of the impossibility of supercooling below MS . However, according to experimental results reported in [37], it has also been possible to supercool an Fe 33,7% Ni alloy down to 4.2 K and to trigger an ”explosive” MT only in a subsequent reheating process, which also included some isothermal holding stages. Further indication of the nonexistence of an unequivocal TC for athermally transforming alloys may also be inferred from the character of incompleteness, being typical of them: The transformation process ceases at a temperature Mf , with 0 < Mf < MS , whilst subsequent cooling will not lead to any further growth of martensite, in spite of the existence of a substantial volumetric fraction ( up to some dozens of percent) of residual, nontransformed parent phase. Investigations on the temperaturedependence of elastic moduli published in [38,39], as well as of dispersion curves of phononspectra [38–41] show that, in most cases, not even a faint tendency towards loss of lattice stability is evident. The observed abnormal course of the temperaturedependency of elastic moduli [38] 22
of alloys of the FeNisystems (> 30% Ni), which already attain a ferromagnetic state of order for T > MS , can easily be attributed to the effect of ferromagnetic ordering [42, 43], instead of lattice instability. This means that in general, a normal temperature characteristic of the elastic moduli of ferromagnetic systems is the case. In other words, an austenitic lattice essentially maintains its inherent stability against certain phononmodes of small amplitude. The results of experiments with small particles (diameter > 10−6 m), reported in [44], convincingly demonstrated that when particles of similar size are cooled down, a MT only occurs in a certain fraction of the involved particles, this being further evidence of the heterogeneous nature of martensite nucleation in certain preferenced centers. The same conclusion can also be drawn from observations of thermocycling, during which repeated (cyclic) growth of parent crystals and of martensite crystals takes place at the same location. A variety of electronmicroscopical observations documented in [45] give evidence of an intimate relationship between dislocations and the process of martensitic nucleation. Even though there is no doubt in general on the heterogeneous character of nucleation, there exists a variety of experiments related to the microscopic mechanism of nucleation [46], like diffuse electron and Xray scattering [47] (see also [45,48]), and measurements of reactive forces against microscopic deformations at temperatures near MS [47], all of them providing evidence of a special state of the austenitic lattice prior to its transformation, manifesting itself by an anisotropic increase of the squared mean of the oscillatory amplitudes of lattice modes with wavevectors of selected orientation (and of selected polarization), as well as in a reduction of the mechanical resistance to small deformation [49]. In the case of a perfect lattice being free of phononmode softening, this particularity can be interpreted as the result of nonlinear (anharmonic) modeinteraction, associated with the emergence of isolated, nearorder regions of displacements (NORD), as proposed in [50]. The investigations performed in [50] mainly deal with constitutive thermodynamic aspects of MT (Investigation of lattice stability against quasistatic lattice deformations, as modeled by a package of ”frozenin” waves). Obviously, the more normal situation would be characterized by a transformed spectrum of elementary lattice oscillations, leading to the emergence of movable nearorder domains of the soliton type [51], their stability being endorsed by the accumulation (localization) of electrons in the vicinity of isolated NORD (in a similar way as in the case of the fluctuational model in [52]). From our point of view, a reasonable qualitative notion of martensite formation, comprising both heterogeneous and homogeneous nucleation, would have to be a nucleation model encompassing the basic process of NORD localization in the vicinity of inhomogeneities produced by single or grouped dislocations. Obviously this point of view is both in accordance with pure thermodynamical concepts [10, 53], because any weakening of the binding energy in the proximity of a lattice defect would compensate for the increase in energy related to the creation of a boundary area, as well as with the Pinningeffect [54] in nonlinear lattice dynamics. This model thus is closely related to the 23
”reactive path” model by Cohen, Machlin and Paranyan [7] in that: 1. A coordinated motion of atoms proceeds by means of ”rapid sequential change of intermediate structures in a given range. . . ” growing ”. . . in a similar way as the propagation of an elastic wave”. 2. ”The activation occurs by means of fluctuating rearrangements of the atomic configuration within the nucleus, and not through changes of its size” 3. Nucleation occurs in the centers of lattice distortion, including dislocation rows. An important feature reported in [50] is the possible loss of stability of NORD, which could be related to their increase in size in conjunction with partial latticesoftening. However, as local softening is always existent in the vicinity of a dislocation, the lateral dimension 2 · r0 of a settling NORD must be larger than the dimension of mobile NORD without defect. In pure dislocation nucleation models (e.g. in [55]), the MS temperature is put into relation with the emergence of the first dislocation loop, whereas the creation of followup dislocation loops is supposed to occur spontaneously. Subsequently, a rapid nucleation process up to macroscopic dimensions would be possible by means of expansion of such dislocation loops, at a speed close to the speed of sound. With the assumption that a nucleus would have the following main linear dimensions: Length as determined by the straight section of the dislocation line, lateral diameter 2 · r, for r ≈ (10−6 ÷ 10−7)m as a realistic gauge for the thickness of a typical lamella, it is possible to assess the period of macronucleation tN by tN ≈ r · c−1 ≈ (10−9 ÷ 10−10 ) s, where c is a speed close to the speed of sound. A model based on the notion of localized NORD thus would have to presuppose an initial quantity r0 of a NORD, being significantly smaller than r ( [50] assumes r0 ≈ 10−9 m), whilst the event of NORDlocalization would simultaneously stimulate the creation of the first dislocation loop. The follow up expansion of these loops would then be characterized by synchronized growth from r0 to a macroscopic size r. It should however be considered that the NORDmodel as defined in [50], is inherently confined to short wave length displacements. For this reason, the existence of soliton solutions with dimensions r0 of about the order of magnitude of r cannot generally be excluded. The transformation of NORD from their initial size r0 ≈ 10−7m into a macronucleus takes place within a period of tN ≈ 10−11 s, as the participating atoms would only have to overcome a distance of about ε· r, within a period tN , where the quantity ε ≈ 0, 1 suggests itself to be taken as a natural gauge of relative deformation during the γ − α MT [56]. We have to remark that the usually assumed shape of the nucleus as a thin, flattened spheroid was mainly determined, on the one hand, by thermodynamical reasons, and on the other hand, by a presupposed inherent similarity between the initial shape of the nucleus and the lenticularly shaped final crystal. The last circumstance led to a nucleation growth model in the pattern of expanding dislocation loops, where 24
the edges of the growing crystal would feature monoatomic thickness in radial orientation. The model of a slowly thickening spheroid for lenticularly shaped crystals requires some further explanation related to its central lamellar zone the midribs  whose constant thickness can, for good reasons, be regarded as a characterizing gauge of the bulk structure. In terms of thermodynamics, this would be analog to a gauge for critical crystal thickness [57], being related to phenomena of transition between different mechanisms of additional deformation (i.e. low thickness by twinning vs. larger thickness by slipping). Thus, in principle, the creation of midribs and their expansion from monoatomic size to their final dimensions of r ≈ 10−6 ÷ 10−7 m would be feasible. Another alternative might be the above mentioned possibility for rapid emergence of a macronucleus, whose dimension r determined the length of latticedisplacement waves excited under nonequilibrium conditions. Thus, if a mechanism for effective maintenance of the wave amplitude would exist in such a way that the amplitude ε of deformation associated with these waves exceeded the thresholdvalue required for initiation of the martesitic transformation, then the growth had to proceed in a wavemode, with characteristic structural gauges of the macronuclei corresponding to certain wavelengths. Obviously, the notion of nonequilibrium conditions, being typical of the nucleation process, will constitute the focus of such a model. It is fairly obvious that the highly pronounced nonequilibrium conditions prevailing in the vicinity of a rapidly growing phase can only be maintained if the process of heat liberation is adiabatic [58, 59]. Then, the −1 temperature difference between the γ  and the α  phase ∆T ≈ Q· Csp (where Q heat energy density, Csp  specific heat), would be comparable with the magnitude of supercooling T0 − MS . This in turn allows to refine the formulation of our basic task: Investigation of a nonequilibrium electronphonon system with the final aim of clarification and substantiation of the principles and conditions for efficient generation of latticedisplacement waves. In the above outlined qualitative pattern, the transition from nucleation to the growth stage features some characteristics of a continuous transition, thus being an indication of a potential instability with respect to rapid growth of nuclei emerging under nonequilibrium conditions. Such a conclusion would however have to presuppose the existence of effective rapid growth mechanisms. This latter circumstance may thus play the crucial role in the transition process of the initial system into a new state. In fact, the following basic rule of nonstationary thermodynamics applies: If a given system can potentially exist in different states, each of them having a relative minimum of free energy, then ” . . . those states emerging at the greater speed will be realized first”. Just this way, the kinetic factor comes to the fore, which is quite natural in a growth stage. Even though the kinetic aspect of the transformation does not belong to the classic realm of thermodynamics, there exists a link between the thermodynamical and the kinetic conditions of such phase generation. In our case however, we shall confine the role of thermodynamics to 25
the determination of the thermodynamic stimulus of the transformation, and of the activation energies required for nucleation and growth. The missing quantity T0 , and therefore the asserted relative stability of the fcclattice at MS temperature, implies a question related to the magnitude of the energy barrier, which has to be overcome by the system during the processes of nucleation and growth. Obviously, this question is closely related to the problem dealing with the large observed magnitude of supercooling T0 −MS ≈ 200 K, which has been clearly formulated in [58, 59]. This specific problem arises from a consideration of the remarkably small temperature difference ∆T = T0 − MS ≈ 45K, being required to satisfy the energy requirement of Ee ≈ 50 kal/mol to carry out the exterior mechanical work during a MT, and of the great observed magnitude of the supercooling. One of the acceptable explanations stated in [7] is that ”. . . the kinetics of the process is determined by the speed at which the transient system overcomes the energy barrier associated with the formation of the nucleation center of the new phase, as further growth of martensite crystals proceeds almost instantly.” Thus, any explanation of the magnitude of supercooling T0 − MS must inevitably consider the key thermodynamic and kinetic process parameters. In the above discussed model of adiabatic generation of a macronucleus, the heating effect Q associated with the transformation, treated in [56], can be interpreted as a result of the distribution of atomic oscillation energy E in the vicinity of new equilibrium states, among all available 3 · NN oscillatory modes of the nucleus (NN  number of atoms in the nucleus), with only a small number of polarization orientations excluded (for anisotropic deformation). We evaluate E by the assumption that during the process of nucleation, the excitation of longitudinal oscillations being polarized in two orientations (called x and y), will be predominant. Let an oscillatory mode be enumerated by a wavevector of components qi (i = x, y). Then, their contribution to E will be Eqi =
1 M ωq2 i uqi 2 NN , 2
(1.1)
where M  atomic mass, ωqi  cyclic frequency, uqi  oscillatory amplitude. Further, the relative deformation ε associated with such oscillations can be determined by the extreme condition εm =
2u 2uq = , λ/2 π
(1.2)
where λ/2 is the distance between two adjacent planes, supposed to oscillate in mutually opposed phases (λ – wavelength). We further assume the same ε for all qi , replacing ωqi by ωqi = c qi , where c  speed of sound, and consider that qx qy attain the value NN x ≈ NN y ≈ 2 rN /a (rN  radius of the macronucleus, a  lattice parameter). Then from (1.1) and (1.2): 26
E=
X i,qi
Eqi ≈
π2 rN NN Mc2 ε2m . 2a
(1.3)
At the instant of nucleation t = tN we get
E π2 ≈ rN c2 εm2 ≈ Q, NN M 2
(1.4)
where Q is the specific transformation heating effect [J/kg]. Using Q ≈ 4 · 104 J/kg (for a Fe30 Ni  alloy according to [22]) we get rN ≈ 10−7 m, a ≈ 3 · 10−10 m, c = 5 · 103 m/s and from (1.4): εm ≈ 10−3 . This way we can reasonably infer a thresholdvalue for the deformation εth of about a magnitude εm ≈ 10−3 , at least for longliving modes with quasimomenta −1 q ≈ qmin ≈ π · rN at the instant t = tN , coinciding with the final instant of the nucleation stage and with the moment of growth initiation. With respect to the effect of external stress on MT, it would be useful to compare our estimate of εm with data published in [13, 49]. The reasons for such comparison  for instance with data of the strain effect are obvious, if we consider that the term λ/2 in (1.2) plays the role of the initial length l of the sample, while the amplitude u corresponds to the incremental length ∆l, and that the quantity λmax = 2 · π/qmin ≈ (10−7 ÷ 10−6 ) m is a multiple of the lattice parameter a. In conclusion, the order of magnitude of these quantities appears to be fairly adequate for a description by continuum mechanics. Useful information can further be inferred from the mere existence of a temperature Melast (in the notion of [49] Melast is close to MS, i.e. Melast − MS ≈ 35 ÷ 40 K), the quantity Melast being such that if a MT proceeded within the temperature range MS < T < Melast it could be induced by elastic stress σm , thus satisfying the inequality σm < σy (σy – yield stress). Remarkably, an evaluation of the stressstrain curve shows that the values of σ ≤ σy correspond to strains εth ≤ 10−3 . This observation may further support our estimate of εth ≈ 10−3 for threshold deformation. Thus in the notion of a developing macronucleus, supposed to be inherently unstable in the growth process, a strongly pronounced supercooling T0 −MS is regarded as an imperative condition for the excitation of oscillations with final (peak) amplitudes (and frequencies) satisfying the condition ε > εth ≈ 10−3 . Moreover, the same condition could be used as a qualitative criterion for lattice stability (or instability) of the γ  phase at the MS  point. 27
1.4
Solved and unresolved problems on the theoretical description of the γ − α martensitic transformation
Any comprehensive reasoning on the theory of phase transitions will inevitably lead to the following two fundamental questions, as noted in [10]: 1. Why does a given phase transition occur? 2. Which is its transformation mechanism? The first question will normally be approached by investigations on the relative stability of different possible phases. In this case, the phase with lowest value of free GibbsEnergy G(P,T) will usually be in the focus of interest. A generalized expression for G is given by the constitutive expression in [60]: G(P, T ) = H − T S = U + P V − T S
(1.5)
where H, U, S, V are the commonly used specific values of enthalpy H, internal energy U, entropy S, volume V and pressure P (relating to 1 mol). A calculus of the (macroscopic) thermodynamic quantities in (1.5) within the frame of a strict (quantumstatistical) approach would be an extraordinarily complicated task, as the Gvalues of different phases differ almost inappreciably, and to the worse, any such calculus cannot be effectively simplified. Nonetheless, today there exist sufficiently clear and substantiated notions on the causes and mechanisms of polymorphic transitions in pure iron. Presumably, the hightemperature transition fccbcc (γ − δ) at Tγ−δ = 1665 K is determined by the entropy term in (1.5), as the contribution to S from atomic oscillations in the more weakly bound bcc lattice, as well as from disordered (large) magnetic moments, is relatively larger for the δphase than for the γphase [61]. The lowtemperature transition fccbcc (γ − α) at Tγ−α = 1183 K, which would appear paradox from the aspect of the oscillatory contributions of the atoms to S, can be put into relation with the reduction of internal energy of the αphase in the ferromagnetic state of order [62–64]. Taking for granted that the answers are already given, we shall refrain from dealing here any more in detail with questions related to phase stability. Of course, a constitutive solution to our initial question ”Why” related to the γ − α MT has not yet been found, as the second part of our question, being related to a ”given phase transition”, belongs to the particularities of the γ − α MT and is intimately linked up with the question for the mechanism of this particular transition. The morphological (phenomenological) features of lowtemperature martensite with habit planes {2 5 9} ÷ {3 10 15} (see 1.2) have successfully been interpreted by the crystallographic theory. A detailed description of its most important results 28
is published in [13, 18]. From a crystallographic point of view, MT are regarded as a lattice deformation process, characterized by a macroscopically invariant plane, the habit plane. This deformation includes pure latticedistortion (PLD), as well as lattice invariant deformation (LID). PLD can either be described within a pattern including two (or more) shear motions, onto which a dilatation mechanism is superimposed, or within the pattern of BainDistortion (BD) with consecutive rotations satisfying the constitutive orientational relationships. The BDpattern is shown in Fig. 1.1, which has been extracted from [13]. Imagine an elementary bct√ lattice cell (with a tetragonality of 2) being partially configured by two adjacent fcccells. Then, in order to transform that bctcell into a cubic bcccell, the bctcell has to be subjected to a compression by 20 % along its [001] axis and to a dilatation by about 13 % along its [100] and [0¯10] axis (or along its [110] and [1¯10] axis). In Fig.1.1, the principal orientations of compression and dilatation are marked by bold arrows. The densely packed (111)γ k(011)α plane is hatched. Fig.1.2 shows an inhomogeneous lattice resulting from LID in the case of shearing Fig.1.2a and twinning Fig.1.2b. It is mandatory to consider LID, because pure BD does not comprise a deformation with an invariant plane (DIP) (during DIP, one of the main components vanishes, whereas the two remaining deformation components feature opposite sign). Thus, if LID is used as a method to introduce auxiliary deformation, it is possible in some cases to attribute the bulk macrodeformation of the transformed region to a deformation with an invariant plane. Among other aspects, the twinning mechanism of lowtemperature martensite was used to prove LID, in that different volumetric fractions of twins were predicted, as confirmed later on by experimental evidence. Among the drawbacks of this approach are those mentioned in [65], as there are: The lack of physical justification for the selection of a specific mechanism of deformation, as well as ” . . . of some of the most essential principles like: attainment of minimum surface energy, minimum active shear parameter, or minimum of atomic motion.” In addition, the aforementioned phenomenological theories are not suitable to reasonably explain ”any change of a crystallographic feature of martensitic transformations in relation to changes of their composition or of transformation temperature.” The thermodynamical approach in [17, 19, 66], which takes into consideration the energy and enthalpy associated with internal stress, within a given system of coexisting γ and αphases, is mainly based on the assumption that the formation of a final structure reflects the tendency of the system to minimize its free energy (i.e. a minimum of elastic energy caused by internal stress), thus giving reasonable justification for regarding the crystallographic pattern of martensite as an isolated case of phases being in immediate contact in an invariant plane, without consideration of the appearance of mechanical stress. In addition, it explains the lamellar equilibrium shape of the crystals, particularities of their internal structure (like autocatalytic twinning) and other general features related to the emergence of crystal groups, under the conditions of a sample with free external boundaries as well as under the conditions imposed by an externally applied field of mechanical 29
tension [67–69]. An interpretation of the kinetic particularities must be based on an evaluation of: a) the level of the energybarriers which have to be surmounted during this type of growth. b) The thermodynamic driving force of the transformation. c) The role of relaxation processes in this environment. To take an example, the observed differences between lathshaped and lamellar martensite might be deducible to differences between the dominating relaxation mechanisms (i.e. slipping processes in austenite and twinning in martensite).
[1¯11]α
zα
zγ
[0¯11]γ
(111)γ
xα
(011)α
yγ
yα xγ
Figure 1.1. Conformance of austenitic and martensitic planes during a fcc → bcc Bain transformation [13]. Planes (111)γ k(011)α are hatched. Bold arrows point to orientations of compression [001]γ and tension [100]γ , [010]γ , respectively. The question about the growth mechanism will lead us into a consideration of the model of a phaseboundary and into an evaluation of its mobility. For example, in [17, 19, 70] there has been investigated a model of a phase boundary arising during a MT, with a transformation pattern characterized by an invariant plane. In Fig. 1.3, which has been taken from [19], the phase boundary is represented by a transition layer together with a transition vector S of variable size and orientation, indicating the locations of atoms (l0  thickness of the boundary layer, being about the size of several lined up lattice parameters). The term fn relates to free energy density, x  coordinate axis oriented parallel to the normal n of the invariant plane of the boundary layer, fna and ∆f indicate the magnitude of the activation energy threshold, or of the thermodynamic driving force, respectively. This representation of a phase boundary thus is akin to that of a ferromagnetic domain [71], which also includes a term related to the free energy gradient. 30
a
c
b
Figure 1.2. Reconstruction of the shape of a transformed region by additional deformation [13]: (a) = Mode of transformation; (b) = Reconstruction of the shape by means of slipping; (c) = Reconstruction of the shape by twinning.
S S = 1/2¯ S
∆f
n x
fna fn
S S = −1/2 ¯
l0
Figure 1.3. Structural pattern of a phase boundary [19] As for the MT of alloys of the Fe  Ni, Fe C systems, a realistic representation of a phase boundary would, at the first sight, have to satisfy the following two, obviously contradicting requirements: the pronounced persistence of metastable austenite at the MS temperature (see also the explanation in 1.3) implies the existence of a finite energy threshold fna . The almost temperatureindependent speed of growth of an individual martensitic crystal (at least within a wide range of temperature) is a typical feature of a thresholdless type of growth or motion. In [17, 19, 70] it is proposed to consider the mobility of a phase boundary analogous to the mobility of a dislocation through a periodic potential as determined by the lattice with its structural periodicity in n  orientation, in a similar way as that described by the FrenkelKontorovaModel. As a result, the f1a threshold is considered instead of the fna threshold, (see Fig.1.4 as taken from [19]), which separates the relatively unstable states in the boundary area (i.e. where the location of individual atoms deviates significantly from the stable location with minimum potential energy in relation to the peaks of the potential ”comb”) from relatively stable ones (i.e. the atoms are located near the bottom of the periodic lattice potential), if put into relation with the driving force ∆f . Thus for ∆f > f1a < fna 31
a boundary would move (jump) nearly unhindered over a threshold, at a speed comparable to the velocity of (transversal) sound waves, nearly independent of temperature. However it has to be considered that a calculus of the above postulated speed of propagation has not yet been performed (as this would not be a typical problem of thermodynamic analysis). Thus the postulate of a large velocity of boundary propagation still needs to be proven. Moreover, according to data published in [30, 31], the velocity of growth of martensite crystals not only exceeds the velocity ct of transversal, but also the velocity cl of longitudinal elastic waves. Thus any concept based on an upper velocity limit ct < cl would be fundamentally inadequate for the description of radial (frontal) growth of a lamellar martensitic crystal, even though an interpretation of lateral growth might be conceivable within such a concept.
S 1/2
fn fn
S¯
0 −1/2 ¯ S
fna fn
F
l0 f1a
F
∆f
¯ 0 1/2 ¯S −1/2 S
S x
Figure 1.4. Determination of the f1a threshold at the phase boundary, analogous to the Peierlsthreshold of a dislocation [19] What’s more, the assumption of supersonic velocity of martensitic crystal growth will inevitably lead into another problem: The usually observed γ − αphase boundaries belong to the semicoherent type [12]. High mobility of semicoherent boundaries usually is put into relation with the existence of parallel rows of slipping dislocations making up a boundary [72]. Under the assumption that the motion of a boundary, including that of a martensite crystal, is produced by slipping dislocations, then we must inevitably conclude that the motion speed v of such dislocations will also take place at the of sound velocity ct . We remember that the supposed motion of dislocations at a velocity exceeding ct is prohibited within the frame of a continuous model [73]. In principle however, this could yet be possible in crystals of a discrete atomic structure [74]. Moreover, we must consider that a dislocation in supersonic motion v > ct would inevitably and per32
manently emit acoustic radiation energy, due to an effect analogous to the emission of Tscherenkovradiation. In accordance with [74], it is possible to calculate the stress σ needed to maintain a dislocation speed v > ct , by the relation σ≈[
υ2 µb − 1] · 2 ct 2πa
(1.6)
where µ  shearmodulus; b  BurgersVector, a  distance between the planes of shear. For example, if v ≈ 2 ct , and b ≈ a were inserted in (1.6), then σ would exceed the theoretical yield stress ≈ 0, 1 · µ, a result which makes no physical sense. The same kind of problem would basically also appear in any investigation of shockwave propagation in solid state matter. Some alternative opinions about the role of dislocations in shockwave propagation are outlined in the papers by Wirthman, Meyers and Moor in [75]. According to Wirthman, supersonic propagation of dislocations (Smithdislocations) should theoretically be possible in conjunction with the propagation of a shockwave at a maximum stress level being equivalent to the yield strength. Meyers and Moor, whose position is based on experimental evidence however reject this point of view, arguing that dislocations generated in conjunction with a shock wave would lag behind the shock wave and soon come to a stop. Rejecting the thesis that the level of stress during the γ − α MT is close to theoretical yield strength, the motion of the phase boundary should rather be regarded as some kind of nonlinear wave process producing dislocations which at the same time set up a boundary between the phases arising immediately behind the propagating wave front. Machlin and Cohen in [76] were first to clearly formulate a wave model as a conceptual approach for resolving the martensitic growth problem. Without getting into details on the meaning of velocities, the authors of [76] propose a pattern of two sequential deformation waves. The first of the waves spreads out into radial orientations starting from a minute plateletshaped martensitic nucleus, thereby causing a homogenous deformation of a lamellarly shaped area, the surface of which (i.e. the habit plane) matches with the invariant plane. As soon as the deformation induced stress delivered by the first wave attains certain amount (presumably the yield limit), the second wave starts to spread into a direction perpendicular to the habit plane, thereby causing shear deformation (being homogenous only at a macroscopic scale). The residual inhomogeneous shear deformation completes the growth process of a martensite lamella. In principle, such wave pattern would make possible a direct interpretation of the crystallographic (geometrical) theory: The first wave produces pure lattice deformation, and the second one the required lattice invariant deformation. But in contrast to the geometrical pattern, in which the invariant (habit) plane can only arise during a combined latticevariant and latticeinvariant deformation, [76] requires that the development of a habit plane must already occur in the first step of pure deformation. Obviously, there do not exist any reasons for assuming that inhomogeneous deformation (i.e. by twinning) 33
takes place only after formation of the lamellar region. At present, there is no doubt about inhomogeneous deformation occurring during a martensitic transformation (transformation twinning according to [13]). Nonetheless, the notion of a clear distinction between two stages of crystal growth still appears to be current. Essentially, the aforementioned basic ideas are also proposed in [77]. In addition, it is postulated therein that the radially propagating wave is of the longitudinal type, leading to a MT in the central area (midrib) of a martensitic crystal. The transformed midribregions thus are about to play the role of secondorder nuclei for excitation of a transversal transformation wave, which would propagate into an orientation perpendicular to the habit plane. In conclusion, it can only be the transversal wave which initiates the growth process in the region adjacent to a midrib. The most important single factor ensuring growth initiation is the high pressure (about 7,4·109 Pa) being produced in the immediate vicinity of the midrib, due to its increase in width by about 5 %. This way, right in front of the transformation wave, short compressive and plastic shear wave pulses are surmised to move about, slowly widening until the growth process has ceased, after which the wavepulses fade down to the level of ordinary elastic waves. The whole scenario is shown in Fig.1.5, extracted from [77]. Fig.1.5 shows a crosssection of a growing lenticular crystal (the drawing plane is assumed to run perpendicular to the habitplane). The midrib is represented by a straight line, splitting the lenticular region into two symmetrical halves, while the arrows are pointing into the orientation of wave propagation. The hatched region represents the region of compressive and shear wave pulses, and the broken line intersecting the crystal indicates how an originally straight line of reference (dotted line in Fig.1.5d) is distorted during and after a MT. Using this pattern of transformation, together with the assumption that the longitudinal and the transversal transformation waves propagate at vl = cl , and vt = ct , respectively, there has been reported in [77] an equation for the shape of the surface of a lenticular crystal, which has been the final aim of that work. We would further like to remark that the notion of dislocation generation under the condition of a high level of mechanical stress being built up in the waves, as postulated in [77], is justified, whilst the motion of the boundary is not put into clear relation with the motion of the dislocations. Even though the values of vl in [77] appear to be estimated too low, and too high for vt (see also the interpretation of the data related to the speed of growth in 1.2), the qualitative model looks quite promising. However, what is obviously missing in [76, 77] is a description of the development of a midrib with an internal twinning structure, which is supposed to take up a leading role during the formation of lenticular crystals. In [31,78,79], the growth of martensite has been treated from the point of view of the shock wave theory. Lokschin also investigated the case of strong shock waves, opening up a possible explanation for supersonic speed of growth. According to estimates in [31, 78], the compressive stress or tension being developed within a 34
a
b
c
t
d l
Figure 1.5. Growth pattern of a lenticularly shaped martensite crystal [77]: (a): Plastic shear and compression waves are propagating ahead of the transformation front; (b) and (c): Crystal growth process has ceased, but abating waves of plastic deformation are still propagating in the aftermath; (d): Waves of plastic deformation faded away, after having excited elastic transverse(t) and longitudinal (l) waves. shock wave amounts to about (1, 4 ÷ 1, 6) · 1010 Pa, being about twice as large as the value used in [77], thus attaining the same order of magnitude as theoretical yield stress. Based on data published in [27], Crussard analyzed the case of weak shock waves with a speed of propagation lower than sonic speed. The common weakness of these treatises is their lack of interpretations of the extensive amount of morphological transformation characteristics. If the role of dislocations during formation and propagation of the phase boundary was not properly considered in the aforementioned models, then the motion of a phase boundary could simply be regarded as the propagation of a lonely front (called ”switching” wave in [80]), akin to a step like excitation (as shown in Fig. 1.3. To the left and to the right of such a ”switching” wave, different values of deformation εα,γ would be produced, being typical of the γ and α  phases. Such a process can usually be described on the basis of a quasilinear parabolic equation 35
(nonlinear diffusion equation), to be dealt with in Chapter 6. Let us now briefly discuss the theories focusing on the role of hyperbolic waves during a MT. Generally, these waves correspond to solutions of nonlinear equations arising from a basic linear hyperbolic equation (i.e. a classical wave equation featuring spatial and temporal derivatives of the second order) for which (harmonic) sinusoidal waves are fundamental solutions. In our opinion, the general interest on waves of this category is due to their potential for simple representations by (quantisized) totalities of phonons. Our next logical step will thus be to pass over to phonon theory, which will finally enable us to take advantage of the well developed and efficient microscopic models of solid state physics, and to establish later on an important link between microscopic and macroscopic descriptions of MT. The assertions in [81] advocate for a description of MT in the wave model. Remarkably in [81], a decidedly passive role is assigned to dislocations, including the proposal to reject a differentiation between the nucleation and growth stages, apparently justified by the lack of observable static nuclei. Thus the kinetics of any kind of MT should in general be allocated within the explosive type. (Even the case of slow macroscopic growth of a martensite crystal can easily be explained within the general notion of explosive transformation, by assuming small microexplosions occurring in sequence, with fairly long interruptions in between). In addition to the above thesis we want to point to another assertion stated in [81]: It is being proposed to interpret the particularities of the martensitic structure as a result of the interaction of a combination of one (or more) lattice oscillation modes, propagating at the velocities of elastic waves). Kayser [82] was first in trying to associate the athermal activation of explosive MT in ferrous alloys with the principle of stimulated emission of phonons, which led to the conceptual notion of a phononmaser 2 effect coming into being at a given amount of supercooling below the equilibrium temperature T0 of both phases. The optimum frequency assumed in [82] is the Debyefrequency νAM ≈ 1013 Hz, while the associated phonon energy hνAM would equate with the free energy difference GA − GM (related to one atom) between metastable (premartensitic) austenite GA and stable martensite GM . The radiation system is supposed to be given by the lattice atoms, which, during the MT, perform a coordinated (cooperative) jump from an energy level GA down to a level GM , simultaneously with a structural transformation. As the initial occupation of the GM  level is assumed to be nil (i.e. when the atoms make up the austenitic lattice) and if the condition GA > GM was given, then the starting scenario would correspond to the utmost possible inversion between the occupations GA and GM . The propagation of the emitted phonons through the transforming lattice is supposed to proceed in such 2
Editorial note: Phononmaser and laser research and development proceeded almost in parallel in their initial theoretical and experimental stages in the sixties, but phononmaser development was abandoned later on due to lack of practical need for phononmasers. See e.g. Phys. Rev. Lett. vol. 12, pp. 592595, May 1964.
36
a way that the amount of phonons would steadily increase, resulting in a steadily increasing amplitude of the acoustic wave, up to a magnitude enabling the creation of lattice defects. Kayser also proposed to interpret the zigzag structures, comprising a macroscopic group of relatively small martensite crystals, grown and confined within the space enclosed by two larger, preexisting lamellae, as a sequence of multiple reflections of stimulated phonon radiation between the lamellae. Fig. 1.6a shows a schematic illustration of the observed zigzag structure (being more commonly known in metallurgy under the term (”lightning” or ”lace” structure), whereas Fig. 1.6b shows the Kayserpattern (arrow lines). Typical of this structure are two groups of lamellae: Any two lamellae selected from the same group are parallel, whilst lamellae belonging to different groups adjoin at an acute angle. We would however like to remark that any two of such totalities of lamellae cannot be built up only on the basis of reflections between nonparallel larger lamellae. Thus the interpretation by Kayser cannot be regarded as consistent. Obviously the structure shown in Fig. 1.6b represents nothing more than an observed phenomenological rule, which however does not reconcile with the classical laws of reflection. The general definition of the radiating system as well as of the radiation frequency also appear to be contestable. In fact, in a well developed twolevel maser (i.e. see [83]), pairs of inversely occupied energy levels would simultaneously exist at certain points of space, and the active radiating subsystem normally is subjected to the FermiDiracStatistik. However in the Kayserpattern, the physical state corresponding to GM energy would only potentially be possible, as the atoms are in a state with GA energy. Furthermore, shortwave phonons generally have a highly pronounced rate of decay, corresponding to short average lifetimes and ranges, thus the argument for the possibility of being generated by the proposed mechanism appears fairly improbable. A more promising description of the emission of radiation in conjunction with atomic jumps is obviously set up by the concept of vacant atomic states, being closely linked with the physical state of quenched austenite (i.e. see [84]). An explanation of the mechanism of phonon generation has also been tried by Zhang in [85]. Refraining here from further and detailed enumeration or discussion of the various theoretical possibilities, we can conclude that, in the aforementioned papers, a more or less reasonable concept of the microscopic mechanism of phonon generation during MT is missing. This can be easily realized by comparing points 2 and 3 of Table 1.2 (next page) which has been borrowed from [85]. In Table 1.2, it has been tried to draw some general analogies (theoretical and phenomenological) between the laser or maser effect and the MT. Moreover, we assume that the requirement of a critical rate of cooling down to MS (pt. 3 in Table 1.2) is not mandatory. In order to suppress diffusion, it would suffice to rapidly pass through the hightemperature region, where diffusion processes predominate, whilst further cooling can succeed at a rather slow rate. For a description of the lateral displacement 37
a
b Figure 1.6. Schematic structural arrangement of typical martensite crystals: (a): Totality of the lenticularly shaped twinned crystals in a realistic pattern [24]; (b): Idealized pattern of multiple reflections of excited phonons [82]. wave, Zhang proposes a wave equation borrowed from LaserTheory: 1 ∂ 2 ξ~ ∂2p ∇ ξ+ 2 2 =− 2, c ∂t ∂t 2~
(1.7)
where: c  speed of sound; ξ~ = [∇, u]  axial vector of rotation is correlated with the antisymmetric rotation tensor [86]; u  vector of translational displacement; ∇  gradient operator in a spatial frame of reference; p  analog to the polarization~ where vector of a lasing medium as used in lasertheory, given by p = c−2 εˆξ, εˆ  matrix of lattice distortion during a latticetransformation. As reported in [85], there have been performed investigations on the characteristics of stationary wave amplitudes, using a phenomenological approach by the commonly known VanderPol and Duffing equations, under the assumption that, in a harmonic approximation, the square of oscillatory frequencies exhibit a critical dependence on temperature, thus resembling a typical characteristic of ”SoftModes”, i.e.: ω02 ∼ (T − T0 ). A discussion of reports related to investigations on the effects of externally applied magnetic fields and of magnetic ordering in austenite on MT will be subject of Chapter 5. 3
A laserresonator, being a characteristic part of most lasers, is not an absolute requirement for realization of laser/maser radiation, as in some radiating systems comprising a sufficiently high
38
Table 1.2. Analogies between the Lasereffect and martensitic transformations Laser 1. Coherent photons 2. Occupational inversion 3. Under the conditions of an occupational inversion, coherent photons are emitted during the transition of electrons to the lower energy level.
4. Resonator3 5. VanderPolEquation
1.5
Martensitic Transformation 1. Coherent phonons 2. Mechanism ensuring a (potential) possibility for stimulated emission of phonons 3. Under given conditions (critical rate of cooling, supercooling down to a certain temperature), the transition of atoms occurs from their initial lattice position of the hightemperaturephase into lattice positions of the low temperature equilibrium phase. Simultaneously with this phase transition, coherent phonons are emitted. 4. Lattice boundary, plane lattice defects, grouped point defects, dislocations etc. 5. VanderPol and DuffingEquation
General physical tasks and objectives
A brief review of existing publications dealing with the spontaneous MT of paramagnetic austenite lead us to the conclusion that the waveapproach, though being regarded as most promising for further development of a microscopic dynamical MTtheory and description of the γ − α MT, presently is only weakly developed. At first, the mechanism of wavegeneration (and amplification, respectively) in the stage of martensite growth has to be determined, and secondly, the substantial variability of crystallographic characteristics of Martensite must be interpreted in the wavemodel, as without such an interpretation, the waveapproach would be largely invalidated with respect to materials science. 1. Let us assume that the process of fast development of a macronucleus of a lateral dimension of about 2 r ≈ (10−6 ÷ 10−7 ) m (see 1.3) occurs within a period of tN ≈ (10−9 ÷ 10−10 ) s. Then it is fairly easy to realize that this postulate represents some kind of specification going beyond the normally used model of fluctuation nucleation. Let us further assume that population inversion density (thresholdinversion), a ”singleshot” or ”superradiance” (Dicke) laser/masereffect can emerge. (Superradiance however mostly is an undesired, potentially destructive and hardly controllable sideeffect in many highintensity lasers.) Moreover, there have also been discovered innumerable cosmic sources of (continuous) laser/maser radiation, clearly demonstrating that laser/maser activity is a natural effect, not requiring sophisticated laboratory equipment like a resonator at all.
39
certain spatial scale l can be defined along an orientation perpendicular to the axis of nucleation, in such a way that l would be complementary to r, as shown in Fig. 1.7. Then l indicates the width of a specific region (we call
µ − µγ
T − Tγ
Tα − Tγ
0
γ  phase
x
α phase
l µ α − µγ
l
γ phase
2r
Figure 1.7. Assumed distribution of temperature T and chemical potential µ at the instant of macronucleation of the αphase. The xaxis is oriented perpendicular to the axis of nucleation. it Bγ−α ) characterized by significant inhomogeneities of such fundamental macroparameters like temperature T and chemical potential µ 4 . In other words, the magnitudes of the spatial gradients ∇T and ∇µ in the a.m. Bγ−α region are relatively large. In order to evaluate the size of l, we start from the assumption that heat liberation as well as a remarkable volume change simultaneously occur in the region penetrated by an elastoplastic wavefront (being closely linked up with the γ − αtransformation). Let us further assume that the wavefront propagates at a speed of c ∼ 103 m/s, through a region transforming within a period tN , rendering: l ∼ c · tN ∼ (10−6 ÷ 10−8 ) m (see also an evaluation of l under 6.3.3). The order of magnitude of the quantities ∇T , ∇µ can easily be assessed from the relations: ∇T ∼
∆T Tα − Tγ ≈ , l l
∇µ ∼
∆µ µα − µγ ≈ . l l
(1.8)
The quantity ∆T is comparable with the degree of supercooling T0 −MS , i.e., ∆T ∼ 100 K (see also the beginning of 1.2) and, as a result, the temperature gradient would become ∇T ∼ (108 ÷ 1010 ) K/m. In assessing ∇µ, we take into consideration that the specific volume of the αphase increases due to the volumeeffect, and that simultaneously the concentration of electrons n, and thus also µ, decrease. Let µ ∼ n2/3 be the generally used relation between µ and n in the freeelectron model (see for example [87]). 4
The designation µ, having been used in 1.4 as the designation of the shearmodulus, will from now on exclusively be used as the designation of chemical potential.
40
Then we get ∆µ 2 ∆V =− . µ 3 V
(1.9)
For an assumed ratio of volume change ∆V /V ≈ 2, 4 · 10−2 , being typical of the Baindeformation, and with µ ∼ 10 eV, we get from (1.9): ∆µ = 0, 16eV, being equivalent to 1860 K at a temperature scale. This way, the quantity ∇µ/kB (kB  BoltzmannFactor) can easily exceed the value of ∇T by one order of magnitude, for the same value of l. It should be noted that our estimate of ∆µ with adequate consideration of the volumeeffect should be 2 essentially correct, due to the use of the relation µ ∼ n 3 for a subsystem of selectrons. Of course the same results can be obtained analytically for a delectron subsystem (see 4.5). The remarkable gradients ∇T and ∇µ however require further analysis under nonequilibrium conditions of the electron and phononsubsystems of the Bγ−α region. A substantiation of such nonequilibrium conditions will then enable us to confine our further task to the determination of the mechanism of generation (or selective amplification) of phonons by nonequilibrium electrons. 2. We recall that the physical basis of the masereffect is that the processes of stimulated absorption are outnumbered by simultaneously occurring processes of stimulated emission in a given region of a system, provided an inverted occupation is given in the radiating system (i.e. in a lasing system the occupation of higher energy levels must substantially exceed that of the lower energy levels). If we choose a group of electrons as a radiating system and further assume that the band model is correct, then it will be straight forward to conclude that inversely occupied energy levels are present wherever electronic flows exist, provided their assumed energy levels are correct. Let fjk denote the nonequilibrium distribution function of electrons in the state (j,k), where j is a band number, k is the wave vector and ~ k the quasimomentum ( ~  Planck’s constant) associated to a given electron of energy εjk . Let us now regard the graphs pertaining to a nonequilibrium distribution of electrons (ref. i.e. [87]) being already known from the theories of heat ( for ∇T 6= 0) and of electrical conductivity (for ∇µ 6= 0). In Fig.1.8, an equilibrium function fk0 (normal line), and a nonequilibrium function fk (dotted line) are plotted, the degree of nonequilibrium being determined by the quantities ∇T Fig.1.8a and ∇µ Fig.1.8b. In case (a), it is clearly obvious that two oppositely oriented electronic flows arise (namely, electrons with energy ε > µ predominantly move from the warmer to the cooler regions, i.e., against the temperaturegradient ∇T , whereas electrons with ε < µ predominantly move parallel to the direction being set by ∇T ). 41
Thus, if the quasimomentum ~ k of electrons is oriented antiparallel to the temperaturegradient ∇T , a nonequilibrium term ∆fk > 0 for εk > µ, with ∆fk < 0 for εk < µ, has to be considered. And viceversa, if ~ k is oriented parallel to ∇T , then ∆fk > 0 for εk < µ and ∆fk < 0 for εk > µ. Thus the states with quasimomentum ~ k oriented antiparallel or parallel to ∇T would be inversely occupied above or below the Fermilevel µ. In Fig.1.8a, two such inversely occupied energy levels are plotted by thin horizontal lines, in relation to the Fermi level µ. In Fig.1.8b, the particular case of parallel electron motion towards decreasing chemical potential, i.e. against ∇µ, is illustrated, where the sign of the nonequilibrium addend to the equilibrium distribution function fk0 is independent of the relation between εk and µ, i.e.: ∆fk > 0 for k ↑↓ ∇µ, and ∆fk < 0 for k ↑↑ ∇µ. The above concept of formation of inversely occupied states related to the nonequilibrium conditions during the stage of growth of the αphase has been proposed in [88–90]. 3. Our investigation of the generation of elastic waves by nonequilibrium electrons should most reasonably start with a definition of the conditions required for the excitation (or amplification) of a plane wave of atomic displacement, in the ideal case of a crystal of infinite dimensions, with homogenous and stationary temperature and chemical potential gradients. From the point of view of quantummechanics, a plane wave of relative atomic
~k ′ ↑↑ ∇T ~
µ
1
~k ↑↓ ∇T ~
0 a ~k ′ ↑↑ ∇µ ~
µ
f (ε)
f (ε) 1
0 b
µ
ε
µ
ε
~k ↑↓ ∇µ ~
Figure 1.8. Equilibrium (normal line) and nonequilibrium (dashed line) electron energy distributions: (a): ∇T 6= 0; (b) ∇µ 6= 0 42
displacement: u(r, t) = u0 cos(ωq t − q r) represents the macroscopic effect of a totality of coherent phonons of energy ~ωq , with wavevectors q. This means that the generation of waves by a masermechanism would become feasible whenever a macroscopic number of inversely occupied electronic states (k, k′ ) was existent, and transitions between them would predominantly result in the emission of phonons, in accordance with the laws of energy and quasimomentum conservation: εik − εi′ k′ = ωjq ,
(1.10)
k − k′ − q = 0, Q.
(1.11)
In (1.10), j is the index of the phononbranch, whereas the equality of (1.11) depends on whether the electronic transitions belong to a normal ”Nprocess” or to a ”Uprocess” [87] (see Fig.1.9). For an Nprocess, the right side of
ε ~q
µ −km
k~′
a ε
~k
km ~q
µ −km
b
k~′ ~k km
ε
~q
µ −km ~k
c
k~′ km
Figure 1.9. Onedimensional pattern of Nprocesses (cases a and b) and Uprocess (case c) km – upper momentum limit in the 1st BZ, q – phononmomentum. The energy difference εk − εk′ is not considered, µ – Fermilevel. (1.11) vanishes, while for a Uprocess, the right side of (1.11) is the vector Q 43
of the reciprocal lattice. This way, our task is equivalent to finding macroscopic sets of pairs of inversely occupied electronic states in kspace, which would have to be equidistant to satisfy the conditions of (1.10,1.11). The main objective in processing with this task will thus be the identification and classification of such pairs of electronic states, starting with the definition of points located in a surface separating inversely occupied states in kspace. Thus it will be important from the outset of our analysis, to identify and preselect such lattice oscillations being characterized by an implicit tendency to become unstable under nonequilibrium conditions. This analysis will be based on the assumption that the structure of the electronic spectrum in the transforming Bγ−α region maintains all relevant properties of the electronic spectrum of the fccphase of iron, this being a significant prerequisite from the viewpoint of the phonongeneration mechanism. If we think of a MT as the manifestation of a particular kind of latticeinstability, it would be reasonable to identify some key features of solidstate instabilities in general. Firstly, it can be stated that, except for some specific aspects of nonequilibrium states, basically the same  finally stated particularity of an electronic spectrum is used to explain latticeinstabilities like the Peierlsinstability of a threedimensional lattice, as well as during a variety of electronic and magnetic phase transitions, within the frame of a wave concept for charge and spindensities [4, 91–94]: The key point thus is: The macroscopicity and collectivity of a number of electronic states, corresponding to (1.10, 1.11). In fact: For the presented examples, there is a requirement for the existence of more or less large regions on the Fermisurface which must nest during a translation by a given vector q. This very vector q thus characterizes the resulting structure. The existence of such particularities must manifest itself through the appearance of densitypeaks of the electronic states in the proximity of the Fermienergy µ [95–97]. Of course, the pairs of electrons that will attract our particular interest later on, must also have energies near µ. 4. By analogy with a photonmaser [98], it can be expected that, in order to realize a phononmaser, mere satisfaction of the thresholdcondition Γκ , (1.12) W 2 R would be sufficient, which already considers that the inverted initial difference of the σ0 populations has to exceed a given threshold σth . This threshold value thus is proportional to the inherent attenuation Γ of radiating electrons, as well as to the rate of damping κ of generated phonons, and inversely proportional to the square of the matrixelement W of electronphonon interaction, as well as to the number of pairs of equidistant electronic states R. It should be noted that DebyePhonons turn out to be incompetitive, due to σ0 > σth =
44
their high attenuation in relation to the attenuation of phonons with longer waves, as indicated by (1.12). 5. It has to be clearly distinguished between a dynamical instability, as manifested by the excitation of elastic waves (in accordance with (1.12)) and the latticeinstability arising as soon as the waves attain a threshold amplitude of εth ∼ 10−3 , as required to initiate plastic deformation (see 1.3). Thus, in order to materialize the lattice instability to be dealt with here, a more demanding condition than that of (1.12) has to be satisfied. 6. As the γ − α MT of ferrous alloys occurs in a wide range of concentrations of its other component (s), causing significant variations of the MS temperatures (from MS < 103 K, for low Niconcentrations, down to MS < 4, 2 K, for 34% Ni in a Fe  Ni  System), we have to identify a specific criterion for an effective working principle of phononmaserexcitation, which must be valid for the observed wide range of temperatures and concentrations. The specific difficulties arising from this task can most easily be overcome by a twoband model of the electronic spectrum of a metal, comprising s and d electrons (a more comprehensive definition of this task will be given under 4.1). 7. After having established a conceptual notion of a phononmaser for single wave generation, let us now get into an interpretation of some morphological characteristics of martensite. It would be most convenient to select the habit plane as a basic characteristic of a MT, as the habit plane is unequivocally linked up with a MT, as already mentioned under 1.2. For further interpretation of MT, it will be convenient to start with an outline of the following geometrical representation, which will play a key role in our further analysis: Imagine a straight line of fixed (nonrotating) orientation, moving with a constant velocity relative to an inertial reference frame (associated, for example, with crystal axes h100i). As a flat surface can geometrically be defined as the location of all points in space through which such a line has passed, then this line in motion will generate a plane. (Analogously, a line can be generated by the trail of a moving point imprinted in a given plane). In our next step, we assume that the moving line itself is defined and generated by the geometric locus of a moving intersection of two flat (nonparallel) wave fronts (i.e. with noncollinear wavevectors). (The idea of using a combination of waves has first been expressed in [81]). Further substantiation of the wave characteristics should aim at defining the class of waves (i.e. longitudinal or transversal), their direction(s) of propagation, and their phaserelationships. It can however be anticipated that the combined action of such waves might suffice to build up favorable conditions for a structural transition. With respect to the γ − αtransformation, longitudinal (or quasilongitudinal) waves, supposed to propagate near to the 45
orientations h001i, h110i will be selected. In addition and in accordance with the pattern of Baindeformation (see Fig.1.1), let us further suppose that the growth of a martensite lamella proceeds by progressive unification with its adjacent areas, which are subjected to the synchronized dilatational and compressive action of the waves intersecting them. In Fig.1.10, two selected perpendicular directions of wave propagation are marked by indices 1 and 2, while the velocities and lengths of the two waves are marked by c1 , c2 , λ1 , λ2 , respectively. The hatched crosssections represent the areas of favorable transformation conditions with respect to the orientations of compressive(acting in direction 1) and tensile stress (acting in direction 2). Each of the waves is shown at a given starting time t0 and at a somewhat later instant t. Obviously in Fig.1.10, the area enclosed by the bold lines represents an idealized crosssection of a lamella with an approximate width of (1/2)λ1,2, thus resembling a prototype image of a growing martensite lamella.
2
1λ 2 1
1λ 2 2
c~2 1
c~1
~c
Figure 1.10. Fundamental growth pattern of a martensite lamella in the notion of two flat longitudinal waves propagating perpendicular to each other: c1 , c2 – wave  velocity, λ1 , λ2 – wavelength. It is easy to conceive from Fig.1.10 that the hatched area of wavesuperposition, as well as the intersecting area of the wavefronts, are simultaneously propagating at the velocity equivalent to the vectorsum (i.e. 46
geometrical sum) of their individual velocities c1 , c2 5 , i.e. q c = c1 + c2 , c = c = c21 + c22 .
(1.13)
As the value of c, on the one hand, characterizes the frontal speed of growth of a martensite lamella, and on the other hand can exceed the longitudinal velocity of sound in direction of c in Fig.1.10, it is possible in principle to explain this way the aligned supersonic growth of martensite crystals (being controlled by a pair of ordinary longitudinal waves), thus inherently representing an important kinetic particularity of the growth stage. This interpretation was proposed for the first time in [99]. We should also keep in mind that the dominating role of longitudinal waves in the formation stage of midribs was postulated in [77] too. If, on the one hand, the types of generated waves were put in relation with the particularities of the electronic spectrum and on the other hand, with the morphology of the end product, then we could expect new explanations of structural and kinetic particularities of the MT (including the effects of changes in concentration of the second component), which might be complementary to some important conclusions drawn from thermodynamic analysis of MT. 8. After having convinced ourselves of the ”functionality” of a twowave pattern, we shall deal in our next step with the various implications related to the coordinated propagation of displacement waves in the model of ”switching waves”, as we will call the isolated, stepshaped fronts of temperature, chemical potential and distortion. This might finally consolidate our understanding of the key phenomena associated with the motion of the interface of a martensite crystal in the growing stage. The following chapters will mainly be devoted to the solution of the tasks defined in above subpoints 3 to 8. In brief, the ultimate objective of this work is to analyze and understand the growth stage of a martensitic crystal during the γ − αtransformation of ferrous alloys, within the conceptual frame of a selforganizing process, during which the mechanism of generation (and amplification) of latticedisplacementwaves by means of nonequilibrium electrons will play a dominant role. To avoid any misunderstandings when reading this monograph, the author recommends to bear in mind that different physical quantities may sometimes be denoted by one and the same symbol. For this reason, the indices appended to symbols, as well as the ”local” definition of abbreviations, will normally be introduced in the ”local” text and should be duly considered. Thus in one instance, εk may represent the energy of an electron of wavevector k, whereas ε may represent linear deformation, and ε˜ represents rel5
In case of nonorthogonality between c1 , c2 , the velocity c would deviate from (1.13)
47
ative volume deformation. Vectors will be represented either by bold letters or by an arrow placed above a letter.
48
Chapter 2 Particularities of an electronic energy spectrum as required for realization of a PhononMaser 2.1
The Hamiltonian Problem
In accordance with No. 1 and 2 of point 1.5 of this monograph we associate to each state of an electron a bandindex j and a wavevector k. Let us further assume that the basic characteristics of the bandstructure of γ  iron will essentially also apply to other ferrous alloys with fcclattice, at least in a coherent potential approximation [100, 101] (also see [102]). Thus our consistent first step will be to analyze the dynamical characteristics of the electronphonon system under nonequilibrium conditions, within the frame of energy of the band spectra of the involved electrons and phonons. We choose the standard formulation of the Hamiltonians for noninteracting electrons He and Phonons Hp , respectively He =
X
εjk a+ jk ajk ,
(2.1)
1 ~ωiq (b+ iq biq + ), 2
(2.2)
jk
Hp =
X iq
+ where a+ jk , ajk , biq , biq  are the creation and annihilation operators for electrons and phonons, respectively. Accordingly, the acoustic branches of the phonon spectrum with frequencies ω and wavevectors q will be enumerated by i = 1,2,3. In consideration of the predominance of singlephonon processes during electronphonon interactions, it is justified to use the Fr¨ohlichHamiltonian Hep as interaction operator, being linear in the operators b+ and b:
49
Hep =
X
+ ∗ + + Wiqjj ′ biq ajk aj ′ k′ + Wiqjj ′ biq a ′ ′ ajk . jk
(2.3)
qkijj ′
In this case the quasimomenta obey to the conservationlaw (1.9b), and Wq is the matrixelement pertaining to electronphonon interaction (Wq * is complexly coupled to Wq ). In the tight binding approximation it is possible to get an estimated value for Wq by limiting the calculus to a linear reduction of the resonance integral G, with respect to atomic displacements, where the magnitude of G determines the width of the electron band [92]. For q < qmax with qmax ∼ π/a, near the boundary of the 1st BrillouinZone (BZ), we get for Normal (Nprocesses) as well as for Umklapp (Uprocesses):
~ Wq ≈ i 2MNωq
12
G(eq , q),
(2.4)
where M  atomic mass, N  number of atoms, eq  phonon polarization vector, i imaginary unit in (2.4) (we omitted the band and branch indices). Apart from the Hamiltonians (2.1)(2.3), the complete Hamiltonian of system H would also have to take into account electronelectron interactions Hee as well as anharmonic phononphonon interactions Hpp , the explicit form of which will however not be used further.
2.2
Form of a nonequilibrium addend to the electronic distribution function and definition of points separating inversely occupied states in a onedimensional electronic spectrum
The task related to the identification of pairs of potentially active electronic states (ES) being involved in the generation of phonons (see subpoint 3 under point 1.5) requires that some additional conditions have to be satisfied, besides those already defined in (1.9). Above all we have to remark that in the context of this monograph, the notion ”potentially active” addresses the population inversion of pairs of ES under nonequilibrium conditions in a transforming lattice. As a population inversion of the kind to be discussed here always coexists with electronic flows, it can be anticipated that the uppermost inversion between pairs of ES will only be realized for such orientations of the groupvelocities vk ↑↓ vk′ of electrons (with wavevectors k, k′ , respectively) being mutually opposed to the relevant gradient of a locally existing spatial inhomogenity. It is easy to convince ourselves of the correctness of this latter statement by writing out a stationary nonequilibrium addend fk − fk0 (for stationary and ho50
mogenous temperature and chemical potential gradients), as determined by the standard kinetic equations of electronic populations fk and using the relaxation time approximations presented in [87]. Our determination of relaxation time τ will be based on the consideration that the impactintegral can be replaced by expression (f − f 0 )τ −1 , where τ is the average relaxation time to equilibrium distribution f 0 . fk −
fk0
∂fk0 yk τ ~ ), ≈ (vk , ∇T ∂yk T
(2.5)
∂fk0 τ ~ (vk , ∇µ). ∂yk kB T
(2.6)
fk − fk0 ≈
In (2.5) and (2.6) fk0  FermiDistribution fk0 =
eyk
1 , +1
yk =
εk − µ , kB T
(2.7)
kB  BoltzmannFactor. It immediately follows from (2.5) and (2.6) that the nonequilibrium addends in brackets simultaneously change their own signs with a change of the orientation of vk , as indicated by the change of sign of the respective scalar products ~ ) or (vk , ∇µ). ~ (vk , ∇T Bearing in mind that ∂fk0 /∂yk < 0, we can easily note the correspondence of equations (2.5) and (2.6) with Fig. 1.8. The requirement of antiparallelism vk ↓↑ v′k bears a more generalized character than the singular requirement of antiparallelism for quasimomenta ~k ↑↓ ~k′ of a pair of ES, as indicated under subpoint 2 of point 1.5. The requirement k ↑↓ k′ is actually satisfied for N and Uprocesses, near the lower and the upper edge of an energy band (cases a and c in Fig.1.9). However it would not be satisfied if an Nprocess occurred at an intermediate location (case b in Fig. 1.9), whereas the requirement vk ↓↑ vk′ would be satisfied in any case. Obviously, a consideration of the onedimensional spectrum Fig. 1.9 shows that mutually opposed velocity orientations correspond to pairs of ES separated by a point corresponding to a quasimomentum p (see below) for which the energy distribution ε(k) features an extreme value. This means that for k = p the group velocity vk =
1 ∂ε(k) p ~ ∂k
vanishes (with p = 0: in case a; p = km : in case c; and 0 < p < km : in case b). This way it will be convenient to select pairs of ES in onedimensional kspace by looking for points p corresponding to equilibrium population, which in this case separate the states k and k′ of an ESpair. 51
2.3
Definition of boundary surfaces separating inversely occupied states for a 3dimensional electronic spectrum
We shall now apply the results of point 2.2 for the case of a 3dimensional electronic spectrum. Let R(q) = {iki, i′ k′ i} be sets of equidistant ESpairs satisfying the conditions of (1.9), which at the same time are potentially active during the creation of phonons with quasimomenta ~q. As already discussed under subpoint 3 of point 1.5, the contribution of stimulated radiative transitions between ES within a set R = {ki, k′ i} can in some instances become a macroscopic quantity, provided that the number of ESpairs in R also is a macroscopic quantity and a population inversion of the majority of such pairs does exist. For simplicity the radiative transitions are supposed to be confined to one electron energy band, and for this reason the band indices will be omitted further on. In the case of an inhomogeneous spatial electron distribution, a population inversion would be ~ existed possible if ESpairs with antiparallel components of velocities v = ~−1 ∇ε along certain directions. This requirement could essentially be satisfied if the ES belonging to one pair were separated in kspace by certain geometrically defined boundary surfaces, including planes, which we shall generally denote as Psurfaces. In such case the general condition (v(k), n(k)) = 0
(2.8)
will apply. Here n(k)  unit normal vector in point k of surface P. This enables us to allocate to each of the Psurfaces a totality of ESpairs with antiparallel velocity components being collinear to the axis of n, being localized in the proximity of a layer with thickness ∼ q (we assume that q ∼ (10−3 ÷ 10−1 )π/a, a  latticeparameter). However, not all of the Psurfaces actually determine a set of ESpairs, as the general requirement of macroscopicity of the number of inversely occupied ESpairs, as well as the need of compatibility with (1.9) have to be equally met. Let a given orientation of the spatial inhomogeneity be denoted by e. Then, in the proximity of those points of the Psurface where n is collinear to e, an inverted population (IP) of ESpairs should actually exist, as in the qproximity of these points the existence of states with antiparallel velocity components along the orientation determined by e would be inevitable. Obviously, the number and density of these specific points mostly depend on the shape of the Psurface, and attain a maximum in the case that the Psurface is a plane. For this reason, among the totality of Psurfaces, the subset of Pplanes (defined by n = const) will be highlighted. By definition, the Pplane is a plane in which the velocity component vn (along to the normal n of the plane) vanishes for all points of the plane. Obviously, planes satisfying this specific definition match with the symmetryplanes of the reciprocal lattice. (We recall the classical rule of reflection which simply states that all normal 52
velocity components conserve their magnitudes and only change their signs, before and after reflection at a plane.) Consequently, on the points of a symmetry plane, the velocity v (as an invariant during a reflective transformation) does not feature nonvanishing components collinear to the normal n of that plane. Of course such symmetry considerations do not exclude in general the possible existence of Pplanes not coinciding with symmetry planes. For this reason we need to find certain specific equations which may enable us to determine such P planes not being defined by symmetry considerations alone, but still being in accordance with the dispersion law. It should be noted that in case that a surface is a Pplane, Eqs. (2.8) must be satisfied for all points of this plane and the next relationship (2.9) occurs ~ (n, dv)p = (n, (dk, ∇)v) p = 0,
(2.9)
where dk corresponds to the requirement (dk,n) = 0. It is further possible to define two independent vectors dk = dk1 , dk = dk2 . Supposing that dk1 = [n, v]p dl and dk2 = vp dl, then we get from (2.9): ~ ~ (n, ([n, v]∇)v) p = 0, (n, (v, ∇)v)p = 0.
(2.10)
If we write the equation for the Pplane in the form (n, k) = C, then it will be possible to find the normalvector n and the constant C by resolving (2.8) and (2.10) for the components of n and C with a given value k = k0 corresponding to the requirement v(k0 ) 6= 0. The vector k0 , which determines a point in the Pplane, possesses two independent components, which can be chosen arbitrarily. For practical reasons however it is more convenient to choose k0 in such a way that Eqs. (2.8) and (2.10) attain their most simple form for k = k0 . In the particular case of a curved surface P, both its normal vectors n and the velocity vectors v change their orientation from point to point, with respect to the orientation of e. Thus the number of ESpairs with antiparallel velocity components ve (collinear to e) located in the qlayer can be small. And vice versa, from the point of view of a population inversion, only such specific ESpairs are highlighted whose mutually antiparallel velocity components are oriented collinear to the local spatial inhomogenity e. In kspace, such ESpairs are separated by boundary surfaces of a different category (we denote them by S or Ssurface) for which (v, e) = 0.
(2.11)
This means that at any point in S, the projection of v onto e vanishes, i.e. v⊥e. According to (2.11) the surface S comprises the geometric loci of all singularity points (i.e. the extremes and flex points) of a function ε(k), if k varies parallel with e. Obviously, the scalar products (v(k), e), (v(k′ ), e) will attain different signs for each pair of points k, k′ located at opposed sides of S, but still remain in the proximity of S (i.e. where k − k′  ≤ 0, 1π/a), provided the intersection of the 53
vectors k − k′ with S corresponds to a relative extreme of the function ε(k) in such ~ s 6= 0. Let (k − k′ , ∇)v ~ intersections, i.e. for (k − k′ , ∇)v s = 0 define a flex point of the function ε(k) on the surface S. Then, in the proximity of such a flex point, there will not occur a change of sign of the scalar product (v(k), e). Consequently, ESpairs k, k′ corresponding to such flex points will not be considered further. The equations of surfaces S can also be written in a form not explicitly depending on e. It will be reasonable to use such a notion when searching for certain Ssurfaces with specific characteristics. Doing this way, the e vectors will not be given from the outset, but can be derived from the already known equations of an Ssurface. We note that in any point of the Ssurface, the velocity vectors v(k) according to (2.11)  are oriented parallel to a fixed plane. Consequently, if three arbitrary points in the Ssurface are defined by vectors k, k1 , k2 we get (v(k), [v(k1 ), v(k2 )]) = 0.
(2.12)
Assuming that k1 = k + ∆k, k2 = k + ∆k′ , we can develop (2.12) by powers of ∆k, ∆k′ , however confining our decomposition of v(k1 ), v(k2 ) to the linear terms. (W(k), [∆k, ∆k′ ]) ≈ 0, where
1X ∂v ∂v W= ei εijn v , , 2 ijn ∂kj ∂kn
(2.13) (2.14)
and e1 , e2 , e3 are the orthogonal unit vectors of a righthand Cartesian frame of reference, with εijn = (ei , [ej , en ]). If ∆k, ∆k′ → 0, then the vector [∆k, ∆k′ ] adopts the orientation of the normal n of the surface S in point k. For this reason, the vector [∆k, ∆k′ ] can be replaced by n when reaching the limit ∆k, ∆k′ → 0 in (2.13). In result, we obtain the general equation for the Ssurfaces we were searching for: (W(k), n(k)) = 0.
(2.15)
In our specific task of search for and identification of the subset of flat Ssurfaces, we shall essentially use (2.15). Formally, our task of finding such planes, determined by a vectorfield W(k), is equivalent to the task of finding Pplanes associated with a velocityfield v(k), as (2.8) and (2.15), which define both the P and S surfaces, are formally equivalent. Thus their resolution will also lead to a resolution of Eqs. (2.8), (2.10), only by replacing v by W. By way of illustration let us analyze a cubic (fcc) lattice, using the definition of the basis vectors of the real and of the reciprocal lattice given in [103]. This will then enable us to use the simplest dispersion law in the tight binding approximation for fcc lattice [104]: ε = ε0 − 2ε1
X ij
(1 − δij ) cos ηi cos ηj , 54
(2.16)
where ε0 , ε1  constants, ηi = (aki /2), a  latticeconstant. In this case, the set of Pplanes will be confined to planes of symmetry with ki = 2mi (π/a), ki ± kj = 4mij (π/a), i 6= j, i, j = 1, 2, 3; mi , mij = 0, ±1,. . . . In our further search for Splanes, it will be convenient to distinguish between the following 2 variants of planes: 1) planes oriented parallel to the coordinate planes (or axes) of the lattice and 2) planes intersecting the coordinate planes or axes. The subset of planes oriented parallel to the coordinate planes can be defined by the condition ki = ci , (i = 1, 2, 3). The constants ci can be determined from the relation 1 1 (n,W)ki =ci,kj =kl =0 = 2B sin ( ci a)(1 + cos ci a)2 , 2 2
(2.17)
where B = 2a5 ~−3 ε31 , being satisfied for ci = 2mi π/a, mi = 0, ±1, ±2,. . . . The specific planes oriented parallel to a coordinate axis, for example the k3 axis, can be defined by the condition n1 k1 + n2 k2 = c12 . The unknown quantities n1 , n2 and c12 are determined by (n,W)k3 =0 = 32BD 2 K(n1 sin η1 + n2 sin η2 ) = 0,
2 4 ~ (n, (W, ∇)W) k3 =0 = 32aB D K{n1 sin η1 [K(cos η1 + K − 2) − − sin2 η1 − sin2 η2 ] + (1 ⇆ 2)} = 0
where
(2.18)
(2.19)
1 1 1 1 1 D = cos η1 cos η2 , K = cos (η1 + η2 ) cos (η1 − η2 ). 2 2 2 2 2
The factor is K = 0, if k1 ± k2 = 2(2m + 1)π/a, m = 0, ±1,. . . . We can easily convince ourselves that the term in brackets in (2.18) can only vanish if the condition n1  = n2  is satisfied, i.e. for planes with k1 ± k2 = 4πm/a. The Eqs. k1 ± k2 ± k3 = 4πm/a defining the planes intersecting all coordinate axes can immediately be identified taking into account that all sections being cut out from the coordinate axes by such planes must be equally sized, as demanded by (2.17), (2.18), (2.19). However, the requirement of (2.15) will not be met on these planes, which means that they would not be Splanes. It should be kept in mind that the requirement for attainment of maximum population inversion , which actually selects the flat Ssurfaces (planes), is not the only one. For this reason, also curved Ssurfaces have to be included in our considerations. The Eqs. defining such surfaces can be derived from (2.11) if certain e are given, as each e is associated with a multisheeted Ssurface, whose shape would change with varying e. Using the spectrum given by (2.16), it is possible to obtain the view about a modification of the shape of Ssurfaces setting e along symmetry axes. For ek[001] (fourfold axis), ek[111] (threefold axis) and ek[110] (twofold axis) the Eqs. describing the Ssurfaces are: 55
S[001] : sin (η3 ) cos
(η1 − η2 ) η1 + η2 cos = 0, 2 2
S[111] : sin (η1 + η2 ) + sin (η1 + η3 ) + sin (η2 + η3 ) = 0,
S[110] : sin
(η1 + η2 ) (η1 + η2 ) (η1 − η2 ) [cos + cos cos (η3 )] = 0. 2 2 2
(2.20) (2.21)
(2.22)
Typical shapes of some sheets of the surfaces (2.20 2.22), being confined within the 1st BZ, are shown in Figs. 2.1 2.3. (In the following, we shall denote those specific sheets of Ssurfaces being located within the 1st BZ as ”reduced sheets”). For ek[001], (2.20) describes a totality of planes: η3 = mπ → k3 = 2mπ/a, m = 0, ±1, ±2, . . . ,
(2.23)
η1 ± η2 = (2m + 1)π → k1 + k2 = 2(2m + 1)π/a
(2.24)
k3 1 W
W X W
2 W X X
Γ
W
k2
k1
W W
Figure 2.1. Image of the reduced Surface S[001] for the dispersionlaw given by (2.16); Sheets 1 and 2 are determined by: k3 = 2π/a, k1 + k2 = 2π/a, where a parameter of the fcclattice. 56
In Fig. 2.1, the hatched quadratic sheet of the 1st BZ corresponds to the plane defined by (2.23) for m = 1 (the opposed quadratic face corresponds to m = 1, and the flat region including the point Γ corresponds to m = 0 ). The vertically hatched rectangle in Fig. 2.1 corresponds to one of the four planes given by (2.24) for m = 0: k1 ± k2 = 2π/a.
k3 X
W
W U W
U
W W U
L W U W
W Γ W
X
k1
U
X W U
k2
W
W
Figure 2.2. Image of one reduced curved sheet of the S[111] surface for dispersionlaw (2.16) For ek[111], all sheets of the surface given by (2.21) are curved. Figure 2.2 shows one of the three reduced sheets. It is possible to obtain the sheet of similar shape by means of the geometric operation of the inversion in relation to point Γ. (The sheet including the point Γ is not shown in Fig. 2.2). For ek[110], (2.22) is satisfied for Splanes with k1 + k2 = 4πm/a (the reduced flat sheet corresponds to m = 0) as well as for curved Ssurfaces (whenever the expression included in brackets in (2.22) vanishes). Figure 2.3 shows one of the reduced curved sheets (the second one is produced by the inversion in relation to point Γ. In Fig. 2.3, showing the intersections of the Ssurfaces (including those not shown in Fig. 2.1  2.3 with planes k1 = k2 for ek[11ψ], it is possible to track their continuous transformation with varying e. For ψ >> 1, the traces of the Ssurfaces attain a steplike shape with pronounced linear (nearly vertical and horizontal) regions, which, for ψ → ∞, will steadily transform into groups of perpendicular straight lines, which also represent the traces of planes (2.20). The 57
k3 X
W
W W W
k1
X
Γ W
X
Λ
L
Λ
W
L
Λ
Λ
k2 W
W
Figure 2.3. Image of the reduced curved sheet of the S[110] surface for dispersionlaw (2.16) trace of that sheet of the Ssurface, which includes the point Γ, will be subjected to the most pronounced changes. This trace changes over from a nearly horizontal section for ψ >> 1, to the almost vertical, for 0 < ψ > 1), threefold (ψ = 1) and twofold (ψ 0, but for on the magnitude of (ξ, jξ
v(s) > cj ξ~, there exists one orientation q for which qmin = 0. (If v(s)c−1 >> j ξ~
1, then this orientation is close to n but if v(s)c−1 ∼ 1, then it will deviate j ξ~ significantly). It has to be taken into account that the orientation of v(s) on the Pplane does not necessarily remain constant. In this case the reduction of qmin , being caused by the deviation between the ξ~ and n, will be achieved due to the decrease in the number of inversely occupied ESstates, already being attached to a smaller region of the Psurface (related to the case ξ~ k n). Thus wherever ξ~ is noncollinear to n, the Pplane can be partitioned into sections Pi . In such cases ~ Curved Psurfaces, each Pi will be associated with an individual orientation of ξ. on the other hand, can only be considered if they can be divided into a totality of sufficiently small sections. Finally, each of them would approximate flat sections. For example, in the proximity of the hexagonal face of the 1st BZ, the shape of the Psurface is close to that of the Ssurface, as shown in Fig. 2.2. On the hexagonal 61
face, the lines LW, which intersect the surface in regions with opposite sign of those electron group velocity components being oriented normal to the surface, belong to the Psurface. This means that those Pregions protruding from the upper side of the hexagonal surface alternate with those Pregions protruding from below. 1 It is reasonable to infer that, in the proximity of the hexagonal faces, the Psurface is divided into roughly six flat regions (with median lines LW), being projected towards those faces of the hexagonal face of the 1st BZ being limited by the lines LK, LU. The normals nj (j = 1, . . . 6) to these regions are grouped in the proximity of one of the threefold axes h111i, and the degree of deviation from nj depends on the magnitude of the velocity component vp of the electrons along the lines LW. Now let us inspect the Ssurfaces. The particularity of this case is that the first addend in (2.27) also exists when S is a plane and ξ~ = ±n (in the case ~ v)p = 0 for ξ~ = ±n). Induced radiative transitions from states of of Pplanes (ξ, higher energy into states with relatively lower energy correspond to such ξ~ pointing towards regions with increasing electronic energy. For this reason ξ~ must have such ~ v(s)) in (2.27) results into a positive quantity. characteristics that the product (ξ, According to (2.31) qmin depends on ξ~ and varies from point to point of the S~ the maximal value of qmin (s,ξ), ~ corresponding surface. Let us denote by qm (ξ) ~ Among the totality of possible ξ~ we shall highlight those specific ξ~ to a given ξ. satisfying the following conditions: ~ v(s)) ≥ 0 for the majority of points of the Ssurface; 1. (ξ, 2. Maximum population difference with uniform sign at opposed sides of the Ssurface; 3. Small (≤ 10−1 π/a) magnitudes of qm . It should however be noted that for a given Ssurface it is possible in principle that not even a single ξ~ may exist for which compliance with all of these conditions would simultaneously be given at all of its points. In such cases the possibility of partitioning the Ssurface into individual sectors S (i) with an individually assigned orientation ξ~ = ξ~i should be considered. The requirement of macroscopicity s(i) Rµ∆ (q(i) ) for each of the desired q = q(i) must however presuppose the correctness of (2.27) for the majority of points of the section S (i) of an Ssurface and can be satisfied at any point of the section for q (i) ≥ qm (ξ~(i) ).
(2.33)
For a given ξ~(i) the inequality (2.33) determines the minimum magnitude of the wave vector of those phonons being emitted during stimulated transitions of elecs(i) trons between ES from the set Rµ∆ (q(i) ). 1
We note that such characteristics of a surface are not related to a specific kind of dispersion law ε(k), as they rather result from pure symmetry considerations [105].
62
It should be noted that the requirement of compliance with the conditions of equidistance (1.9) enables us to compare the Ssurfaces being linked up with different e and to sort out those ones which, for a given q, dispose over the largest total area Σs(q) of the S(q)regions within the reduced sheets of the Ssurface. Obviously the number of ESpairs being active immediately after their generation in the proximity of S(q) must be proportional to Σs(q) . Taking the spectrum (2.16) as an example, there exist for e k [001] and e k [110] each a planar (see sheet 2 in Fig. 2.1) and a curved (Fig. 2.3) reduced sheet of the Ssurfaces, for which the vector q k [110] is highlighted from the point of view of maximum population inversion. Now, let us compare these particular sheets of the Ssurfaces. It is easy to realize that both of the requirements of maximum population inversion, ~ v) as well as for conservation of the sign of the populafor positive amount of (ξ, √ tion difference, are satisfied for ξ~ = ±1 / 2 (e1 + e2 ) in half of the section S[001] . However, for small values of ε1 and q < 0, 1π/a, the majority of points of this section does not satisfy Eq. (2.27). This is due to the fact that in S[001] , the quan√ ~ v) varies within the wide range between 0 and 2 2aε1 , whereas the term tity (ξ, m−1 = −~2 a2 ε1 remains constant. Due to the small variations of δ (not exceeding 0, 1π/a), (2.27) is valid only for a small number of points in sheet 2 of the surface S[001] . As a result, the associated amount of pairs of equidistant states is small ~ And viceversa, in and would not even significantly increase with variations of ξ. case of a curved surface (2.22) (see also Fig. 2.3) then (2.27) could be satisfied for the same ξ~ in a region being comparable with that of the sheet S[110] of the surface S, located within the 1st BZ. The dimensions of this region depend on ε1 and q. The first addend in (2.27), being related to the surface (2.22), indeed vanishes √ for ξ~ = (1/ 2)(e1 + e2 ), while the factor m−1 = −~2 a2 ε1 sin2 1/2(η1 + η2 ) varies. Considering that m−1 → 0 for (η1 + η2 ) → 0, we must exclude from the possible range of variables η1 , η2 the specific range
η1 + η2  ≤ 2 arcsin [2~ cj ξ~ (qε1a2 )−1 ]1/2 ,
−η1 + η2  ≤ η1 − η2 ≤ η1 + η2 ,
in which δ ≥ δmax = q/2. For example, taking cj ξ~ = 5 · 103 m/s, a = 3, 5 · 10−10 m, ε1 = 10−19 J, we obtain η1 + η2  ≤ π/4 for q = 0, 2π/a, and η1 + η2  ≤ π/2 for q = 0, 02π/a. The results of this estimate indicate that for S[110] , the part of the area to be excluded amounts to about 10 % in the first case and to about 30% in the second case. As the area Σ of the sheet S[110] is large (Σ ∼ 10π 2 /a2 ), the number of equidistant pairs of states in the proximity of the sheet S[110] also becomes large. Thus in the case of the dispersion law defined by (2.16), and with due consideration of the conditions of equidistance, a comparison between flat and curved Ssurfaces turns out in favor of the curved surfaces. 63
2.5
Potentially active pairs of electronic states in the electronicspectrum of fcc iron
Within the framework of our final aim to describe the γ − α MT, our interest will now focus on an analysis of the Ssurfaces of the fcc iron lattice. A detailed analysis however appears to be difficult, as this would imply substantial knowledge on the spectrum ε(k) as well as on the velocityfields v(k), within a region limited by isoenergetic surfaces ε(k) = µ ± ∆. The data published in the relevant literature however only refer to symmetry lines (predominantly relating the bccphase of iron), whereas data on the velocity field are totally missing. Thus is would be reasonable to investigate to which extent the results obtained for the model spectrum (2.16) can be used further. Above all we have to remark that all symmetry planes of the reciprocal lattice: ki ± kj = 4πm/a are Splanes, independent of the underlying spectrum ε(k). Yet any of the Splanes corresponds to a vector e, oriented in the normal of the plane. This immediately follows from symmetry considerations. The velocity v, being an invariant with respect to reflective transformations in the symmetryplane, can’t feature a nonvanishing component oriented normal to the symmetryplane and thus must completely lie within the symmetryplane. Based on this consideration it can be concluded that the reduced sheet 1 of the surface S[001] (see Fig. 2.1) at e k [001] also remains conserved for the ε(k) spectrum of iron. However, there exist no reasons to surmise that the reduced sheet 2 of this surface maintains its shape. Even the slightest modification of the dispersionlaw (2.16): ε = ε0 − 2ε1
X ij
(1 − δij ) cos ηi cos ηj + 2ε2
X
cos 2ηi
(2.34)
i
taking into account the interaction with the second neighbor from [104], results into a curved sheet 2, associated with an expansion of its area. Depending on the sign of ε2 , the curvature of sheet 2 will take shape within the 1st BrillouinZone (1st BZ) for (ε2 > 0), or be oriented towards the faces of the 1st BZ for (ε2 < 0), as shown in Fig. 2.5. Thus the flattening of sheet 2 follows from particularities of the dispersion law. It can further be stated for the iron spectrum that sheet 2 will intersect the hexagonal surfaces of the 1st BZ in the same horizontal WLWlines as sheet 2 in figs. 2.1 and 2.5. Symmetry considerations in fact lead to the conclusion that the velocity v is oriented along the lines WL (as well as WX), i.e., vW LW ⊥ek[001], whereas the horizontal lines WLW belong to sheet 2 of surface S[001] . In the case of an iron spectrum, the intersecting region of sheet 2, comprising the square surfaces of the 1st BZ k1 = 2π/a, k2 = 2π/a can only go along the line WXW if the dispersion ε vanishes in the lines WX, in the same way as for the spectrum (2.16), or in other words, if the velocity vector v vanishes along these lines. Otherwise the intersection would be located either along the curved line Λ, being defined by the requirement (v, e)Λ = 0, as shown in Fig. 2.5a, or in 64
k3 L
W
W Γ
k1 W
k2
W
W
W
L a k3 L
W
W Γ
k1 W
W
k2
W W
L b
Figure 2.5. View of reduced curved sheets 2 of the surface S[001] for the spectrum (2.34): a  Parameter ε2 > 0; b  Parameter ε2 < 0. The intersection of surface S[001] with the plane k3 = 0 is shown by the horizontal dashed line. singl points W, as shown in Fig. 2.5b. We emphasize that from the point of view of materialization of a masereffect the curved sheets 2 imply a promising advantage over the flat sheets. The ESpairs located in the proximity of the flat sheets 2 cannot contribute to the generation of phonons with qk[001], as they don’t feature inverted populations in this direction, and for q k [110], their contribution would only be small, as already mentioned. This means that for q k e k [001] and flat sheets 2 only ESpairs located in the proximity of the flat sheets 1 would have the potential to actively contribute to phonon generation. However, in the case of curved faces 2, phonon generation with q k [001] would not be generally forbidden. Therefore, an appreciable increase of the number of ESpairs being active during phonon generation with q k [001] can be expected, if compared with the spectrum (2.16). For e k [111], the shape of the reduced sheet of surface S[111] , as shown in Fig. 2.5, must not differ appreciably from the reduced sheet of surface S[111] of the iron spectrum ε(k). This way the lines WLW at the hexagonal face of the 1st BZ, and the lines UXU at the square faces of the 1st BZ will also belong to the surface 65
S[111] of iron, as the velocity there is oriented perpendicular to [111], due to the symmetry requirements. It should also be noted that the aforementioned remarks on the intersecting lines of face 2 of surface S[001] with the square surface of the 1st BZ also apply to the allocation of lines WXW to surface S[111] . For spectrum (2.16) and for that of iron at e k [110], the common features of the reduced sheets of the surface S[110] are the vertical lines WXW, being located on the square faces of the 1st BZ, k1 = 2π/a, k2 = 2π/a, and the horizontal lines WLW located on the hexagonal surfaces of the 1st BZ, being an immediate result of the orthogonality relation for the velocity v⊥[110] in these lines. It will however be necessary to specify the intersection lines of the surface S[110] with the horizontal square surfaces of the 1st BZ (in the same way as in the previous cases), as well as the location of the lines WAW (see Fig. 2.3).
ε, Ry 0,6
µ
X5 W1′
K2
L3
X5
L3
W1′
0,4 0,2 0
Γ
X W
L
Γ
KX
L
UW
Figure 2.6. Extract of the calculus in [110] of the dispersion curves of ferromagnetic nickel with fcc lattice. The solid lines indicate spindown states, dashed lines spinup states, µ = Fermienergy. Let us now deal with questions related to the possible existence of electronic bands in the energyspectrum of fcc iron, featuring weak dispersion at the reduced sheets of the Ssurfaces, which at the same time dispose of an acceptable energetic interval ∆ ∼ 0, 2eV in the proximity of the Fermienergy µ, in accordance with inequality (2.25). As the bcc lattice modification of iron predominates in the temperature range between 0 and 1183 K, most calculus related to structure deal with this modification. Nonetheless, the results published in [106–109], dealing with the energy spectrum of the fcc lattice modification of iron [106, 107], as well as with nickel in [108–110], will enable us to answer the first part of the question. The similarity between the energy spectra of iron and nickel, becoming evident from a comparison of the results in [107] for spinup subbands with the results in [108–110], enables us to use the more comprehensive calculus of [110] for Ni, with the aim to reveal those bands featuring a weakly pronounced dispersion. Figure 2.6 shows data published in [110], related to those branches of the εL3 energy spectrum featuring the weakest dispersion of the lines corresponding to the 66
above discussed Ssurfaces. As can be seen in Fig. 2.6, the energy along the lines LW, LU and LX is close to εL3 , and along the line XW is close to εX5 . According to [106], the difference between the energies εX5 − εL3 ≈ 0, 02Ry ≈ 0, 27 eV. (It should be noted that in [106] only the curves ε(k) for the γphase of iron along ΓX, ΓL, ΓK, as well as the term  energies in the points Γ, X, K, L are presented).
g(ε), (Ry · atom)−1 25 20 15 10 εL3 µ
5 0
0,4
0,2
0
0,6
ε, Ry
Figure 2.7. Density of states (DOS) for the nonmagnetic state of nickel with fcclattice [110]. The loci of the Fermienergy µ and of the energy εL3 are labeled. Thus it can be inferred from the available details of energy spectra that there is an appreciable probability for the existence of Ssurfaces with weak energy dispersion. 2
g(ε), (eV · atom)−1
2
1
g(ε), (eV · atom)−1
1
µ
µ 0
0 1,4
1
a
0,6
1,4
ε,Ry
1
b
0,6
ε, Ry
Figure 2.8. DOSfunctions of iron with fcclattice from [111], for two different electronic configurations of the iron atoms: a − 3d7 4s1 ; b − 3d6 4s2 The second part of our question will be more difficult to answer: Which are the mutual arrangements of the energy level µ and of the energies ε(s) on the S67
surfaces or, put in another way: How can the size of the interval ∆ = µ − ε(s) be unambiguously determined on the basis of existing calculations of electronic spectra, with a required precision of at least ≤ 0, 1eV . If we denote by εL3 the spatial average energy on the Ssurface, then we will note from the calculus in [108–110] that εL3 is localized in the peak area of the DOS g(ε), whose energy is close to the top of the 3dband, as shown in Fig. 2.7. Provided the electronic configuration is known, and after having determined the location of µ, it would be reasonable to assume ∆ = εL3 −µ. However, the precise electronic configuration of iron atoms in the solid (metallic) state is not precisely known and the quantity εL3 − µ varies significantly with changes in the electronic distribution between the 3d and 4s states. In figure 2.8, which has been extracted from [111], the characteristics of the curves g(ε) are compared for the 3d74s1 , 3d 6 4s 2 configurations. The change of configurations is associated with a reduction of the difference between the peakenergies ε ≈ εL3 (in the proximity of the top of the dband) and µ from ≈ 0,6 eV down to ≈ 0,2 eV. In the last case, the peak degenerates to a step like shape. The intermediate configuration 3d 6,54(sp) 1,5 of the γ and α phases of iron has been used in [112]. (However an explicit form of the g(ε) is not presented in [112]). It should be noted here that the results of the calculated configurations (3d9,4 4s0,6 in [108,109] and 3d 8,6 4(sp) 1,4 in [110]) differ appreciably for the fcc modification of Ni. If preference was given to the selfconsistent calculus in [110, 112], then the configurations 3d6,5 4(sp)1,5 for Fe and 3d8,6 4(sp)1,4 for Ni would be in harmony with the lemma of increased probability of population of states with a fraction of selectrons, during passage from the elements of the mean of the 3dgroup towards its end [113]. A value of ∆ = εL3 − µ ≈ 0,4 eV can be expected, which would be intermediate in relation to the ∆ = εL3 − µ, for the configurations 3d 7 4(sp) 1, 3d 6 4(sp) 2. One point however, being related to the vague interpretation of paramagnetism of the γ phase of iron, is important enough to deserve a remark: Experimental results published in [114, 115] clearly show that the magnetic susceptibility of the γ phase is less by a factor of about 1.5 ÷ 2 in comparison with that of the α or δphase and, moreover, does not obey to the CurieWeiss law [62]. In [62], these facts are reasonably explained by the Paulicharacteristics (including exchange amplification) of the paramagnetism of the γ phase. In contrast, the experimental results of diffuse magnetic neutron scattering published in [116, 117] provide clear evidence of a remarkable amount of magnetic moment density in the γ phase (being of an order of magnitude of Bohr’s magneton µB per atom). As stated in [62], it is possible to interpret these observations without contradiction by the theory of spinfluctuations, stating that the average spinmoment of a given ”knot” vanishes, due to permanent statistical fluctuations, and thus cannot be observed or derived from magnetic susceptibility measurements under static conditions. However, if the measurements are performed at a timescale being comparable with the average lifetime of these fluctuations (like neutron diffraction), then the spin moment fluctuations can clearly be observed. 68
In a paramagnetic state, the existence of disordered local magnetic moments of finite magnitude implies that the local DOS varies from point to point, with the same probability for a spinup or a spindown condition of a spinpolarized state. Thus, in such cases there must also exist spinup ↑ and spindown ↓ states located on Ssurfaces, with identical difference ∆ = ε(s) − µ. As described in [118], the average DOS is broadened and characterized by displaced and diffuse peaks of the DOS function, if compared with a ferromagnetic (or nonmagnetic) state. We should also recall that in [119, 120], the existence of two atomic states (γ1 and γ2 ) of iron in the γphase has already been hypothesized, essentially stating that a γ1 state coexists with a smaller atomic volume V1 and a smaller magnetic moment, together with a γ2 state characterized by a relatively larger atomic volume V2 > V1 and larger magnetic moment. In [107, 112, 121, 122] (see also [123]), this hypothesis received some verification within the frame of the simple Stonermodel. As has been shown therein, for an existing exchangesplitting of the bands into
g(ε), (Ry · atom)−1 40
NM
20
20
F
0
0
F
µ 20 0
0,4
ε, Ry
Figure 2.9. DOSfunctions of iron with fcclattice. NM  nonmagnetic state, F  ferromagnetic state (lower curve  spinup, upper curve  spindown) [122] spinup ↑ and spindown ↓ subbands, together with the assumption of steady increases of the lattice parameters at certain a = a0 (a0 ≈ 3, 58 ˚ A in [122] and ˚ 3, 63 < a0 < 3, 71 A in [107]), a stable ferromagnetic state with a magnetic moment of (2, 3 ÷ 3)µB per atom will arise, being separated from states with vanishing magnetic moment by an energy gap of 0.1 eV [112] (in [120] an energygap of 0,037 eV is given). In Fig. 2.9, borrowed from [122], both the DOS functions g(ε) of the nonmagnetic and of the spinpolarized state are shown for a ≈ ao . Obviously, the peak of the nearly filled spinup ↑ subband is located below the Fermilevel, 69
in the proximity of µ, µ − εL3 ↑ ≈ 0, 2 eV. If we took the location of µ between two large peaks of the DOS function g(ε) of the nonmagnetic state as a criterion for selection of the electronic configuration, then the electronic configuration of iron would be near the 3d74s1 configuration (as can be confirmed by comparison with Fig. 2.8a). However, due to the existence of exchangesplitting, the values of the parameters ∆ ∼ 0, 2 eV are also possible for this configuration. It should be noted that the value εL − µ ≈ 0,78 eV for the nonmagnetic state of the γphase (published in [122]) is larger than the corresponding value of 0,6 eV published in [111]. As the martensitic transformation temperature MS of pure iron (or of iron with small content of nickel or carbon) is MS ∼ 103 K, it would be possible for the iron atoms to simultaneously coexist in both states γ1 and γ2 , with the same probability at T ∼ MS . If we assigned to the state γ1 the configuration (3d ↑)3 (3d ↓)3 (4sp)2 , which does not feature a local magnetic moment, and to the state γ2 the configuration (3d ↑)5 (3d ↓)2 (4sp)1 , featuring an atomic moment of 3µB , as surmised in the modified Weisspattern [124], then the states located above and below the Fermilevel µ, being linked up with the γ1 , γ2  states of iron, would be interchangeable on the Ssurfaces (with values ∆ ∼ 0, 2 eV). On the basis of energy spectrum calculus however, substantial difficulties arise in unambiguously determining both the magnitude and the sign of the chemical potential difference µα − µγ of the electrons in the α and γ  phase (Let’s remind that the specified difference is the significant characteristic of a nonequilibrium condition of an electronic system). According to [111], the chemical potentials of nonmagnetic phases are practically indistinguishable in the configuration 3d7 4s1 . For the configuration 3d6 4s2 , a value of µα − µγ ≈ −0, 2 eV is proclaimed. However, the calculus in [125], which was performed by the cluster method (for the configuration 3d64s2 ), delivered µα − µγ ≈ + 0, 2 eV, the sign thus being opposed to the aforementioned sign. However, it should be remarked that the limitation to three regions of nearest neighbors, used in [125], presumably is inadequate for a sufficiently precise evaluation of the small difference µα − µγ . Thus the calculus by the augmented plane wave method in [111] should be given preference. There still remains one unconsidered aspect: During the γ − α  MT (with exception of FeNi alloys with a Nicontent of > 30 %), the MT is associated with a transition from the paramagnetic γ into the ferromagnetic α  phase (we recall that the Curietemperature Tc = 1041 K of the α  phase of iron is higher than the MS temperature at the onset of a martensitic transformation). This means that µγ of paramagnetic and µα of ferromagnetic iron must be compared among themselves. Estimates in [118], based on a DOS model, indicate that during the process of ferromagnetic ordering, the magnitude of µα decreases, that would be an argument in favor of a negative sign of the difference µα −µγ < 0. Of course this question could most easily be resolved by a proper experimental method, taking advantage of the fact that the large temperature hysteresis between martensitic transformations of FeNi alloys and their reverse transformation (see Pt. 1.2) 70
enables us to measure the difference of the contact potential at one and the same temperature between a sample which has undergone practically the total γ − α  MT (as with FeNi alloys containing up to 28 % Ni), and an austenitic sample of same composition. In our further evaluations, a value of µα − µγ = −0, 16 eV will generally be assumed. This latter value was determined under adequate consideration of the volumeeffect of the MT, as described in Pt. 1.5. A more detailed treatment of this question will be resumed under Pt. 4.5.3. Some additional remarks 1. In addition to the ES with least dispersion (see Fig. 2.6), there may also exist active ES belonging to other energy bands. For example, in the proximity of point X, potentially active ES are those associated with point X2 and energies εX2 ≈ εL3 . 2. From the point of view of compliance with the energetic criterion (2.25), a curvature of sheet 2 of surface S[001] oriented towards the faces of the 1st BZ, would be more favorable (see Fig. 2.5b ), as on the one hand, the dispersion along line ΓK is remarkably pronounced, and on the other hand, a curvature towards the center of the 1st BZ (see Fig. 2.5a) would come into conflict with the conditions implied by (2.25), for the largest part of sheet 2, and would thus finally lead to a contraction of the region adjacent to lines LWL. 3. A weak dispersion ε (k) (comparable with the dispersion of the phononbranches) in the essential sections of lines LW and LV of the Psurfaces in the proximity of the hexagonal Brillouinfaces (as well as for similarly shaped S[111] surfaces) opens up the possibility for participation of ESpairs being mutually separated by these surfaces  on the generation of longwave phonons with quasimomentum ~q, whose orientation would significantly deviate from the threefold axes of symmetry [111] towards the twofold axes of symmetry [1¯10], [10¯1], [0¯11] (also see the remarks following (2.31) of Pt. 2.4). We also remind that the component of electron group velocity being oriented normal to the Psurface would vanish by definition of (2.8). This in turn implies that the nonequilibrium addends relating to the occupation of states on both sides of a Pplane would essentially be proportional to the projection of e (e  orientation of spatial inhomogeneity) onto the normal n of the Pplane. In contrast to the Ssurfaces, which vary with variations of the orientation of e, the Pplanes are independent of e. Thus only the magnitude of occupational inversion would depend on e. Therefore it will be necessary to correct our conclusions initially inferred from the analysis of ES located in the proximity of Ssurfaces, if they should also apply to ESpairs located in the proximity of flat (or nearly flat) sections of Psurfaces. To take an example: Instead of the generation of phonons with quasimomenta qkh110i strictly aligned with twofold axes of symmetry, which would be most 71
obvious due to the extensiveness of the Sh110i surfaces (see Fig. 2.3), there must be expected a deviation of q with respect to the axis h110i. As the area Σ of the reduced Ssurfaces steadily changes with varying e, a deviation of e from the axis [110] by a small angle of let us say 100 , (e k [11η], η ≈ 0,3) could not significantly diminish the area of the reduced surface S[11η] , if compared with S[110] . The additional contribution to the generation of phonons with q k [11η] comprises about one sixth of the ESpairs located in the proximity of the Pplanes, in the surroundings of the hexagonal faces of the 1st BZ with normal vectors parallel to [¯111], [1¯11], corresponding to areas of √ n oriented 2 Pplanes ∼ 2 3(π/a) , thereby not only compensating for the losses but leading to a surplus of area. This means that a consideration of ES located in the proximity of Pplanes ensures a low generation threshold for waves whose wavevectors q lie within orientations confined by a cone centered around [110], with respect to the threshold for q k [110]. The deviation of q from [110] will however be essential for an interpretation of the particularities of the morphology of the product of the γ − α MT (see Chap.5), as well as for any reasoning about the actually occurring choice of the pathway of a martensitic reaction.
4. The conclusion on the existence of Ssurfaces with weak energy dispersion in the proximity of values ε = εL means that the shape of the isoenergetic surface ε = const ≈ εL3 must be more or less akin to the shape of the Ssurfaces. As in the case of ferromagnetic Ni discussed in [108] [110], the location of the Fermilevel with partially filled minority subband ( electron spindown ↓ oriented against the orientation of the magnetic field) is close to the energies εL3 ↓ ( εL3 − µ ≈ 0,3 eV), the method of Fermi  surface calculus can be used. In Fig. 2.10, the intersections extracted from [109] are depicted (see also [126]) and the overview of the sheet corresponding to the dlike sheet of the Fermisurface in [127] (5β in accordance with the designations used in [109]). Obviously, the curved surface pronouncedly protrudes towards the orientation of the WKWrib of the 1st BZ. Thus condition (2.25) is satisfied for the similarly curved sheet 2 of surface S[001] . In kspace, the sheet of the Fermisurface is more remotely located from sheet 1 of the S[001] surface than from sheet 2, featuring the shape of a doublesaddle in the region opposite the square surface of the 1st BZ. Obviously with increasing energy, the isoenergetic surface will come closer to the faces of the 1st BZ, which in turn will enhance the effectivity of those ESpairs being located in the proximity of the vastly extended curved surfaces S[110] , S[111] (see also Figs. 2.2, 2.3). 72
2.6
Summary of Chapter 2
A consideration of the crucial conditions for phonon generation to be satisfied by a radiative electronic subsystem led us to the following conclusion: Potentially active ES in kspace are localized near regions of Ssurfaces being limited by isoenergetic surfaces ε(k) = µ ± ∆. In kspace such S surfaces separate ES with the ~ k ε(k) on the direction of opposite signs of group velocity projections v(k) = ~−1 ∇ the local spatial inhomogeneity e. Even if the dispersion law ε = ε(s) on the S surface was arbitrarily chosen, the conditions for inversely occupied and equidistant ESpairs would still demand a slow rate of change of the electron energy on the S surfaces, hence satisfying the inequalities (2.25) for the macroscopic majority of points on the S surface. It can thus reasonably be expected for systems with high density of electron states in the proximity of the Fermilevel to satisfy this requirement. Those S surfaces (as well as the associated orientations of e) for which the greatest part of their area is located within the 1st BrillouinZone (BZ) (for reduced sheets) are highlighted, as they correspond to (2.27) and, at the same time, satisfy the requirement of sign invariance of the population difference of ES associated with a given pair k, k′ , where a phononwavevector q connects the pair of points defined by k, k′ , at opposed sides from S. The quantity q is limited from below, where the minima of q are mainly determined by the characteristics of the groupvelocities vs , as well as by the inverse effective masses m−1 s on the S surfaces (note that the inverse effective masses are essentially independent of the orientation of q, see eq.(2.27)). For q k e, the smallest value of q = qmin attains an order of magnitude of (10−3 ÷ 10−2π/a). As the vast majority of points of the reduced sheets of the Ssurfaces are located within the 1st BZ, and not at its boundaries, the elementary processes of phononemission with wavevectors q ≥ qmin can be regarded as Nprocesses, as they are determined by electronic transitions of the type k → k′ being localized in the proximity of the S surfaces. Thus, under the pronounced nonequilibrium conditions locally prevailing in a γ − α  MT region, there will predominantly be emitted or amplified longitudinal (or quasilongitudinal) phonons, as both the scalar products (eq , q), and the matrixelements (2.4) of electronphononinteraction would vanish for pure transversal waves related to Nprocesses. The emission of phonons with q vectors collinear with e becomes most probable under condition of maximum population inversion. Using the conservation law of quasimomentum (1.9) and the nonequilibrium addenda, to the electronic distribution function expressed in (2.5), (2.6), it is easy to find the relative orientation of q and e according to the sign of the expression m−1 s , (ε − µ)s on the Ssurface, for two different sources of nonequilibrium. Table 2.1 shows the relative orienta~ , e k eµ k ∇µ. ~ tion between q and the unit vectors defined by e k eT k ∇T Positive −1 m s → (+) correlate with the points of minimum, while negative m−1 s → (−) correlate with the points of maximum of the function ε(k) on the Ssurface. For 73
example, for m−1 s < 0 → (−), (ε − µ)ε > 0 → (+), e k eµ in Table 2.1 we get q ⇈ eµ . The latter statement means that for µα < µγ , there will be generated (or amplified) the longitudinal waves propagating from the growing martensite crystal (into the austenite area being free from martensite). Thus it can also be concluded from Table 2.1 that for e = eµ the relative orientation of q and e is independent of the sign of the term (ε − µ)s , whereas such a dependence does exist for e = eT . This latter conclusion immediately results from the consideration that for ∇µ 6= 0, there must exist an electron flow oriented from regions with relatively larger chemical potential µ towards regions with lower µ (thus being linked up with charge transfer), while for ∇T 6= 0, there must exist two mutually opposed electron flows of equal density, however not contributing to effective charge transfer in that region (see also the legend to Fig. 1.8). Table 2.1. Orientation of the wavevectors of generated phonons relative to the orientation of spatial inhomogeneity
(ε − µ)s + –
m−1 s
+ q ↓↑ eT q ↓↑ eµ q ⇈ eT q ↓↑ eµ
– q ⇈ eT q ⇈ eµ q ↓↑ eT q ⇈ eµ
Considering that Tα > Tγ and bearing in mind that µα < µγ , (see also final statement of Point (2.5)) the antiparallelism of eµ and eT becomes evident. Then the effect of the sources of nonequilibrium for the states with (ε − µ)s > 0 will partially be counterbalanced (in that the nonequilibrium addenda of (2.5) and (2.6) are mutually subtracted), whereas they will mutually be amplified for (ε − µ) < 0 (i.e. the nonequilibrium addenda of (2.5) and (2.6) add up). Of course, during the process of generation and amplification of longitudinal waves propagating ahead of the growing martensitic phase, the dominating quantity is the inhomogeneity (gradient) of the chemical potential µ and not the temperature ~ . This conclusion is evident as the order of magnitude of the difference gradient ∇T µα − µγ = −0, 16eV is about one order of magnitude greater than that of the temperature difference Tα − Tγ (after the temperature is adequately converted into its energy equivalent). Following an evaluation of our electronic bandanalysis under Point 2.5 it appears to be most likely that the value of the parameter ∆ is approximately some tenths of eV for fcciron lattice, and that ESpairs in the proximity of the surfaces S[001] , S[110] , S[111] can be active during the generation of longitudinal phonons with orientations q in the proximity of symmetry axis. The most important results of our analysis of electronic spectra under the particular aspect of the general requirements for realization of a phonon maser are 74
published in [55, 88, 89, 128–130].
75
W
X
W
K
K
W
5β
W X
X
a U X
U L
L 5β
K
K
b
c Figure 2.10. Sheet of the dlike band (5 β with spindown) for Ni with fcc lattice: a  sectional view by the plane (001); b  sectional view by the plane (011) [126]; c  general view [127].
76
Chapter 3 Constitutive equations of the electronphonon system and the threshold wave generation conditions The theoretical finding of pairs of electronic states with the inverted population (see the previous chapter) is the most essential stage in our aim to disclose the phonongeneration mechanism. Next it is necessary to get a determination of the physical conditions required for the functioning of a phonon maser (see SubPt 4 in Pt.1.5) or, put in another way, to determine the threshold value of an inverted population difference. Thanks to the already existing comprehensive theory of the masereffect (for example in [98, 131–133]) this task does not comprise any fundamental difficulties and can thus be resolved on the basis of wellproven approaches and methods. The simplest approach is semiphenomenological. Then the crucial interaction of a radiating subsystem (in our case the nonequilibrium 3d electrons) with a radiating field (in our case a specific class of longitudinal phonons) has to be defined as precisely as possible, while the creation of the inverted population (i.e. the pumping), as well as dissipation processes, are treated by a phenomenological method.
3.1
Threshold conditions for singlemode generation
Following [132,133] we shall start with a brief consideration of the simplest derivation of the expression for a thresholddifference of population (1.12), related to the case of singlemode generation. As the generation of phonons normally begins with that specific mode for which the required population difference is minimal, it would be reasonable to start with a consideration of singlemode generation. Thus 77
in this case we start with our analysis by sorting out one specific Hamiltonian H1 from the general set of Hamiltonians 2.12.3 of an electronphonon system: H1 = ~ ωq b+ q bq +
X
εp a+ p ap +
p
X
+ + ′ Wq∗ bq a+ k ak + Wq bq ak′ ak .
(3.1)
k
+ Here b+ q , bq and ap , ap are the phonon and electron creation and annihilation operators, respectively, and Wq is the matrixelement of electronphonon interaction. Then, our next step is the decomposition of the complete Hamiltonian H of our task into the sum
H = H1 + H2 , The Hamiltonian H2 describes the action of other subsystems like heat reservoirs, on the segregated system (3.1). In (3.1), we omitted the indices of bands related to electronenergies and operators (in the case of a 3d  electron band), as well as the polarization index of phononenergies and operators (the polarization is supposed to be longitudinal); ~  Planck’s constant. In the Heisenbergrepresentation, the following constitutive equations of motion can be assigned to any operator x: ∂x i i i ≡ x˙ = [H, x] = [H1 , x] + [H2 , x] ≡ x˙ 1 + x˙ 2 . ∂t ~ ~ ~ Using the commutation rule [b+ p , bq ] = δq,p ,
(3.2)
+ [b+ q , bp ] = [bq , bp ] = 0
and the anticommutation [a+ p , aq ]+ = δq,p ,
+ [a+ p , aq ]+ = [ap , aq ]+ = 0,
we find from (3.1) and (3.2) that the following expressions describe the phonon + + field operators b+ q , electronpolarization operators dk,k′ = ak ak′ and the operator ′ + of the populationdifference σkk′ ≡ σ = a+ k ak − ak′ ak′ (where k, k correspond to those used in (1.9)): i X ∗ + + b˙ + Wq dk,k′ , q = (i ωq − κq ) bq + ~ k
i d˙+ = (i ωk,k′ − Γ)d+ − Wq b+ q σ, k,k′ k,k′ ~ 2i ∗ + σ0 − σ 2i + Wq dk,k′ b+ W d ′ bq , σ˙ = q − tσ ~ ~ q k,k b˙ q = (b˙ + )+ , ~ ωk,k′ = εk − εk′ . q
78
(3.3)
Here, Γ is the electronattenuation. Let us now discuss (3.3): As our interest is focused on the average values of the operators in (3.3), we can ignore the fluctuational action of heat reservoirs in (3.3), without introducing any significant error. Then, the effect of dissipation can be considered phenomenologically by introduction of relaxation times tσ of electron populations, of phonon attenuation κq , and of electron attenuation Γ. (It is agreed that an attenuation Γ for the dipole  moment dk,k′ of transition between a pair of electronic states (ESpair) k, k′ , emitting phonons with the quasimomentum q, is of the same order of magnitude as the electronic states attenuations, i.e., Γ ∼ Γk ∼ Γk′ ); σ0  inverse initial population difference of states k, k′ located on opposite sides of the Ssurface, being produced by electronic flows (driftpumping mechanism), as well as by other noncoherent processes in absence of maser radiation. In principle, the constitutive set of equations (3.3) represents an analog to the Blochequations of magnetic resonance theory. This becomes obvious from [134, 135] and by comparing σ, d+ , d with the projections of the spinoperators S z , S + , S − , and the parameters tσ , Γ−1 with the longitudinal and transversal relaxation times T1 , T2 , respectively. This immediately leads to the restriction (3.4) already known from [134]: T1 ≥ T2 : tσ ≥ Γ−1 .
(3.4)
In the phonon generation (stimulated emission) regime, the number of quanta of the mode to be emitted becomes macroscopic and the operators b+ q , bq represent satisfactory approximations of c  number functions of time. From the above presentation it becomes obvious that, in the generation regime, the equations of the system (3.3), averaged by a density matrix of the system, are identical with the classical expressions, if all operators were replaced by their average values. In below equations, this replacement has already been considered. Hence, the previously used designations of operators now simply pertain to their averages. The oscillatory dependence on time can then simply be eliminated by adoption of the quantities ˜b+ = exp [−iΩq t] b+ , q q
˜bq = exp [iΩq t] bq ,
d˜+ = exp [−iΩq t] d+ ,
(3.5)
d˜ = exp [iΩq t] d,
with consideration of the case of exact resonance: ~Ωq = ~ωq = εk − εk′ = ~ωk,k′ .
(3.6)
Under stationary conditions, we get from (3.3)  under consideration of (3.5) and (3.6)  the following system of nonlinear algebraic equations: i ∗ X ˜+ − κq˜b+ W d ′ = 0, q ~ q ′ k,k k
79
i (3.7) Γd˜+ + Wq˜b+ q σ = 0, k,k′ ~ i Γd˜k,k′ − Wq∗˜bq σ = 0, ~ σ0 − σ 2i 2i ∗ ˜+ ˜ + Wq d˜k,k′ ˜b+ W d ′ bq = 0. q − tσ ~ ~ q k,k The stationary value of the population difference σ, being the result of a balance between gains and losses, is the threshold value σth . Assuming the existence of solutions ˜b+ q 6= 0, we find from the first of two equations of system (3.7) that X k
σth =
′
~2 Γκq . Wq 2
(3.8)
We note that the attenuation Γ included in (3.8) represents certain mean attenuation of the dipolemoment d of the pairs of state k, k′ , being localized in the vicinity of the Ssurface. It is further convenient to introduce an average value σth for those σth associated with the Ssurface, by substituting in (3.8) in accordance with the meanvalue rule: X σth = σ ¯th Rq . (3.9) k′
Here Rq  number of ESpairs of state k, k′ which emit phonons with quasimomentum ~q during k − k′ transitions. As the energy of the pairs of state k, k′ must settle within certain interval ∆ (see (2.25)), the substitution in (3.9) requires from σ ¯th to be associated with certain constant amount of energy ε¯ within the interval ∆: ε − µ ∈ ∆. This requirement is equivalent to the replacement of a nonisoenergetic Ssurface by an isoenergetic one. Considering the weakly pronounced dispersion of ε(k) near the Ssurfaces, such a substitution suggests itself as natural. Using (3.9) and omitting the mean value sign (horizontal dash on top of σth ) we can write (3.8) in the form σth =
~2 Γκq . Wq 2 Rq
(3.10)
It immediately follows from (3.10) that σth becomes the less, the greater: the lifetimes of the quasiparticles Γ−1 , κ −1 ; electron  phonon interaction; the number of pairs of state with inverted population Rq , being proportional to the area ΣS(q) of the reduced sheet of the Ssurface. If we express (with the aid of the last of the three Eqs. of (3.7)) the value d˜+ by + ˜b and ˜bq and insert the result into the first of Eqs. (3.7), then, by consideration q of (3.10), we get 2 σ 4t W  0 σ q + + −1 ˜b ˜b ˜bq ) − 1 = 0, (3.11) (1 + q q σth ~2 Γ 80
with the two solutions: ˜b+ = 0, q ˜b+ ˜bq = q
σ0 < σth ,
σ0 ~2 Γ −1 , Wq 2 4tσ σth
(3.12)
σ0 > σth ,
(3.13)
which clearly verify that the displacement amplitude 2~2 uq = MNωq
12
˜bq
(3.14)
is vanishing below and nonvanishing above the generation threshold, thus indicating essentially classical characteristics of the displacement. In fact, it is obvious −2 ˜ from (3.13) and (2.4) that for σ0 > σth the number of phonons ˜b+ ∼N q bq ∼ Wq  becomes a macroscopic quantity. Consequently, the energy of this mode is comparable with the energy of the remaining noncoherent phonons. In order to evaluate σth , the relaxationparameters κq , Γ and the number of pairs of active states Rq must be known. To perform such evaluation, we can use as an upper limit of the parameters κq , Γ their respective values in the high temperature domain, where scattering by short  wave phonons predominates ( i.e. where T exceeds the Debyetemperature TD ). For an evaluation of κq , let q ωq enables us to use (without getting into contradiction to the conservation laws of energy and momentum) as the maximum number of electronic states Rq the quantity (Rq )max ≈ 2qΣq δ −1 , 3 Nδ ≈ 4 · (2π/a)3 ∼ qmax .
(3.21)
In (3.21): δ  volume of the reciprocal space covering one wave number, the factor 2 is due to the required consideration of two possible spinorientations, Σq  area of one sector of the package of sectors oriented parallel to the reduced sheet of the Ssurface, without being more distant from it in q  space than one unit of quasimomentum ~q of the generated phonons, this way ensuring the transition of electrons from the volume Σq q of the states with quasimomenta ~k into the same volume with quasi momenta ~k′ , being located at opposite sides of the Ssurface. Further assuming that Σq ≈ 20(π/a)2 , we get Σq δ −1 =
5a q N, 8π
Rq =
5a q N. 4π
(3.22)
This means that for q ∼ (10−3 ÷10−2 )π/a the number of pairs of state being active during phonon generation is about (10−3 ÷ 10−2 ) times from the total number of states 2N. After substitution with (3.22), (3.16), (2.4) in (3.10) and using M ≈ 10−25 kg, G ≈ 10−19 J (G ≈ 0, 6 eV), Γ ∼ (1011 ÷ 1012 ) s−1 , we finally get σth ≈ 10−4 ÷ 10−3 . Using the expressions (2.5), (2.6), being related to additional nonequilibrium terms in the energy distribution of electrons, in conjunction with the energy conservation law (1.9), we can express the inverted initial occupational difference in the pattern 83
σ0 (∇T ) = fk − fk′ ≈
i yk ∂fk0 h ~ − ~ωq ,   kB τ (vk′ − vk )∇T kB T ∂yk
(3.23)
i 1 ∂fk0 h ~ ′ σ0 (∇µ) = fk − fk′ ≈   τ (vk − vk )∇µ − ~ωq . (3.24) kB T ∂yk Table 3.1 shows the values of σ0 obtained for some representative yk = (εk − µ)/kB T (after omission of the last term in (3.23) and (3.24)), using: T = 103 K, ∇T = ∆T (10 vk τ )−1 , ∇µ = ∆µ (10 vk τ )−1 , ∆T = 100 K, ∆µ = 0, 15 eV = 1, 74 kB T . It is obvious from Table 3.1 that the crucial condition for excess generation of phonons σ0 > σth is easily satisfied for σ0 (∇T ), as well as for σ0 (∇µ), in the latter case even with an excess of the order of magnitude (since 2 · 10−1 > σ0 (∇µ) > 10−2 > 10 · σth ). We have however to remark that for q ∼ (10−3 ÷ 10−2)π/a, the value of the projection vk towards the orientation given by the heterogeneity gradient attains an order of magnitude of about 103 m/s. At the other hand, if 10 average free path lengths of electrons of about 10vk τ ∼ 10−8 m were taken as a natural scale of the average size of an heterogeneity, and further assuming τ ∼ 10−12 s, then we would get a length one order of magnitude less than half wavelength, as given by the expression λ/2 ∼ 4π/q ∼ 10−7 m. From the point of view that a MT can be described as a diffusionless lattice deformation process, then at least λ/2 would fit into our assumed scale of the heterogeneity (see also the treatment of (1.2) in Pt. 1.3 and SubPt. 7 of Pt. 1.5, as well as Chap. 6). In this case however, for an evaluation of ∇T and ∇µ, it would be more realistic to use a value of 102 vk · τ , instead of 10 vk · τ (thus in this case the values of σ0 in Table 3.1 would have to be reduced by one order of magnitude), and for σth ∼ 10−3 the condition σ0 > σth would only be satisfied for the σ0 (∇µ). However, assuming σth ∼ 10−4, then the condition σ0 > σth would easily be satisfied for both the thermal and the chemical potential of heterogeneities ( σ0 (∇T ) and σ0 (∇µ) ). We shall resume our consideration of a realistic spatial scale of an inhomogeneous (nonequilibrium) distribution of T and µ in Pt. 3.3 (from a different point of view).
3.2
Threshold conditions for two and threemode wave generation and characteristics of a phase transition of a radiation system
We shall now deal with multiphonon processes involved in the generation and amplification of waves, using some reasonable and justified approximations within the basic objectives of our analysis. In our notion of the γ − α MT, the electronic transitions between the states k,k′ , occurring in the vicinity of the Sh111i surface 84
Table 3.1. Inverted initial population difference as a function of the parameter y y 0 1 1,54 2 3
∂f 0 /∂y 0,5 0,197
σ0 (∇T ) · 103 0 3,94
0,156 0,105 0,045
σ0 (∇µ) · 102 17,4 6,86
4,78 4,2 2,7
5,43 3,65 1,57
σth · 103 (0, 1 ÷ 1)
under participation of two or three longitudinal phonons, are supposed to be of real importance. The quasimomenta of these phonons are oriented either along the two  and fourfold symmetry axes (during a twophonon process), or along the fourfold symmetry axes (during a threephonon process). This statement is put into relation with the assumption that predominantly the longitudinal waves, which propagate in the h001i and h110i orientations, initiate the process of Baindeformation (see (1.1)). It would be further interesting to find the conditions for multimode generation and to compare them with the conditions for singlemode generation. Such a comparison would then enable us to find a criterion for identification of such cases where multiphonon processes carry out independent or supportive functions for singlemode generation, during a γ − α  MT. To disclose and enlighten the outstanding features of twomode generation, it is convenient from the outset to omit singlephonon processes and define a specific model Hamiltonian as the Hamiltonian of the electronphonon system: + H = ~ωq b+ q bq +~ωp bp bp +
X
εk a+ k ak +W (q, p)
X
+ + + b+ p bq ak ak′ +bp bq ak′ ak . (3.25)
k
k
Here, b+ , b, a+ , a are the phonon and electron creation and annihilation operators, respectively. During the summation of quasimomenta of the electrons ~k we shall however only consider those states located in the vicinity of the surface S[111] (see (2.2)). In (3.25), the quasimomenta ~q and ~p are oriented parallel to the axis [001] and [110] (q⊥p), thus the following conservation rules are satisfied: εk′ − εk − ~(ωq + ωp ) = 0,
k′ − k − q − p = 0,
Q.
(3.26)
Here, Q  vector of the reciprocal lattice, to be considered in the case of UProcesses. However, as the quasimomenta ~q, ~p can be judged as small quantities in relation to the quantity ~π/a, the importance of Uprocesses is only appreciable for a small fraction of the totality of transitions with quasimomenta ~k, ~k′ , in the immediate proximity of the lines LW, XW. Thus we will later 85
consider Nprocesses, selecting zero in the righthand side of the quasimomentum conservation law (3.26). With quasimomenta ~q, ~p σth2 , there exist two other valid solutions, in addition to ˜bp = 0: (˜bp )1,2
21 1 R = (σ0 − σ1,2 ) 6= 0. 2 κp tσ
(3.31)
For σ0 = σth2 , we get from (3.29) and (3.31): σ0 σth2 σ1 = σ2 = = ; 2 2
(˜bp )1 = (˜bp )2 = ˜bpth
1 1 R σth2 2 = 2 2 κp tσ
(3.32)
The correct expressions for ˜bq can be obtained by replacement of p by q (p ⇆ q). The investigation on the stability of these solutions and their interpretations will be performed by considering the transition in the generating mode as a particular kind of phase transition of a radiation system, as proposed by Haken in [98, 135, 137]. The role of the ordering and temperature parameters will be represented by ˜b and −σ0 respectively. The analog expression for free energy B can easily be found by considering Eq.(3.30) as an extreme condition dB = 0. d˜b Then, after omission of the irrelevant constant, we get: B ≡ B2 (˜b) = ϕ(˜bp ) + ϕ(˜bq ), " # 2 ˜b4 4 t W κ 1 R σ σ p 0 2 p ϕ(˜bp ) = κp ˜b2p − ln 1 + . 2 16 tσ ~2 Γ κq
(3.33)
The expression ϕ(˜bq ) can be obtained from ϕ(˜bp ) by the changing p ⇆ q. Now it is easy to verify that the function B2 (˜b) attains a single minimum in the region σ0 < σth2 , corresponding to ˜b = 0. For σ0 = σth2 , a flex point ˜bt arises, being a forerunner of additional extremes taking shape in the region σ0 > σth2 . The additional minimum B2 is associated with the value ˜b2 (3.31), while the maximum 87
corresponds to ˜b1 , which indicates an instability of the solution ˜b1 and a stability of the solution ˜b2 . This is a distinct indication for the emergence of a scenario of a typical 1st order phasetransition (see (3.1)), where the value σ0 = σth2 determines the limit of absolute loss of stability of the phase with nonvanishing magnitude of order parameter. The analog of the critical temperature of a 1st  order phase transition is the critical value of occupation inversion σ0 = σc , at which the minimum values of the function B2 match, i.e. B2 (˜b = 0) = B2 (˜b2 ) = 0.
(3.34)
We can now determine ˜b2 by substituting the expression for σ2 from (3.29) in (3.31). After insertion of ˜b2 in (3.33), we are able to express (3.34) in such a manner that we can determine σc : h i2 −2 1/2 −2 1/2 2 = 0, (3.35) 1+ 1−ψ − ln 1 + ψ 1 + 1 − ψ −1 where ψ = σc σth2 . The numeric solution of (3.35) renders:
ψ ≈ 1, 25,
σc ≈ 1, 25 σth2.
For σ0 > σc we get B2 (˜b2 ) < B2 (0), indicating a higher relative stability of the phase corresponding to ˜b 6= 0. After further analysis, we can realize a decrease of the maximum of B2 (˜b1 ), which plays the role of a potentialbarrier between the states with ˜b = 0 and ˜b2 6= 0, as well as a decrease of the actual value of ˜b1 with increasing parameter σ0 σc−1 > 1 (B2 (˜b1 ) → 0 only for σ0 σc−1 → ∞ ). As the value of σ0 is limited (σ0 < 1), the satisfaction of Eqs. ˜b1 = 0 and B2 (˜b1 ) = 0, indicating an absolute loss of stability of the phase with vanishing orderparameter, will only be possible at σc = 0. However, if σc ∼ σth 6= 0, it is not possible to introduce a value σc corresponding to the temperature of absolute loss of stability of the hightemperature phase. A consideration of threemode generation with frequencies ωk ,ωp and ωq would lead us to qualitatively similar conclusions. For this reason, we will only denote the expressions for the threshold and for the critical occupational differences. σth3 = where
1 3 4 Γ t2σ ~2 κk κq κp 3 , R
W3 ≡ W (k, p, q) =
σc ≈ 1, 41 σth3
(3.36)
i G k p q ~3/2 . (2MN)3/2 (ωk ωp ωq )1/2
We can realize the difference between two and three phase generation on the one hand and singlephase generation on the other hand, which can thus be defined 88
as a secondorder phase transition of a radiation field at threshold occupational differences σth1 (3.10), which we shall write once more, for comparison, σth1 =
Γ κq ~2 i~1/2 G q , W ≡ W (q) = 1 R W1 2 (2 M N ωq )1/2
(3.37)
and which can be interpreted as an analog to the expression of the Curietemperature. In fact, if we regard (3.11) in 3.1 as a prerequisite for a minimum of the free energy equivalent B1 (˜b), then we get: # " 2 ˜2 ˜b2 σ0 R κ 4 t W  b σ 1 B1 (˜b) = . (3.38) − ln 1 + 2 8 tσ ~2 Γ It can easily be verified that  in the region σ0 < σt1  the function B1 (˜b) attains a minimum at ˜b = 0, and in the region σ0 > σth1 another minimum at ˜b 6= 0. This is a clear indication of a non  stability of the ordered state below the generation threshold, and of the disordered state above the generation threshold. Moreover, a typical feature of 2nd order transitions can be inferred from the smoothly changing of the order parameter while approaching to σ0 = σth1 . The expressions σc ∼ σth 2,3 also differ significantly from σth1 . By definition, σc implicitly includes a timevariable tσ , in addition to the parameters specifying −1 −1 σth1 . We thus determine the relations σth2 σth1 and σth3 σth1 , using the assumption that frequencies of a given order of magnitude will be generated in a single mode, as well as in two or three modes, respectively. Then we get from Eqs. (3.29), (3.36) and (3.37), within an accuracy given by factors of order σth2 G ∼ σth1 ~
tσ Γ
1/2
;
" #4/3 1/2 σth3 G tσ ∼ . σth1 ~ Γ
1/2
(3.39)
Thus for ~−1 G tσ Γ−1/2 < 1, multimode generation could formally start sooner than singlemode generation. It has however to be considered that this inequality can only be satisfied by a reduction of G or by raising of Γ within the region of the threshold condition σthj > 1, j = 1, 2, 3, being unattainable in reality due to the limitation σ0 < 1. But also the parameter tσ has a natural lower limit. According −1 to (3.4), (tσ )min = Γ−1 , but (σth2 σth1 )min ∼ G(~ Γ)−1 , and for the previously −1 used values G ∼ 10−19 J, Γ ∼ 1012 1/s we get σth2 σth1 ∼ 103 . Thus the role of processes with two and three participating phonons can mainly be attributed to the amplification (and possible synchronization) of modes generated by singlephonon processes. Our common consideration of single and twophonon processes has been performed for the most favorable case of generation, being characterized by electronic transitions with one or two participating phonons, occurring in the proximity of different Ssurfaces. To take an example, during the generation of a pair of waves along the orientations ∆−[001] and Σ−[110], it is possible to analyze singlephonon 89
B2 σ0 < σth2 0 B2 σ0 = σth2
−˜bn
0 B2
˜bn
σth2 < σ0 < σc −˜b2 −˜b1
0
˜b1 ˜b2
B2 σ0 = σc
−˜b2 −˜b1
0
˜b1 ˜b2
Figure 3.1. Image of the function B2 (˜b) at different values of occupational difference σ0 . processes in the proximity of the surfaces S[001],[110] , and twophonon processes between states in the proximity of S[111] . Omitting some usual considerations, −1 −1 being negligible for our purposes, and considering σ0 σth2 ≥ σth1 σth2 as a small quantity, we can present a stationary solution for the simplest case of equalities: ˜b2 = ˜b2 = ˜b2 for the numbers of generated phonons; R∆ = RΣ = R for the numbers ∆ Σ of pairs of electronic states; σ0∆ = σ0Σ = σ0Λ = σ0 and tσ∆ = tσΣ = tσΛ = tσ (for the longitudinal relaxation times), confined to the states located in the proximity of different Ssurfaces. Then our solution is: ˜b2 = 0, σ0 < σth1 , 2 ! 2 σ 2 σ ~ Γ 0 0 ˜b2 ≈ , 1+ −1 4 W1 2 tσ σth1 σth2
(3.40) σ0 > σth1 ,
being distinguished from the solution for singlemode generation (3.13) by a fac90
−1 2 tor 1 + (2 σ0 σth2 ) , thus clearly indicating the amplification effect by twophonon processes.
3.3
The lattice strain induced by the generated waves
For realization of martensitic transformation, in accordance with the wavemodel, it is necessary that the amplitudes of the generated waves have exceeded the threshold (ut (λ, T )), which essentially depends on the wavelength λ and on the temperature T. The maximum of ut (λ) can be evaluated by geometrical considerations alone, taking into account that  for pure Baindeformation [13]  the transition to new equilibrium conditions is associated with a relative displacement of 0, 1a (a latticeparameter) of the atoms neighboring in the orientation h001i. This means that an instability must be expected for relative lattice displacements greater than ≈ 0, 05a. If such displacements were associated with a wave, then the amplitude of such waves would obviously be ∼ 0, 05 λ/2 = ut (λ). The value ut (λ) being independent of temperature can be put into natural correspondence with the threshold ut (λ, T0 ), where T0  equilibrium temperature between austenite and martensite. The supercooling below the equilibrium temperature ( for definiteness, the straight MT under cooling is considered ) must occur with the decreasing of austenite stability and hence: ut (T, λ) < ut (T0 , λ). Let’s remind (see Pt. 1.3) that waveamplitudes creating the thresholddeformation εth of about 10−3 are anticipated in the proximity of MS . In evaluating the stationary amplitudes u of the generated waves, we can disregard the influence of electronphonon interaction associated with multiphonon processes. Then, using the link between u and ˜b by (3.14), as well as the expressions (3.40) and (3.37), we get the following relation:
2~ uq = MNωq
21
12 Γ σ ~ 0 ˜bq ≈ . −1 Gq tσ σth1
(3.41)
The deformation ε in turn is linked up with the amplitude by the relation (1.2) in Pt. 1.3: 12 2 σ0 2~ Γ ε = uq q ≈ . (3.42) −1 π π G tσ σth1 −1 Assuming tσ = Γ−1 , σth1 ∼ 10−3 , σ0 σth1 − 1 ≈ 1, 6  corresponding to the value σ0 (∇µ), y = 2 in Table 3.1  and using the quantity 102 vk · τ as a natural gage of heterogeneity (see end of Pt. 3.1), with G ∼ 10−19 J and ~ Γ ∼ 10−22 J, we get 91
from (3.42): ε ≈ 3, 2/π · 10−3 . As a result, the existence of waves with amplitudes ensuring a lattice deformation near the elastic (yield) limit, should be reasonably possible. We further note that for λ/2 ∼ 10−6 m and ε ∼ 10−3 the waveamplitude (u = ε λ/4 ≈ 5 · 10−10 m ≈ 1, 4a) becomes even greater than the latticeparameter. Let us now discuss the applicability of our estimates, taking into account that they are based on stationary solutions. Above all, the lifetimes of spatially inhomogeneous distributions of temperature and chemical potential have to be evaluated. Let these times be t∇T , t∇µ and, taking into account that such heterogeneities rapidly fade away, mainly as a result of conduction and diffusion processes, we can obtain an estimate of these times t∇ , becoming clearly obvious from dimensional considerations: t∇T ≈
lT2 , dT
t∇µ ≈
lµ2 , dµ
(3.43)
where lT, µ  characteristic gages of inhomogeneity, determining ∇T ≈ ∆T · lT−1 , ∇µ ≈ ∆µ · lµ−1 ; dT and dµ  heatconduction and diffusion coefficients, respectively. The typical value of dT ≈ 10−5 m2 /s for T > TD can easily be obtained from below equation (3.44), by linking up dT with heatconductivity λt , specific heat capacity Csp and density ρ: dT =
λt , ρ Csp
(3.44)
where λt = 34 W/mK, ρ = 7900 kg/m3 , Csp ≈ 4, 6 · 102 J/kg K (the specific heat capacity has been derived from the DulongPetitLaw, being substantiated for T > TD ). Taking into account that the term dµ is a coefficient of proportionality which combines an electric current density j with the gradient ∇nγ of conduction electron concentration in the γ  phase, we are able to express the term dµ by the specific conductivity σγ of the γ  phase. For this purpose, we start with an appropriate 2/3 conversion of the expression for currentdensity j, presupposing that µ ∼ nγ : j=−
2 σγ µγ σγ ∇nγ . ∇µ = − e 3 e nγ
(3.45)
After division of both sides of (3.45) by the electron charge e, we get: j 2 σγ µγ =− 2 ∇nγ ≡ −dµ ∇nγ , e 3 e nγ
dµ =
2 σγ µγ . 3 e2 nγ
(3.46)
After insertion of σγ ≈ 106 m−1 Ohm−1 , nγ = 1029 m−3 , µγ ≈ 10 eV = 1, 6 · 10−18 J into (3.46), we get dµ ≈ 4 · 10−4 m2 /s.1 1
The order of magnitude of the current density j being generated by the chemical potential gradient 106 eV/m in the transformation front is 1012 A/m2 for σγ about 106 m−1 Ohm−1 and substantially greater than any drift current observed in semiconductors.
92
Obviously in our assessment of the quantities ∇T , ∇µ the usage of the quantities ∆ T ∼ 102 K ∼ (T0 − MS ) and ∆µ = µα − µγ  ≈ 0, 15 eV can be justified if the nucleation time tN is less or of the same order of magnitude than that the time of existence of the gradient t∇ . Otherwise, conduction and diffusion processes would smooth down the jumps of temperature and concentration at the phase boundary. In the nucleation model of the macronucleus, we can determine the minimum values (lT )min and (lµ )min from the requirement tN = t∇ , using (3.43), further assuming tN ∼ 10−11 s (see treatise under Pt. 1.3), which would correspond to a nuclear radius rN ∼ 10−5 cm and to a speed of propagation of the nuclear boundary of V ∼ 103 m/s: (lT )min = (tN dT )1/2 ∼ 10−8 m, (lµ )min = (tN dµ )1/2 ∼ 6 · 10−8 m. If ∇µ was considered as a stationary quantity, then the quantity lµ ∼ 10−7 m would be a natural gage. We remind that, at the end of Pt. 3.1, we came to a similar conclusion (which however resulted from different considerations). The issue related to the applicability of stationary estimates of the amplitudes u = ust and deformations ε = εst is more complex. In fact, the transition to virtually stationary values of u, ε, within certain characteristic period tu = tε , will not depend on the values of u0 , ε0 at the starting moment t0 , provided tu ust , ε0 > εst , the stationary estimate then would deliver the lower limit of u, ε (for σ0 > σth1 ). For an evaluation of tu , the nonstationary solution of ˜b(t) must be known. However, it cannot be found for the general case, but in the vicinity of the threshold for singlemode generation, the equation for ˜b leads to the VanderPol equation (see for example § (3,a) in the lectures of HakenWeidlich [132]): D=κ
d −D dt
˜b+ + β ˜b+ ˜b ˜b+ = 0,
σ0 −1 , σth1
β=
4 tσ κ W1 2 σ0 . Γ σth1 ~2
(3.47)
Formally, the VanderPol equation can be obtained if the temporal derivatives ˜ ˜˙ + of system (3.7) are only reestablished for the quantities ˜b+ q , bq , by writing  bq for the right side of the first Eq. (3.7), instead of zero, leaving the other equations unchanged (Of course, this is an adiabatic approximation, which means that the 93
radiating subsystem will immediately be subordinated to the orderingparameter ˜bq ). Then, d˜ and σ must be excluded, and a decomposition of the resulting factor −1 4 tσ W1 2 ˜+ ˜ 4 tσ W1 2 ˜+ ˜ 1+ b b ≈ 1 − bq bq q q ~2 Γ ~2 Γ
(3.48)
˜ must be performed with an accuracy up and including to the linear term in ˜b+ q bq . As we already excluded the dipolemoment d˜ and the occupation difference σ in our search for a stationary equation for ˜b+ q , we can immediately use Eq. (3.11). It delivers the nonstationary equation for ˜b+ q in an adiabatic approximation, by multiplication with −κq and addition of ˜b˙ + to the left side: q
˜b˙ + = κq ˜b+ σ0 q q σth1
˜ 4 tσ W1 2 ˜b+ q bq 1+ ~2 Γ
!−1
− 1 ≡ −χ ˜b+ q.
(3.49)
With consideration of (3.49), we immediately get (3.47) from (3.49). Eq. (3.49) will be further used in Chapter 6, so that we can now deal with to the more simple Eq. (3.47). Assuming that the quantity ˜b attains the value ˜b0 , due to fluctuations at the starting time t = 0 , we get from (3.47): ˜b =
1 β − 2 b0 D
−2 D t
e
β + D
−1/2
.
(3.50)
It follows from (3.50), that for D > 0, t → ∞, ˜b → (D/β)1/2 6= 0, but ˜b → 0, for D < 0, t → ∞. It also is obvious from (3.50) that the only relevant characteristic time is: tu = (2 D)−1.
(3.51)
Here, the following observation is striking enough to attract our attention: As a general rule, during approach to the starting temperature of a secondorder phase transition, the tendency of tu to infinity for σ0 → σth1 would be analog to the critical degradation of fluctuations of the ordering parameter. Even though the VanderPol equation is not applicable for states located significantly beyond the threshold, an evaluation of the order of magnitude of tu can nonetheless be performed on the basis of Eq. (3.51). Assuming an attenuation −1 κ ≈ (10−4 ÷ 10−3 )ω, in accordance with (3.16), we can realize that for (σ0 σth − 1) of order 1 the resulting time tu evaluated on the basis of Eq. (3.51) must be not less than (10κ)−1 . Hence only the inequality tu >> t∇ is satisfied in the region of parameters interesting for us: ω ∼ 1010 ÷ 1011 s−1 , tu ≥ (10−8 ÷ 10−9 ) s. In accordance with our above treatise, it must be concluded from this latter inequality that our stationary evaluations of u and ε, having been obtained on the basis of 94
(3.41), (3.42), would only be justified for hard modes of excitation, i.e. u0 ≤ ust , ε ≤ εst .2
3.4
Conclusions from Chapter 3
From the above analysis of the equations for a nonequilibrium electronphononsystem, it is possible to draw the following conclusions: 1. Electronphonon processes with participation of a single phonon play a dominating role during the generation of longitudinal latticedisplacement waves, while the role of multiphonon processes is limited to the amplification of waves. 2. Wave generation takes place through relatively longlived ES with an average lifetime of about τ0 ≥ 10−12 s. 3. Among two nonequilibrium sources in electronic subsystems, being defined by the existence of ∇T and ∇µ, the latter one, being caused by the inhomogeneity of the chemical potential µ, is the more effective one in generating longwave phonons (q ∼ (10−3 ÷ 10−2 )π/a). 4. In the case of largesized reduced sheets of the Ssurfaces (Σ ≥ (π/a)2 ) with weak energydispersion near the µvalue, as well as for chemical potential gradients ∇µ ∼ 106 eV/m (1010 K/m in a temperaturescale) the generation of longitudinal elastoplastic waves, being linked up with latticedeformations close to the limits of elasticity of about ε ∼ 10−3 , becomes possible. 5. For some characteristic temporal gauges, the following chain of inequality conditions may be suggested: tu >> t∇ > tN > τ0 ∼ tσ .
(3.52)
The central term t∇ > tN of (3.52) determines a relation between t∇  the lifetimes of ∇T and ∇µ, respectively  and the time of macronucleation tN ≥ 10−11 s, which, in turn, also implies minimal spatial gauges lT ∼ 10−8 m, lµ ∼ 10−7 m for stationary evaluations of ∇T = ∆T · lT−1 , ∇µ = ∆µ · lµ−1 . The first term tu >> t∇ shows that a realization of the deformation level obtained from an evaluation of (3.42) (for stationary conditions) only becomes feasible for hardmode waveexcitation. Within the frame of the developed model of the γ −α MT as a deformation process, being controlled 2
Editorial note: If a transformation energy of ( 0, 01 ÷ 0, 1) eV per atom is assumed, then the maximum possible powerdensity (power per unit surface) of the transformationwavefront would be of an order of magnitude of ≈ (0, 1÷1)GW cm −2 , determining the level of external energy flow being necessary for the martensitic transformation start.
95
by the thresholddeformation εth ∼ 10−3 of the carrierwaves, this means that the thresholdlevel εth must arise simultaneously with beginning growth i.e. for t0 = tN . This latter conclusion matches very well with the interpretation of the observed pronounced supercooling of the γphase below the phaseequilibrium temperature T0 (including a significant freeenergy excess for compensation of the energy required for builtup of the phase boundary, and of the elastostatic distortion field), thus being an essential prerequisite for the excitation of oscillations with an amplitude sufficiently large to produce permanent latticedeformations of about ε0 ∼ 10−3 in the nucleation stage (see Pt. 1.3 and Pt. 1 of the task defined by Pt. 1.5). Such deformation levels thus will be sufficient to overcome the threshold separating the metastable state of fcclattice from the more stable state of bcclattice (at T = MS ). The treatise of Chapter 3 is mostly based on the papers [140, 141] and, to a lesser extent, on [56], the results of which have been improved in this chapter, mainly by the replacement of the Pplanes of the simplified model by Ssurfaces and by the specification of the rather illustrative quantitative estimates presented in [140, 141]. Some additional remarks 1. The tasks of development of kinetic equations for a nonequilibrium electronphonon system, as well as the analysis of threshold conditions during singlemode generation within the conceptual notion of isoenergetic Psurfaces with inhomogeneous distribution of temperature has been treated in [142–146] and summarized in [147], within the frame of the method of the nonequilibrium statistical operator of Zubarev and Kalashnikov [148–150]. The results presented in these works, as far as they relate to the γ − α MT, are alike to the results of Pt. 3.1, at least in a qualitative aspect. They can be taken as a justification of the semiphenomenological approach, being characterized by the introduction of relaxation constants to consider dissipative processes. Furthermore it has been shown in [146, 147] that a system of equations with mixed coordinate and momentumrepresentation, resulting from a reduction of the macrovariables f, σ, d, b by powers of the respective gradients, attains a local spatial form matching with (3.3), with sufficient precision until the first nonvanishing terms. However, in this case the macrovariables σ, d, b must be considered as functions of the xcoordinate being oriented parallel to the orientation of highest heterogeneity e. This representation highlights that the probability for the presence of an electron within in the immediate vicinity of a point x, with simultaneous presence of electronic flows, will largely depend on the orientation of the groupvelocity v of that electron in relation to e, and that in one and the same point in space states with inverted occupation can exist. The spatiallylocal nature of such describing justifies the application of the findings obtained in the quasimomentum rep96
resentation to an analysis of the nonequilibrium state in the proximity of the propagating phase boundary. 2. Generally speaking, the drift mechanism for the creation of a population inversion is well known, being used for example at generation and amplification of elastic waves in semiconductors (see [151, 152]). Usually, the conditions for wave generation by a drift mechanism focus on the requirement that the electron drift velocity vd must locally exceed the speed of sound c, i.e. vd > c. Thus this condition is equivalent to that formulated by Tscherenkov for phonon radiation generation by drifting electrons. Within the frame of our designations, the condition vd > c is equivalent to the condition σ0 > 0, being an essentially weaker requirement than σ0 > σth1 . Obviously from (3.24), the condition σ0 > 0 is equivalent to the equation ~ µ > ~ ωq = ~ c q. (vk′ − vk ) τ ∇
(3.53)
Taking into account that the states k, k′ are located in the vicinity of the Ssurface, and that the dispersionlaw for these states along the direction e  is a quadratic function (see Chapter 2), we get:
vk′ − vk = ~ [s − k′ − (s − k)] m−1 s = ′ −1 = ~ (k − k ) ms = ~ q m−1 s ,
(3.54)
where s  vector designating the intersection point s of the vector k − k′ = q with the Ssurface, m−1  reciprocal effective electronmass in point s. s After substitution by (3.54) in (3.53), we get the condition for Tscherenkovradiation: vd = τ ∇µ m−1 s > c.
(3.55)
For ∇µ ∼ 106 eV/m = 1, 6 · 10−13 J/m, τ ∼ 10−12 s, ms ≈ 3 m0 ∼ 3 · 10−30 kg, we obtain vd ≈ 5 · 104 m/s, the magnitude of which exceeds the speed of longitudinal waves by about one order of magnitude and thus is sufficient for satisfaction of the threshold condition σ0 > σth1 , within a temperature region of T ∼ 103 K. However, the realization of waves carrying a deformation amplitude of ε0 ≥ 10−3 requires the larger values of ∇µ, corresponding to vd ∼ 105 m/s. The region of vd ∼ (104 ÷ 105 ) m/s also is typical of semiconductors [151]. To have ended this comparison, we remind that the generation of elastic waves in a semiconductor requires the considerable driftvelocities as well as the large values of the electronphonon interaction matrixelements (semiconductorspiezoelectrics). In the case of the γ − α  MT, this interaction is not large. Instead, the number of pairs (k, k′ ) of 97
active electronic states is large, whereas in turn this factor is of minor importance for semiconductors. Of course, neither the drift mechanism of pumping nor the existence of electrical conductivity are exclusive prerequisites for the emergence of a phononmasereffect. Alternative principles of a masereffect are also known (see for example [136, 153, 154]). 3. Finally, we remark that, besides stimulated emission of radiation, in an inversely occupied radiation system the spontaneous collective superradiation (Dicke)8 , with the intensity being proportional to the square of the number of pairs of active states, is also possible (see for example [134,154,155]). As the time for the development of superradiation must be less than the relaxation time Γ−1 ∼ τ0 of the dipolemoment, the generation of a superradiation pulse is not possible for the frequencies ν of phonons below τ0−1 . Then, assuming τ0 ∼ 10−12 s, it is meaningless to discuss this effect for phononradiation with quasimomenta q ∼ (10−3 ÷ 10−2 )π/a or with frequencies νq < τ0−1 . Thus the masereffect is the predominant generation mechanism of phonons with the relevant region of wavevectors.
98
Chapter 4 Coordination between of the γ − α martensitic transformation temperature and the optimum wave generation temperature in ironbased alloys 4.1
Definition of the task
Our previous analysis suggests that, in the growth stage of martensite, the existence of latticedisplacement waves with deformation amplitudes of ε ∼ 10−3 is a real possibility. Let us remind that the evaluation of the fulfilment of the general thresholdconditions has been performed for the hightemperature region, where the frequency of collisions with shortwave phonons is large. Then there is reason to think that this evaluation in order of magnitude is satisfactory not only for pure iron but also for the iron based alloys. However, to generalize our conclusions and to obtain the optimum conditions of wave generation over the full range of concentrations of the alloying elements (for example up to 10% Mn or up to 34% Ni) and of carbon (up to 1,8 weight%), a special investigation is required. On the one hand, the existence of a high level of population difference σ0 in accordance with (3.23), (3.24) would require that the magnitude of the parameter y = (ε −µ)(kB T )−1 must not exceed a few units, as the multiplier ∂f 0 /∂y rapidly diminishes with increasing y (see Tab.3.1), and hence also the value σ0 . On the other hand, with increasing concentration of Ni the temperature (MS ) is decreasing (practically, down to 0 K for 34 % Ni), thus the value of y would have to increase. This difficulty cannot be resolved (vide infra) by the formal assumption about the necessary reduction of the magnitude (ε − µ) to ensure practical stability or reduction of the parameter y. Moreover, the assumption that the increasing of Ni concentration causes a 99
requisite reduction of the difference ε − µ, due to the filling of the energy band (the model of hard zone) by excesselectrons (two electrons per Niatom), cannot generally be supported, as this model leads to the wrong conclusion about the increasing of MS for a FeMnsystem, because the difference ε − µ must increase with increasing Mn concentration. In reality, investigations on binary alloys of the FeNi system (up to 28% Ni), as well as of the FeMn system ( up to 10% Mn) clearly show the decreasing of MS with increasing concentration of the alloying element for the common type (the packetmartensite) of γ − α  transformation, therewith the decrease is more pronounced for the Mnalloys. So, a comparison of data [7] and [156] shows that a reduction of MS , down to the level of 500 K, requires concentrations of 20% Ni or only 10% Mn. Assume that the energies of 3d electronic states, belonging to the Ssurface, are characterized by a given mean εd (see also the context to Eq.(3.9)). Then we can define the following model antithetical to the hardzone model: In alloys of iron with elements of close neighbors in the 3d row of the transition metals (substitution alloys), the value εd − µ is considered as nondepending (or weakly depending) on composition and thus conserving the value that is the same as in pure γ  iron. This means is that the alloying element builds up own 3d subbands, which overlap with the 3d  bands of iron without a charge exchange flow among the components of alloy. (Hypothesis of minimum polarity [100]). Furthermore, we will assume that the magnitude of the threshold difference σt retains a value not exceeding 10−3 (as estimated for the region of high temperature), in alloys undergoing a martensitic transformation. Then, fulfilment of the threshold condition σ0 > σt can be justified within of the twoband model, for a wide region of concentrations Cae of alloying elements, using the assumption that the magnitude of attenuation Γs of mobile s electrons is comparable with the value (εd − µ)~−1 and many times larger than the attenuation Γd of the 3d  electrons, which are active during the generation of phonons (the typical lifetime of s  electrons τs ∼ 10−15 s in 3d metals corresponds to the value ~ Γs ∼ 0, 6 eV). The population of states with energies εd > µ can be kept up fd0 ≥ 0, 1 by an effective scattering mechanism into d states of s  electrons with energies εs that are corresponding to the condition εd − µ −
~ Γs ~ Γs < εs − µ + ~ ω < εd − µ + . 2 2
(4.1)
In (4.1) ~ ω is the energy of a shortwave phonon, whose participation is required for satisfaction of momentum conservation law, if the uncertainty of the quasimomentums of s  electrons is small (in (4.1), the value ~ Γd is disregarded compared to ~Γs ). Thus, for large Γs , the magnitude of thermal excitation kB T ∼ (εs − µ) can be much smaller than εd − µ, without reduction of the dstate occupation. In a similar way, the mechanism of d  s scattering ensures that the states with the energy εd , located below the Fermilevel, despite of an inequality µ − εd > kB T have the occupations fd0 < 1 significantly deviating from unit at the cost of an additional (nonthermal) broadening of the d  electron distribution function. 100
From the above analysis it is clear that the increase of concentration C of the alloying supplement (C < 1/2), which causes a rapid increase of the attenuationpart Γs (C) ∼ C(1 − C) of total attenuation, linked with the scattering on substitution atoms, Γs being combined with a temperaturereduction, by the following condition:
~ ω + kB T +
~ Γ(C, T ) ∼ εd − µ. 2
(4.2)
It has to be noted that the temperaturedependent contribution Γs (T ) connected with the scattering on thermally activated heterogeneities (vacancies, phonons, magnons etc.) is decreasing with decreasing T and must smooth down the behavior of Γs (C, T ), by stabilizing the broadening of the delectron distribution function, within a wide range of T and C. Logically, at first we must obtain a modification of the equilibrium distribution function f 0 → f˜0 in such a way that f˜0 must simultaneously consider the distribution function broadening determined by the factors T and ΓS . After that it is necessary to analyze the behavior of the derivatives ∂ f˜0 /∂µ, ∂ f˜0 /∂T which determine the magnitude of the population difference σ0 , together with the gradients ∇µ and ∇T . Hence we have to find such region of the variables ( T and Γ) in which (for a fixed value of εd − µ) the value σ0 attains a maximum that only slightly varies with simultaneous variations of T and Γ. The temperature belonging to this optimum region might then be defined as the optimum temperature T˜ for the martensitic transformation process. If the electronic configurations of the atoms of lattice matrix and of the alloying element are known, it will be possible to determine the dependence T˜(C), by calculating Γs (C) and identifying the correlation between T˜ and Γ(C, T˜). Then, the concentrationdependencies of T˜(C) and MS (C) will be compared. It is also possible to deal with the inverted task:
i we require a close relation between the dependencies of T˜ (C) and MS (C);
ii we choose the electron configuration of one of the alloying components;
iii we find the electron configuration of the atoms of the other component. It is the latter definition of task, allowing us to gather the additional information which will be used in the fourth chapter, during a comparison of the interdependence between T˜(C) and MS (C), in the substitution alloys (FeNi, FeCo, FeMn) and in the interstitial alloys (Fe  C). 101
4.2
Modified electronic distributions and their derivatives in the case of a rectangular spectral density function
A statistically disordered lattice of the binary substitutional type can be considered as the medium comprising an ideal (periodic) arrangement of lattice knots, for which the probability of occupation of a knot (lattice point) with atoms of either one of its two components is equal to C and 1 − C, respectively, where C  concentration of the dissolved component. The missing of a longrange order in such lattice, being caused by the stochastic nature of its singleknotpotentials, causes the states with predetermined quasimomenta to become nonstationary. Therefore  within the general notion of some kind of periodic ”effective” medium  one of the approaches for the description of substitutional alloys is characterized by the introduction of an effective NonHermitian Hamiltonian with complex eigenvalues, the imaginary part of which determines the extinction rate of electronic states [100]. The calculus of meanvalues of electronic operators comprises both thermodynamic and configuration averaging, which have to be performed independently from each other for systems without a shotrange order. As an example, the modified electronic distribution f˜0 of our interest is given by the expression f˜k0 =
Z∞
[1 + exp (
−∞
ε − µ −1 )] A(ε, k)dε, kB T
(4.3)
where the spectral density A(ε, k) is a configurationally averaged probability in a given alloy for the existence of an electron of energy ε in a state with quasimomentum ~k. Usually, the spectral density obeys the Lorentz (BreitWigner) formula: " 2 #−1 1 1 A(ε, k) = ~ Γk (ε − εk )2 + ~ Γk , (4.4) 2π 2 where Γk  extinction of an electron in a state with energy εk , where the extinction corresponds to the width at half of the height of the function A(ε, k). Furthermore, the normalization condition is satisfied: Z∞
A(ε, k)dε = 1.
(4.5)
−∞
Obviously from (4.4), (4.5), the spectral density (SD) function gradually transforms into the δ  function for Γk → 0 lim A (ε, k) = δ (ε − εk ) ,
Γk →0
102
(4.6)
and the distribution (4.3) into the FermiDirac distribution: −1 ε − µ k 0 0 lim f˜ = f˜k = 1 + exp . Γk →0 kB T
(4.7)
This is quite reasonable, as the condition Γk = 0 would implicitly require a reestablishment of longrange ordering, as occurring during gradual transition of a binary alloy into a singlecomponent system with C → 0. A simple analytical expression for f˜k0 can easily be found by choosing a rectangularly shaped spectral density function with a height of ~Γk −1 and a width of Γk , being symmetrically arranged with respect to the energy εk : 1 A (ε, k) = ~Γk
~Γk ~Γk Θ ε − εk − − Θ ε − εk + , 2 2
(4.8)
where Θ  Heaviside unitfunction Θ(ε) =
1 0
ε ≥ 0, ε < 0.
After insertion of (4.8) in (4.3), we get: 1 + exp (y − η ) 1 k k 0 , ln f˜k = 1 + 2ηk 1 + exp (yk + ηk )
(4.9)
(4.10)
where yk = (εk − µ)(kB T )−1 , ηk = ~ Γk (2 kB T )−1 . It can easily be verified that the limit condition (4.7) is satisfied for (4.10), so that we get for the lowtemperature case T → 0 1 εk < µ − (~ Γk )/2 1/2 + (µ − εk )(~ Γk )−1 µ − (~ Γk )/2 ≤ εk ≤ µ + (~ Γk )/2 lim f˜k0 = T →0 0 µ − (~ Γk )/2 < εk (4.11) a distribution with a scattering width ~ Γk , as shown in 4.1. Moreover, the normalization condition for an electronic distribution f˜k0 = 1/2 at εk = µ is satisfied, independent of T. Disregarding the dependency on k of the extinction Γ within a coherent potential approximation [100], we note that f˜k0 remains constant along isoenergetic areas with εk = const. in quasimomentum space, as f˜k0 = f˜k0 (εk ). Accordingly, we shall design our spectral function by A(ε, k) = A(ε, εk ). Taking for granted that (4.3) represents the energetic distribution function 0 ˜ f (εk s ) ≡ f˜k0 s of the selectrons in an alloy, we can now show that, for a given dsscattering mechanism with involvement of shortwave phonons, the equilib0 rium distribution: f˜kd = f˜0 (εk d ) of delectrons of energy εd in an alloy of the 103
same energy εs = εd is nearly equal to the function f˜0 (εs ). According to [157], the modification of the normalized integral of electronphonon collisions, being required after consideration of scattering at the substitutional atoms, can be reduced to a replacement of the δ  function, thus reflecting strict compliance with the conservation of energy requirement, by the Lorentzfunction: ∂ f˜kd ∂t
!
= col
2π X Wp 2 {A(εk′ s , εkd + ~ ωp)[Np (f˜k′ s − f˜kd ) + ~ ′ kp
+f˜k′ s (1 − f˜kd )] + A(εk′ s , εkd − ~ωp )[Np (f˜k′ s − f˜kd ) − f˜kd (1 − f˜k′ s )]}
(4.12)
where Wp   modulus of the matrixelement of electronphononinteraction, Np  phonondistribution function. Proceeding further with the integration of the εk ′ s , under consideration of the definitions (1.1) and (1.3), and in order to find 0 the equilibriumdistribution f˜kd , we require that the collisionintegral (4.12) must vanish. Then we get approximately f˜0 (εkd + ~ ωp ) + [ f˜s0 (εkd + ~ ωp) + f˜s0 (εkd − ~ ωp) ] Np 0 . f˜kd ≈ s 2 Np + 1 + [ f˜s0 (εkd + ~ ωp ) − f˜s0 (εkd − ~ ωp ) ]
(4.13)
If we develop (4.13) by powers of ω ′ = ~ ωp (εkd − µ)−1 , then we get in a zeroorder approximation 0 f˜kd ≈ f˜s0 (εd ).
(4.14)
By consideration of (4.10), the linear supplement in the right hand side of (4.14) ∂ f˜s0 (εd ) (1 − 2 f˜s0 (εd ))~ ωp ∂(εd − µ)
can be written in the following form
1 sinh Γ ′ (T ′ )−1 (1 − 2 f˜s0 ) ω ′, 2Γ ′ cosh Γ ′ (T ′ )−1 + cosh (T ′ )−1 where Γ′ =
~Γ , 2 (εkd − µ)
T′ =
kB T . εkd − µ
(4.15)
(4.16)
Let εkd − µ ≈ 0, 2eV, and ωp be of an order of magnitude of half of the Debyefrequency, then we get ω ′ ≤ 10−1 . An order of magnitude of about 0,1 also applies to the product of the other factors in (4.15), so that the corrective factor, being linear in ω ′ , becomes at least one order of magnitude smaller than in (4.14). Therefore, in an analysis of the nonequilibrium addenda to the function f˜d 104
∆f˜kd (∇µ) ≈
0 ~ τ vk ∇µ ∂ f˜kd , ∂µ′ εd − µ
µ′ =
µ , εd − µ
(4.17)
0 ~ kB ∂ f˜kd τ vk ∇T , ∂T ′ εd − µ it is possible to replace the function f˜d0 by f˜s0 (4.3) for εk = εkd . Under the presumption that this replacement has been performed all over, we can omit in our subsequent analysis the indices d, zero and tilde in our notation of the function ~ τ v∇T ~ , we only need to f˜d0 → f . After having fixed in (4.17) the values of τ v∇µ, ′ ′ analyze the derivatives ∂f /∂T , ∂f /∂µ for our envisaged determination of the optimum values of Γ and T (see Pt. 4.1), as a function of the dimensionless variables Γ′ and T ′ (4.16). It is convenient to use these variables, as the value of εd − µ will remain unchanged, according to our assumption in Pt.4.1. In the case of the spectral density (4.8) we can obtain from (4.10) the derivatives ∂f /∂T ′ , ∂f /∂µ′ by direct differentiation:
∆f˜kd (∇T ) ≈
∂f 1 = ∂T ′ 2 Γ′
h 1 + exp (y − η) i y sinh η + η(cosh η + exp y) + , ln 1 + exp (y − η) cosh y + cosh η ∂f 1 sinh η = , ∂µ′ 2Γ′ cosh y + cosh η
(4.18)
(4.19)
where η = Γ′ T ′ −1 , y = T ′ −1 . The results of our calculus of the derivatives ∂f /∂µ′ and ∂f /∂T ′ on the basis of (4.18) and (4.19) are presented in Figs. 4.2 and 4.3. In these figures, the group of thin lines represents the constant values of the functions ∂f /∂µ′ , ∂f /∂T ′ (being labeled at each line), while the dashed lines 1 and 2 are defined by the conditions ∂ ∂ ∂f ∂f (4.20) ′ = 0, ′ = 0. ′ ′ ′ ′ ∂T ∂µ ∂Γ ∂µ Γ T
These lines correspond to the maximum values of the derivatives ∂f /∂µ′ , ∂f /∂T ′ of the variables T ′ and Γ ′ and pass through those points where the parallels to the vertical and horizontal coordinate axes touch the isolines. The area enclosed by the lines in Fig. 4.2 represents a region of values of the parameters T and Γ for which the occupational inversion σ0 (∇µ ) attains maximum values, only slowly varying with T and Γ. Obviously, it is justified to define an optimum temperature for phonongeneration, which decreases with increasing extinction Γ, by highlighting within this region the point corresponding to pure iron. Thus the behavior of the derivative ∂f /∂µ′ suggests the existence of an optimum temperature T˜1 , the derivative of which obeying to the condition ∂ T˜1 /∂C < 0, where C = Cae is the concentration of the alloying element. The jump of the value of ∂f /∂µ ′ from 0 up to 0,5, during the transition from Γ ′ < 1 to Γ′ > 1 (at the point 105
f˜0
1
µ
ε
h ¯Γ Figure 4.1. Modified SD  function at a temperature of 0 K.
T′
2
0,224 0,227 0,234
1 0,5
0,23 0,3 0,4 0 1
2
Γ′
Figure 4.2. Calculated values of the derivative ∂f /∂µ′ (Γ′ , T ′ ), for the case of a rectangular SD function: ——  isolines with constant values of the ∂f /∂µ′ function (Lines 1 and 2 are defined in the text). Γ′ = 1 we have ∂f /∂µ′ = 0, 25) and for T ′ → 0, is obvious from Eq. (4.19), which attains the following form for T ′ → 0: ∂f 1 ≈ . ′ ′ ∂µ 2Γ [1 + exp (1 − Γ ′ )(T ′ )−1 ] This jump is due to the extremely rapid decay of the modeled spectral density function (4.8) within a variation of the energy εk by ± 1/2Γk , and there is no reason for expecting such a jump for a smoother behavior of A(ε, εk ). A comparison of Figs. 4.3 with 4.2 obviously shows that the crucial difference among the behavior of ∂f /∂T ′ vs. that of ∂f /∂µ′ is due to the existence of an ascending section of line 1 for Γ′ > 1, which could serve as the basis for the definition of an optimum phonon generation temperature T˜2 , which would increase 106
T′ 1,0 0,15
0,2 0,3 0,435 0,5
0,4
1
0,35
1 2
0,1 0
0,5
1,0
1,5
2,0
Γ′
Figure 4.3. Calculated values of the derivative ∂f (Γ ′ , T ′ )/∂T ′ , for the case of a rectangular SDfunction:——–  isolines.
with increasing value of Cae : ∂ T˜2 /∂Cae > 0. As the abrupt ”slump” at Γ ′ → 1, T ′ → 0, along line 1 (at point Γ ′ = 1, T ′ = 0, ∂f /∂T ′ = 1/2 ln 2 ≈ 0, 347) is caused by the already mentioned particularity of the spectral density function (4.8). It can be anticipated that this ”slump” will vanish when getting over to the more smoothly changing functions A(ε, εk ), and that the ascending section of line 1 will broaden out. We also note that the quantity ∂f /∂T ′ diminishes more rapidly with increasing Γ ′ than ∂f /∂µ ′ . A convincing explanation for this behavior can immediately be concluded from (4.3), if one considers that derivations on T and µ lead accordingly to factors being odd and even on ε concerning the point µ in the integrand.
If we summarize the results of our calculus with usage of a rectangularly shaped spectral density, it can be concluded that they provide strong evidence for the existence of optimum conditions for phonon generation, within a wide concentration region of the alloying element, a possibility we already tentatively anticipated in Pt. 4.1, on the basis of qualitative thoughts. However, a more detailed treatise of the task of Pt. 4.1 could reasonably be performed by determination of the derivatives ∂f /∂T ′ and ∂f /∂µ′ on the basis of the Lorentzexpression of spectral density, as will be done in the next chapter. 107
T′ 1,0 0,200,19 0,21 0,22
0,18 0,17
0,16
0,13
0,14
0,15
0,12
0,11
0,5 1 2 0
0,07
3
0,10 0,13 0,14 0,15
0,5
1,0
1,5
2,0 Γ′
Figure 4.4. Calculated values of the derivative ∂f (Γ ′ , T ′ )/∂µ′ , for the case of a Lorentzshaped SD function:——–  isolines.
4.3
Region of T ′, Γ ′ values with optimum conditions for phonongeneration in the case of a Lorentzshaped SDfunction
An explicit determination of ∂f /∂µ ′ , ∂f /∂T ′ on the basis of (4.3) proves to be difficult in the case of the Lorentzform (4.4) of the function A(ε, εk ). That’s why a numeric calculus of T ′ has been performed, the results of which are presented in Figs. 4.4,4.5. Let us now compare in pairs Fig.4.4 with Fig. 4.2 and 4.5 with 4.3. A comparison of the first pair of results shows that, during a transition to a smoothly changing spectral density (4.4), the optimum region of parameters T ′ , Γ ′ is being retained, even though lines 1 and 2 of the maximum value of ∂f (T ′ , Γ ′ )/∂µ ′ exchange their relative positions (in Fig. 4.2, line 2 is located above line 1 and in Fig. 4.4 below line 1). In addition, in the region between lines 1 and 2, the values ∂f /∂µ ′ of the Lorentzform A(ε, εk ) slowly decrease with increasing Γ ′ and with decreasing T ′ , while the function ∂f /∂µ ′ in Fig. 4.2 behaves nonmonotonously, especially in the vicinity of the point T ′ → 0, Γ ′ → 1. The solid line 3 in Fig. 4.4 is the projection of the ”crest” of the profile of function ∂f /∂µ′ on plane (Γ ′ , T ′ ). The function T ′ ( Γ ′ ) with lines 1, 2, 3 describes the reduction of T ′ with increasing Γ ′ , in a similar way as relation (4.2). This means that they can be used as a basis for determination of the temperature T˜1 . The characteristic difference between Figs. 4.5 and 4.3 consists in the missing ”slump” of line 1, which  for 0 < Γ ′ ≤ 0, 8  slightly changes in the proximity of T ′ ≈ 0, 4, attaining its minimum at T ′ ≈ 0, 39, Γ ′ ≈ 0, 42, being approximated by a straight line for Γ ′ > 0, 8 108
1,0
T′ 0,15
0,05
0,10
0,20 0,25 0,30
0,5
1
0,35 0,40
2
0 0,5
1,0
1,5
2,0
Γ′
Figure 4.5. Calculated values of the derivative ∂f (Γ ′ , T ′ )/∂T ′ for the case of a Lorentzshaped SDfunction : ——–  isolines.
T ′ ≈ 0, 25 + 0, 175Γ ′.
(4.21)
Of course, also a parabolic approximation might be possible. Obviously, by usage of the function T ′ (Γ ′ ), corresponding to (4.21), it would be feasible to determine the temperature T˜2 , which increases with increasing Γ ′ . Line 2 in Fig. 4.5 is shifted towards the lower T ′ , Γ ′ region, both in relation to Fig. 4.3 and to Fig. 4.4 and could thus in principle be used for the introduction of temperature T˜1 , provided the starting temperature of the martensitic transformation of the main alloying component is close to it. Let us surmise that the function T˜1,2 (Γ ′ )  being the mapping of the function T˜1,2 (C) onto the plane (Γ ′ , T ′ )  is known. Then, in order to determine the explicit expressions for T˜1,2 (C), we must first discriminate those fractions of total electron extinction Γ being dependent on the concentration of the alloying element: Γ(T, C) = Γ(T ) + Γ(C).
(4.22)
In paramagnetic alloys, at temperatures larger than or close to the Debyetemperature TD , the extinction Γ(T ) is mainly caused by selectron scattering at phonons and magnetic moment fluctuations. The first of these processes leads to a contribution Γ(T ) exhibiting linear variation with temperature, while the second one only weakly depends on T  for temperatures above the Curietemperature Tc (or the Neeltemperature TN respectively)  and rapidly diminishes for T < Tc . Measurements of the specific electric resistance ρ [158] (see also §3 of Ch. 25 in [159]) have shown that the contribution to scattering by magnetic inhomogeneities for T > 500 K exceeds phonon scattering by about the same order of magnitude. In the region of temperature T < 1100 K, being relevant for martensitic transformations, ρ decreases monotonously with decreasing T. Even though 109
the function ρ(T ) is nonlinear, we shall use below, for simplification, the linear approximation ~ Γ(T ) = a0 kB T , where a0  dimensionless parameter. Obviously, we can already anticipate that a0 must be a onedigit number greater than 1, as the contribution of pure phononscattering already amounts a0 ≈ 1 in the case of transitionmetals. In principle, it is also possible to include in (4.22) the part being largely independent of T and C, being caused by scattering on static defects (i.e. dislocations, alloying atoms of a third element etc.), but we shall assume that the growth of martensite crystals will proceed within a region being practically devoid of such defects, thus confining ourselves to the contributions of only two terms in (4.22). The usage of the ratio (4.22) takes into account that phonon scattering leads to a more scattered energy distribution function, essentially resulting in the need for replacement of the δ  function by a Lorentzline of finite width [160]. In this context we should remind that during any consideration of the washout of the Fermi distribution, the equivalence of different scattering mechanisms will always be confirmed, which inevitably leads to the question about the justification of a well defined Fermisurface in alloys. Among other arguments, it is being emphasized that a case is possible for which ”. . . an alloy in the proximity of absolute zero temperature represents a better model of an ideal lattice than that of a pure metal lattice at room temperature ” [161]. The extinction Γ(C) is mostly caused by scattering of selectrons on alloying elements. In a modeled alloy with diagonal disorder and weak scattering, the following form is true [100]: ~ Γ(C) = 2 π gs (µ) δ 2 C(1 − C).
(4.23)
M Here δ = (εae s − εs )  difference of the energy levels of sstates of alloying components; gs (µ)  density of selectronstates of the matrix at Fermilevel (per spinorientation). Thus for a numeric assessment of Γ(C), the quantities gs (µ) and δ must be known. They can be determined if the width Ws of the sband, the parameter a0 , and the amount of selectrons donated by the alloying element Zae (with matrix ZM ) into the common sband, i.e. if the electronic configurations of the alloying elements are known. In fact, we have a parabolic sband:
√ gs (ε) ∼ ε,
0
ZWs
3 gs (ε) = 2
gs (ε) dε = 1,
ε Ws3
21
(4.24)
.
Considering that the occupied part of the sband accepts ZM /2 electrons, i.e. 110
0
Zµ
gs (ε)dε =
ZM , 2
(4.25)
we get, after insertion of (4.24) in (4.25):
µ Ws
12
=
ZM 2
13
.
(4.26)
Finally we can express (4.26) and (4.24) gs (µ) as a function of ZM : 3 gs (µ) = 2 Ws
µ Ws
21
3 = 2 Ws
ZM 2
13
.
(4.27)
According to [100], the parameter δ is linked up with the difference ∆Z = Zae − ZM by means of the relation ∆Z = − I(µ) =
Z∞
−∞
2 arctan [π δ gs (µ) (1 − δ I(µ))−1 ]; π 1 + x 3 gs (η) x ln dη = −2 , µ−η 2 Ws 1−x
(4.28)
(4.29)
1 ZM 3 x= . 2 In the following, we shall designate by ZM the number of electrons donated into the sband by the iron atoms, using ZM = ZF e . Obviously, the justification for introduction of the MS (C)  like function of T˜1,2 (C), can be given on the basis of the analysis performed, by mapping the function MS (C) onto the plane (Γ ′ , T ′ ), with subsequent determination of those specific values of the parameters a0 , δ, εd −µ, for which the obtained representations M˜S (Γ ′ ) are located in the vicinities of the dashed lines in Figs. 4.4 and 4.5. Doing this way, it will be possible to bring in accordance various experimental data with the defined above laws.
4.4
Mapping of the functions MS (C) into the T ′ , Γ ′ region of optimum phonongeneration, with analysis of the electronic configurations of atoms in binary substitutional alloys
The variation of MS (C) with concentration mentioned in Pt. 4.1 belongs to the kind of results which have been determined with massive specimen. Besides these 111
data, there is currently being collected experimental data related to superrapid quenching (up to 5 · 105 K/s) of foils with a thickness of ∼ 10−4 m (see for example [162–164] for binary alloys and [165, 166] for steel). It could be shown that in different regimes of coolingrates of steel and ironbased alloys there can be realized four ”stages” of martensitic transformations. An extrapolation of these data towards pure iron delivers the following temperatures MSi of these ”stages”: MSI = 820, MSII = 720, MSIII = 540, MSIV = 430 ˚C. The existence of various MS  stages is explained in [164] with the hypothesis of structural particularities of the moving phaseboundaries, as well as by different diffusion mechanisms in their vicinity. During changes of composition, the amount of ”stages” will usually decrease, mainly due to the different rates of change of MSi during the alloying process, resulting into overlapping of the stages. Let us now inspect more in detail the Fe  Ni and Fe  Co systems. For this purpose, the corresponding functions MSi are shown in Figs. 4.6 and 4.7. For FeNialloys, the following inequalities apply for the derivatives (slopes) of the functions MSi (C): 
d MSII d MSI d MSIII d MSIV > > > , dC dC dC dC
d MSi < 0. dC
This means that all MSi decline with increasing concentrations of C. By contrast, in FeCoalloys, the temperatures MSI , MSIII , MSIV increase with increasing C, while MSII decreases: d MSII d MSIII d MSIV d MSI  > > > . dC dC dC dC If, according to [164], the second MTstage was combined with the motion of a phaseboundary embodying a Cottrellatmosphere, then the abnormal MSII behavior could be attributed  at least in the case of FeCoalloys  to solute carbon, as the high mobility of carbon atoms can contribute to the rapid formation of a Cottrellatmosphere. We note here that for Fe Calloys, the slope d MSII /d C < 0 is of an order of magnitude of the slope d MSII /d C, thus exceeding the corresponding derivatives of FeNi, FeCo  alloys. This would be evidence for the correctness of our above assumption. As the theory of electronscattering in substitutional alloys also has to take into account the effects of latticedeformation, the function MSII (C) will not be analyzed here. We also have to point at another particularity of the function MSI (C) in FeCoalloys: In the region of small concentrations of C, MSI remains almost constant, i.e. d MSI /d C ≈ 0. But if C ≥ 7 %, then a pronounced slope d MSI /d C > ˜ I (Γ ′ ) and 0 appears. Assuming an inherent similarity between the functions M S T˜2 (Γ ′), this particularity can easily be explained: It can be taken for granted that the temperature MSI (0), when represented on plane (Γ ′ , T ′ ), corresponds to the coordinates T ′ ≈ 0, 4, Γ ′ ≈ 0, 42, in the vicinity of which (as explained in Pt. 4.3) there also is located the minimum of curve T˜ ′ , where the transition of T˜ ′ (being 112
MS , 0 C 800
I
600 II
400
III
IV
200
IV
0
10
20
30
CN i,w% Figure 4.6. Variation with nickelconcentration (weight %) of the temperatures ˜ i , in ironnickelalloys [162]. M S essentially independent of Γ˜′ ) towards the function (4.21) takes place. Then we choose this point as the starting point and get from (4.16): kB MSI (0) T = ≈ 0, 4; εd − µ ′
α0 kB MSI (0) Γ = ≈ 0, 42, 2 (εd − µ) ′
(4.30)
from which we can simultaneously determine the values of two parameters: a0 ≈ 2, 1 and (εd − µ)/kB ≈ 2, 5 MSI ≈ 2750 K. If these values were considered as fixed and characteristic of the fcc phases of iron, then it would be possible to perform the mappings of MSi onto plane (Γ ′ , T ′ ), simply by varying the parameter ∆Z, being determined by (4.28). This way, it has to be considered that in the case of weak scattering, the parameter δ, being linked with ∆Z, must be a small quantity in relation to the width Ws of the sband. Let Ws = 10 eV, which  for an assumed width Wd = 5 eV of the dband  would correspond to the 10fold difference of the average densities of the s and delectron states. For the FeNi  system, we shall use the two nickelatom configurations 3d 9,44s0,6 and 3d 8,6 4s1,4 , as configurational references, as proposed in [110, 167]. During our projection of the graphs MSi (C) on plane (Γ ′ , T ′ ) we choose 5 points being borrowed from [162]: For C1 = 0 (starting points), C2 = 5%, C3 = 12% (in the proximity of C3 , the curves MSIII (C) and MSIV (C) intersect), C4 = 22% (in the proximity of C4 , the slope of curve MSIV (C) changes), C5 = 30% (in the proximity of C5 the curves MSI (C) and MSIV (C) intersect). We further note that for a Niconcentration CN i > C5 , the slope of the graph MS (C) abruptly increases, so that variations of Niconcentrations by about 4% from 30% up to 34% will 113
MS ,0 C 1000 I III 800
IV 600
II
400 20
40
CCo, w%
Figure 4.7. Variation with cobaltconcentration (weight %) of the temperature ˜ i , in ironcobalt alloys [164]. M S cause a decrease of MS from 250270 K close to 0 K. Then we have to introduce ˜I = M ˜ IV of the intersection of the the additional requirement that the point M S S first and second stage must fall on the line of extremes 2 (see Fig.4.4), the end of which, close to Γ ′ ≈ 1, exhibits a section of rapid, nonlinear decrease of T ′ , with only small variation of Γ ′ . For the a.m. parameters a0 , Ws , ZN i = 0, 6 and ∆Z > 0, it will quite easily be possible to show that, on the basis of (4.16), (4.22), (4.23), (4.27)  (4.29) and by variation of ∆Z, the condition for location of the ˜I = M ˜ IV on line 2 at ZF e = 0, 91 can be met. The magnitude of the slope point M S S ′ ˜I = M ˜ IV remains high. For comparison, we note that at ∂f /∂µ ≥ 0, 16 at point M S S ˜I = M ˜ IV on line 1) the slope ∂f /∂µ ′ ≈ 0, 13 is significantly ZF e = 1, 02 (point M S S ˜ i (Γ ′ ) for ZF e = 0, 91, corresponding to the lower. Fig. 4.8 shows the graphs M S ˜I = M ˜ IV configuration 3d 7,094s0,91 of ironatoms. During deviations of the point M S S from line 2, being associated with a variation of Z in the region 0, 88 ≤ Z ≤ 0, 93, the magnitude of ∂f /∂µ ′ ≈ 0, 16 remains unchanged. For ∆Z < 0, the ironatoms will attain configurations with a number of selectrons less than 0,6. Even though apparently, such a configuration might not be materialized, a consideration of the case ∆Z < 0 may still be useful, from a methodological point of view. An analysis of (4.23), (4.27)  (4.29) in fact leads to the conclusion that, within our notion, the contribution to total extinction Γ(C), related to scattering on solute charged atoms, will vanish in the following three specific cases: At ∆Z = 0 (neutral effect), for ZM → 0, x → 0, gs (µ) → 0 (in this case, the Fermilevel corresponds to the bottom of the sband coinciding with the 114
T′ 1
0,5
3
2 I III IV
0
0,5
1
Γ′
˜ i (Γ ′ ) for FeNialloys with ZN i = 0, 6, ZF e = 0, 91 (or Figure 4.8. Graphs of M S ˜ i were drawn from the starting points with ZN i = 1, 4, ZF e = 1, 04): The graphs M S (I, III, IV), which correspond to pure iron; lines 1, 2 and 3 are identical to those in Fig. 4.4. baseline of the density of states function) and for ZM → 2, x → 1 (in this case, the Fermilevel corresponds to the upper edge of the fully occupied sband). In these particular cases and in accordance with (4.22), (4.30), total extinction is mainly related to the effects of phononscattering and magnetic inhomogeneities, so that ˜ I (C5 ) = M ˜ IV (C5 ) has the coordinates the relation Γ ′ = 1, 05 T ′ applies. Point M S S T ′ ≈ 0, 1, Γ ′ ≈ 0, 1, lying outside of the optimum region, ∂f /∂µ ′ ≈ 0, 04, thus being one fourth as large as the corresponding values in the proximity of line 2 (see Fig. 4.8). For a given value of T ′ , the approach to the optimum region will also depend on the increase of Γ ′ , through the scattering effect of the impurities. ˜ i (Γ ′ ) in Fig. 4.8 corresponds A path being almost equivalent to that of curves M S to ZF e ≈ 0, 09, for a configuration 3d 7,91 4s0,09 of the iron atoms, being close to the 3d 8 4s0 configuration. Full correspondence of the paths of these curves however is not possible, as for ∆Z < 0, the values of Γ ′ are limited. The existence of the maximum Γ ′ at fixed T ′ , for certain ZF e lying within an interval 0 < ZF e < 0, 6 is obvious, as the extinction Γ ′ takes on minimum equivalent values Γ ′ ≈ T ′ , at the borders of the interval (ZF e = 0, 6 (∆Z = 0), ZF e = 0). The condition ′ Γ ′ = Γmax ≈ 0, 936 at T ′ = 0, 1 also matches with the above mentioned value of ZF e ≈ 0, 09 with the configuration 3d 7,914s0,09 of the iron atoms. It is also obvious from Fig. 4.8 that, at the point with coordinates T ′ = 0, 1, Γ ′ ≈ 0, 936, the slope ˜I = M ˜ IV . is ∂f /∂µ ′ ≥ 0, 16, but line 2 is out of reach for the point M S S ˜ For ZN i = 1, 4 and ∆Z < 0, the location of point MS (C5 ) on line 2, with coordinates T ′ = 0, 1, Γ ′ ≈ 0, 96 (the same as for the case with ZN i = 0, 6, ∆Z > 0), corresponds to the value ZF e ≈ 1, 04 with the ironatom configuration 115
3d 6,96 4s1,04 . After similar considerations as those done in the case of ZN i = 0, 6, ∆Z < 0, we can find out for the difference ∆Z > 0, corresponding to the inequality 1, 4 < ZF e < 2, an ironatom configuration 3d 6,114s1,89 , being close to the ˜ S (C5 ) has the coordinates T ′ ≈ 0, 1, configuration 3d 64s2 , for which the point M ′ ′ Γ = Γmax ≈ 0, 65. Even though this point does not merely reach line 2, the corresponding slope ∂f /∂µ ′ ≥ 0, 15 at this point is quite high. Thus the assumption on the existence of two ironconfigurations in the γ  phase, being close to the 3d 7 4s1 and 3d 64s2 configurations with ZN i = 1, 4 (see Pt.2.5), is compatible with the requirement of conservation of optimum generation conditions for phonongeneration in FeNialloys, for both of these configurations. In [163], the processing of data for the FeMn  system has been performed in a similar way. As referenceconfigurations, there were used ironatom configurations like those determined above for the FeNisystem. In addition, satisfaction of the requirement of conformity for points MSIV , within the systems FeNi and FeMn, with CN i = 22% and CM n = 11%, respectively, was imperative. The results obtained are listed in Table 4.1. Table 4.1. Charge numbers of manganese and ironions ZF e ZM n ∆ZF e−M n
0,09 0,84  0,75
0,91 0,53 1,37 0,38  0,46
1,04 1,49 0,63  0,45 0,41
1,89 1,19 0,7
To ease our comparison, Table 4.2 also shows the specifications of the quantities Z and ∆Z, pertaining to the FeNisystem. For ”average” ironconfigurations near 3d 7 4s1 (being equivalent to ZF e = 1), the following conclusion is obvious: To obtain a slope of the relationship MS (C) in FeMnalloys, doubly exceeding the corresponding slope in FeNialloys, it will suffice that the manganeseatoms must only donate 0,1 more electrons into the sband than the Niatoms. For ”marginal”configurations near 3d 84s0 , 3d 6 4s2 , this difference would amount to 0,2 electrons per atom. Table 4.2. Charge numbers of nickel and ironions ZN i ZF e ∆ZF e−N i
0,6 0,09 0,91  0,51 0,31
1,4 1,04 1,89  0,36 0,49
Now let us use the previously determined ironatom configurations for our ˜ i (Γ ′ ) of FeCoalloys. By varying the parameter ∆Z, foundation of the curves M S ˜ i (Γ ′ ) for the function T˜ ′ (Γ ′ ), which come close it is easy to obtain the lines M S 116
˜ i (Γ ′ ) are depicted for an ”averto line 1 in Fig. 4.5. In Fig. 4.4, the curves M S 7,09 0,91 age” ironatomconfiguration 3d 4s and ∆Z = 0, 2, being in accordance with ˜ I (Γ ′ ) with line 1 (dashed line in Fig. the correspondence of the path of curve M S ˜ i correspond to a Coconcentration of 40%, and attain 4.4). The ends of lines M S maximum values at MSI , MSIII (see Fig. 4.7).
T′ 0,5
1 I III IV
0
0,5
1
Γ′
˜ i (Γ ′ ) for FeCoalloys with ZF e = 0, 91, ZCo = 1,12 (or Figure 4.9. Graphs M S with ZF e = 1, 04, ZCo = 1, 24); line 1 is identical to that in Fig. 4.5. The same general path of curves as those with ∆Z = 0, 2 also results for ∆Z = −0, 21, corresponding to a cobaltatomconfiguration 3d 7,88 4s1,12 . Table 4.3 shows the specifications of some other atomconfigurations. Table 4.3. Charge numbers of cobalt and ironions ZF e ZCo ∆ZF e−Co
0,09 0,29  0,2
0,91 0,71 1,12 0,2  0,21
1,04 0,83 1,24 0,21  0,2
1,89 1,6 0,29
A comparison with Fig. 4.4 shows that the coordinates of the ends of lines I ˜ ˜ III , being about T ′ ≈ 0, 4, Γ ′ ≈ 0, 7, correspond to a point on line 3, MS , M S and that the coordinates of the end of line MSIV correspond to a point on line 2, with a slope ∂f /∂µ ′ ≈ 0, 18. In this connection, it is also possible to relate the decrease of MSI , MSIII for CCo > 40% to the onset of shifting of the mapped ˜ I, M ˜ III on line 3, thus ensuring a smooth decrease of the slope ∂f /∂µ ′ . points M S S ˜ IV for CCo > 40% can shift along the line of At the same time, the point M S ′ constant slope ∂f /∂µ ≈ 0, 18, with smooth increase of MSIV . Obviously, this interpretation requires an approximated ”equality” of two nonequilibrium sources, during a martensitic γ − α  transformation in FeCoalloys, while in FeNi and 117
FeMnalloys, the chemical potential gradient ∇µ serves as the dominating nonequilibrium source.
4.5
Discussion of the results on substitutional alloys
On the basis of reasonable electronic configurations, our consideration shows that it is possible, in principle, to obtain satisfactory accordance between experimentally ˜ i (Γ ′ ) and the theoretically obtained relationship T˜ ′ (Γ ′ ), provided that the M 1,2 S spectral density A(ε, εk ) is chosen in the form of a LorentzSDfunction, as it has to account for the complete extinction of selectrons. It would also be interesting to discuss the problems related to the amount ˜ i  mappings and of conformity existing between the parameters used for the M S other relevant data, and how sensitive the evaluations of the ∆Z  quantities would behave against variations of key parameters, within the frame of an alloying model with diagonal disorder.
4.5.1
Determination of the parameter a0 and of electronic atomconfigurations on the basis of electrical and optical characteristics of alloying components
Let us start with the parameter a0 . To determine the function ρ(T ) of the electric resistance  within a temperatureinterval 0 < T < 1100 K  we use the linear extrapolation for data of [158]. Then we can determine the average slope of the curves ρ(T ): ∆ρ/∆T ≈ 10−9 Ohm · m /K. If we now use the Drudeformula (see for example [87, 168]) 1 e2 n ~ e2 n ~ e2 n = ∗ −1 ≡ ∗ = ∗ . ρ m τ m Γ m a0 kB T we get for a0 : a0 =
e2 n ~ ∆ρ , m∗ kB ∆T
(4.31)
(4.32)
where e, m∗  charge and effective electronmass, n  electron concentration. If we further hypothesize that each ironatom donates one electron into the sband (ZF e = 1), we get an selectron concentration of ns ≈ 8 · 1028 m−3 . Then we determine from (4.32) using m∗ = free electron mass = m0 = 9, 1 · 10−31 kg a value of a0 ≈ 17, 2, being 8times as large as the previously mentioned value a0 = 2, 1. For a0 ≈ 17, the extinction Γ at point MSI ≈ 1100 K would be about 1,6 eV ˜i (Assumed selectron lifetime τ ≈ 4 · 10−16 s). For εd − µ ≈ 0, 24 eV, point M S in plane (Γ ′ , T ′ ) had coordinates T ′ ≈ 0, 4, Γ ′ ≈ 3, 3, and the level of the value ∂f /∂µ ′ would decrease to 0,08. We remark that the projection of point MSI into 118
the surroundings of the point (T ′ ≈ 0, 1, Γ ′ ≈ 1), including reestablishment of ∂f /∂µ ′ ≈ 0, 15 ÷ 0, 16 at Γ ′ ≈ 1, 6 eV, is possible for εd − µ ≈ 0, 8 eV, as shown in [121] for the case of the nonmagnetic state of fcciron. Even though in [169] the value τ ∼ 10−16 s was used for an interpretation of the thermoelectric effect in Nickel, the quantity τ most probably had been underestimated, and the quantities Γ and a0 overestimated. This is due to the fact that the Drudeformula (4.31), being correct for the case of a freeelectron gas, does not account for the hybridization of s and dbands in transition metals. As shown in [111] by calculations, the density of the sstates gs is only akin to the density of states of free electrons in the proximity of the bottom of the sband. However, in the overlapping region of s and dbands, the sstate density does not exhibit a monotonous increase with increasing energy ε, and thus will only attain values gs (µ) of an order of magnitude of 10−2 1/(eV atom), in the proximity of the Fermilevel µ. Thus, for correct interpretation of data substantiating the function ρ(T ), it will be more advisable to use the general formula (4.33), which links up both quantities ρ and gs (µ): 1 2 2 ~ e2 v2 gs (µ) = e2 v2 τ gs (µ) = , ρ 3 3 a0 kB T
(4.33)
where v2  squared mean value of selectron velocities at the Fermisurface [168]. The quantity gs (µ) indicates the number of states for a spinprojection within an energy and volume unit interval. For an atom concentration of 8 · 1028 m −3 , we get the following correspondence for different units of energy density: 1 1 = 5 · 1047 . (4.34) eV · Atom J · m3 Let v ∼ 106 m/s, ∆ρ/∆T ≈ 10−9 Ohm m /K. Then we can determine from (4.33), (4.34) that a value of gs (µ) ≈ 2, 3 · 10−2 1/(eV atom) is assigned to a0 = 2, 1, thus amounting to only one fifth of the gs (µ) as estimated on the basis of (4.27), using ZF e = 1. Without doubt, the results of optical measurements in the far infrared (at wavelengths of about 10, 6µ m) reported in [170] are interesting, as they enable us to evaluate data related to the plasma  Ω and relaxationfrequencies τ −1 for ”pure” s and hybridized sdtypes of the chargecarriers in Fe and Ni meltings, and their solutions with Cr, at T = 1873 K: Ω2s = 15 · 1030 s−2 , Ω2s−d ≈ 33 · 1010 s−2 , −1 τs−1 = 2, 4 · 1014 s−1 , τs−d ≈ 4 · 1014 s−1 ,
o
Ω2s ≈ 29 · 1030 s−2 , Ω2s−d ≈ 40 · 1010 s−2 , −1 τs−1 ≈ 2 · 1014 s−1 , τs−d ≈ 3 · 1014 s−1 .
o
Fe (4.35) Ni
Firstly, we note a remarkable conformity among the above data (4.35) and those published in [158], related to the specific resistance ρ. For example we get from 119
[158] ρ ≈ 1, 4 · 10−6 Ohm m for iron at T ≈ 1900 K, and an evaluation of the data shown in (4.35) results in ρs−d = ρs =
−1 τs−d ≈ 1, 35 · 10−6 Ohm · m, ε0 Ω2s−d
τs−1 ≈ 1, 8 · 10−6 Ohm · m, 2 ε0 Ωs
where ε0 = 8, 85 · 10−12 F/m  dielectric vacuum field constant. Secondly, the squared ratios of the plasmafrequencies, Ω2s−dN i ≈ 1, 21, Ω2s−dF e
Ω2sN i ≈ 1, 93, Ω2sF e
being proportional to the ratios of electronconcentrations in Ni and Fe, are greater than 1, a result being in accordance with our initial assumption of the proximity of the effective electronmass m∗N i ∼ m∗F e , for our chosen configurations 3d 8,64s1,4 , 3d 74s1 for Ni and Fe, respectively. Thirdly, a calculus of the ns  concentration of selectrons, being included in the formula of the plasmafrequency e2 ns , (4.36) ms ε0 shows that, using ms ≈ m0 , the value of ns , amounting to only one sixteenth of 8 · 1028 m−3 , corresponds to ZF e = 1. This means that the mean density g¯s of sstates (being related to the energyintervals of occupied states in the sband) is smaller by about one order of magnitude than the g¯s value of free electrons. This is an immediate indication of the existence of collective selectrons of the ironatoms, predominantly in hybridized sdstates. For our determination of ms−d , we keep in mind the condition ZF e = 1 and apply formula (4.36) for Ω2s−d . After insertion of ns → ns−d ≈ 7 · 1028 m−3 we obtain an effective mass ms−d ≈ 6, 7m0 . Fourthly, considering that the specific resistance of iron ρ decreases during a change of temperature T from 1900 K to 1100 K by about 20 ÷ 21% [158], we get the following relaxationfrequencies of iron at T = 1100 K, instead of the values shown in (4.35): Ω2s =
τs−1 ≈ 1, 9 · 1014 s−1 ,
−1 τs−d ≈ 3, 2 · 1014 s−1 .
(4.37)
From this, we can easily evaluate a0 : −1 ~ τs−d ~ τs−1 ≈ 1, 3, a0 s−d = ≈ 2, 2. (4.38) kB T kB T By comparing the results obtained from our interpretation of the concentrationdependency MS (C) with measured optical data, it is possible to draw the following conclusions:
a0 s =
120
1. The above used value of a0 ≈ 2, 1 corresponds to a washed out distribution of hybridized sdcarriers. 2. Out of two referenceconfigurations of nickel, the configuration 3d 8,64s1,4 should be preferred, and from possible ironconfigurations, those being close to 3d 7 4s1 . 3. The value of the parameter εd − µ ≈ 0, 24 eV indicates a spinpolarized state of ironatoms, i.e. εd − µ = εd↑ − µ (see Pt.2.5). 4. The location of cobalt in the periodical system of elements, i.e. between nickel and iron, suggests that out of the two ”average” configurations of its atoms, with ∆Z ≈ ±0, 2 (see Table 4.3), the one enabling a rational explanation of the function MS (C) in FeCoalloys, being close to 3d 7,84s1,2 , i.e. with ∆Z ≈ −0, 2, should be chosen. In accordance with the above interpretation of a scenario with plasmafrequencies of scarriers, it can be anticipated, that the inequalities: Ω2sF e < Ω2sCo < Ω2sN i , Ω2s−dF e < Ω2s−dCo < Ω2s−dN i will be satisfied. However, it has to be taken into account that the partition of the frequencies Ω1,2 and τ1,−12 for two carriergroups is no trivial problem, if the frequency of light ω < τ1−1 , τ2−1 and τ1−1 , τ2−1 are of the same order of magnitude [171]. Thus for example the effective values Ω2ef = −1 (32 ± 1, 2)1030 s−2 , and τef = (0, 8 ± 0, 04)1014 s−1 , as determined in [172] at T = 295 K for bcciron, fit very well with (4.35), taken from [170], for Ω2s−d −1 and τs−d , under the assumption that the absorption of light is of Drudelikecharacter, and if one considers both that the plasmafrequency only weakly varies with temperature, and that the relaxation frequency declines with decreasing T (for a0 = 2, 1 and T = 295 K we get τ −1 = a0 kB T ~−1 = 0, 81 · 1014 s−1 ). The information on frequencies of the ssubsystem however remained hidden. Therefore it cannot be excluded that the values determined for cobalt Ω2 = 31 · 1015 s−2 , and τ −1 = 0, 37 · 1014 s−1 (see [171, 173]) belong to hybridized sdelectrons. 5. Assuming that our conclusions drawn from an alloyingmodel with diagonal disorder in the parabolic band of the selectrons are correct, this would suggest that the density of states (DOS) gs (µ) ≈ 0, 12 1/(eV atom) has been determined realistically, with our model for hybridized sd electrons near the Fermilevel of the γ  phase. Among the papers dealing with the measurement of the specific electric resistance of FeNialloys, we want to emphasize [174–176]. In [174] the ”jumps” of the specific electric resistance ρ, in the region of temperatures MS and AS , are reported, being most probably directly linked up with the γ − α MT and the α − γreverse MT (ρα < ργ ) occurring during the temperaturecycles. During investigations of alloys with 30% Ni [175], only weak variations of optical data were observed after a γ − α  MT. The paper [176] 121
focuses on measurements of the function ρ(T ) , in the adjacency of magnetic phase transformations. [156]reports on the behavior of ρ(T ) in FeMnalloys, while [177–179] is related to FeCsystems. In our opinion however, a more comprehensive consideration of these results would require additional data on Ω and τ −1 , which could in principle be obtained from optical measurements near the MS  temperatures, for a variety of alloys, in a similar way as with the data for ρ, being presented in [174]. Thus we shall confine ourselves to only two qualitative remarks. 1 The values of ρ(MS ) prove to be almost equivalent for various alloys with the same MS temperature, an observation satisfying our initial requirement for compliance of the extinction Γ ′ for FeMn and FeNialloys, with identical MS  temperature. 2 In FeNi, FeMnalloys, the function ρ(MS ) slowly declines with decreasing MS , i.e. with increasing Mn and Niconcentrations, an observation which, at the first sight, would contradict with our hypothesized increase of selectron extinction Γ, with decreasing MS . However, we have to take into account that, for a given ds, sd scattering mechanism, the increase of Γ delivers the larger contribution to conductivity by the delectrons, leading to a decrease of specific impedance. In this case, the increase of Γ leads to the same class of effect as an increase of photonfrequency, the latter one resulting in an increase of the contribution of delectrons to optically induced conductivity [172].
4.5.2
Effect of variations of latticeparameter and the sband width on the difference of the charge numbers ∆Z of alloying components
Due to results of energy band analysis (see for example [106]) we will not only have to expect significant deviations of m∗ from m0 , but also an anisotropy of the values m∗ and gs (µ), mainly caused by the sdhybridization of electronic states. If the value Ws in formula (4.27) was varied for the isotropic function gs (µ), is could easily be estimated which electronic configurations will lead to ˜ i (Γ ′ ) as previously determined, for new values of the same optimum functions M S Ws . According to the band spectrum of iron [106], the ”widths” of the sband, related to the orientations ∆ and Λ of the 1st Brillouinzone, are close to the above used value Ws ≈ 10 eV, whilst the ”width” of the sband in Σ  orientation is Ws ≈ 15 eV. A calculus shows that, for example for ZN i = 0, 6, the transition Ws ≈ 10 eV to Ws = 15 eV is associated with a transition of the configurational set 3d 7,14s0,9 , 3d 8,3 4s0,7 , 3d 9,4 4s0,6 (relating to iron, cobalt and nickel, in sequence) into the configurational set 3d 7,14 4s0,86 , 3d 8,324s0,68 , 3d 9,4 4s0,6 . This means that the variation of the ∆Z  quantity does not exceed 0,04. Of course, for known 122
electronic configurations, the deviation of ∆Z could also be larger than 0,04, but we should not overestimate its exactness, under a qualitative aspect. We also note that formula (4.28), establishing the link between ∆Z and the δ parameter (Friedelsummation rule [100]), is only correct in the region of small concentrations of an alloying element. Consequently, the description of the initial path of the curves MS (C) would be most realistic for small Cconcentrations. However, if the function MS (C) does not significantly deviate from a linear function in a sufficiently large range of concentrations, then a more generous application of the results obtained by means of (4.28) would be justified. For alloys with concentrations C = 0, 2 ÷ 0, 4, our results undoubtedly only are of qualitative nature. We also note that the parameter δ Ws−1, whose magnitude must be less than 1 (being a prerequisite for the applicability of formula (4.23)), has not exceeded the region of 0, 23 ÷ 0, 15, for Ws = 10 ÷ 15 eV, with exception of the case ZF e = 0, 09, ZM n = 0, 84, and δ Ws−1 = 0, 28 ÷ 0, 18 resembling the least probable ”marginal” configuration 3d 7,91 4s0,09 of iron atoms in an FeMnalloy. Now let us discuss the sensitivity of our calculated results against variations ∆a of the latticeparameter a, essentially depending on temperature and composition of an alloy. It is commonly known that a homogenous distribution of the impurities [180] firstly causes a uniform change of the lattice parameter of an ”average” crystal, as well as of the function a(C) of the concentration of a solute, and secondly, the inhomogeneous local static displacements of the lattice, in the adjacency of an impurity atom. The local variation of volume in the adjacency of the impurity atom requires a correction of the quantity ∆Z (4.28), which for an isotropic medium, according to [138], comes to a replacement of the function ∆Z by ∆Z ′ = ∆Z − ZF e
∆V 1 + σF e 1 da = ∆Z − ZF e , 3 a 1 − σF e a dC
(4.39)
where σF e ≈ 0, 3  Poisson’s number. The corrected expression (4.39) reflects the fact that the shielded charge of the impurity atom must be corrected by consideration of the excessive volume ∆V occupied by the additional atom (in relation of the matrixatom). To give an example, for FeMnalloys, the parameter a(C) = 3, 575 − 0, 072 CM n (in Angstr¨om), according to [156], where CM n Mnconcentration. Let ZF e = 1, then we get for the second term in (4.39): ZF e
1 + σF e 1 da ≈ 0, 037. 1 − σF e a dC
(4.40)
According to data in [181, 182], a function a(CN i ) for FeNialloys is nearly inexistent in the ranges of temperatures above 575 K and concentrations CN i < 0, 3, being of interest for a comparison of the functions MS (C) of FeNi and FeMnalloys (see Fig. 4.10). Thus, if we ignored the corrective factor for ∆Z in FeNialloys, we would note that the difference ZM n − ZN i ≈ 0, 1, which originally had been obtained from a comparison of the values shown in Tables 4.1 and 4.2 in 123
Pt. 4.4, is correlated by nearly 40 % with the corrective factor (4.40) of FeMnalloys, being related to the case of ”average” ironatom configurations (ZF e ≈ 1) and ∆Z < 0. In other words, the actual number of electrons donated by each Mnatom into the sband can be less than values shown in Table 4.1 in Pt. 4.4, thus ZM n − ZN i ≈ 0, 06.
a, ˚ A 3,62
4 3,58 3
2 3,54 1
3,50 0
0,2
0,4
0,6
0,8
Fe
1
Ni
Figure 4.10. Variation of the latticeconstant of FeNialloys with FeNiconcentration, at different temperatures [181, 182]: 1 = 0 K, 2 = 288 K, 3 = 575 K, 4 = 875 K. Now let us get over to an estimate of the increment ∆(εd − µ) of the parameter (εd − µ), being caused by the homogeneous variation of the parameter a, using the tight binding approximation. Above all we have to note that the reduction of a must be associated with increasing probability of transitions of the delectrons between the knots, with enlargement of the width of Wd  of the dband. And viceversa: The width Wd must decrease with increasing a. If we further assume that the relation εd − µ Wd−1 will remain unchanged during the variation a → a ′ = a + ∆a, i.e. εd − µ Wd−1 = εd′ − µ (Wd′ )−1 , then ∆(εd − µ) = εd − µ Wd−1 ∆Wd .
(4.41)
It has to be noted that the correspondence of the incremental signs of ∆Wd , ∆(εd − µ) in (4.41) is independent of the sign of the difference εd − µ, as long as the energy εd is related to a nonpolarized (in terms of magnetism) state of 124
ε′d↓
εd↓ εnp d
ε′d np
µ
µ′
εd↑
ε′d↑
Figure 4.11. Graph of energy levels showing the opposite signs of the increments ∆(εnp d − µ) ∼ ∆Wd > 0 and ∆(εd↑ − µ) < 0, during enlargement of the width of the dband (for Wd′ > Wd ) in the case of εd↑ < µ. electrons εd = εnp d . However, if polarization exists there are two energy levels εd↑ , εd↓ which emerged after the fission of εnp d . The energy level εd = εd↑ is characterizing the lower energy level of the pair. Then the signs ∆(εd − µ) and ∆Wd will only correspond for εd↑ > µ. But if εd↑ < µ, then the signs will be opposed (see Fig. 4.11). In this case, the ratio (4.41) must be changed: −1 ∆(εd↑ − µ) = −εnp d − µ Wd ∆Wd ,
εd↑ < µ.
(4.42)
As already discussed above under Pt. 2.5, it is both possible for the γ  phase of iron to materialize a nonpolarized state with εd > µ as well as a spinpolarized state with εd↑ < µ. However, when using (4.41) in the first case, we have to equalize εd − µ in both the left and right hand side of (4.41), but in the second case, the np difference εd↑ − µ can significantly deviate from εnp d − µ. But also εd − µ can deviate from εd − µ in (4.41). If we further took εd − µ = µ − εd↑ ≈ 2, 5 kB MSI (0), being equivalent to 2750 K (see (4.30)) at a temperature scale or to 0,237 eV at an energy scale, and the quantity εnp d − µ ≈ 0, 78 eV (in accordance with [122]), then we would note that the value ∆(εd↑ − µ) attains a sign opposed to that of ∆(εd − µ), being about 3,3 times larger in magnitude. The quantity Wd and its increment ∆Wd can easily be estimated, using the relation from [183] 6, 83 ~2 rd3 Wd = , m0 r05
(4.43)
where rd  atomic parameter, which, in the case of iron, equates to 0, 8 ˚ A = 8·10−11 m, r0  radius of the atomic sphere, m0  electronmass. Taking into account that, for an fcclattice, 4 a3 π r03 = , 3 4 then we are able to express the quantities Wd , ∆Wd as a function of a: Wd =
749, 3 ~2 rd3 , m0 a5
∆ W = −5 Wd
125
∆a . a
(4.44)
For a = 3, 6 ˚ A = 3, 6 · 10−10 m we get from (4.44) Wd ≈ 4, 85 eV. Let us now regard the increment ∆Wd associated with cooling of the γ  phase of iron. According to the data in [184] we can assume a linear heat expansion coefficient β ≈ 2, 15 · 10−5 K−1 . Then, as a result of cooling by ∆T = −100 K ∆a = β ∆ T = −2, 15 · 10−3 , ∆ Wd = 1, 075 · 10−2 Wd . a By insertion of (4.45) in (4.42), (4.41), we get
(4.45)
∆(εd − µ) = 0, 237 · 1, 075 · 10−2 eV ≈ 2, 55 · 10−3 eV, ∆(εd − µ) = −0, 78 · 1, 075 · 10−2 eV ≈ −8, 39 · 10−3 eV,
−1 −1 or kB ∆(εd↑ − µ) ≈ 30 K, kB ∆(εd↑ − µ) ≈ −100 K at a temperature scale. During the cooling process, the starting points MSi (C = 0), if mapped onto a plane (T ′ , Γ ′ ) in accordance with (4.30), will settle a straight line 1,05 T ′ = Γ ′ , ˜ III, IV so that a variation of the parameter εd − µ will shift the starting points M S along this straight line. In a nonpolarized and polarized state, respectively, the ˜ IV are (T ′ ≈ 0, 245, Γ ′ ≈ 0, 257) and (T ′ ≈ 0, 298, coordinates of edgepoints M S ˜ IV are: Γ ′ ≈ 0, 313), whereas in Figs. 4.8, 4.9, the coordinates of the point M S ′ ′ IV ˜ will shift T ≈ 0, 256, Γ ≈ 0, 269. In case of a spinpolarized state, the point M S from the line of constant slope ∂f /∂µ ′ ≈ 0, 14 towards the line of constant slope ∂f /∂µ ′ ≈ 0, 17. Obviously, this shifting of the points is favorable for realization of optimum conditions for phonon generation. Simultaneously, the shifting of point ˜ IV causes a slight reduction of the gradient ∂f /∂µ ′ ≤ 0, 14, in the case of a M S nonpolarized state. For this reason, the polarized state has certain advantage. The mappings of points MS , corresponding to alloys with a concentration Cae greater than a few percent, can be performed by consideration of the following: Firstly, we must consider the reduction of the coefficient β, the values of which being about 1,5 to 2fold smaller (for ironalloys) during approach to roomtemperature (and for FeNiInvaralloys 10 times smaller) if compared with γ  iron, and secondly, by adequate consideration of the dependence of the latticeparameter on the composition of the alloy. Following [181, 182] the value a ≈ 3, 58 ˚ A corresponds to a Fe  30% Ni alloy. It remains almost invariant with varying temperature below 288 K (see Fig. 4.10), whereas at a temperature MSI = 1093 K, corresponding to the value εd − µ (see (4.30)), a ≈ 3, 64 ˚ A. In Tables 4.4, 4.5, there are presented the ZF e for the polarized state of ironatoms, as determined by the ˜I = M ˜ IV on line 2 (at T ′ ≈ 0, 137, Γ ′ ≈ 0, 92) requirement of location of point M S S and line 3 (at T ′ ≈ 0, 137, Γ ′ ≈ 1, 17 ), taking into account, in each case, the increment ∆a = −0, 06 ˚ A. The data in Tables 4.4, 4.5 only relate to ”average” configurations of ironatoms, in accordance with the assumption in Pt. 2.5 on the polarization of states with a configuration close to 3d 74s1 . A comparison of the data are presented in Tables 4.2, 4.3 also shows that a variation of the latticeparameter a leads
126
Table 4.4. Chargenumbers of nickel and ironions with consideration of the ˜I = M ˜ IV on line 2 lattice parameter variation for the case of location of point M S S (see explanation in the text) ZN i ZF e ∆ZF e−N i
0,6 0,87 0,27
1,4 1,10  0,30
Table 4.5. Chargenumbers of nickel and ironions with consideration of the ˜I = M ˜ IV on line 3 lattice parameter variation for the case of location of point M S S (see explanation in the text) ZN i ZF e ∆ZF e−N i
0,6 0,90 0,30
1,4 1,06  0,34
to a noticeable effect on the quantity εd↑ − µ, which will diminish by 6, 4 · 10−2 eV (or about 27%) for ∆a = −0, 06 ˚ A, as well as on the quantity ∆Z, the reduction of which will lead to an additional deviation of Z from 1, by 0,06. For ”marginal”configurations, if put into relation with the nonpolarized state of iron, a consideration of ∆a = −0, 06 ˚ A will result into an increase of ∆Z by about 1/3 of the corresponding increment of ∆Z in the polarized condition of iron. This way, in the spinpolarized state of ironatoms, the ZF e  values for ZN i = 0, 6 are lying in a range of 0, 87÷0, 91, and for ZN i = 1, 4, in a range of 1, 04÷1, 10. As to differentialmodules of electronnumbers, associated with the sband of atoms of binary substitutional alloys, we obtain the following inequalities: ∆ZF e−Co < ∆ZF e−N i  < ∆ZF e−M n .
(4.46)
It has to be noted here that the value ∆ZF e−Co ≈ 0, 2, being used in Table ˜ I with 4.3, nearly corresponds to an approximated conformance of the function M S the sector of line 1 in Fig. 4.5 From the point of view of maintenance of a high level of the slopes ∂f /∂µ ′ , ∂f /∂T ′ during variations of the Coconcentration, a conformance of the figures ZF e und ZCo would also be favorable, i.e. ∆ZF e−Co = 0. For ∆ZF e−Co = 0, the contribution to extinction being caused by scattering ˜ i  points at at charged impurities, also vanishes, i.e., Γ(C) = 0, while the M S the (T ′ , Γ ′)  plane shift upwards from their initial locations along the straight ˜ I change with variations of Coline 1, 05 T ′ = Γ ′ . The coordinates of point M S concentration from C = 0 to C = 0,4 from (T ′ ≈ 0, 4, Γ ′ ≈ 0, 42) to (T ′ ≈ 0, 426, ˜ III , M ˜ IV shift into positions close to Γ ′ ≈ 0, 447), and, for C = 0,4, the points M S S 127
˜ I or M ˜ III for C = 0. It can further be seen from Figs. 4.4, 4.5 that that of M S S the slopes ∂f /∂µ ′ and ∂f /∂T ′ increase at the same time. For FeNi and FeMnalloys, the vanishing of the quantities ∆ZF e−N i , ∆ZF e−M n is most unfavorable, as ˜ i along line Γ ′ = 1, 05T ′ will lead to rapid reduction of the downshift of points M S the magnitudes of slopes ∂f /∂µ ′ , ∂f /∂T ′ . We further note that in the above performed analysis of the scattering by impurities, we omitted a consideration of nondiagonal disorder existent in binary alloys, being caused by electronic transitions between the knots of the components of binary alloys [100]. Obviously, any additional contribution to extinction Γ(C) will cause a decline of the quantity ∆Z. Thus the above determined ∆Z  values should be regarded as estimates lying above the true differences of the number of electrons donated into the sband by the alloying components.
4.5.3
Estimation of the chemical potential differences of some γ  and α  phases, for the subsystem of delectrons
Let us use formula (4.43) in order to calculate the chemical potential difference ∆µ = µγ − µα between austenite and martensite, the magnitude of which will determine the amount of inverted occupational difference σ0 , in addition to the slope ∂f /∂µ ′ . We recall that an elementary assessment of ∆µ, relating to selectrons, has already been performed in Pt. 1.5. With regard of the necessary correspondence of the ∆µ  assessments for different (s and d) electrons, we now assess ∆µ for the subsystem of delectrons. Let us count µ from the bottom of the dband upwards, assuming that the ratio µ Wd−1 applies for both the γ and the α  phases. Then we get: µγ Wd α ∆ µ = µγ − µα = (Wd γ − Wd α ) µγ . (4.47) = 1− Wd γ Wd γ
If we regard the already used quantity εnp d − µ ≈ 0, 78 eV as the energydifference between the upper edge of the dband and the Fermilevel of the γ  phase, we get for Wd γ ≈ 4, 85 eV the value µγ ≈ 4, 85 − 0, 78 = 4, 07 eV. Taking further in consideration that, for a bcclattice, the volume associated to one atom is
4 1 π r03 = a3α , 3 2 we then can express by formula (4.43), in a similar way as previously done with (4.44), the value Wdα by means of the latticeconstant aα , and determine the ratio Wd α aγ 5 ≈ 0, 961, = 1/3 Wd γ 2 aα
(4.48)
using therein the ratio aα = 0, 8aγ , being typical of the Baindeformation (see Fig. 1.1 and its legend). If we now insert µγ = 4, 07 eV in (4.47), under consideration of 128
(4.48), then we get ∆µ ≈ 0, 16 eV, being in good accordance with the previously performed estimate for the subsystem of selectrons.
4.6
The MS (C) function for steel and degree of ionization of carbonatoms
In principle, one could try to extend the approach for an analysis of the concentrationdependence of MS , from binary substitutional alloys towards interstitial alloys, among which the FeCsystem would be the most interesting one. We can take for granted that carbonatoms will only occupy the octahedral interstitial voids in austenite [13]. Let us further surmise that those ironions, in the closest adjacency of which a carbonatom is localized, can be characterized by a chargenumber ZF eC , and that these ironions will adopt the role of the ”alloyingelement”ions, substituting the ”normal” ironions by a combined charge number ZF eC , being different from ZF e . Then our search for Γ(C), which represents the contribution to selectron extintion by scattering at the impurity atoms, can be reduced to the task of determination of electronscattering at octahedral clusters of 6 atoms, whose concentration is identical with the concentration of carbon. This task however is neither trivial nor has it been completely resolved (see for example [102,185]). Thus we shall confine ourselves on a qualitative reflection and start with an estimate of the lower limit by hypothesizing that, during the process of clusterscattering, the selectrons will only interact with one of the six ”solute” ions (i.e. that one being nearest to the selectron). In this case, our analysis of MS (C) can be performed in the same way as in the case of a substitutional lattice in Pt. 4.4, 4.5. According to [165], the rate of reduction of MS with increasing carbon concentration is about fourfold or twice as large as that for FeNi or FeMnalloys. Thus for instance, a temperature MSIV ≈ 473 K in FeC, FeMn and FeNisystems corresponds to about 4,6 Atom  % C (1 weight% C), 10,5 atom % Mn and 22 atom  % Ni. In Table 4.6, there are presented some values of ZF eC , which have been determined for the same parameters as those used in Pt. 4.4, i.e. Ws = 10 eV, εd − µ ≈ 0, 237 eV, without account on the effect of variable lattice parameter. Table 4.6. Effective chargenumbers of ironatoms included in octahedral clusters with interstitial carbon atoms ( ZF eC ), and of ironions without association to carbon (ZF e ) ZF e ZF eC ∆Z
0,09 1,08  0,99
0,91 0,42 1,53 0,49  0,62
129
1,04 1,62 0,52  0,58 0,52
1,89 0,86 1,03
By comparison of the data shown in Tables 4.6 and 4.1, we note that  for ”average” ironconfigurations  a twofold increase of the rate of reduction of MS would requires an increase of ∆Z  by about 0, 1 ÷ 0, 15. We recall that we came to a similar conclusion in Pt. 4.4, after having compared the rate of change of the MS temperature in FeNi and FeMnalloys. The measured magnetic susceptibility of FeCalloys, as reported in [186], points to an increase of electronconcentration in the dband with increasing concentration of carbon. In a local interpretation, dband occupation by carbonelectrons is associated with hybridization of the 2p wavefunctions of the carbon with the 3dfunctions (eg  symmetry) of the iron. Such hybridization can associate with a reduction of the chargenumber of the ironatoms in an octahedral cluster. Further hypothesizing that the difference between ZF eC and ZF e is only caused by the additional charge transfer from the carbonatom, it is suggested to keep in mind only the following two ZF eC  values of Table 4.6 : ZF eC = 0, 42 (at ZF e = 0, 91) and ZF eC = 0, 52 (at ZF e = 1, 04). ZF eC = 0, 88 (at ZF e = 1, 89) should be omitted, as the adoption of one electron per ion (with ∆Z = 1) would result in complete ionization of the carbonatom, given an equivalence of six ironions per cluster. The degree of ionization of the carbon atom is 6 ∆ Z = 6 (ZF e − ZF eC ) ≈
2, 94, 3, 12,
ZF e = 0, 91 , ZF e = 1, 04
(4.49)
i.e. one carbonatom may donate about three electrons into the dband. Consideration of the homogenous change of the latticeparameter (see Pt. 4.5.2) would lead to a reduction of (εd↑ − µ) to 0,215 eV, for FeCalloys (1 weight % C) at T = MSIV ≈ 473˚K. In Table 4.7, there are presented the corrected ZF eC values, by adequate consideration of the increments of the lattice constant a (the values of ZF e were extracted from Table 4.4, as determined from the requirement ˜ IV in the adjacency of line 2 in Fig. 4.4 (at T ′ ≈ 0, 19, of location of point M S Γ ′ ≈ 0, 82), relating to an FeCalloy with 1 weight % carbon. In calculating the corrective factor for inhomogeneous volume change, we have to consider that the quantity ∆Z in Table 4.7 must equate to the quantity ∆Z ′ in (4.39). Table 4.7. Chargenumbers ZF e , ZF eC with consideration of a variable latticeparameter a ZF e ZF eC ∆Z
0,87 0,42 0,45
1,1 0,59 0,51
Taking advantage of the concentrationdependency of the latticeparameter of 130
austenite given in [13]: aγ = (3, 578 + 0, 645C)˚ A , where C  fraction of carbonatoms, we can determine from (4.39) 1 + σF e ZF e da 0, 47, ZF e ≈ 0, 87 ′ ∆Z = ∆Z + ≈ (4.50) 0, 57, ZF e ≈ 1, 1 1 − σF e 6a dC The factor 1/6 in the second term in (4.50) considers that only one sixth of the inhomogeneous volume increase caused by the insertion of the carbonatom can be assigned to each ironion in the octahedral cluster. The ionization degree of the carbonatoms 6 ∆Z ≈
n
2, 82, 3, 42,
ZF e ≈ 0, 87 , ZF e ≈ 1, 1
which had been determined under consideration of the changes of the austenitic lattice parameter, moderately differs from the results of (4.49). The quantity 6∆Z ≈ 3, 42 presumably is the upper margin for the degree of ionization of the carbonatoms, as the hypothesis which transforms the effect of selectron scattering at the complete cluster to scattering at only one of its six ironions, can only be substantiated for a larger number of ions involved in selectron scattering, which in turn would lead to an increase of ZF e , with corresponding decrease of ∆Z. However, we note that our conclusion on the maximum value of 6∆Z ≈ 3, 42 is ˜ IV for FeCalloys (1 weight % C) arrives at based on the condition that the point M S ˜ IV arrives at the adjacency the adjacency of line 2. If we required that the point M S of line 3 in Fig. 4.4 then the degree of ionization would increase to 6∆Z ≈ 3, 78. This value is an intermediate in relation to the values 3,5 and 3, 9 ÷ 4, which had been determined in [186] and [187], by analysis of the magnetic susceptibility of FeCsystems, within the notion of a quasirigid dband with ZF e ≈ 1, and by consideration of data of carbondiffusion in a constant electric field (electrotransfermethod).
4.7
Summary of Chapter 4
Our assessments of substitutional (FeNi, FeMn, FeCo) and interstitial alloys (FeC) will now enable us to draw a basic conclusion on the possibility of preservation of the conditions for efficient phonon generation by nonequilibrium 3delectrons, within a wide range of concentrations of the second alloying component. The methodological basis of our investigations was the usage of a SD  function, which, besides thermal scattering, also takes into account the effect of scattering (washout) caused by the inhomogeneity of the system. We note that establishment of a modified equilibrium distribution of delectrons (see Pt. 4.2), whose degree of ”washout” is mainly determined by the rate of extinction of selectrons, is limited by the time τd−s characterizing dselectron scattering. As the nonequilibrium addend to the electronic distribution cannot come into existence prior 131
to the formation of the real equilibrium distribution, the time τd−s will determine the minimum time τσ for establishment of an inverted occupational difference σ0 (pumpingtime). From this perspective, the value of τσ ∼ 10−12 s, as determined in Chapter 3 in our evaluation of the deformation ε, appears quite acceptable. Our analysis of the behavior of nonequilibrium addends to the electronic distribution functions revealed the existence of certain region of temperatures T and extinction Γ with optimum conditions for wave generation (Electron extinction depends on the concentration C of the second alloying component). Within this region, during simultaneous change of the key parameters T and C, a high magnitude and slow variation of the nonequilibrium addends are typical. The next step in our analysis comprised a mapping of the real relationship MS (C), between temperature and concentration, into the region of optimum values of parameters T and Γ. As for Γ, the contribution of scattering by impurities has already been emphasized, and resulted in our consideration of weak scattering, being intimately related to the diagonal disorder in the system matrix. (Characteristic of this matrix is that it reflects the effect of solute atoms substituting the matrixatoms in the lattice knots, with conservation of the transition integrals among the latticeknots). Our choice of the electronic configurations of the Niatoms as a reference configuration, based on published data, enabled us to determine the electronic configurations of iron, cobalt manganese and carbon, in accordance with the mapping of the relationship MS (C) into the region of optimum values of the parameters T and Γ. Among the analyzed substitutional alloys, the difference ∆Z, indicating the number of electrons donated by an alloying atom into a common sband, proved to be least for FeCoalloys: ∆ZF e−Co = (0 ÷ 0, 2) and largest for FeMnalloys: ∆ZF e−M n = (0, 4 ÷ 0, 5), for the case of an ironatom configuration near 3d 7 4s1 . Interestingly, within our model with diagonal disorder, there can be realized a twicefold rate of reduction of MS (C) in FeMnalloys with increasing manganeseconcentration, in relation to the rate of decrease of MS (C) in FeNialloys with ∆ZF e−M n − ∆ZF e−N i ≤ 0, 1. This result could also be confirmed by comparison of the rates of reduction among the FeMn and FeCsystems. Good accordance with the values of 0, 2 ÷ 0, 3 eV, mentioned in Pt. 2.5, is also given for the parameters εd − µ = (0, 17 ÷ 0, 26) eV, which we used for the mapping of the function MS (C). We recall that the value εd − µ ≈ 0, 237 eV has been chosen as an initial value (at a temperature MSI (0) = 1093 K), and that the range of the εd − µ values depends on the lattice parameter. From a quantitative point of view, an evaluation of the derivative ∂f /∂µ ′ , which  besides the quantity ∇µ  determines the initial occupational inversion σ0 , appears to be important. It follows from Fig. 4.4 that, in the vicinity of line 2 of the maximum values of the function ∂f (Γ ′ , T ′ )/∂µ ′ , the inequalities 0, 21 ≥ ∂f /∂µ ′ ≥ 0, 15 are satisfied, enabling us to use the value ∂f /∂µ ′ ≈ 0, 15 as a minimum, in our evaluation of σ0 . We further note that the value ∂f /∂µ ′  ≈ 0, 1, as used in Pt. 3.3 in our evaluation of the deformation ε (see (3.42)), was 1,5 times 132
less than the above value. We further note that the character of the isolines in Figs. 4.4, 4.5 (mirrored C˜ S (C) strictly follows the path shaped curves) does not require that the function M of lines 2 or 3. In the general case, which must not necessarily relate to ironalloys, ˜ S on the a variety of possibilities is permissible. For instance, the mapping of M ′ ′ plane (T , Γ ) (for low MS temperatures and εd − µ  values near εd − µ ≈ kB MS ) can attain the coordinates (T ′ ≈ 1, Γ ′ ≈ 0), thus going far beyond of the limits of the region bordered by lines 1 and 2. The value ∂f /∂µ′ ≈ 0, 2 however is large in this point and remains almost unchanged during a shifting motion along the isolines, being caused by increases of Γ ′ with simultaneous reduction of T ′ . Thus, ˜ S are located in the adjacency of T ′ ≈ 0, 4, Γ ′ ≈ 0, if the startingcoordinates of M ′ then the value ∂f /∂µ ≈ 0, 18 can only be conserved with increasing Γ ′ , if the temperature initially decreases and later on increases. A situation is also possible in which the temperature MS , along certain section of the branches (steps) of the functions MS (C), decreases with increasing C, but increases along other sectors of the branches. This situation is illustrated in Fig. 4.12. Obviously, the motion ˜ I with increasing Γ ′ . away from point I along the isoline leads to a reduction of M S Cooling (without change of composition) will shift the system away from point I to point II. The shifting away from point II, along isoline ∂f /∂µ ′ = const, is ˜ II , for increasing Γ ′ , until the intersection of associated with an increase of M S ˜ I and M ˜ II is reached. A similar behavior of the branches M i (C) can branches M S S S also be observed in FeMoalloys [164, 188]. Of course, during an analysis of the functions MSi (C) for ironbased alloys, the thermodynamic limitation T0 (C) − MS (C) ≥ ∆T min ∼ 102 K,
(4.51)
may not be ignored. This limitation shows that, during a γ − α  MT, the point MS is set off by a limited quantity of about 102 K, below the temperature T0 of phaseequilibrium. In the case of a reduction of T0 (C) with increasing C (∂T0 /∂C < 0), the condition ∂MS /∂C > 0 would contradict with the limitation (4.51), thus all functions MSi (C) must decrease with increasing C, as can actually be observed in the cases of FeNi, FeMn and on FeCalloys. However, if T0 (C) increased with increasing C (∂T0 /∂C > 0), then the MSi could either increase with increasing C (FeCo, FeAlalloys), or decrease (FeCralloys), without contradicting to (4.51). At the same time, the high level of ∂f /∂µ ′ remains conserved, while, in an alloyingmodel with diagonal disorder, the choice among these two possibilities will be determined by the quantity ∆Z, being the difference among the chargenumbers of the alloying components. For small ∆Z ≤ 0, 1, an increase of MS , and for large ∆Z > 0, 3, a decrease of MS would be favorable. As to the general case, instead of a ∆Z  comparison, we have to compare, for various alloys, the derivatives ∂Γ(C)/∂C. This way the relations (instead of inequalities (4.46)) 133
∂f ∂µ′ = const
T′ I
1
2 MSI = MSII
II
3
Γ′ Figure 4.12. One of the variants for description of two stages of the concentrationrelationship MSI,II (C), mapped on the plane of variables Γ ′ , T ′ : Shifting motion along the isolines ∂f /∂µ ′ = const: Starting at point I and proceeding along route 1 corresponds to a reduction of MSI , with increasing concentration of the alloying elements. The motion along route 3 from point II is reflected by an increase of MSII . Route 2 describes a cooling process without variation of composition.
∂Γ ∂Γ ∂Γ < < ∂ C F e−Co ∂ C F e−N i ∂ C F e−M n are materialized in an alloying model with diagonal disorder. Thus our presentation of the concentrationrelationship MS (C) opens up the possibility of sustaining a high level of occupational inversion, in a wide range of variations of temperature and concentration of alloyingelements, thus delivering a simple explanation for the reasons of the different characteristics of the MS (C) functions of ironbased alloys, including alloys with elements marking off the limits of the region of existence of the γ  phase (a more comprehensive list of elements than that mentioned in Chapter 4 is given in [7]). The data on which Chapter 4 is based were published in [90, 189, 190]. The analysis of the electronic configurations of ironatoms in Fe  Ni  alloys, published in [190], has been used partially [191].
134
Chapter 5 Interpretation of a variety of characteristic morphological features of martensite within the notion of a phononmaser
In ironbased alloys, the structural product of the γ − α  transformation, mainly bcc or bctetragonal martensite, exhibits a large variety of morphological features (see Pt. 1.2). This morphology undoubtedly contains valuable information on the dynamical mechanism of the martensitic transformation (MT). Its disclosure will thus be essential in our search for potential methods of externally influencing a MT. Thus it would be helpful to define certain models which will then enable us to gather such information. The notion of a phononmaser (see Chapter 2.3) focuses on nonequilibrium conditions emerging in the adjacency of the boundary of the growing phase, as well as on the possibility of generation of latticedisplacement waves with amplitudes being sufficiently large to initiate the necessary plastic lattice deformation. This enabled us to interpret the growthstage of martensite as a process being controlled by certain waves propagating through the premartensitic lattice phase. It should be emphasized that our task to explain the mechanism of wave generation includes the disclosure of an inherent link between the waves and some specific particularities of the electronic spectrum. Within the notion of the wavemodel, our interpretation of morphological features of martensite will define such a link to observable macroscopic features (i.e. habitplanes), which will then allow us to analyze the physical causes of changes being linked up with variations of composition or of external boundary conditions. 135
5.1
Habitplanes in FeNi, FeCalloys
The qualitative pattern of definition of a habitplane, which represents a fundamental morphological feature of martensite, has already been outlined in SubPt.7 of the definition of our task under Pt. 1.5. Within our aim to resolve this task, let us start with a qualitative matching of characteristic latticeplanes and waves.
5.1.1
Matching of a plane with a pair of waves
It is generally possible, in principle, to link up planes with waves: Firstly, by directly associating them with the wavefront of a plane wave, and secondly, by associating them with the geometrical pattern of those points defined by a frozenin trace of a moving line of intersection of two plane wavefronts, propagating into different orientations. As the first case is rather trivial, let us consider more in detail the second case: Let c1 and c2 be two nonparallel wavevelocity vectors, taking into consideration that their vectorproduct [c1 , c2 ] is collinear with the line of intersection of the wavefronts, which propagates with velocity c. Then we will be able to define a vector N , being collinear with the normal vector of the plane defined by the vectors [c1 , c2 ] and c, by the following vectorproduct N = [c, [c1 , c2 ]] = c1 c22 − c2 c21 .
(5.1)
Relation (5.1) immediately resolves the task of determination of N for given c1 , c2 . The resolution of the inverted task however (i.e. the search for a pair of waves associated with a given N), is ambiguous from the outset. Nonetheless, with the aid of (5.1), it is possible to determine conditions limiting the degree of ambiguity. As N is a linear combination of the vectors c1 , c2 , the vectors c1 , c2 define a plane. Thus their vector triple product will vanish, for any factorial combination of them: N [c1 , c2 ] = c1 [N, c2 ] = c2 [N, c1 ] = 0.
(5.2)
Inserting the factor c2 c21 in (5.1), we get a representation of (5.1) in the form: N k n1 κ − n2
(5.3)
where n1 = c1 c−1 1 ,
5.1.2
n2 = c2 c−1 2 ,
κ = c2 c−1 1 .
(5.4)
Habit (225)
Getting over to an interpretation of the real habitplanes, we recall (see Pt. 1.2) that in FeC, FeNisystems, the observed habitplanes are: Near {557} ÷ {111} (up to 0,6 weight % C, up to 29% Ni), {225} (0,6  1,4 weight .% C), {259} ÷ {3 10 15} (1,4  1,8 % C, 29  34% Ni). In accordance with Pt. 7, SubPt. 1.5 of the definition of our task, as well as with our conclusions from Chapters 2 and 136
3, we shall define, in our description of the waves, pairs of longitudinal (quasilongitudinal) waves, propagating close to the perpendicular orientations h001i and h110i of a fcclattice. This way, we can hypothesize that the martensitic transformation is initiated by waves propagating through the austenitic parent areas, delivering or exceeding the required thresholddeformation ε ∼ εt of austenite. In addition, the displacement of lattice atoms, being immediately linked up with the waves, feature just the kind of phase relations being required to perform a Baindeformation (the geometric pattern of the Baindeformation has been treated in Pt. 1.4, see also Fig. 1.1). Let us start with a consideration of martensite with habit planes {225}: Our particular interest in this habit group is based, on the one hand, on that the crystallographic theory encounters the greatest explanatory difficulties [13] with this group, and on the other hand, on the intermediate position of martensite with these habits, in relation to its carbonconcentration, which may facilitate a comparison of habit planes of martensite belonging to the first and to the third group. From the outset of our consideration, we note that, if we choose the velocity of one of the waves propagating in direction c1 k [00¯1] ( Orientation ∆: 4th  order axis of symmetry), then, according (5.2) and (5.3), it will be possible to define the type (h h l) habit, where h, l> 0, by choosing the second wave with a velocity c2 k [11η], using the condition κ=
c2 l−η h = p . c1 h 2 + η2
(5.5)
Moreover, if we choose waves with reasonable long wavelengths (see the treatise in Chap. 2), it may be justified to surmise that their role mainly consists in selecting those macroregions (or mesoregions) comprising the most favorable transformation conditions. Under such a point of view, it suggests itself to perform our interpretation of the particular features of the inner structure of a martensite lamella (with a thin structure), using the notion of coordinated action of longand shortwaves. It may be reminded that a lamella with habit (225) consists of thin twinning lamella (110), among which the main axes [100] and [010] of Baindeformation alternate in turn. Thus obviously, if we confined ourselves to a description of pure Baindeformation, it would be justified to choose the velocity of one of the longitudinal waves c1 = c∆ in direction [00¯1]. The coordinated action of such wave with the shortlength displacement waves will then result in a tension of the lattice in the orientation [001], being also required for Baindeformation with compressiveaxes [100] and [010]. As to the wave along [11η], both type of twins have equal relevance to it, like in the previously discussed case. Furthermore, if the wave is of the longitudinal type, it will support the Bainpressure alternating among the directions [010] and [100], the more, the closer η is to zero, i.e. the closer c2 is oriented towards Σ. For a given alloy, the value κ0 = κ(η0 )  corresponding to habit (225)  is 137
defined by the intersection between the curves determined experimentally κe (η) and theoretically κT 1 (η): κ(η0 ) = κe (η0 ) = κT 1 (η0 ). According to (5.5), the curve κT 1 (η) descents monotonously  within the interval 0 < η < 1  from κ(0) ≈ 1, 77 down to κ(1) ≈ 0, 87. Obviously, an unequivocal solution κ0 exists within the interval 0 < η < 1, if the path of curve κe (η) ascends monotonously, with an initial value κe (0) out of the interval: 0, 87 < κe (0) < 1, 77. As longitudinal waves normally satisfy the inequality c ∆ < c Σ < c Λ , the requirement of monotonous ascent of curve κe (η) also is satisfied, in addition: κe (0) = c Σ c−1 ∆ > 1, thus the only remaining restriction is κe (0) < 1, 76. Under consideration of the aforementioned restriction, which most certainly will be satisfied for the systems of our interest, there must exist an unequivocal solution. The results of our analysis are presented in the first part of Fig. 5.1, where the nearly horizontal curve κe represents the weakly pronounced dependence on orientation of a longitudinal wave during a transition from the Σ  to the Λ  orientation, resembling a 3rd order of symmetry axis. As already mentioned, those c2 orientations being close to the Σ  orientation will find our greatest interest. Obviously from Fig. 5.1, this approximation occurs with increasing κe (0).
κ 2
κT1 κT2 κe ≈ κc 1
1
ηc
−ηc
1
η
Figure 5.1. Graphic pattern for determination of the η0 , which determines the orientation [11η0 ] of propagation of a quasilongitudinal displacementwave. Shown is the ”critical” case: The value η0 = ηc corresponds to the habit plane (225) and the value η0 = −ηc to habit plane (557). Then functions κT (η) and κe (η) are defined in the text.
138
5.1.3
Habit (557). Criterion for transition from habitus (557) to (225)
The affiliation of habitus (557) to the type (h h l), also being common with (225), and the possibility of their coexistence in the limit region of carbonconcentration near 0,6 % C, suggest to describe these lamellae by a pair of waves c1 k [00¯1], c2 k [11η], in a similar way as habitus (225). Even though such a description is possible, the solution of the equation κ(η0 ) = κT 2 (η0 ) = κe (η0 ) is defined in the negative region −1 < η0 < 0. In the left side of Fig. 5.1, the curve κT 2 (η) has been drawn in accordance with (5.5), for the habit (557), which ascends monotonously from κT 2 (0) ≈ 1 up to κT 2 (−1) ≈ 1, 386. The larger κe (0) > 1 becomes, the more the direction of velocity c2 will deviate from that of Σ. In other words, it behaves just the opposite way as in the case of habit (225). Obviously, there must exist a value ηc (let us call it the critical value), for which κT 1 (ηc ) = κc = κT 2 (−ηc ) ≈ κe (0). This equation corresponds to ηc ≈ 0, 55, with κc ≈ 1, 285. The quantitative criterion for separation of these cases, for which apparently the dynamical conditions for development of only one of the habits must be more favorable, has a simple structure: (225) − −κe (0) > κc , (557) − −κe (0) < κc .
(5.6)
Obviously, both habits can coexist in the region κe (0) ≈ κc . Further assuming that an increase of carbonconcentration leads to a slow increase of κe (0), and that the value κc is attained near 0,6 % C, then any further increase of κe (0) > κc must be associated with a transition from habit (557) to (225). This specific effect of carbon can be explained in a qualitative manner: Those carbon atoms accumulating in voids [13] hybridize their 2p  functions with the 3dfunctions of the iron atoms with eg  symmetry (as shown under Pt. 4.6), and thus reduce the effective positive charges Z of the ions, in the field of which the free 4selectrons are moving. This must cause a local reduction of longitudinal velocity of sound, as  in accordance with the ”jelly”model [192]  the velocity of sound is c ∼ Z 1/2 . Presumably due to the anisotropy of the 2pfunctions in FeCsystems, the increase of the parameter κe (0) = c Σ c−1 ∆ is mainly associated with the decrease of c ∆ with increasing carbonconcentration (note that any comparison of the c Λ  values of different alloys must be performed at the same temperature). In the more general case, a situation is also conceivable in which an increase of κe (0) is related to the more rapid increase of the velocity c Σ in relation to c ∆ . Remarkably, the lack of a noticeable region of Niconcentration for habit (225) in FeNisystems is in accordance with our criterion (5.6). Experimental evidence reported in [38] shows that κe (0) can only attain the value κc for 33 % Ni in ferromagnetic austenite. In this case, κe (0) attains the values 1, 12 ÷ 1, 15 until reaching magnetic ordering, clearly being less than κc . Having applied this approach for the case of perpendicular waves 139
c1 k [η/2 η/2 ¯1], c2 k [1 1 η]  where c1 already is nonparallel to [00¯1]  and with consideration of the variation of habit from (557) to (111), we get the results listed in Table 5.1. Table 5.1. Values κc , ηc , θc , for three pairs of habits habitpairs (225), (557) (225), (667) (225), (111)
ηc 0,1962 0,2619 0,3166
κc 1,3083 1,1923 1,1061
θc , Degree 7,8966 10,4913 12,6197
Here, θc  angle between [11ηc ] and [110]; ηc being determined on the basis of equivalence of the velocitymodules ratios κ = c2 c−1 1 , for different habits of the types (h1 h1 l1 ) and (h2 h2 l2 ), as given by √
2 h1 h2 + l1 l2 , h1 l2 − h2 l1 while κc can be determined by substituting η = ηc in the expression √ c2 (l − h η) 2 κ= = . c1 2h+lη ηc =
2 + b2 − b,
b=
(5.7)
(5.8)
In (5.7) and (5.8) the indices l = l2 = 5, h = h2 = 2 correspond to positive η. As can be seen from the data in Table 5.1 for perpendicular wavepairs c1 and c2 , an increase of κ supports the transition from the habit (557) to (225), in conjunction with a reduction of the angle of deviation θ among the axes of symmetry of second and fourth order. We also note that the deviation of the first wave from the axis [00¯1] opens up the possibility to significantly reduce the deviation of the second wave from the axis [110], in comparison with the case c2 k [00¯1]. Of course, for κ ≈ κc , a coexistence of crystals with habits (557) and (225) is possible. This way, e.g. in [165] a similar kind of coexistence has been observed during rapid quenching of steels with < 0, 6 % C
5.1.4
Habits {15 3 10} ÷ {9 2 5}
The characteristic feature of martensite with these habitplanes is associated with internal twinning. For the habits (15 3 10) and (9 2 5), the Bainpressure axes in the twins correspond to [010] and [001]. Thus, in analogy with habit (225), we have to choose as the first wave contributing to lattice expansion of both twins during Baindeformation, the longitudinal wave with velocity c1 k [¯100]. Then we determine from (5.2) the velocity of the second wave: c2 k [η 0, 3 1] and c′2 k [η 0, 4 1] (in the following, we mark with ′ the results relating to the description of habit (9 2 5)). If we construct, on the basis of (5.4), the curves κT (η) within 140
a region 0 ≤ η ≤ 0, 3, and κT′ (η) within a region 0 ≤ η ≤ 0, 4, then we can easily convince ourselves that they descend monotonously, attaining the following values at the limits of those regions: κT (0) ≈ 1, 44, κT (0, 3) ≈ 1, 1; κT′ (0) ≈ 1, 67, κT′ (0, 4) ≈ 1, 22. Obviously, there exist unequivocal solutions of the equations κe (η) = κT (η), κe (η) = κT′ (η), corresponding to the experimentally determined curves κe (η), κe′ (η), which ascend monotonously with increasing η, in the regions: 1, 1 < κe (0) < 1, 44; 1, 22 < κe′ (0) < 1, 67. Let us now take the data of [38] for Fe  33% Ni and use them to calculate the longitudinal velocities of sound, related to the axes of symmetry of cubic crystals [193], in order to determine κe (0) ≈ 1, 1, κe (0, 3) ≈ 1, 22 for the second wave: c2 k [0, 22 0, 3 1], c′2 k [0, 34 0, 4 1]. It should be noted here that the twins no longer can be treated equally in relation to the second wave, if compared with the case of habit (225). Obviously, the second wave delivers more pressure towards direction [001]. The experimental result published in [13] gives evidence for our conclusion that the thickness of the respective twins effectively is more in comparison to the width of the twins with Bainpressure directed in axis [010]. A very convenient form of notation of axes and planes, being particularly useful for the description of morphologic characteristics of twinned martensitic crystals, can easily be obtained for any given habit, out of a totality {h k l} under the assumption h < k < l. Then the direction h0 0 l/l i for {h k l}habits {3 10 15} ÷ {2 5 9} (the position of the 1 corresponds with the position of the largest modulus of the index l ) will be collinear with the direction of wavepropagation with velocity c1 , which initiates the γ − α  transformation in the phase of tension. The axis h0 k/k 0i (position of the 1 corresponds to the position of the intermediate module of index k) determines the direction of the main Bainpressure axis and the axis hh/h 0 0i (the position of the 1 corresponds to the position of the smallest module of index h) the direction of the Bainpressure axis for the volumetrically smaller twin components. The twinningplane can be noted in the form { h/h k/k 0}. The same symbols can also be used for definition of the direction of the normals h h k l i to habits { h k l }, in a stereographic projection, being commonly used in crystallographic analysis. Namely: the pole h h k l i is located within a stereographic triangle, its corners h0 0
l i, l
h0
h l i, k l
h
h k l i h k l
(5.9)
correspond with the projections of the axes of symmetry of the fourth, second and third order, respectively. Following (5.9), e.g. the normal [15 ¯3 10] corresponds with the stereographic triangle [100]  [101]  [1¯11]. We can easily convince ourselves that there exists a totality of twentyfour orientational variants, all of them corresponding with the normals h h k l i. By consideration of the notes in the previous section we see that the corner h0 0 l/li of the triangle, being confronted with the { h k l}  habit, indicates the direction of the austenitic ex141
pansion during formation of a martensite crystal. We also note that the corner h h/h k/k l/li of the stereographic triangle points into the direction of the normal of the plane of densely packed austenite, out of a totality of four planes {111}, belonging to the orientational relationship of the lattices of the γ  and α  phases (see Pt. 1.2), with respect to a materialized habit of the { h k l} family, which also feature the smallest angle with the habitplane in relation to the remaining {111} planes. The latter circumstance most likely is linked up with the minimization of free energy of the phaseboundary, during its gradually staged microscopic coupling, as commonly known for grainboundaries [194].
5.2
Grouping laws for packetmartensite crystals
Research on lath or packetmartensite is a highly demanding scientific task. The papers [24, 195–205] provide us with a relatively comprehensive and contemporary image on the development of concepts and the structure of packetmartensite. The habits of packetmartensite near to {557} were firstly mentioned in [195], for Fe  0,2% C, Fe  0,6% Csystems (and confirmed in [197, 205]), where the conformance of a pair of Millerindices only is approximated. Thus in reality, the normal of the habitplane is located within the stereographic triangle (see end of Pt. 5.1) corresponding to its habit, and not at the border of two triangles. In our wavepattern used in Pt. 5.1 for a description of habits { h h l }  {557}÷{225}, an unequivocal orientation of the habits near {557}, {225} will arise if the directions defined by c2 k h11ηi are ”split” into pairs h1 ± η1 , 1 ∓ η2 , ηi , η1,2  < η. Then we get instead of {h h l} the corresponding expression {h ±δ1 , h ∓δ2 , l}, where δ1,2  < 1. Using (5.3) and the relation c1 k [00¯1], c2 k [1 + η1 , 1 − η2 , η] we can determine the vector N, being collinear to the normal of the habitplane N k [ 1 + η1 , 1 − η2 , κ
p
(1 + η1 )2 + (1 − η2 )2 + η 2 + η ],
(5.10)
where κ = c2 c−1 1 . Then we can determine from (5.10), e.g. for η1 = η2 = 0, 03, η = − 0, 21, κ = 1, 2, the habit (4,79 4,51 7), whose normal is located within the stereographic triangle [001]  [101]  [111]. Let us further assume that, for initiation of a γ − α  transformation resulting in packetmartensite, there are required certain phaserelationships among the relative displacements of the lattice atoms associated with the waves, in a similar way as for lamellar martensite (see Pt. 5.1.4). Then we compare in the crystals with habits of the type {5 + δ1 , 7, 5 − δ2 }, for δ1,2 > 0, the direction of expansion  h010i and the direction of compression h100i, where positions 1 correspond with those habitplane indices where the modules attain the largest or the mean value, respectively. Further assuming that the strainamplitudes of the waves are sufficiently large to initiate plastic deformation, (see Chap.3), then it will be possible to determine the direction of macroshear S (lacking the correct sign), as the pair of waves 142
propagating into directions h001i, h1+η1, 1−η2 , ηi, will prefer one of the twelve slipsystems {111} h1¯10i of the fcclattice. The real selection will then be performed in accordance with the Schmidrelationships for shearstress δc (see e.g. [206]): δc ∼ cos ϕ1 cos ϕ2 ,
(5.11)
resulting from the requirement of maximum angular factor modulus (5.11) for the mechanical stress associated with the waves. ϕ1 , ϕ2 in (5.11) are the angles between the direction of applied normal stress (being close to the direction of propagation of the longitudinal wave) and the directions of the normal h111i to the slip plane  {111} or shear h1¯10i, respectively. As a result of this analysis, the habits {5 ± δ, 5 ∓ δ, 7} will naturally form groups of sextets { h k l} close to the common slip planes {111}. An example of such grouping is presented in Table 5.2, for η < 0. This grouping corresponds to a package of crystals [196–198] Table 5.2. Directions of wave propagation and some characteristics of packetmartensite (slipplane (111)) Nr.
Habit
Direction of c2
1
(5 + δ1 , 5 − δ2 , 7)
[1 + η1 , 1 − η2 , η]
2
(5 − δ1 , 5 + δ2 , 7)
[1 − η1 , 1 + η2 , η]
3
(7, 5 + δ1 , 5 − δ2 )
[η, 1 + η1 , 1 − η2 ]
4
(7, 5 − δ1 , 5 + δ2 )
[η, 1 − η1 , 1 + η2 ]
5
(5 − δ1 , 7, 5 + δ2 )
[1 − η1 , η, 1 + η2 ]
6
(5 + δ1 , 7, 5 − δ2 )
[1 + η1 , η, 1 − η2 ]
Direction Compressive Direction c1 axis S [00¯1]
[100]
[¯101]
[00¯1]
[010]
[0¯11]
[¯100]
[010]
[1¯10]
[¯100]
[001]
[10¯1]
[0¯10]
[001]
[01¯1]
[0¯10]
[100]
[¯110]
with six orientations close to the common plane (111), forming part of the orientational relationship. Obviously there exist three similar groups of crystals with six orientations in each group, comprising other common planes out of the totality of {111}. It is also obvious from Table 5.2 that, if the crystals with six orientations are equally partitioned in such a package, then, during a martensitic transformation, the region occupied by such a package must be subjected to a quasiisotropic volumetric change, as the directions of maximum compressive and tensile stress correspond to all three variants of Baindeformation, while the alternating orientations of latticedisplacement S make possible a macroscopic neutralization of totalized local displacements within a packet. In [196–198], just these rules were pointed out. 143
Due to a missing more stringent definition of the term ”Packetmartensite crystal” it came about that, apart from methodological problems, different results were obtained in the determination of the number of orientations associated with martensite packet crystals. Thus in [199], one or two, in [205] only one, and in [196–198], six orientations within a common plane {111} were considered. If one describes the term ”packet” as a totality of martensitecrystals (with habits near {557}) and with six orientations close to a common plane out of {111}, as practically done in [196–198], then the determined reduced number of orientations must be associated with a certain local zone of the packet, which would comprise a reduced number of orientations. In [202], the existence of four zonal types was determined in one packet. Type 1 represents triplets of orientations, i.e. habittriplets of numbers 1, 3, 5, or 2, 4, 6 as shown in Table 5.2. Type 2 represents pairs of orientations, i.e. habitpairs 1, 4; 2, 5; 3, 6 as shown in Table 5.2. Type 3 represents pairs of twinorientations, corresponding to pairs of habits 1, 2; 3, 4; 5, 6 as shown in Table 5.2. Type 4, with only one orientation, corresponds to any of the habits shown in Table 5.2. For equal volumetric fractions of crystals with different orientations in zone of type 1, a quasiisotropic change of volume in conjunction with neutralization of sheardeformation may be possible. In the zone of type 2 (as well as in the zones of type 3 and 4), the volumetric changes become anisotropic, but a neutralization of displacementdeformation still is possible. This however is no longer possible for zones of type 3 and 4, that is becoming evident by comparison of the Sdirections in Table 5.2. Obviously, the used definition of the packet implicitly takes for granted that the transforming austenite comprises a sufficiently large volume. In other words, this definition is critical with respect to the austenitic volume size. The results obtained with pseudomonocrystals in [203, 204] fit well with the findings in [196–198]. In [200], being related to the case of coexistence of lamellae with habits {225} and laths, a package is defined as a totality of ”blocks” composed of lamellae and laths (each lamellae being connected with laths embodying two twinningorientations), in such a way that within this definition, the requirement of six orientations lives on for packetmartensite. A comparison with the a.m. data [202] shows that, due to the presence of lamellae with habits {225}, to which a dominant role during formation of packets is assigned in [200], only the zone of type 3 is segregated out of four types of local packing zones in lathshaped crystals. We also note that the association of plane (111) in Table 5.2 with the plane of least slip resistance correlates well with the concepts in [13] on stressrelaxation, during the isothermal martensitic transformation by shearprocesses within the austenitematrix surrounding the martensite crystal. The orientation S, being precisely determined by the Schmidrule (with exception of the sign), correlates with the macroscopic direction of displacement of a martensite crystal of this orientation [200, 201].
144
5.3
5.3.1
Effect of the magnetic state of austenite and of an externally applied magnetic field on the martensitic γ − α  transformation Possible causes for the transition of habitplanes
After our matching of the habits with pairs of waves, it will be easy to estimate which parts of the electronic spectrum are actively involved in a martensitic transformation. Following such general characteristics, it is possible to associate crystals with habitplanes near {557}, {225}, as the pairs of waves, propagating near the axes of symmetry of the second and fourth order, can be put in relation with the electronic states being localized in the vicinity of the Ssurfaces: Sh001i , Sh110i (see Chap. 2). In the case of the habit (15 3 10), already mentioned under Pt. 5.1.4, the direction of c2 defines an angle θ1 = 20, 3˚, θ2 = 69, 8˚, θ3 = 34, 7˚ in relation to the axes [001], [110], [111]. It is therefore justified to assume that the habits {15 3 10} need only to be matched with the waves propagating near the fourthorder symmetryaxes, being linked up with the Sh001i surfaces. Thus the causes for the first and second change of habits, i.e. {557} → {225} in FeCsystems, and for the second change, i.e. {225} → {259} in FeCsystems and {557} → {3 10 15} in FeNialloys, apparently must be different. In the first case, no change of the class of waves governing the growth of a martensitic lamellae occurs; while the velocityvector c2 of the second wave remains within the directional cone near h110i, and only the sign of the projection c2 on the direction h00¯1i (close to direction of propagation of the first wave (see Pt. 5.1.3)) changes. The causes for this behavior may be: 1. Increase of the velocityratio κ = c2 c−1 with increasing carbon1 concentration, leading to improved conditions for Baindeformation for κ > κc (see Table 5.1) (i.e. to smaller thresholddeformation εt ), in case of changing sign of the projection of c2 on h00¯1i. 2. The appearance of a shortwave displacement component, being responsible for the thin (twinned) structure of macrolamellae in the case of crystals with habits {225}. From a dynamical point of view, the appearance of shortwave displacement (of about half the wavelength with an order of magnitude of about the thickness of twins) at lower temperatures (related to the MS  temperature of lathmartensite) should be possible in principle, as a reduction of T will inevitably lead to a reduction of phononextinction and, consequently, also of the thresholdvalue σt of an inverted occupational difference (see (3.10) in Pt. 3.1). The latter argument fits well with the commonly used interpretation in [13], stating that during a martensitic transformation, the relaxation of internal stress at low temperatures is mainly linked up with 145
twinningprocesses. The second change of habits apparently is caused by a reduction of the activity of electronic states localized near the Sh110i surfaces, in relation to the states located near Sh001i . The relative passiveness near Sh110i may be related to the magnitudes of the parameters Γ and εd − µ, at the surfaces Sh110i and Sh001i . We recall that εd represents certain meanvalue ε¯ of the energies of the delectrons on the Ssurface and Γ is an extinction of selectrons of energy εs ≈ εd . As a common cause of the different values of the Γ parameter at different Ssurfaces, it is possible to define the anisotropy of sdscattering, the degree of which varying with concentration of the alloying elements. The variation of εd − µ for non spinpolarized states with εd −µ > 0 (see Pt. 4.5) is mainly caused by a the variation of the latticeparameter a, whereas the rate of variation of εd − µ may differ for different Ssurfaces, due to the noncorrespondence of the rates of change of energies εd . If, for example, the tight binding approximation in [104] was used with consideration of the first and second neighbors, as well as the expressions of the matrixelements Vij ∼ a−5 for the electronic transitions among the knots given in [183], then it would easily be recognized that the characteristic energies (see Pt. 2.5) εX5 , εX2 , εL3 decrease with increasing a, while the rate of decrease is largest for εX5 and least for εL3 . For spinpolarized states, the value of εd↑ − µ < 0 will also depend on the magnitude of exchangesplitting, which probably increases at temperatures below the magnetic ordering temperature, and in the case of anisotropic splitting, may be an additional cause of passivation of electronic states near Sh110i for the FeNisystem (with CN i > 29%), in which magnetic ordering of the γ  phase precedes the martensitic transformation. The influence of the magnetic state of austenite on reaction kinetics has been highlighted in [207] and [208], in connection with a qualitative consideration of the causes of a selective influence of a magnetic field on the kinetics of the γ − α transformation. The most important law published in [15] is related to the effect of magnetic field bursts with fieldstrengths H up to 2, 8 · 107 A/m (≈ 350 ke) on FeNialloys. This law states that a magnetic field stimulates the athermal transformation into lamellarmartensite of FeNialloys with Niconcentration of more than 25 %. In addition, such magnetic field burts cause a nonmonotonous increase of the point MS by ∆MS , as depicted in Fig. 5.2. According to [15], the positive shifting ∆MS > 0 is deducible from the larger inherent magnetization of the α  phase, and, consequently, from the larger incremental freeenergy reduction of the α  phase in a magnetic field, in relation to the γ  phase. Nonmonotonous character of the shifting ∆MS is attributable to the exceptionally large volumetric magnetostriction of the paraprocess defined in [209, 210], with consideration that the lower concentration limit of the nonmonotonous magnetic field relationship corresponds with the lower limit of the ∆MS  relationship (see Fig. 5.3, borrowed from [211]). A similar correlation also exists for steel with a superparamagnetic γ  phase [209, 212] as well as for FeNiMnalloys with F e70+x Ni30−2x Mnx (0 < x < 4), which have been in146
∆MS ,K 60
20
0
30
26
CN i,w%
Figure 5.2. Relationship between the shifting of MS in a magnetic field of 2, 6·107 A/m and Niconcentration (weight %) [15] vestigated in [213, 214]. A linear extrapolation of the relationship between the volumetric increment ∆V /V and the quantity H, as shown in Fig. 5.4 (borrowed from [209]), results in a value of ∆V /V ∼ 10−3 for H = 2, 8 · 107 A/m. The growth of specific volume in a magnetic field also correlates well with an increase of magnetization [213]. This suggests that ”quasiferromagnetic” ordering exists in a strong magnetic field, being also associated with the transition towards athermal transformation kinetics [208]. The emergence of this state presumably is caused by magneticfield induced exchangesplitting, which in turn results from the dependence of the exchange integral on the atomic distances (lattice parameter) or specific volume, respectively. As a reasonable basis for analysis and description of this effect, the exchangestriction model may be suggested (see e.g. [215]).
5.3.2
Single peak density of states (DOS) model, exchangesplitting and electronic redistribution
If the Fermilevel µ of the nonmagnetic state of the γ  phase of a FeNialloy is located at the boundary of a steplike change of the DOSfunction (right in front of the last peak of the density of states function of the dband in Fig. 2.9), then the process of exchange splitting must be associated with an overflow of a part of the selectrons into dstates [216,217]. By comparison of a modeled DOS with two characteristic values g1 and g2 , as shown in Figs. 5.5a and 5.5b, it becomes evident that the exchangesplitting ∆εexch must lower the Fermilevel by forcing the spinup states into states with greater occupational density g2 . The new Fermilevel µ′ of the subsystem of delectrons (dashed line in Fig. 5.5b) can be determined using the condition of equality of the hatched areas for the subbands d ↑, d ↓ as shown in Fig. 5.5b. With consideration that the difference of the areas of the d ↑, d ↓ subbands  below the level µ′  determines the atomic magnetic momentum µ ¯ µ−1 B 147
∆V V
· 106
30
10
10
30
CN i,w%
Figure 5.3. Relative change of volume due to magnetostriction in a magnetic field of 8, 4 · 104 A/m [211] (Niweight %) (expressed in units of Bohr’s magneton µB ), then we get for the ferromagnetic phase ∆ εexch =
¯ g1 + g2 µ , g1 g2 2 µB
µ − µ′ =
g2 − g1 µ ¯ . g1 g2 4 µB
(5.12)
In the parabolic sband, being characterized by a monotonously changing density of states gs (see Pt. 4.3), the variation of the Fermilevel µ = µs of the subsystem, being related to exchangesplitting of the selectrons, can be ignored, i.e., a separate consideration of the s and dband will deliver µ′ = µd < µs = µ. If an equality of the Fermilevels of d and selectrons was required, then it would be possible to estimate the number of electrons flowing over from the s into the dband (related to a singe atom): ∆ns ≈ 2 gs (µ) (µ − µ′ ),
(5.13)
where the factor 2 accounts for both projections of the electronspin (note that in Pt. 4.3 we have gs (µ) with only one spinprojection). For a width of the sband Ws = 10 eV, and ZM ≈ 1, we get from (4.27) gs ≈ 0, 12eV −1 atom−1 . Further assuming that the width of the dband Wd = 4, 5 eV, and the width of the rectangular peak 0,5 eV, g1 ≈ 1 eV−1 atom−1 , g2 ≈ 2 eV−1 atom−1 , µ ¯µ−1 B = 1, 7, which, in accordance with [218], almost represents the alloy F e0,65 Ni0,35 , then ∆εexch ≈ 1, 28 eV,
µ − µ′ ≈ 0, 21 eV,
∆ns ≈ 0, 05.
(5.14)
Of course this pattern features an illustrative character, in that it only gives us an estimated order of magnitude µ−µ′ ∼ 0, 1 eV, ∆ns ∼ 10−2 . Presumably, the value 148
∆V V
· 106
60
30
0
5
10
15
H · 10−5, A/m
Figure 5.4. Relative change of austenite volume in the steel 40X2H20 in a magnetic field up to 1, 5 · 106 A/m , at temperature of 77 K [209] ∆ns ≈ 0, 05 is too large, as firstly, in the nonmagnetic case shown in Fig. 5.5a, the shape of the DOSpeak, as well as the location of the Fermilevel, correspond to the maximum value of ∆ns , and, secondly, the relative shift of the d and sbands has not been properly taken into consideration. According to [111], the transition from configuration 3d6 4s2 to 3d7 4s1 of the γ  phase of iron is associated with an upward shift of the dband by 5,5 eV  at an energetic scale  due to an increase of the repulsive energypotential of the delectrons. Then, due to an selectron overflow of ∆ns = 10−2 into the dband, we get the following estimate for the upward shift of the dband: ∆µ′ = 5, 5 · 10−2 eV. If we further consider that for gs ≈ 0, 12 eV−1 atom−1 , an selectron overflow of ∆ns = 10−2 would reduce the value of µ = µs by 4, 2 · 10−2 eV (using the same g1 and g2 ), we got a value of only ∆ns ≈ 0, 022, being less than half of our initial estimate (5.14). Thus, the reduction of the Fermilevel µ − µ′ proves not to be greater than 0,11 eV. Of larger interest however is the shift of the Fermilevel being related to the bottom of the dband: In the ferromagnetic state, the bottom of the dband is equal to the bottom of the d ↑  subband. Let us designate by ∆µd↑ the shift (towards the upper edge of the band). Then the quantity ∆µd↑ can be determined, using the condition of equality of the hatched areas in Fig. 5.5b: ∆µd↑ =
g1 ∆ εexch 1 ≈ ∆ εexch ≈ 0, 43eV, g1 + g2 3
(5.15)
where the value ∆εexch has been taken from (5.14). A substantial difference among the values ∆µd↑ and µ − µ′ , namely the weak dependence on the relative shift of the s and dbands, (note that the shift ∆µd↑ is mainly caused by redistribution of electrons within the d ↓→ d ↑ subbands) as well as disappearing difficulties related to the selection of the origin of energyreference, are arguments in support 149
g2
a
g1
d↑
µ 0
ε
Wd g1
d↓ g2 g2
b
g1
µ′ µ
d↑
∆εexch ε
0 g1
d↓ g2
Figure 5.5. Modeled (singlepeak) DOSfunction of delectrons, in the paramagnetic (a) and ferromagnetic (b) phase
of ∆µd↑ , when compared with the measurement conditions of the parameters ∆µd↑ and µ − µ′ . Obviously in our model, the heating process, being associated with the destruction of ferromagnetic ordering, will result in a relocation of the Fermilevel relative to the dband, by about the same magnitude as (5.15), linked with a shift corresponding to the inverted electron overflow d ↑→ d ↓ (d → s). These findings are in accordance with data presented in [220, 221], in which a relationship between the Fermilevel and the temperature of invaralloys has been observed, during photoelectronic Xray spectroscopy. During heatup of two FeNialloys with about 34,87 atom% Ni and 35,8 atom% Ni, from 100 K to 600 K, the shift ∆µd↑ towards the bottom of the dband was about 0,51 eV and 0,36 eV, respectively. Considering of the simplified character of our model, this correspondence of the measured values with our estimate by (5.15) appears fairly well. We should however note here that, during magnetic ordering, the associated s → d redistribution of electrons must result in a reduction ∆Cl of the elastic modulus Cl , which, according to the BohmStaverformula [192], is proportional to the ionchargenumber Z, while a variation of Z must correspond with the quantity  ∆ns . Thus obviously 150
ε
µ
Figure 5.6. Contribution of iron  (dashed line) and nickelatoms (solid line) to the singlepeak DOS function of the F e0,6 Ni0,4  alloy [219] ∆Z Cl , Z and with ∆Z ≈ − 0, 02, Z ≈ 1, we get ∆Cl ≈ − 0, 02Cl , being about 10% of the of the elastic modulus reduction1 associated with the magnetic ordering process, as reported in [38]. Despite their low amount, the number ∆ns of electrons participating on the s → d  transition can be regarded as an informative parameter, due to the high sensitivity of the isomershift δ of the γ  nuclear resonance absorptionline, in conjunction with to the s → d  transition. In particular, the γ  resonance increases during s → d  transitions and decreases during d → s  transitions (see e.g. [222]). If we now use the relationship between the isomershift of F e57 and the chargedensity of the 3d and 4selectrons (see Fig.16 in [222]), in the configuration 3d8−z 4sz , for Z ≈ 1, ∆Z ≈ − ∆ns ≈ − 0, 022, then we can determine that the isomershift increases by ∆δ ≈ 6, 4 · 10−5 m/s. This estimate matches fairly well within the interval of ∆δ = (0, 6 ÷ 1) · 10−4 m/s, as reported in [223] for the isomershift in F e − (28 ÷ 75)% Nialloys during magnetic transitions (however a somewhat less ∆δ = (4 ÷ 5) · 10−5 m/s has been reported in [224], for Fe33% Nialloys). Singlepeak DOSmodels have successfully been developed for the fcclattice structure of FeNialloys (see e.g. [219, 225, 226]). Using a realistic (nearly triangular) shape of the peak, the following characteristics of such DOSfunctions were obtained, on the basis of a coherentpotential approximation: ∆ Cl ≈
• An appreciable difference among the DOSfunctions for subbands d ↑ and d ↓, being evident in Fig. 2.9; • Changes of the shape of the subband DOSfunctions (in most cases, the shape of the d ↓  band) will vary with the composition of the alloy; 1
The basic contribution to a softening of elastic modulus gives the redistribution of delectrons. So e.g. at µ ¯ = 1, 7µB from states with small density g1 into states with major density g2 0,85 electron/atom overflows. Then ∆Z/Z ≈ ∆C/C ≈ −0, 85/7.
151
• Splitting of the DOS into partial contributions of Fe  and Ni  atoms. An example for this splitting, pertaining to the F e0,6 Ni0,4  alloy, borrowed from [219], is shown in Fig. 5.6. The relative success of the hardzone model used for these estimates can mainly be deduced to the conservation of the shape of the d ↑ band for partial components of the iron and nickelatoms, as well as to the weakly pronounced variation of the DOS of the d ↓ band at the Fermilevel, with varying alloying composition. It has to be noted however that the considered mechanism of variation of the isomershift through s → d  overflow is limited to such Niconcentrations starting from which the process of d ↓→ d ↑  electron redistribution doesn’t cause an appreciable downshift of the Fermilevel of the delectrons subsystem. According to the data in [219], this particular concentration is about 40% Ni, thus the process of s → d  overflow can contribute the most part to ∆δ, within the region of concentration of our interest of 29 ÷ 34% Ni. Our qualitative notion of these processes however deserves at least another remark, namely: Due to significant inhomogeneities of concentration and magnetic order (see e.g. [227,228]), the transition into a magnetic state of order is remarkably blurred. Thus, with decreasing temperature, the structure of an inhomogeneity can vary from a quasiparamagnetic up to a chaoticallyfrozen spin distribution, akin to a spinglass ( [229]). According to [230,231], the cause of the emergence of a noncollinear magnetic structure is the blended character of exchangeinteraction, being a common feature of many binary transitionmetal alloys. For example, the exchangeintegrals of pairs of FeFe atoms in FeNi  alloys are of negative sign, i.e. JF e−F e < 0, and of Fe  Ni , Ni  Ni pairs, of positive sign, i.e. JF e−N i > 0, JN i−N i > 0. The notion of an antiferromagnetic character of the exchange interaction of FeFe in iron and its alloys with fcclattice has for the first time been postulated in [232]. The values of exchangeinteractions JF e−F e = − 9 meV, JF e−N i = 39 meV, JN i−N i = 52 meV, as determined in [233], are evidence in support of these concepts, i.e., below the Curie temperature Tc , strictly (collinear) magnetic structure not exists in the premartensitic austenite, thus the assumption of a ferromagnetic state of the fccaustenite should only be regarded as a reasonable approximation. During various neutronspectroscopic investigations on austenitic FeNi  invar alloys (see e.g. [234–236] and further references therein), there have been discovered superstructures of the γ ′ , γ ′′ , γ ′′′ type. The first of them already appearing in the paramagnetic region T > Tc > MS , the second one at T ≤ Tc (T > MS ), being linked up with the onset of ferromagnetic ordering, while the third one appears at T ≤ TN (TN  Neeltemperature, TN < MS ) and reflects the onset of antiferromagnetic longrange ordering. We note that the γ ′′ phase has been considered as an intermediate phase in [237, 238], thus ensuring the necessary symmetrylink between the γ  and the α  phases, which will finally lead to the Nishiyama orientational relationship of the γ  and α  phases. Evidence of a rather complex nature of the magnetic transition is also given by 152
the results of [239] (more detailed see [240]), in which two different stages of the magnetic transition of austenite have been determined, in a temperatures range of 0, 8 ≤ T · Tc−1 ≤ 1, on the basis of a very detailed analysis of the isomershift of FeNialloys with (28, 5 ÷ 31, 3) wt.% Ni. The first stage occurs in a temperature range of about 25÷30 K below Tc and is characterized by an increase of the isomershift of F e57 nuclei in the ferromagnetic areas of the fccphase, by about (∆δ)f m ≈ 5 · 10−5 m/s, while the δvalues of the paramagnetic areas remain unchanged, i.e. (∆δ)pm = 0. In the second stage, the isomershift decreases, exhibiting slightly larger incremental decreases of (∆δ)pm ≈ −6 · 10−5 m/s in the paramagnetic areas than in the ferromagnetic areas, with (∆δ)f m ≈ −4, 5 · 10−5 m/s. The positive shift (∆δ)f m in the first stage matches fairly well with the estimates of the shift ∆δ being associated with s → d  electron overflow. However, experimental results reported in [239, 240], which aimed at an explanation of the particularities of the second stage of the magnetic transition, by relating them to the increases of hydrostatic pressure during formation of an ”infinite” ferromagnetic cluster within the system, provided ∆δvalues which would only correspond to an isomershift of about 15 to 20 % of the observed values. Thus it cannot be excluded that the missing (main) part of the observed effect is related to the processes of d → d  electron redistribution between iron and nickelatoms, being mainly caused by the significant relative differences among their affected spectral density regions, i.e. where the partial contributions of the iron and nickelatoms are largest. Thus for example it is obvious from Fig. 5.6 that the increase of exchangesplitting must lead to a reduction of the number of d ↓  electrons of the ironatoms, and to a corresponding increase for the nickelatoms. This kind of d ↓→ d ↓  electron redistribution among alloying components must result in a decrease of isomershift, as the decrease of the number of delectrons of ironatoms must elevate the chargedensity of selectrons at the nucleus [222]. Such minor effects however, as well as those of a possible polarization of quasiparamagnetic areas, in conjunction with the formation of internal or external antiferromagnetic order (being put in relation with the ferromagnetic areas), will not deserve further consideration in our further analysis.
5.3.3
Oriented latticegrowth of athermal martensite in an externally applied magnetic field
The orientational effect of an externally applied magnetic field on the growth of martensite crystals mainly consists in a preferred orientation of the long axes of martensite crystals parallel to the magnetic field, as highlighted in [15, 241]. The conclusions in [242] on the orientational effect of a magnetic field had been drawn from investigations of the magnetic anisotropy of a specimen exposed to a magnetic field during and after a γ − α  MT. A thermodynamical analysis in [15] explains the predominance of smallangle orientations among martensitelamellae in cubic crystals, mainly by attributing them to the minimization effect on the 153
magnetic field energy contribution to the thermodynamic potential, being closely related to the proper magnetic field produced by the magnetic spinmoments of electrons in the ferromagnetic α  phase. As commonly known for the specific case of an ellipsoidal magnetic specimen, this energy resembles a quadratic function of all magnetizationcomponents, the coefficients of which being proportional to the components of the demagnetizationtensor. For smallangle orientations, the proper magnetic energy is proportional to the square of magnetization and to the least of the three eigenvalues of the demagnetizationtensor, being many times less than 1 for small slices (lamellae). And viceversa, for lamellae with largeangle orientation, the demagnetization factor is of an order of magnitude of 1, thus its contribution by proper magnetic energy becomes largest. It has however to be considered that the orientational influence of the demagnetizationfields, as well as that of magnetic anisotropy, on the growth of martensite crystals not exceeding 8 · 105 A/m ∼ 104 Oe, dwindles with increasing externally applied magnetic field strength, finally disappearing for magnetic fields of H ≥ 107 A/m ∼ 105 Oe [209]. Within this context, in case of strong magnetic fields, those factors which increase with increasing external magnetic field can come to the fore. Among them, there is the nonequilibrium addend to the electronic distribution function. Let us assume that the athermal martensitic transformation would only be related with those electronic states being localized in the proximity of the Sh001i surfaces (see Pt. 5.3.1). Thus we shall consider the effect of a magnetic field H on the nonequilibrium addend f − f 0 of the electronic distribution function f 0 . In accordance with [243], we can use the following approximation, being linear in H: f − f 0 = − Φ′ Φ′ = (τ P , v) +
∂f 0 , ∂ε
(5.16)
eτ ~ ) (τ P , v), ( H, [v , ∇] c0 ~
where e  electron charge; τ  average free path time of existence of an electron; c0 ~  gradientoperator in k  space, while the explicit form of the  speed of light; ∇ vector P, including the temperature, chemical and electrical potentialgradients, not being worth to be considered in our further analysis. We shall further confine our analysis to the calculus of the contribution of nonequilibrium addends to the electronic distribution functions, related to states in the proximity of the reduced 1st face of the S[001] surface, which in this case corresponds with the squareshaped border of the 1st BZ. In our calculus of the groupvelocity v and its derivatives, it will be justified to use a dispersion law in the tight binding approximation, which considers fairly satisfactory the particularities of the electronic energy spectrum within a weakly dispersed band, being enumerated by X5 on sheet Nr.1. For example, we can obtain from (2.16) ε = 4 ε1 = const along the line X5 W (weak dispersion will only appear after consideration of the resonancetransition integrals with the second neighbor). Let Hk [001] and assume 154
that the predominant contribution to the rate of change with k under the numeral ~ k brings in v, then we get from (2.16) and (5.16): of ∇ 2 e τ 2 ε21 a3 H ( Jx + Jy + Jz ), c0 ~ 3 Jx = sin x (cos x + cos z) (1 + cos z cos y) Py ,
Φ′ − (τ P , v) =
(5.17)
Jy = − sin y (cos y + cos z) (1 + cos z cos x) Px ,
(5.18)
Jz = sin z sin x sin y (cos x − cos y) Pz , vx = 2 ε1 a ~−1 sin x (cos y + cos z), vy = 2 ε1 a ~−1 sin y (cos x + cos z),
(5.19)
vz = 2 ε1 a ~−1 sin z (cos x + cos y). In (5.18), (5.19) we used instead of the designations η1 , η2 , η3 in (2.16) the designations x, y, z, without index. During Uprocesses among states in the proximity of the sheets Nr. 1, the velocity component oriented normal to sheets Nr. 1 inverts its sign ( the Vx,y,z in (5.19) include odd sinefunctions), and the differences of the nonequilibrium terms ∼ (τ P , v) will sum up, which, in effect, leads to maximum inverted occupational difference (IOD) for ESpairs. As a result of (5.18), the fieldterms containing the Jx , Jy and also deliver an additional contribution to the IOD, being related to ES  pairs located in the proximity of the sheets Nr. 1 with normals [100] and [010], have the same characteristics. The term ∼ Jz however is odd with respect to the inversion x ⇆ y, Therefore, ES pairs near sheet Nr. 1 with normal [001] do not contribute to IOD as Jz is integrated in the region which is symmetric with relation to the x ⇆ y inversion. Within usual definitions, this behavior of the fieldsupplements reflects transversal thermomagnetic and galvanomagnetic effects. As a result, a field H k [001] will support the generation of waves with q near [100] and [010]. Thus, in accordance with the twowave pattern, there can be expected habits {l k h}, whose smallest angle with H will be ( l  >  k  >  h ), where the underlined indices mark their ¯ . . . Accordingly, {l h position being fixed, i.e.; {l k h}  (l k h), (k l h), (k l h) k} and { h k l } represent the totalities of the medium and large angle habits. For H k h111i, this orientational effect must vanish. This latter conclusion is important in order to clarify the causes of the observed orientations, as there also exist thermodynamical reasoning [15] in favor of the smallangled orientation of the first martensite lamellae, being independent of the orientation of H. The lack of an appreciable orientation at H k h111i, in relation to H k [001], would imply that the dynamic mechanism plays a decisive role. Of course, the effect of H on the generation of latticedisplacement waves becomes appreciable as soon as the magnitude of fieldsupplement becomes comparable with the initial supplement (τ P , v). It is however more convenient to average the supplemental terms when performing such comparison, by integrating the expressions (5.17) and (5.18) over those areas being parallel to faces Nr. 1. Then their ratio will be 155
ψ ≈
e τ a2 ε1 Py H. 5 c0 ~ 2 P x
(5.20)
For Py ≈ Px , τ ∼ 10−12 s, a = 3, 5 · 10−10 m, ε1 = 5 · 10−20 J (corresponding to the width of the band ∆ε = 16ε1 = 5 eV), H = 8 · 106 A/m ∼ 105 Oe (being typical experimental results published in [15]), we get from (5.20) ψ ≈ 0, 2. Thus the fieldsupplement is a nonnegligible quantity. It has however to be emphasized here that the conclusion related to the transversal character of the thermo and galvanomagnetic effects at H k [001], having been drawn during our previous consideration of the electronic states in the proximity of the Sh001i surfaces, will remain valid during an analysis of the nonequilibrium terms for states in the proximity of the curved sheets Nr. 2 of surfaces Sh001i . To convince oneself, it will suffice to recall the definition (2.11) ~ appearing in the of a Ssurface, taking into consideration that the vector [v, ∇] fieldsupplement (5.16) is perpendicular to v. Consequently, the scalar product ~ ) vanishes for v k H attaining a maximum for v ⊥ H. This means that ( H, [v, ∇] our conclusion of the preference of smallangled orientations of martensite lamellae for H k [001] also applies for the field supplements to the electronic distribution function f in the proximity of sheets Nr. 2 of the Sh001i surfaces, thus being a general conclusion. In the case of magnetically ordered austenite, the local fieldinduction vector has to be used instead of vector H and also the effect of magnetostriction has to be taken into account as the emerging lattice deformations can modify the orientational effect. At H k [001] and for a magnetostrictive constant of λ100 < 0 there will be produced compressive stress in the orientation [001] and, in the orientations [100], [010] equal magnitudes of tensile strains (see §2, Chap. 23 in [159]). Considering the rule of matching between the compressive and tensile axes and the habit planes indices, as discussed in Pt. 5.1.4, then there can also be expected mediumangled {l h k} habits, in addition to the smallangled {l k h} habits. It is worth to note that if H is oriented near [001], so that a larger dilatation along one of the transversal axes is ensured, e.g. along [010], then the emergence of {k l h} and {h l k}, with two fixed indices positions will be most likely for the small and mediumangled habits . For λ100 > 0 (i.e. dilatation along [001]), also largeangled habits {h k l} must arise, apart from the smallangled habits. We emphasize that the above orientational effect of an externally applied magnetic field can be discriminated with satisfactory reliability from orientational effects related to uniaxial elastic stress (like that produced by magnetostriction or by externally applied stress), which would result in the appearance of mediumangled (for compressive stress) and large angled (for tensile stress) orientations of the lamellae in athermal martensite. In sufficiently strong magnetic fields, the contribution of a nonequilibrium electronic fieldsupplement to the orientational effect, which would have to become more pronounced with increasing H, can be discriminated from the background 156
of statical orientational effects are caused by the existence of demagnetizationand anisotropy magnetic fields, the general impact of which will decrease with increasing H. In [244], the predominance of smallangled orientations of martensitic lamellae has been reported, based on reproducible experiments with samples of 50X2H22, 77X2H22 steel, being characterized by low autocatalysis of the γ − α  transformation, both in magnetic field bursts and in constant field conditions. In these cases, the orientational relationship is most pronounced if H is oriented parallel to the h001iaxes. This matches fairly well with our above prediction drawn from our analysis of the effect of the nonequilibrium field supplement. Characteristic of this effect is that an increase of H over a critical magnitude of Hc = 1, 1 · 107 A/m (related to the steel 50X2H22, where Hc is the magnetic field for which, at a given temperature Texp = 203 K, the first martensite crystals emerge, i.e. Texp − MS ≈ 100 K) results in an increase of the orientational effect, if H k [001]. Similar results were obtained for the steel 77X2H22 (at Texp = 77 K, with a critical field Hc ≈ 8, 76 · 106 A/m). Unfortunately, the results reported in [244], pertaining to H k h111i, only relate to the specific case H = Hc , thus the dependence of the orientational relationship on the magnetic field strength H has not been investigated. In accordance with the above considerations, it can also be concluded that in the special case of H k h111i an increase of H must lead to a reduction of the orientational effect. In general, the results presented in [244] give evidence in support of our findings based on the notion of the control of the growth process of athermal martensite by longitudinal waves propagating near the h001i directions and, accordingly, also on the dominating role of the electronic states being localized near the Sh001i surfaces.
5.4
Summary of chapter 5
Following our interpretation of the morphological characteristics of martensite within the notion of a twowave pattern, the main conclusions that we can draw here are: 1. The habits of the FeNi and FeCsystems can be associated with a twowave pattern, where one of the waves, belonging to the longitudinal type, propagates in the h001i direction, while the second wave is of a quasilongitudinal type, which can be determined on the basis of experimental data of elasticmoduli at a given temperature MS . 2. The habits near {557} and {225} are characterized by the pairs of waves propagating near the perpendicular axes of symmetry of the fourth and second order h110i, h001i. By means of the criterion discriminating the most favorable conditions for materialization of habits {557}: κ = c Σ c−1 ∆ < κc 157
and {225}: κ = c Σ c−1 ∆ > κc enables us, in principle, to explain the default of habit {225} in FeNisystems. 3. The habits near {259}, {3 10 15} are only associated with those waves propagating near the fourthorder axes of symmetry. Possible causes for the passivation of electronic states (located near the surfaces Sh110i ), being associated with wavegeneration in the h110i  direction, can be the anisotropy of sdscattering processes and differences of the parameter εd − µ, depending on the size of latticeparameters as well as on the magnetic state of austenite. 4. The largescale growth process of martensite is being controlled by long displacement waves, acting in coordination with short displacement waves which form the fine structure. It is possible e.g. to describe the formation of a twinningplane {110} analogous to that of a habit plane, in such a way that a twinningplane resembles the imprinted path of the moving line of intersection of a pair of perpendicular shortwave fronts, including the pairs of waves propagating perpendicular to h001i. This of course does not impede the description of the transformation of small areas within the concept of stationary waves, as shortwave displacements can perform a multitude of oscillations within half a period of the longwave oscillations, whenever favorable transformation conditions materialize, thereby enabling the lattice to perform the transformation under optimized conditions. The oscillation period can easily be estimated if one considers that the widths of the macroand microlamellae of the twins is within the order of magnitude of half of a wavelength each of the long and the short displacements. Of course, the general possibility of twinning being driven by the need for periodic discharge of accumulated elastic strain energy, through lattice rearrangement, is no contradiction to our twowave lattice control pattern, which only emphasizes the main component. On the other hand, the longwave displacements, featuring a slower rate of decay than shortwave displacements, are effective carriers of information controlling the transformation of various regions of the specimen. Longwave displacements thus can attain a leading role in the formation of crystal ensembles. 5. The knowledge of phaserelationships characterizing atomic displacements being most favorable for the initiation of the martensitic transformation by waves enables us to define rules related to the comparison of habits with the directions of compressive and tensile stresses of the Baindeformation (based on a stereographic projection) (see end of Pt. 5.1.4). Using these rules it is easily possible, among other things, to determine the predominant orientation of martensite crystals, based on an orientational relationship with the unidirectional elastic stress field arising at temperatures above the MS temperature. 158
6. The rules derived from observations on packetmartensite are in accordance with the conceptual view of martensite growth in which growth is controlled by pairs of elastoplastic waves. Within this notion, the deviations of the habit planes of lathcrystals from the relevant pairs of Millerindices, resulting in unequivocal orientation of martensite lamellae, can be put in relation with the orientational deviations from the {1¯10} planes of the waves propagating near the h110i axes. 7. The new mechanism of controlled lattice growth of athermal martensite within an externally applied magnetic field, having been predicted after an analysis of the nonequilibrium fieldsupplement to the electronic distribution function, is confirmed by experimental analysis on the morphology of ensembles of martensitic monocrystals, emerging within the austenitic singlecrystals when being subjected to the orientational action of an external magnetic field. Some additional remarks 1. The simple formalism establishing a link between the habitplane and a given pair of waves can be used for a phenomenological analysis of the involved longitudinal and transversal waves, independently of causes and conditions of their emergence, like generation under nonequilibrium conditions, local lattice deformation associated with the nucleation of phases, or even excitation by external sources. To take an example reported in [90], experiments have been performed which aimed at an interpretation of habits of the type {h h l}, being observable during the β → γ ′ , β ′′  martensitic transformation of copper and gold based alloys [245], using a combined transversal and longitudinal twowave pattern. 2. An experimental verification of the relationship between a twowave pattern and the habits must, in the first step, comprise the determination of the κ  parameters for a given pairs of waves at MS , as well as the selection of the preferable parameters. Of course it suggests itself to confine our measurements to those velocities of sound (for cubic crystals, at the orientations ∆, Σ, Λ) being sufficient for determination of the elastic moduli. This will then enable us to calculate κ for any given pair of waves. In the second step, it will be possible, by means of a pair of external hypersound generators (ν∼ 109 ÷ 1010 s−1 ), to excite the selected pair of waves in the single crystal. This would raise, during a crystallographic analysis, the probability for discovery of a habitplane (already being known at the outset). It should be noted here that the knowledge on the orientations of propagation and the types of the waves which materialize a thermodynamically relatively stable habit, should make it possible to perform such experiments even with lowpower generators. Moreover, using highpower generators, it should be 159
possible to achieve habits not occurring under natural conditions, in a given type of crystal. For example, a habit (225) in the FeNisystem. Most promising would be an experiment for the case of a parameter κ being close to the critical value κc . This way, using a predetermined orientation of c1 , e.g. c1 k [00¯1], it should be possible to materialize the cases shown in Table 5.3, simply by varying the orientation of c2 . Table 5.3. MillerIndices of some habitplanes formed by a pair of waves, for a variety of orientations of the second wave velocity c2 (c1 k [00¯1]) Orientation of c2 [1 + η1 , 1 − η2 , η] [1 − η1 , 1 + η2 , η] [1 + η1 , 1 − η2 , η] [1 − η1 , 1 + η2 , η]
η −ηc  ≤ η < 0 0 < η ≤ ηc 
Habit (5 + δ1 , 5 − δ2 , 7) (5 − δ1 , 5 + δ2 , 7) (2 + δ1 , 2 − δ2 , 5) (2 − δ1 , 2 + δ2 , 5)
A large variety of possibilities for exertion of direct influence on directed generation and growth of martensitic structures in austenitic single crystals is opened up by the combined application of magnetic, hypersound and conventional treatment. We also want to point at future potential for development of methods with two or three sources of ultrasound aiming at direct control of the direction of crystallization immediately out of the melting (upon cooling) and in the amorphous condition (upon heating), while these methods can be of interest both for stationary as well as for moving waves. In the latter case, it should be possible e.g. to produce of a chessboardpattern structure with alternating amorphous and crystalline regions, by usage of two external sources of perpendicular waves. 3. The attractiveness of the twowave pattern is mainly due to its potential to materially demonstrate the possibility of flexible behavior of a dynamic system, still being able to preserve the conditions for realization of thermodynamically favorable phasecoupling, in spite of variations of key parameters (in our case κe (0)). The materialization e.g. of habit (557) could thus be attained due to the increasing deviation of the orientation of the velocity vector c2 from the direction h110i, occurring coincidentally with an increase of the parameter κe (0). As the energy being released during the transformation serves as the source of a nonequilibrium, those waves producing the most favorable conditions of generation (as needed for preservation of temperatureand chemical potential gradient) will develop and predominate. Due to the continuous feedback effect, the system will enter into a condition enabling it to flexibly follow and adapt itself to the most favorable thermodynamical path, on the one hand, by its ability to tune the spectrum of generated waves 160
(i.e. mode selection), and on the other hand, to select various velocities c2 out from an orientational cone around the h110i axis. Obviously, this point of view is free of contradictions with general thermodynamical reasoning and broadens them by an image of transformation dynamics. 4. Within the approach combining martensite growth with wave generation by nonequilibrium electrons, it is obvious that the conceptual view of nuclear growth can be complemented by means of a solitonlike description of the motion of the phaseboundary, as the conditions required for their generation (i.e. temperature and chemical potential gradients) exist in the proximity of the boundary. The most important results relating to an interpretation of morphological characteristics of martensite, within the frame of a wavepattern, have been published in [99], [56], [246–248]. The redistribution of electrons during the development of ferromagnetic ordering within a singlepeak DOS environment is discussed in [216, 217], the results of which were used in [124].
161
Chapter 6 Wavemodel of motion for a martensitic lattice boundary The wave model under development for reconstructive martensitic transformations is essentially based on the conceptual view of the stage of growth of the new phase as a lattice deformation propagating in a wavemode. As already discussed in Chap. 1, there exists sufficient experimental evidence for a metastable condition in the lattice of the premartensitic γ  phase at MS temperature. This means the transition into the new lattice structure is inevitably associated with the need to overcome the interfacial energy barrier, for any degree of supercooling, only becoming possible if the magnitude of lattice deformation ε exceeds a given threshold value εth (MS ). In our wavemodel, we got ε = 4 uλ−1, where u  waveamplitude and λ  wavelength, further assuming εth (MS ) ∼ 10−3. Under a condition of strongly pronounced supercooling, the transformation of the austenitic lattice is associated with release of transformation heat and with a sudden (jumplike) increase of volume. From the outset, the emerging martensite crystal exerts a thermal, electrical and mechanical influence on the interfacial region Bγ−α between the phases, thereby causing a deviation of the local thermodynamic state from equilibrium conditions. Under such nonequilibrium conditions, amplification of atomic oscillations is generally possible, through the generation and selective amplification of displacementwaves by means of nonequilibrium electrons (i.e. instability of lattice oscillations by phononmaser action). The displacement waves in turn ensure a latticedeformation close to thresholddeformation. With regard to the aforementioned, it is obvious to consider the nonequilibrium region Bγ−α as an active and highly excited medium, being capable to generate, preserve and amplify cooperative waves, which in turn induce a transition at ε ∼ εth (MS ). This way the phononmaser effect can be defined as an effect based on positive feedback, by conversion of a fraction of the released transformation energy into the energy of displacement waves. Further surmising that these waves in turn ensure the overcoming of the energetic barrier, then it is conclusive to interpret martensitic lattice growth as a selfsustaining 162
wavelike process, during which the transforming Bγ−α region propagates in conjunction with lattice displacement waves.
163
6.1
Coordinated propagation of a displacementwave with a switchingwave of chemical potential or temperature
We designate in general by a vector u the displacement of atoms participating on an arbitrary wave motion in a nontransformed lattice area. Let us further theorize that the wave is longitudinal with wavelength λ = 2 π/q >> a, where a  latticeparameter; q  modulus of the wavevector q. Then, in a continuous lattice model, we can express the equations of motion for displacements u in the following way, using a frame of reference where the xaxis is collinear to u: u¨ − c2 u′′xx = χ c u′x, χ = −κq
(6.1)
(
−1 ) σ0 G2e tσ ′ 2 1− 1 + 2 (ux + q 2 u2 ) . σth ~ Γe
(6.2)
Here, c  velocity of sound; κq  waveextinction without phonongeneration; tσ period for emergence of an occupational inversion σ0 ; σth  thresholdinversion; Γe  extinction of electrons active during generation; Ge  resonance overlap integral, which determines the width of an electronic band in tight binding approximation. Eq. (6.1) can most easily be derived by confining our consideration of phonon generation to singlemode (related to the case of perfect resonance) and to adiabatic approximation, leading to Eq. (3.49) for slowly varying phononfield amplitudes ˜b+ , ˜bq . The expression of effective extinction (6.2) is the same as in (3.49). The q transition to expression (6.2) can easily be performed by insertion of the explicit form (2.4) of matrixelement W1 in (3.49), using the relations ˜b+ q
M N ωq ≈ 2~
12
˜bq ≈ M N ωq 2~
exp [−i(ωq t − q x)]
12
u˙ +u , i ωq
u˙ exp [i (ωq t − qx)] u − , i ωq
∂u ≡ u˙ ≈ −c u′x ∂t ˜ for the transformation of ˜b+ q , bq in (3.49). Eq. (6.1) can be resolved, provided the class of relationship among the parameters appearing therein and the parameters x and t can be substantiated. Most important is the relationship σ0 = σ0 (x, t), whereas the relationships of the remaining parameters (c, κq , σth , tσ , Γe , Ge ) with x and t is more or less irrelevant and can thus be ignored, without introducing any significant error. According to (3.23), (3.24), the quantity σ0 (x, t) implicitly also depends on local temperature T, 164
chemical potential µ and on their local gradients. Assuming steady motion of the phaseboundary with a velocity V ∼ c, then it suggests itself to describe temperature and chemical potential by means of ”solitary fronts” which propagate with the velocity of sound: i.e. switchingwaves (see e.g. [80, 249]). Thus the frontal width l of such a switching wave practically determines the thickness of the transforming region Bγ−α , being characterized by highly pronounced gradients ∇T , ∇µ, −1 which in turn satisfy the thresholdconditions D0 ≡ σ0 σthM − 1 > 0 for phonon generation. Taking this into proper consideration, we can assume σ0 = σ0 (x−Vt). As the amplification of a displacementwave only is possible within the region of Bγ−α , propagating at velocity V, a coordinated propagation of stationary switching waves and displacement waves can only be realized if V = c. Taking this for granted, then we can search the solution of Eq. (6.1) in form of expression u = u(x − c t) ≡ u(ξ).
(6.3)
After insertion of (6.3) in (6.1) we get a set of equations ∂u = 0, ∂ξ
∂u ∂ξ
2
+ q 2 u2 −
D0 (ξ) = 0, β0
(6.4)
where β0 = ~−2 G2e tσ Γ−1 e . The first equation in (6.4) delivers a trivial solution, not matching with our expected spatially inhomogeneous distribution of local displacement at the starting moment. Solutions of the second equation of (6.4) only exist for D0 ≥ 0, i.e. in the Bγ−α region. If we characterize the region of Bγ−α by means of inequalities −l ≤ ξ ≤ 0, further assuming that T and µ linearly depend on ξ  within the Bγ−α region  then we can use the following expression for D0 ξ ∈ [−l, 0]; const1 ≥ 0, D0 (ξ) = (6.5) const2 < 0, ξ∈ / [−l, 0].
Thus the solution of the second equation in (6.4), being confined to the region Bγ−α , will look as follows: 1 u (ξ) = q
D0 (ξ) β0
12
sin (q ξ + ϕ).
(6.6)
The value of the phaseterm ϕ in (6.6) can be determined from the additional conditions imposed on u at the starting moment t = 0, at the boundaries of the segment [−l, 0]. Solution (6.6) is based on the requirement of equality of the velocities of the displacementwave and of the switchingwaves for T and µ. Within this context it is reasonable to discuss here the limitations imposed on our modelparameters by the above requirement. According to [80], a switchingwave can be defined by a nonlinear equation of the diffusiontype: 165
′′ ψ˙ = F (ψ) + d ψxx ,
(6.7)
where d  diffusion coefficient, ψ  dimensionless variable of the type ψ = ψT = (T −Tγ )/(Tα −Tγ ), or ψ = ψµ = (µ−µγ )/(µα −µγ ) and F (ψ)  nonlinear function. Assuming that F (ψ) ≥ 0 and Eq. F (ψ) = 0 only has two solutions, namely ψ = 0 and ψ = 1, corresponding to the values of ψ in the γ  and α  phases, then we get for velocity V [80]:
1 dF ′ 2 2 (d Fψ (0)) = 2 d dψ
ψ=0
21
≡ Vmin ≤ V.
(6.8)
In accordance with (6.8) the equality V = c is possible for Vmin ≤ c. We estimate Vmin by assuming that Vmin 6= 0. For it, F (ψ) must be materialized. A function F (ψ), being compatible with the conditions F (0) = F (1) = 0, Fψ′ (0) 6= 0, can always be expressed in the form F = τ −1 ψ (1 − υ(ψ)),
(6.9)
where υ(ψ) = 1 only for ψ = 1 and υ(0) = 0, τ  constant with temporal dimension. It follows from (6.9), that Fψ′ (0) = τ −1 and Vmin = 2(d/τ )1/2 : Vmin = 2
dT, µ τ
12
.
(6.10)
In the case of a temperaturewave (Twave) the coefficient d ≡ dT is the temperature conductivity (dT ∼ 10−5 m2 s−1 for ironalloys). In the case of chemical potential (µ  wave), the coefficient d ≡ dµ can be determined in accordance with (3.46) by means of the specific conductivity σγ in the form of dµ =
2 σγ µγ 3 e2 nγ
and dµ ∼ 4 · 10−4 m2 /s.
Let us come back to the condition V = Vmin = c and estimate τ from (6.10) for c = 5 · 103 m/s. This delivers τ ≡ τT ∼ 2 · 10−12 s, τ ≡ τµ ∼ 6 · 10−11 s. Using a linear approximation for the profile of the frontal region of the switching wave, we get for l the following relationship with τ , using the condition Vmin = c: l = A τ c, where A  a figure not larger than a few units, depending on the form of expression υ(ψ) in (6.9). For υ(ψ) = ψ, e.g., we have A = 4, according to [249], thus l = lT ∼ 4 · 10−8 m or l = lµ ∼ 10−6 m, respectively. Taking into account that the optimum size of the region being deformed by the displacementwave corresponds to λ/2 in the wave model, then we can assess the minimum value q in (6.6) using the relation l ∼ λ/2 = π/q: q = qT ∼ 10−2 π/a for l = lT and q = qµ ∼ (10−4 ÷ 10−3 )π/a at l = lµ . 166
Strictly speaking, expression (6.5), when used for resolving (6.4), would require the following form of the function ψ: ψ = θ(−η − 1) − η [θ(η + 1) − θ(η)], η=
(6.11)
(x − c t) ξ ≡ , l l
which will only be satisfied after replacement of expression (6.9) for F (ψ) by a rectangularly shaped pulsefunction: F (ψ) =
1 θ (ψ) θ (1 − ψ). τ
(6.12)
In (6.11), (6.12) the function θ  Heaviside unitfunction: 1 , ψ > 0, θ (ψ) = 0 , ψ < 0. Such an approximation of the wave profile and of F (ψ) should be fully satisfactory for a qualitative consideration, after having determined the speed of propagation of the switchingwave.
6.2
Coordinated propagation of a pair of displacementwaves with the switchingwave of T (µ)
Let us extend the results of Pt. 6.1 to the case of a pair of longitudinal waves propagating with the velocities c1 and c2 in noncollinear directions of axes x1 and x2 , in that we surmise, as done in Chapter 5, that the formation of a martensite lamellae of thickness ∼ λ1 , ∼ λ2 (λ1,2  wave lengths) is performed by the association of the areas subjected to synchronized tensile and compressive stress, the main axes of which being oriented parallel to x1 and x2 , respectively. If we start our conceptual view with a pair of waves of type (6.6), featuring infinite flat fronts, it will be obvious that the specific region in which the combination of tensile and compressive stress being required for a martensitic transformation (also combined with the release of transformation energy) is granted, is identical with the region of waveimposition, propagating in the same direction and with the same velocity c = c1 + c2 (if c1 ⊥ c2 ), that is the line of intersection of the (perpendicular) wave fronts. Consequently, the stationary wave pattern must correspond with the region Bγ−α bound in both x1 and x2 directions and moving with velocity c. In other words, a stationary propagation of the pair of displacementwaves in cooperation with the switching wave is feasible, if the latter one propagates with a velocity V 167
= c = c1 + c2 . This also means that, in the case of a displacementwave, the requirement V = c is to be replaced by the requirement Vx1 = c1 , Vx2 = c2 . Within our following considerations, the actual orientation of the axes x1 and x2 will be of no fundamental importance. Thus we shall further on consider x1 ⊥ x2 . With consideration of (6.6) it is possible to note the expression for the displacements ui , with i = x1 , x2 in the form 1 ui = qi
D0 i β0 i
12
sin (qi ξi + ϕi ).
(6.13)
However, the term D0i already depends on two variables ξ1 = x1 − c1 t and ξ2 = x2 − c2 t, as the region of Bγ−α , in which D0 i > 0, is in simultaneous motion both in the x1  and x2  directions, while featuring limited dimensions ∼ l1 , l2 in both directions. This means that each of the expressions (6.13) describes a stationary wave bundle moving together with the switching wave. The most simple switchingwave model (see Fig. 6.1), corresponding to the wave beams (6.13), can be prescribed by the expression c2 c2 c1 ψ = 1 + η2 − θ(η2 ) θ − η1 − η2 − 1 + θ η2 + c1 c2 c1 c2 c1 c2 + 1 − η2 θ − η1 + θ(η2 ) − θ η2 − η2 − 1 − c1 c1 c2 c1 c2 η2 + 1 − θ − η1 + η2 − 1 , − η1 [θ(η1 + 1) − θ (η1 ) ] θ η1 + c1 c2 (6.14) η1 = (c1 ξ1 + c2 ξ2 ) d˜−1 ,
η2 = (c2 ξ1 − c1 ξ2 ) d˜−1 ,
where d˜ = c1 l1 + c2 l2 ; the coordinates η1 , η2 are mutually perpendicular and located in the plane ξ1 and ξ2 , where the axis η1 is oriented parallel to V. If the definition of the Heaviside θ  function is taken into consideration, it will be easy to understand that the first row of Eq. (6.14) describes the distribution of the reduced temperatures (chem. potentials) ψ in the region OA3 A1 A′1 , the second row in the region OA3 A2 A′2 , and the third row in the region A1 O1 A2 A3 as illustrated in Fig. 6.1. Put in another way, (6.14) is subdivided into terms corresponding to the flat sectors of the triclinic surface ψ. The peripheral points of the plane (x1 , x2 ), supposed to be reached by the switchingwave at an instant t, are the points of segment A1 A2 of the straight line η1 = 0 (see Fig. 6.1) on which ψ = const = 0. Consequently, this segment belongs to the switchingwave front (note that in an orientation perpendicular to x1 and x2 , the switchingwave front is unlimited). The velocity of motion of the points belonging to the segment A1 A2 , related to the frame of reference x1 , x2 , is easy to find, after having noted that the conditions η˙ 1 = 0, η˙ 2 = 0 are 168
ψ
1 A′2 ψ x1
O
A′1 A2
A3
c~1
x2
η2 ξ1
O1
c~2
A1 ξ2
~c η1
Figure 6.1. Model of a switchingwave propagating in conjunction with two wavebeams. The coordinates of the points are: A1 : (η1 = 0, η2 = − c1 /c2 ), A2 : (η1 = 0, η2 = c2 /c1 ), A3 : (η1 = −1, η2 = 0); further explanations are given in the text. satisfied for any point of segment A1 A2 , from which it can be concluded that  in the frame of reference x1 , x2  the velocity r˙ of the wavefront is equal to V = c1 + c2 . Obviously, for η˙ 2 → ±0 the expression (6.14) transforms into (6.10). Then it will be possible to determine the expressions for the time τ and the coefficient of diffusion d, assuming that the quantity V = (c21 + c22 )1/2 corresponds to the minimum velocity of the switchingwave 2 (dτ −1 )1/2 , and by consideration of the relationship ψ˙ = ψη′ 1 η˙ 1 = −η˙ 1 = τ −1 , resulting from (6.7), (6.10) and (6.11), where ˜ η˙ 1 = − c2 /d: d˜ 1 1 ˜ , d = V 2 τ = d. (6.15) 2 V 4 4 For a given d, relationship (6.15) delivers the connection between l1 and l2 , and thus also among the lengths of the displacementwaves, propagating along the x1 and x2 directions, because l1 ∼ λ1 ∼ q1−1 and l2 ∼ λ2 ∼ q2−1 . Finally we have to note that, within the notion of a solitary wave front separating regions with different stationary values of T and µ, the description of T and µ only is an approximation, as the diffusionprocesses proceeding perpendicular to V will modify the profile of a twodimensional wave with increasing time. Thus the real profile of the T  and µ  waves would only feature a shape near their τ=
169
stationary value if they were located close to the Bγ−α region.
6.3 6.3.1
Stationary wave of relative spatial deformation ε˜ during the γ − α  transformation ε˜  triggerswitching displacementwaves

wave
in
absence
of
The displacementwaves generated in the Bγ−α region ensure the lattice deformation required for a cooperative overcoming of the energythreshold separating the structural α and γ states. These structural α  and γ  states are characterized by different values of static (permanent) displacements. However, the states of the α  and γ  phases feature different T , µ  values, a fact not having been explicitly considered in our previous treatise. We shall now focus our analysis on the static deformations and only consider the relative change of volume during the transformation or, put in other words, characterize the γ  and α  phases by their relative volume deformation ε˜, where ε˜γ = 0 and ε˜α = 2, 4 · 10−2, being a value typical of the volume effect of the Baindeformation (see also Pt. 1.4). The tildesign (∼ ) is introduced to distinguish the relative volume deformation ε˜ from the associated linear deformation ε being produced by a displacementwave. In a system comprising two stable states (˜ ε = ε˜α , ε˜ = ε˜γ ), being separated by certain barrier, the propagation of a triggerswitching wave (TSW) is possible in principle [80, 250]. However, for its generation, an initial level of excitation (˜ ε = ε˜0 ) is required, which must at least exceed the thresholdvalue (˜ ε = ε˜th ). It is also known that an ε˜  wave of the triggering type, propagating along the xorientation, satisfies the relationship ε˜˙ = dε˜ ε˜′′xx + F (˜ ε),
(6.16)
for which, in contrast to (6.7), the nonlinear function F (˜ ε) for ε˜ = ε˜γ = 0, ε˜ = ε˜th > 0, ε˜ = ε˜α > ε˜th must vanish. The most simple expression for F (˜ ε) thus may look as follows: 1 ε˜ (˜ ε − ε˜th ) (˜ ε − ε˜α ), (6.17) τε˜ where τε˜  constant with the dimension of time. The stationary solution ε˜ = ε˜ (x − Vε˜ t) ≡ ε˜ (ξ) of waveequation (6.16), comprising a nonlinearity (6.17), will look as follows: F (˜ ε) = −
ε˜ =
1 ε˜α [1 − tanh (2 ξ lε−1 ˜ )], 2
(6.18)
1 4 (2 dε˜ τε˜) 2 . ε˜α
(6.19)
lε˜ =
170
In contrast to the T  and µ  waves  resembling so called phase  switching waves (PSW) [250]), which dispose of a velocitycontinuum V ≥Vmin  a TSW only features a single (discrete) velocity: Vε˜ =
dε˜ 2 τε˜
12
(˜ εα − 2 ε˜th ).
(6.20)
In order to interpret these results, we recall that Eq. (6.16) can be expressed in the notation of the LandauHalatnikovEqaution (see e.g. [251]): δΦ ε˜˙ = − Γ , δ ε˜ where Γ  kinetic coefficient (not to be confounded with electronextinction); Φ fraction of free energy depending on ε˜; δ Φ/δ ε˜  functional derivative of Φ by ε˜, ( 2 ) Z 1 1 ∂ ε˜ A 2 1 , (6.21) ε˜ + B ε˜3 + G ε˜4 + P Φ= dV 2 3 4 2 ∂x where A/G = εth ε˜α , B/G = − (˜ εα + ε˜th ) , ΓG = τε˜−1 , Γ P = dε˜. Our model (6.21) for Φ represents a 1st order phase  transformation, because A > 0, B < 0, G > 0. If, in addition, dB/dT < dA/dT < 0, then the elastic moduli will feature a normal temperature dependence during cooling, ε˜th and the level of the energythreshold Φ0 (˜ εth ), which separates the states ε˜ = ε˜γ , ε˜ = ε˜α , will subside and remain a finite quantity. If we use the notation Φ0 for Φ at ∂ ε˜/∂ x = 0, and consider that Φ0 (˜ εγ ) = 0,
Φ0 (˜ εα ) =
Φ0 (˜ εth ) =
V A ε˜α2 (2 ε˜th − ε˜α ) , 12 ε˜th
(6.22)
2 V A ε˜th (2 ε˜α − ε˜th ) , 12 ε˜α
where V  volume of the system, it becomes obvious from (6.20) and (6.22), that Vε˜ ∼ (Φ0 (˜ εγ ) − Φ0 (˜ εα )), being proportional to the drivingforce of the transformation, and Vε˜ = 0 at T = T0 , being corresponded by the value of ε˜th = 1/2 ε˜α. We should however remark that, in order to excite a TSW, being in motion with nonvanishing velocity Vε˜ at a temperature T near T0 , there would be required large initial values of ε˜0 of about ∼ 1/2 ε˜α. The frontal width lε˜ of a TSW, as defined by (6.19) (with linear approximation of its profile), is determined by parameters A and P in the function (6.21), in the form lε˜ = 4
2 ε˜th P A ε˜α
171
21
.
(6.23)
To perform an evaluation of lε˜, let us first express P by means of the specific surfaceenergy Es and A by the additional assumption
Es =
Z∞
dx P
−∞
∂ ε˜ ∂x
2
.
(6.24)
After substitution by (6.18) in (6.24), and with consideration of (6.23) we get: 1 Es = 6
ε˜α P A 2 ε˜th
21
ε˜α2 ,
(6.25)
i.e. P = 72 Es2
ε˜th . A ε˜α5
Using (6.22), we can express ε˜th by the following notation: "
∆Φ0 ε˜th = A˜ εα3 2 A˜ εα2 − 12 V
!#−1
.
(6.26)
According to the calculus in [58], it is justified to assume for the γ − α  transformation of ironbased alloys: ∆Φ0 (MS )/V ≈ (4/3) Q, where Q  specific reactive heat (it will be surmised that one fourth part of ∆Φ0 /V is needed for the formation of the phaseboundary, thus providing an explanation for the factor (4 / 3) associated with Q). E.g. for the alloy H30: Q ≈ 3 · 108 J m−3 [22]. Thus we get for A ≈ 2 · 1011 J m−3  being a typical value of the compressive modulus  from (6.26): ε˜th ≈ 5, 4 · 10−4. Taking a value of 0,2 J m−2 for Es [252], we can determine from (6.25) and (6.23): P ≈ 10−6 J m−1 , lε˜ ≈ 1, 9 · 10−9 m ≈ 5 a, i.e., the width of the front lε˜ is about 5 times as large as the latticeparameter of the γ  phase. Some additional remarks: 1. The data presented in [252] mainly relate to the surface energy of a static phaseboundary, whereas, in our above compilation of Es , we used the solution (6.18) pertaining to a moving phaseboundary, which, strictly speaking, would only be justified for the case of a temperature close to T0 , and with Vε˜ ≈ 0. In case of an arbitrary temperature, the value Es of a static phaseboundary can however be calculated using the general approach related to 172
the determination of the boundary energy of a ferromagnetic domain in [71]: Es =
! 21 ( p ε2α PA 6 2 (n − 1) (n2 − n + 1) − 2 27 n2 p 2 3 (n − 2) (n − 2) (n − 1) + √ (2 n − 1) (n − 2) (n + 1) × − n ) 2 (2 n − 1) + 3 p2 n (n − 1) p × ln (6.27) n − 2 + 3 n (n − 2)
where n = ε˜α ε˜th . A comparison between (6.27) and (6.25) shows that for T = T0 , (˜ εα = 2 ε˜th ), (n = 2) the expressions for Es match, as required. For T = MS , if n >> 1, we get from (6.27):
Es
( 1 √ √ (P A n) 2 2 √ ε˜α 6 2 − 3 + ≈ 27 2 ) 4 + 3 √ 2 1 + 4 ln √ ≈ 0, 3 (P A n) 2 ε˜α2 , 3+1
(6.28)
being about 2,5  fold larger than the result obtained from (6.25). Thus we obtain with Es ≈ 0, 2 J m−2 the values P ≈ 4 · 10−7 J m−1 and lε˜ ≈ 2 a. 2. In the papers [17, 19], dealing with Es , a ratio of Φ0 (˜ εth ) lε˜, V was used, which can also be expressed by Es ≈
1 Es ≈ 3
P A ε˜th ε˜α
21
ε˜th 2− ε˜α
2 ε˜th ,
(6.29)
after consideration of (6.22), (6.23). At T = T0 , ε˜α = 2 ε˜th , Eq. (6.29) realistically delivers the order of magnitude of the quantity Es , however at T = MS and ε˜α ≥ 10 ε˜th , the ratio between Es , as determined from (6.25) or (6.27), and the value of Es derived from (6.29), is of an order of magnitude of (˜ εα /2 ε˜th )3 ≥ 104 , thus we can conclude that the assessment from (6.29) is not realistic in principle. 3. If the motion of the phaseboundary resembles a thermally activated process, being controlled e.g. by a diffusionprocess, then the quantities Vε˜ and thus also Γ, dε˜ and τε˜ should exhibit a strongly pronounced (exponential) dependence on temperature. 173
4. In order to determine Γ, dε˜ and τε˜ by means of our model (6.21) of the potential Φ, it should suffice to know the experimentally determined value Vε˜ , provided the quantities A, ε˜α , ε˜th , P are previously given. We shall use the expressions suffixing Eq. (6.21), and write Vε˜ in the form
Vε˜ = Γ
PA 2 ε˜th ε˜α
12
(˜ εα − 2 ε˜th )
(6.30)
thus highlighting the proportionality between Vε˜ and Γ. 5. Besides the potential (6.21) there is frequently used a potential which only depends on even powers of ε, i.e. ε˜ 2 , ε˜4 , ε˜6 . In this particular case, being qualitatively analogous to that relating to (6.21), it is easily possible to perform a consideration of the triggeringswitching wave (TSW), using the results of [253].
6.3.2
Effect of the displacementwaves on the velocity of the ε˜  switchingwave
The relationship between the velocity Vε˜ and the temperature, in conjunction with the parameters included in (6.20), is not typical of the γ − α  MT. That is no surprise, as the mechanism being responsible for the cooperative character of the transformation is not expressed explicitly neither in Eq. (6.16) nor in Eq. (6.21). In the twowave model however, the cooperative nature of the latticetransformation is linked up with displacementwaves, which, during their propagation, ensure the attainment of the thresholddeformationlevel in the Bγ−α region. As soon as this thresholddeformation is surpassed, irreversible deformations up to the value of ε˜ = ε˜α will be produced, resulting in the development of an ε˜  wave. Obviously, this conceptual view of martensite crystal growth must take for granted the motion of the ε˜wave into xdirection with a velocity c, being equal to the geometric sum of the velocities of each individual displacement wave. That becomes a possibility when, as a result of the interaction of the ε˜  TSW and the displacement waves, the ε˜  TSW is converted into a wave featuring more than one discrete velocity Vε˜, i.e. a velocity continuum, like a PSW. In mathematical terms, the effect of the displacement waves at the points of the Bγ−α region is expressed in such a way that there occur in sequence the events of approaching, confluence and finally, of disappearance (socalled ”FoldingCatastrophe” [254]) of two singular points ε˜γ and ε˜th . As a result, only a singular stable point ε˜α will remain, to which the system tends (see Fig. 6.2). In the latter case, the ε˜  wave can generally propagate with any arbitrary velocity, since the region deformed by the displacement waves becomes unstable against any positive fluctuation. As the aforementioned vanishing process of particular points, propagating with velocity c in space, is caused by the action of 174
3 2 1
ε˜γ
ε˜′γ
ε˜t
ε˜α
ε˜
Figure 6.2. Development of a ”Catastrophe” of the foldingtype: Curve 1 path of the function (6.17) in absence of displacement waves; Curves 2 and 3 are associated with the confluence and disappearance of discrete points ε˜γ , ε˜th , respectively. displacement waves, just this velocity proves to be the only one highlighted in the velocity continuum of the modified ε˜  wave. The vanishing of the discrete points ε˜γ and ε˜th of the function F (˜ ε) can be taken into consideration by adoption of an addend of the ”fieldtype” in (6.21): −˜ σ (˜ εu ) ε˜, where σ ˜ (˜ εu )  pressure and ε˜u  volume deformation associated with the displacementwaves. If we further infer that σ ˜ (˜ εu ) = K ε˜u , with K > 0, and equalize the conditions for confluence ′ ε˜γ , ε˜th → ε˜γ = ε˜′th ≈ ε˜th /2 of the discrete points ε˜γ and ε˜th with the condition ε˜u = ε˜′γ , then we can determine K = A/2. Thus, within the framework of our considered model, ε˜th (MS ) = ε˜′γ ≈ ε˜th /2. This way our consideration of displacement waves, which ensure the cooperative lattice transformation in the growthstage, leads to a conceptual view of the motion of the martensite latticeboundary with a velocity c, only weakly depending on T , its magnitude corresponding to that of the velocity of sound. More than that, if c is the geometric sum of c1 , c2 , than c can even exceed the velocity of sound in the direction given by c. We recall that supersonic speed of growth has been observed during the passage of a detonation wave through steel [30, 31].
6.3.3
The ε˜  ModifiedSwitchingWave
Let us now consider in more detail the ε˜  ModifiedSwitchingWave (˜ ε  MSW), related to the case of the confluence of the discrete points ε˜γ , ε˜th (Curve 2 in Fig. 6.2): ε˜γ′ = ε˜t′ ≈ ε˜th /2. Such a wave can generally be described by an equation of the form 1 ′′ ′ 2 ε˜˙ = dε˜ ε˜xx + (˜ ε − ε˜th ) (˜ εα − ε˜) , τε˜ 175
(6.31)
in which, by way of contrast to (6.16), the nonlinear function F (˜ ε) only features ′ two values ε˜th , ε˜α , corresponding to the requirement F (˜ ε) = 01 . Let us now introduce the designations Z=
′ ε˜ − ε˜th , ′ ε˜α − ε˜th
τ˜ =
τε˜ , ′ 2 (˜ εα − ε˜th )
(6.32)
12
(6.33)
and a dimensionless time t˜ and spatial coordinate x˜: t t˜ = , τ˜
x˜ = x
Then we can write Eq. (6.31) in the form
1 dε˜ τ˜
.
Z˙ t˜ = Zx˜′′x˜ + Z 2 (1 − Z) .
(6.34)
Z (ξ) ≡ Z x˜ + c˜ t˜ ,
(6.35)
The solution Z is of the travellingwave type Z = Z(ξ)
where c˜  dimensionless wavevelocity
c˜ = c corresponds to the equation
τ˜ dε˜
12
,
(6.36)
Zξ′′ξ − c˜ Zξ′ + Z 2 (1 − Z) = 0.
(6.37)
ϕ = −˜ c Zξ′
(6.38)
In case of large values c˜ 2 >> 1 it is possible to use a simplified procedure for resolving Eq. (6.37), by introduction of a row of additive terms with increasing powers of the small parameter c˜−2 . This procedure is described in detail in [249]. Taking the velocity c = c1 + c2  as given (see Pt.6.3.2) and the condition c˜2 >> 1 as satisfied, then we will be able to assess the frontal width of the ε˜  SW. Following [249], we designate
and transform (6.37) into the coordinate frame of a phase plane: 1 dϕ ϕ − Z 2 (1 − Z) = . c˜ 2 d Z ϕ
(6.39)
Let us now search for a solution of (6.39) in the form of
1
2 ϕ Z, c˜−2 = g0 (Z) + c˜−2 g1 (Z) + c˜−2 g2 (Z) + · · · .
(6.40)
Notice that equation (6.31) has the solution (6.18) for the solitary wave front propagating with velocity (6.20)
176
After insertion of (6.40) in (6.39) and equalizing the terms with identical powers (˜ c−2 ) we get: g0 (Z) = Z 2 (1 − Z), g1 (Z) = g0
d g0 = Z 3 (1 − Z) (2 − 3 Z) , dZ
(6.41) (6.42)
d (g0 g1 ) = 2 Z 4 (1 − Z) (1 − 2 Z) (5 − 6 Z) . (6.43) dZ We determine the dimensionless frontal width ˜l of the ε˜  PSW from [249] by the ratio g2 (Z) =
˜l ∼
1 Zξ′ (Z0 )
,
(6.44)
in which Z0 is a solution of the equation dϕ =0 (6.45) dZ corresponding to the flex point of the function Z(ξ), i.e. Zξ′′ξ = 0 for Z = Z0 . From (6.45) and (6.40)  (6.43) we can immediately find 2 14 −2 + c˜ + O c˜−4 . (6.46) 3 27 After insertion of (6.46) in (6.40), and with consideration of (6.38), we get Z0 =
Zξ′ (Z0 ) = Making use of (6.44), (6.47), we get
1 4 + O c˜−5 . c˜ 27
(6.47)
˜l ∼ 27 c˜. (6.48) 4 If we turn over to dimensional quantities with consideration of (6.36) and (6.33), we get from (6.48) l ∼ 7 c τ˜ =
7 c τε˜ 7 c τε˜ , ≈ 2 ′ ε˜α2 ) (˜ εα − ε˜th
(6.49)
′ in which the condition ε˜th ε˜th , i.e. in the frontal area of the ε˜  MSW. Thus it is justified to introduce the following additional condition: l ∼ lµ ∼ lT ∼ λ/2,
(6.50)
dε˜ P ε˜th ε˜α P ε˜th ε˜α3 = ≈ . τ˜ τε˜ τ˜ A A τε˜2
(6.51)
where λ  length of a displacementwave with magnitude of about (10−7 ÷ 10−6) m. For the aforementioned region of λ we can determine from (6.50) and (6.49) ′ 2 with c ∼ 5 · 103 m/s τε˜ ∼ 2 (10−15 ÷ 10−14 ) s. The time τ˜ = τε˜/(˜ εα − ε˜th ) , which, according to (6.49), determines the frontal width l, is of an order of magnitude of 10−11 s for ε˜α ∼ 2, 4 · 10−2 . Now it is easy to convince ourselves that, for τε˜ ∼ (10−15 ÷ 10−14 ) s, our initial assumption c˜2 >> 1, used for our above analysis, is satisfied. Thus we can also use the relationships linking up the quantities dε˜, τε˜ with Γ, P, A, ε˜α , ε˜th , appearing in Eq. (6.21), to determine
From (6.51), we can determine for P ∼ 4 · 10−7 J/m, A = 2 · 1011 J/m3 , ε˜th ∼ 10−3 , ε˜α ∼ 2, 4 · 10−2 , τε˜ ∼ (10−15 ÷ 10−14 ) s the value of dε˜/˜ τ ∼ (102 ÷ 104 ) m2 /s2 . Then we obtain from (6.36) the quantity c˜ 2 for c ∼ 5 · 103 m/s, delivering c˜ 2 ∼ (105 ÷ 103 ) >> 1. Remarkably, for the same values of P, A, ε˜t h, ε˜α , and τε˜ ∼ 10−14 s, we obtain a kinetic coefficient Γ ∼ 10−2 m3 /(J s), and then, in accordance with (6.30), the velocity of the TSW Vε˜ ∼ 10 m/s is almost three orders of magnitude smaller than the speed of growth of a martensite crystal. Large values of c˜ 2 justify the omission of two addends of an order of magnitude of c˜−2 and, all the more, those of an order of magnitude of c˜−4 , c˜−5 appearing in Eqs. (6.47), (6.46) without introducing any significant error. This also means that, when breaking down Eq. (6.40), it is justified to confine our further analysis to the first addend. This approximation corresponds to an omission of the second derivative Zξ′′ξ in Eq. (6.37). After elementary integration of Eq. (6.37) we are able to find the expression defining the shape of the ε˜  modifiedwave: Z ξ . (6.52) = exp (1 − Z) exp (Z −1 ) c˜ 178
Z 1
10
5
l˜
0
5
10
ξ/˜c
Figure 6.3. PhaseSwitchingWave (PSW) profile of relative volume deformation. As a result of (6.52), we obtain Z → 0 for ξ → −∞, and Z → 1 for ξ → +∞. Fig. 6.3 shows the profile of the ε˜  wave, as obtained from Eq. (6.52), as well as the width ˜l as obtained from Eqs. (6.44) and (6.48). It is obvious from Fig. 6.3 that the waveprofile is asymmetric in relation to the point with coordinates Z = 1/2, ξ/˜ c = −2, which does not correspond to the flex point (Z = 2/3, ξ/˜ c ≈ −0, 807) of the function (6.52), and is characterized by a more moderate variation at Z → 0 in relation to a variation at Z → 1. This in turn justifies to some degree the usage of the bandstructure of the fccphase of iron for an analysis of the conditions for displacementwave generation.
6.4
Summary of Chapter 6
Let us summarize as follows: 1. Within the framework of the wavemodel, our qualitative approach as proposed in Chap. 6 is mainly based on the presumption that several of the mutually  connected processes, which are propagated in a wave regime, determine the growth mechanism of martensite crystals. 2. In the particular case of missing atomic displacementwaves, the width of the moving boundary between the adjacent phases is mainly determined by the frontal width lε˜ of the ε˜  TSW, corresponding to some latticeconstants. In the case of nonvanishing atomic displacementwaves, which ensure the required thresholddeformation, the ε˜  wave transforms into a modifiedswitching wave of frontal width l, being characterized by a displacementwavelength λ. For λ/2 ∼ (10−7 ÷ 10−6 ) m, the quantity l is about two to three orders of magnitude larger than lε˜. The region Bγ−α , comprising 179
highly pronounced inhomogeneities of temperature and chemical potential, basically corresponds with the frontal structure of the modified ε˜  wave. The complicated structure of the waveprocess justifies the introduction of the special term ”transformationwave”, closely related to the growth stage of martensite, also having been used in [77], but without specification of the wavestructure. 3. The cooperative character of the structural transformation, being the most typical phenomenological feature of martensitic transformations, is ensured by a phononmaser effect occurring in the Bγ−α  region, which transforms a fraction of total reaction energy into energy of the atomic displacement waves. 4. The specification of the pattern of growth control of a martensite crystal by a pair of waves, as developed in Chap. 5, is reduced with the replacement of the lattice displacement waves with infinite frontal dimensions by wavebeams. The notion of wavebeams, i.e. of displacementwaves with finite frontal dimensions, suggests itself for the description of the growth process of a cylindrical macronucleus (see Pt. 1.3), whose lateral dimension will just determine the minimum dimension of the wave front. 5. In order to provide further evidence for our interpretation by the notion of wave beams, it may be of crucial interest to investigate how efficiently crystalgrowth can be stimulated by means of two external sources of hypersound, and its relationship with the dimensions of the wavefront sources, with the aim of an improved specification of the transformation pattern treated in the final part of Chap. 5. In particular, getting over to closely located and properly oriented linear emitters with lateral dimensions of about ≤ 10−6 m might make possible the simulation of a generation mechanism with longwave components of the displacement waves, during the development of a single nucleus. It cannot be excluded that a single linear emitter (with the special orientation) may be a successful tool for simulation of the development of a single cylindrical macronucleus. It is obvious from the description of the habits near {557}, {225} in the twowave pattern that, in order to excite waves propagating near the axes h00¯1i, h110i, the emitter must be oriented in the direction of h1¯10i, lying in the habitplane. The success of such an experiment might be evidenced by the emergence of crystals with a limited choice of habits (i.e. from 1 to 4) of the type (h ± δ, h ∓ δ, ±l) with δ < 1. Such result would testify the benefit of nucleation of the martensitic crystals in elastic fields of dislocations with typical Burgersvectors of fcclattice structures. It would also be promising to try to simulate the process of energy irradiation during the nucleation process, by means of narrow (with lateral dimensions of about ∼ 10−6 m) 180
directed electron, ion or photon beams, with a profile ensuring a linear trace of interaction on a single crystalsurface, with a period of interaction of ti ∼ 10−10 ÷ 10−11 s. 6. The mutual interaction of wave beams among themselves and with PSW of the T  or µ type is expressed by the requirement of their coordinated propagation, i.e. V = c = c1 + c2 . 7. In the case of the γ −α  MT, the volumetric effect as well as the macroscopic shear with a typical magnitude of 0,2, serve as macroscopic characteristics. It can however easily be shown that the aforementioned model of thermodynamic potential (6.21), being related to the macroshear, will deliver a thresholdlevel of macroscopic shear exceeding the threshold of volume deformation by one power, even for an Avalue equivalent to the minimum shearmodulus C ′ = (C11 − C12 )/2. Thus it can be expected that macroscopic sheardistortion will only play a subordinate role, in that it would only appear in regions which already lost their stability by volume deformation, due to the action of longitudinal displacement waves. In other words, the relative volumetric change (actually playing the role of an orderingparameter) might be the better choice as a macroparameter. This point of view is close to the position of the author of [77], highlighting the leading role of longitudinal waves during the development of the central zone (the ”midrib”) of lenticularly shaped martensite crystals. 8. In the case of lenticularly shaped martensite crystals, the quantity c determines the greatest (frontal) midribgrowth velocity and thus features an important characteristic of the process. This circumstance implies the requirement for a precise measurement  by more than only of its order of magnitude  of the velocity c by an independent measuring principle. For example, the method described in [27] could be improved by triggering the martensitic transformation of certain specimen exhibiting a pronounced twostage transformation, by means of a strong magnetic field [34, 36]. On the one hand, this would allow a distinguished identification of the first, rapidly processing transformation stage and, on the other hand, a reduction of possible orientations of martensite, by proper consideration of the orientation of the premartensitic austenitic single crystals (see Pt. 5.3.3), in addition to allowing an improved determination of the dimensions of the crystals. Some additional remarks: 1. In [255], the temperaturefield at the boundary of the growing martensitic crystal with the shape of an ellipsoid cylinder with small ratio of the crosssection axes has been treated. The task treated in [255] is like the freezingproblem of humid ground [256]: The equation of heatconduction is devoid 181
of sources, and the speed of boundary motion is assumed to be proportional to the temperaturegradient within the boundary. However, this approach differs remarkably from the one we used. Nonetheless, it is interesting to note that the estimate of the radius of curvature of the martensiteboundary ρ ∼ 10−6 m (as determined in [255]), at which adiabatic crystal growth mode becomes effective, confirms the possibility of adiabatic growth of the cylindrical macronucleus with a radius of an order of magnitude of about 10−6 m. 2. The description of martensitic growth as a latticedeformation process suggests itself as most natural. In our above consideration, we distinguished between the deformation controlling the growth process of martensite, by means of displacementwaves, and the observable macroscopic deformation. Obviously, from a phenomenological point of view, this interpretation represents one of some possible variants of description, within the framework of a pattern of cooperating micro and macroscopic ordering parameters [1]. We also drew the attention to [257], focusing on the selection of an orderingparameter not being deducible to the observed macrodeformation, and on the applicability of a strictionmodel for an interpretation of thermodynamic laws, being typical of thermoelastic martensite. 3. For large propagation velocities of the phase boundary, it is generally required to take into consideration the systematic motion of the electrons with the velocity of local lattice motion analogously to the systematic motion of the electrons with the local velocity of ions in an elastic wave (see e.g. Chap. 3 in [258]). The results published in [29, 259] give evidence for the draggingeffect of electrons by a moving boundary. However it is easy to prove that the contribution of such dragging effect on the occupational inversion would only be of an order of magnitude of ∆σ0 ∼ 10−4 and thus have no appreciable effect on the rate of phonongeneration, as becoming obvious after comparison with the σ0  values in Table 3.1. 4. In addition to the description of the phase boundary by means of a functional of type (6.21) we also would like to draw attention on the work of Lihachev [260], which, within the framework of continuummechanics, suggests to consider boundary layers in the solid state (without specifying their structure) as independent planardefects. The results related to the qualitative analysis of coordinated propagation of switching and displacementwaves, which simulate the motion of the phaseboundary during the γ − α  MT, are published in papers [261–264]. The substantiation of Chap. 6 mainly follows the work published in [262].
182
Synopsis and outlook Based on analysis of experimental data and theoretical notions, a new conceptual approach for the description of rapid (frontal) crystal growth during fcc bcc (γ − α) martensitic transformations in ferrous alloys has been developed. The particularities in the course of this transformation (e.g. supersonic velocity of growth, anomalous magnitude of supercooling below the point of phaseequilibrium, missing phonon mode softening in the temperature region before the onset of a martensitic transformation) are considered as strong evidence for setting off the spontaneous martensitic transformation as a pecular kind of ”limiting case” among diffusionless transformations, contrasting most pronouncedly with the opposed ”limiting case” of structural transformations, described most conveniently under the notion of softphonons. Basically, the martensite growth stage is considered as a process of propagation of lattice deformation, being controlled by wavelike atomic displacements of relatively large wavelengths λ ∼ (10−7 ÷ 10−6 ) m. However, the cooperative character of atomic displacement can only become effective if significant deviations from equilibrium conditions in the subsystem of 3delectrons are present, thus implying the requirement of the existence of 3delectron subsystems embodying a macroscopic number of pairs of equidistant, inversely occupied states. This way, electronic transitions among inversely occupied electronic states lead to the generation of cooperative macroscopic latticedisplacement waves by stimulated emission of phonons (phononmaser effect). Because, from a quantummechanical point of view, the propagating atomic displacement wave represents a macroscopic amount of phonons of nonvanishing frequency, the previously defined notion of martensitic transformations, being essentially based on the propagation of displacement waves, is equivalent to a description within the conceptual framework of ”hard” phonon modes, conforming to the new scientific tendency of theoretical research on γ − α  martensitic transformations. The survey of results presented in the final sections of Chaps. 2 to 6 of this monograph is showing that the tasks determined in Pt. 1.5 have been resolved, at least at a qualitative level. Nonetheless, let us now review once more the most important findings considered essential for the new description of the γ − α martensitic transformation in ferrous alloys, as well as some remarkable quantitative keyevaluations obtained for the stage of nucleation of martensite, as well as some predictions derived from the theory and their future developments, respec183
tively. Most important findings 1. In the stage of rapid martensite crystal growth there exists a boundary area between the phases being characterized by intensive electron currents within coexisting strongly pronounced temperature and even more important  chemical potential gradients. 2. An electronic drift current leads to an inverted occupation of those pairs of electronic states being localized in the proximity of the S  surfaces in quasimomentum space. S  surfaces are defined by the condition that the ~ or ∇µ ~ projection of electronic group velocity towards the orientations of ∇T must vanish at all points of the Ssurfaces. 3. The number of pairs of inversely occupied electronic states of the 3d  bands of iron is a macroscopic quantity. 4. The process of generation of atomic displacement waves is energized by stimulated emission of phonons during transitions of the nonequilibrium 3delectrons between the inversely occupied states. This process is similar to the radiation of photons in a maser. 5. The displacement waves controlling the process of martensitic crystal growth are of the longitudinal type (or quasilongitudinal) with frequencies of ν ∼ 1010 s−1 (region of hypersound) and amplitudes ensuring the required level of lattice deformation of ε ∼ 10−3 needed for initiation of the γ −α  martensitic transformation. The mode of initial excitation of waves during the nucleation stage of the α  phase is a hard mode. 6. Certain combinations of displacement waves are important but not separate waves. Thus for instance, the stage of rapid growth of a martensitic lamellae is correlated with the propagation of a pair of perpendicularly oriented waves, stimulating the process of flat lattice deformation of a combined tensilecompressive type. 7. The displacement waves exist in the shape of the wave bundles propagating in coordination with the spatially limited front of a wave of relative volume deformation and making the function of ”pilotwaves”, paving the way for the martensitic reaction in their wake. Key quantitative evaluations ~ is the main non1. Obviously, the electronic (chemical) potential gradient ∇µ equilibrium source within an electronsubsystem. The assessment of the ~ requires that the difference of chemical phase potentials ∆µ = quantity ∇µ 184
µγ −µα as well as the width l of the region among the phases are known. The value ∆µ ≈ 0, 16 eV has been determined for the s  and d  electron sub systems under Pts. 1.5 and 4.5.3. The quantity l can be assessed by means of Eq. (6.49). Taking into account that the constant τε˜ included in (6.49) plays the role of the minimum timeconstant characterizing the Baindeformation process, it suggests itself to take the physically consistent value τε˜ ∼ 10−14 s, corresponding to the period in which a lattice  atom will be displaced  at nearsound velocity  by a distance of about 0, 1 a (a  latticeparameter). Then we get from (6.49) the value l ∼ 10−6 m and ∇µ ∼ ∆µ/l ∼ 105 eV/m. 2. Within the frame of the proposed wavemodel of martensitegrowth the requirement for satisfaction of the condition σ0 > gth for displacementwave generation, as outlined under Pt. 3.1, attains a key role. An assessment of the inverted population difference of a pair of electronic states, associ~ ated with an electron drift in a field ∇µ, delivers σ0 (∇µ) ≥ 10−3 . The −4 −3 thresholdvalue σth ∼ 10 ÷ 10 had been determined under Pt. 3.1 from Eq. (3.10). After further evaluation of σth , it becomes obvious that the number of pairs of inversely occupied states Rq , being proportional to the area Σq of the reduced sheet of the Ssurface, is of paramount importance. For Σq ≈ 20(π/a)2 , the condition σ0 > σth is satisfied for ordinary values of the matrixelements of electronphononinterection Wq (Wq is taken in the tight binding approximation ). We emphasize that the instability of a metal lattice, being linked up with the amplification of an acoustic wave by the mechanism of stimulated emission of phonons (see e.g. [265]) has generally been supposed as not realizable in metals. 3. The magnitude of maximum lattice deformation εm maintainable in a displacement wave also is of fundamental importance. An evaluation of εm has been performed under Pt. 3.3 by means of Eq. (3.42), being correct for stationary conditions. Using this methodology, a value of εm ∼ 10−3 was obtained for σ0 ≈ 2, 5 σth . The inequality tu >> t∇ , being included in Pt. 3.3, refers to the settling time  tu  of the stationary amplitude (or of the deformation εm ) within the displacement wave. The lifetime of the chemical potential gradient t∇ shows that a usage of the stationary εm  estimate is only justified for a hard mode of wave excitation. With this approach, it is possible to link up the growth of martensite with displacement waves, while we believe that near MS the austenitic lattice remains essentially stable against deformations being less than 10−3 , thus suggesting the following conclusion: the nucleation process of martensite crystals is associated with the hard mode excitation of displacement waves of an estimated strain amplidude εm ∼ 10−3 . 185
4. An evaluation of the threshold value ε˜th (MS ) of relative volume deformation ε˜ at temperature MS also is of crucial importance. The point here is that coordinated propagation of displacement waves with an interphase boundary would only be possible if the relative volume deformation ε˜u within the displacement waves exceeded the value ε˜th (MS ). Otherwise, (˜ εu < ε˜th (MS )), the motion of the phase boundary would be described by a triggeringswitching wave with the sole velocity being distinctly smaller than the magnitude of the sound velocity. In Pts. 6.3.2, 6.3.1, there has been shown that ε˜th (MS ) ≈ 2, 5 · 10−4, so that the condition ε˜u > ε˜th (MS ) is easily satisfied for εm ∼ 10−3 . Proposed experiments for further verification of the growth model 1. Measurement of the contactpotential difference ∆ϕ among the γ  and α  phases (see Pt. 2.5). The value and sign of ∆ϕ are needed to determine the inverted occupational difference σ0 ∼ ∆ϕ, as well as the direction of ~ (see legend of table propagation of the displacement waves in relation to ∇µ 2.1). 2. Measurement of the ratio of the velocity moduli of the longitudinal waves κe = ch110i c−1 h001i in austenite at the temperature MS , as a function of the concentration of the alloying element Cae , in order to check the criterion for the first change of the habitplanes ({557} → {225}). A positive result of the experiments would be an increase of κe with increasing Cae while approaching to the concentration at which the habit {225} obviously becomes stabilized (see Pt. 5.1.3). 3. Precise measurement of the rapid frontal growth velocities of martensite crystals and comparison with the values c ≈ c1 + c2  predicted by theory, while the velocities c1 and c2 could be calculated on the basis of measured elastic moduli of austenite at MS . 4. Observation of oriented growth of the martensite crystals during simultaneous influence of hypersound and strong magnetic fields, as well as of the effects of laser radiation pulses impinging on the surface of a specimen, directed along a trace near to a linear form. We note here that the discovery of a predicted orientational effect in a magnetic field of H ∼ 107 A/m [244], exceeding in order of a magnitude both demagnetization and magnetic anisotropy fields, delivers strong evidence in favor of the masereffect during phonongeneration, and, moreover, confirms our conclusion on the connection of the second change of habit {557} → {3 10 15} in the FeNisystem, and {225} → {259} in the FeCsystem, with exclusion of the quasilongitudinal waves with velocity directions near the secondorder axes of symmetry of the fcclattice from the total spectrum of generated waves. 186
If we mention further research, we want to note, above all, that a comprehensive understanding of the processes occurring in the stage of growth of martensite crystals should also contribute to the definition of physical models of the preceding stage of nucleation, as well as of the subsequent stage of accommodation of the coexisting phases. This way, for instance, the requirement for coordination of the nucleation stage with the growth stage, caused by the nonequilibrium conditions at the interphase boundary and being controlled by displacement waves, will lead to new findings on the rapid emergence of the macronucleus, as treated under Pt. 1.3. Synthesis of concepts of the heterogeneous nucleation and of the wave growth of martensitic crystals The presently achieved success in improved understanding of the nucleation stage can mainly be attributed to the consolidation of the notions of heterogeneous (dislocation) nucleation as well as of the wavecontrolled growth of martensite [266–272]. A calculus of the elastic fields of linear dislocations, being typical of the parent γ phase, have shown that even single mixed dislocations can play the role of nucleation centers (NC) of martensite crystals. NCcharacteristics and macroscopic morphological features of martensite are (genetically) mutually linked up. In result there exist 24 different variants of matching patterns in the ”NCcrystal”. The elastic field of dislocations disarranges the original lattice symmetry by selecting regions being most favorable for martensitic nucleation. Such a region features the shape of a perpendicular parallelepiped, its edges being oriented along the eigenvectors ξ~i of the strain tensor εˆ, its eigenvalues εi satisfying the following conditions: ε1 > 0,
ε2 < 0,
ε3  S2 , to surmise that the plane with the normal N1 is distinguished, and that the anticipated orientation of macroscopic shear is close to S1 . And viceversa, for S2  > S1 , the components N2 and S2 will be discriminated, respectively. In the case of the straight γ − α  transformation, the results of this approach are in good accordance with experimental results. With this approach, all macroscopic morphological characteristics of martensite attain a reasonable interpretation within the conceptual notion of nucleation at dislocations, where dislocations act as centers of forces disturbing the original lattice symmetry, their effect not being confined to the nuclear volume. These findings match in detail with the ideas of the wave theory of growth, presupposing that the transformation starts with the emergence of an excited state with the shape of a parallelepiped, built up of vectors ξ~i , its pairs of edges oscillating in opposed phase, thereby exciting controlling displacement waves orientated in the wavenormal n1,2 close to ξ~1,2 . In the most simple approximation of the equations n1 = ξ~1 ,
n2 = ξ~2 ,
the requirement of correspondence of NW DS with the wavehabit (5.3) delivers the following condition: 1 c2 ε1 2 κ= ≈ c1 ε2  188
which, if satisfied, ensures the possibility of a kinematic agreement of the wave description with the deformation description of the habit. Obviously, given the case that the ratio of tensile and compressive deformation in the wavemode corresponds with κ 2 , then dynamic agreement will also be achieved. We further note that for the γ −α  transformation, which proceeds with increase of specific volume: ε1 > ε2 . Consequently, c2 > c1 , so that the tensile strain can be prescribed by the wave propagating with the smaller velocity c1 , whereas compressive strain can be prescribed by the wave propagating with the larger velocity c2 (In the case of the α − γ  transformation, the situation will just be inverted). Specifically, the latter finding provides a physical criterion for the realistic choice of phase tuning of the waves controlling the transformation, as outlined in Chap. 5, as well as for the selection for the principal axes of tensile and compressive strain. Undoubtedly, the rules of deviation of the normal n1,2 of the controlling waves from the axes of symmetry of an ideal cubic lattice are dictated by the symmetry of the elastic field of the NC in the nucleation stage, in conjunction with a hard mode of wave generation. It is further worth to note that the orientation of the axis ξ~3 of the cylindrical nucleus of the α  phase can significantly deviate from the line of dislocations (most pronouncedly for the 30˚  dislocation line). Our specification of the nucleation stage, which also enabled us to define the orientation ξ~3 , besides lifetime, energy and spatial contour of the state of excitation, suggested possibilities for their physical simulation [273, 274]. The effect of laser impingement close to a linear trace, with a period of ∼ 2·10−11 s and sufficient power density for atomic vaporization, could induce the onset of a γ − α  in Fe31,5 Nisingle crystals, at a temperature some degrees above MS , however only in cases where the orientation of the trace of impingement of laser radiation was close to the calculated orientation ξ~3 on the flat surface of the specimen. Obviously, besides the envisaged precise measurement of the speed of growth of α  martensite, the already obtained results are fundamental for proving true the developed dynamical theory of the transformation. In order to get over to the dynamical description of the final stage, it would be useful, from our point of view, to represent the displacement waves by extremely small bundles of waves (with one of its transversal frontal dimensions of an order of magnitude of about one half wavelength), existing in the form of halfwave pulses (the dimensions of such pulses of order λ/2 in their direction of propagation). In fact, given a level of deformation ε ∼ 10−3 , with λ/2 ∼ 10−6 m, the utmost displacement associated with the wavepulse would be umax ≈ 1/4 ε λ, i.e., of similar order of magnitude as the latticeparameter. Consequently, such wavepulses must destroy the continuity of the medium, by causing the following effects: Generation of structural de189
fects; rotational distortions of the transforming lattice (being equivalent to the onset of ”rotational modes” [275]), which reestablish the macroscopic continuity of the medium, as known from [11, 13, 275], also leading to the emergence of a characteristic relief at the surface of the specimen subjected to a γ − α  transformation. Of course, all these processes, including the nucleation stage, are closely associated with the stage of growth and thus can only partly be put in relation with the stage of accommodation of coexisting phases. Nonetheless it is reasonable to classify as fundamental the identification of processes controlling the martensitic transformation, as well as a more detailed investigation of the microscopic mechanism of their development, within the frame of a comprehensive description of the growth mechanism of martensite. The identification of dislocation centers linked with martensitenucleation opens up new possibilities for an interpretation of the laws and rules governing the formation of latticeensembles, by definition of the spectrum of new centers of nucleation, being immanent in the newly emerged α  phase crystal. Further progress of the general theory of martensitic γ − α  transformations will undoubtedly be associated with the following topics:  Theoretical research on the dynamics of latticefluctuations including investigations on the effects of elastic dislocation fields on the nucleation stage of martensite. It can already be anticipated that the fluctuations leading to the above defined state of latticeexcitation in the form of an elongated parallelepiped, are most probable;  Specification of the area in which the state of excitation is localized, within the field of dislocation (i.e. the shortest distance to the line of dislocation), as well as of its probable transversal dimension;  Specification of the structure of the electronic spectrum in the proximity of the dislocationnucleation center (DNC) and of the Bγ−α  region. Doing so, the following aspects have to be considered: 1) The potential coexistence of a mixture of electronic configurations of the ironatoms (the basic pattern of calculus of a bandspectrum has already been proposed in [276]); 2) The effect of latticedistortions on the shape of the Ssurfaces as well as of energydispersion at the Ssurfaces, in the proximity of the Fermisurface. Finally, we remark that Ssurfaces resemble individual objects in quasimomentum space, thus classifying electronic states with respect to their contribution to transportprocesses. Furthermore, for investigations and interpretations of phenomena in transitionmetal alloys, which can most con190
veniently be described on the basis of a firstorder coherentpotential approximation [277], it will be necessary to evaluate the possible existence of Ssurfaces with large areas. Obviously, our proposed wavemodel of growth control for an α  crystal will be universally applicable for most rapidly proceeding (1st  order) martensitic transformations, being related to a dislocationnucleation mechanism. The thresholddeformation for such martensitic transformation comprises combined tensile and compressive strain, their main axes being oriented perpendicularly. For atoms in an intermediate phase region, the energy barrier can be overcome in a cooperative manner by a wavemode. This way, the controlling displacementwaves imprint macroscopic characteristics in the martensitecrystals, however without determining the final positions of the atoms. The latter will mainly depend on the pattern of local interactions among the atoms. The atomic displacements towards their new equilibriumpositions can be initiated by waves of shorter wavelength (in relation to the controlwaves), both in the pretransitional stage and in the growthstage. Such an additional system of waves, in parallel with the accommodationprocesses, must define the internal fine structure of the martensite plates.
191
Final conclusions
As a final conclusion, it can be stated that the obtained results provide sufficient evidence of the onset of a new qualitative stage of research on the large field of γ − α  martensitic transformations, within the frame of the waveapproach, thus making possible, on principle, to establish and to describe the following fundamental chain of relationships of cause and effect: • dislocationnucleationcenter • initial state of excitation • nonequilibrium conditions • particularities of the electronic structure • spectrum of the generated displacementwaves • observed morphological characteristics. It is apparent that just the growthcontrolling displacementwaves carry the information about the elastic field created by the nucleationcenter in the region of nucleation location, thereby ensuring a genetic correspondence of the characteristics of macroscopic martensitecrystals with those of the nucleationcenter. It is also obvious that, within the developed dynamical theory of γ − α  martensitic transformation, the growthcontrolling displacementwaves play the role of the previously missing link among microand macroscopic description. Our general conclusion is that the new comprehensive model of growth of the martensite crystals in a wave regime is basically consistent with observations and phenomenological theories, now being complemented by contemporary dynamics of lattice, and also by thermodynamical and quantum theoretical aspects, missed or only partially considered in previous theories. The author hopes that nearfuture research will confirm most of the predictions, enabling an extension of the insights of the wavemodel of α martensitegrowth in ferrous alloys onto a variety of other solidstate martensitic transformations.
192
Bibliography [1] Iziumov Iu.A. and V.N. Syromiatnikov. Fazovye perekhody i simmetriia kristallov. M.: Nauka, 1984. [2] Vaks V.G. Vvedenie v mikroskopicheskuiu teoriiu segnetoelektrikov. M.:Nauka, 1973. [3] Gufan Iu. M. Strukturnye fazovye perekhody. M.:Nauka, 1982. [4] Brus A. and Kauli P. Strukturnye fazovye perekhody. M.: Mir, 1984. [5] Vaks V.G., Zinenko V.I., and Shne´ıder V.E. Mikroskopicheskie teorii strukturnykh fazovykh perekhodov tipa poriadokbesporiadok v kristallakh. UFN, 141(4):629–673, 1983. [6] Strukov B.A. and Levaniuk A.P. Fizicheskie osnovy neto´ elektricheskikh iavleni´ı v kristallakh. M.: Nauka, 1983.
seg
[7] Kaufman L. and Ko´en M. Termodinamika i kinetika martensitnykh prevrashcheni´ı. Uspekhi fiziki metallov, IV:192–289, 1961. [8] Warlimont H., Hausch G., Prasetyo A., and Renaud F. Relations between elastic properties and diffusionless structural transition. Proceedings of the first JIM Int. Symposium on ,,New aspects of martensitic transformation“, pages 153–158, 1976. [9] Warlimont H. On the classification of structural phase transformation. J. Microsc. Spectrosc. Electron., 2:333–344, 1977. [10] Kristian D. Teoria prevrashcheni´ı v metallakh i splavakh, volume 1. M.: Mir, 1978. [11] Umanski´ı Ia.S. and Iu.A. Skakov. Fizika metallov. M.: Atomizdat, 1978. [12] Kurdjumov G.V. Iavleniia zakalki i otpuska stali. M.: Metallurgizdat, 1960. ´ [13] Kurdjumov G.V., Utevski´ı L.M., and Entin R.I. Prevrashchenia v zheleze i stali. M.: Nauka, 1977. 193
[14] Lysak A.I. and Nikolin B.I. Fizicheskie osnovy termichesko´ı obrabotki stali. Kiev: Tekhnika, 1975. [15] Krivoglaz M.A., Sadovski´ı V.D., L.V. Smirnov, and i dr. Zakalka stali v magnitnom pole. M.: Nauka, 1977. [16] Bernshte´ın M.L., Za´ımovski´ı V.A., L.M. Kaputkina, and i dr. Termomekhanicheskaia obrabotka stali. M.: Metallurgiia, 1983. [17] Ro´ıtburd A.L. Sovremennoe sostoianie teorii martensitnykh prevrashcheni´ı. Nesovershenstva kristallicheskogo stroeniia i martensitnye prevrashcheniia, pages 7–32, 1973. ´ ´ [18] Ro´ıtburd A.L. and Estrin E.P. Martensitnye prevrashcheniia. In Itogi nauki i tekhniki. Metallovedenie i termicheskaia obrabotka, pages 5–102. M.: VINITI, 1970. [19] Roitburd A.L. Martensitic transformation as a typical phase transformation in solids. Solid state physics: Advance in research and application, 33:327–390, 1978. [20] N. Seljakow, G. Kurdjumov, and Goodtzow N. Eine r¨oentgenographische untersuchung der struktur des kohlenstoffstahls. Zeitschrift f¨ ur Physik, 45:384–408, 1927. [21] Fridkin V.M. Dinamika reshetki i fazovye perekhody. kristallografiia, 2:262–296, 1979.
Sovremennaia
[22] Vinnikov L. Ia., Georgieva I.Ia., and i dr. Vydelenie ´energii pri obrazovanii martensita v zhelezonikelevykh splavakh i osobennosti ego struktury. Metallofizika, (55):24–27, 1974. [23] Robin M. and Gobin P.F. Etude par amplification electronique rapide de la propagation de la martensite dans un alliage ferrumnickel. Scripta Metall., 11:669–674, 1977. [24] Izotov V.I. and Khandarov P.A. Klassifikaciia martensitnykh structur v splavakh zheleza. FMM, 34:332–338, 1972. [25] Georgieva I.Ia. and Nikitina I.I. DAN SSSR, 186(1):85–87, 1969. [26] Zambrzhitzki´ı V.N., Maksimova O.P., and Shcherbedinski´ı G.V. O novom kineticheskom variante martensitnogo prevrashcheniia. DAN SSSR, 272(1):90–94, 1983. [27] Bunshah R.F. and Mehl R.F. Rate of propagation of martensite. Trans. AIME, 197:1251–1258, 1953. 194
[28] Mukherjee K. On the dynamics of martensitic transformations. Trans. AIME, 242:1494–1501, 1968. [29] Robin M., Lormand G., and Gobin P.F. Electrical emission associated with the martensitic burst of feni alloy. J.Phys. (Fr.), 43(12):485–490, 1982. [30] Lokshin F.L. Skorost’ martensitnogo prevrashcheniia. Nauchnye doklady vyshe´ı shkoly, (2):205–208, 1968. [31] Lokshin F.L. Dinamicheskaia teoriia martensitnogo prevrashcheniia, volume 771/85. Tr. Novocherkas. Politekhn. instituta, 1967. [32] Takashima K., Higo Y., and Nunomura S. The propagation velocity of the martensitic transformation in 304 stainless steel. Phil. Mag. A., 49(2):231– 241, 1984. [33] Arski´ı V.N. Vremya obrazovaniia martensitnogo kristalla. Metallovedenie i obrabotka metallov, (11):26–29, 1966. [34] Sadovski´ı V.D. and Romashev L.N. Rost kristallov martensita, obrazovavshikhsia pod de´ıstviem impul’snogo magnitnogo polia. DAN SSSR, 238(2):342–344, 1978. [35] Schastlivtsev V.M., Romashev L.N., Iakovleva I.L., and Sadovski´ı V.D. ´ Elektronnomikroskopicheskoe issledovanie struktury kristallov martensita, zarodivshikhsia pod de´ıstviem impul’snogo magnitnogo polia. FMM, 52(4):773–782, 1981. [36] Schastlivtsev V.M., Iakovleva I.L., and Romashev L.N. ´ Elektronnomikroskopicheskoe issledovanie struktury kristallov martensita, zarodivshikhsia pod de´ıstviem impul’snogo magnitnogo polia. FMM, 52(2):271–279, 1983. ´ ´ [37] Serebriakov V.G. and Estrin E.I. Pereokhlazhdenie ,,vzryvnogo“ martensitnogo prevrashcheniia v monokristallakh splavov FeNi. DAN SSSR, 237:322–324, 1977. [38] Haush G. and Warlimont H. Single crystalline elastic constants of ferromagnetic face centered cubic FeNi invar alloys. Acta Met., 21(4):401–414, 1973. [39] Delaey L., Gobin P.F., Guenin G., and Warlimont H. Premartensitic phenomena. Proceedings of the International Conference on Martensitic Transformations ICOMAT79, pages 400–414, 2429 June, 1979. [40] Hallman E.D. and Brockhause B.N. Crystal dynamics of nickeliron and copperzinc alloys. Canadian Journ. Phys., 47(10):11–17, 1969. 195
[41] Endoh Y. Lattice dynamics in ferromagnetic invar alloys. J. Magn. and Magn. Mat., (10):177–182, 1969. [42] Zverev V.M. and Silin V.P. Zavisimost’ skorosti zvuka ot namagnichennosti v ferromagnitnykh metallakh. Preprint T19272. M.: FI AN SSSR. [43] Zverev V.M. and Silin V.P. K invarno´ı probleme. Kratkie soobshcheniia po fizike, (6):46–49, 1984. [44] Cech R.E. and Turnbull D. Heterogeneous nucleation of the martensitic transformation. Trans. AIME, 206:124–132, 1956. [45] Vinta´ıkin E.Z. Martensitnye prevrashcheniia. Itogi nauki i tekhniki. Metallovedenie i termicheskaia obrabotka., 17:3–63, 1983. [46] Iurchikov E.E. and Men’shikov A.Z. Issledovanie sostoianiia austenita pered martensitnym prevrashcheniem metodom ´effekta messbau´era. FMM, 32(1):168–170, 1971. [47] Tiapkin Iu. D., Pushin V.G., Romanova P.P., and Bu´ınov N.N. Issledovanie struktury γ  i αfaz v splavakh zhelezonikel’ vblizi tochki martensitnogo prevrashcheniia. 1. diffuznoe rasseianie ´elektronov i rentgenovskikh luche´ı. FMM, 41(5):1040–1047, 1976. [48] Kondrat’ev V.V. and Pushin V.G. Predperekhodnye sostoianiia v splavakh vblizi martensitnykh prevrashcheni´ı. Fazovye prevrashcheniia i struktura metallov i splavov. Sverdlovsk: UNTs AN SSSR, pages 18–25, 1982. [49] Sarrak V.I. and Suvorova S.O. Ob osobennostiakh sostoianiia austenita v predmartensitnom intervale temperatur. Izv. AN SSSR, Metally, (6):90– 97, 1982. [50] Kondrat’ev V.V. O termodinamichesko´ı usto´ıchivosti strukturnykh sostoiani´ı pri martensitnykh prevrashcheniiakh. FMM, 47(1):102–109, 1979. [51] Falk F. GinzburgLandau theory and solitary waves in shapememory alloys. Z. Phys. B., 54:159–167, 1984. [52] Krivoglaz M.A. Fluktuonnye sostoianiia ´elektronov. UFN, III(4):618–654, 1973. [53] Ro´ıtburd A.L. Zarozhdenie na dislokatsiakh pri martensitnykh prevrashcheniiakh. DAN SSSR, 256(1):80–84, 1981. [54] Gurevich A.B. and Mints R.G. Lokalizovannye volny v neodnorodnykh sredakh. UFN, 142(1):61–84, 1984. 196
[55] Petrov Iu. N. Defekty i bezdiffuzionnoe prevrashchenie v stali. Kiev: Naukova dumka, 1978. [56] Kashchenko M.P. and Vereshagin V.P. Dynamic lattice stability during reconstructive martensitic transformations in the phonon maser model. Phys.Met. Metall., 58(3):28–34, 1984. [57] Ro´ıtburd A.L. Neutron scattering study of the magnetic structure of cupric oxide. FTT, 10(12):3619–3627, 1968. ´ and Vefer F. K termodinamike austenitno[58] Krizement O., Gudremon E., martensitnogo prevrashcheniia. In Fazovye prevrashcheniia v stali, pages 263–271. M.:Metallurgizdat, 1961. [59] Mogutnov B.M., Tomilin I.A., and Shvartsman L.A. Termodinamika zhelezouglerodistykh splavov. M.: Metallurgiia, 1972. [60] Landau L.D. and Lifshits E.M. Statisticheskaia fizika. M.: Nauka, 1976. [61] Ziner K. Rol’ ´entropii v stabilizatsii faz. In Usto´ıchivost’ faz v metallakh i splavakh, pages 96–109. M.:Mir, 1970. ´ [62] Dovgopol S.P. and Zaborovskaia I.A. Elektronnaia struktura, magnetizm i stabil’nost’ faz 3dmetallov i splavov v tverdom i zhidkom sostoianiiakh. Obsory po teplofizicheskim svo´ıstvam veshchestv. M.: IVTAN, 1982. [63] Miodownik A.P. The effect of magnetic transformation on phase diagrams. Bull. Alloys Phase Diagr., 2:406–412, 1982. [64] Hasegawa H. and Pettifor D.G. Microscopic theory of the temperature – pressure phase diagram of iron. Phys. Rev. Let., 50:130–133, 1983. [65] Barret Ch.S. and Massal’ski´ı T.B. Struktura metallov. PartII. M.: Metallurgiia, 1984. [66] Ro´ıtburd A. L. Teoriia formirovaniia geterofazno´ı struktury pri fazovykh prevrashcheniiakh v tverdom sostoianii. UFN, 113(1):105–128, 1974. [67] Patel J.R. and Cohen M. Criterion for the action of applied stress in the martensitic transformation. Acta Metall., 1(5):531–538, 1953. [68] Kosenko N.S., Ro´ıtburd A.L., and Khandros L.G. Vliianie vneshnego napriazheniia na termodinamiku i strukturu produktov martensitnogo prevrashcheniia. In Martensitnye prevrashcheniia: Dokl. mezhdunar. konf.”ICOMAT77”, pages 74–78. Kiev: Naukova dumka, 1978. 197
[69] Pankova M.N. and Ro´ıtburd A.L. Orientiruiushchee vliianie vneshnego napriazheniia na martensitnoe prevrashchenie v splavakh na osnove zheleza. FMM, 58(4):716–726, 1984. [70] Ro´ıtburd A.L. O nekotorykh ocobennostiakh rosta kristallov v kondensirovannykh sistemakh. Kristallografiia, 7(8):292–299, 1962. [71] Landau L.D. and Lifshits E.M. ’Elektrodinamika sploshnykh sred. M.: Nauka, 1982. [72] Ro´ıtburd A.L. Osobennosti razvitiia fazovykh prevrashcheni´ı v kristallakh. In Problemy sovremenno´ı kristallografii, pages 345–369. M.: Nauka, 1975. [73] Khirt Dzh. and Lote I. Teoriia dislokatsi´ı. M.: Atomizdat, 1972. [74] Kottrel A. Teoriia dislokatsi´ı. M.: Mir, 1969. [75] Udarnye volny i iavleniia vysokoskorostno´ı deformatsii metallov. M.: Metallurgiia, 1984. [76] Machlin E.S. and Cohen M. Habit phenomenon in the martensitic transformation. Trans. AIME, 191:1019–1029, 1951. [77] Meyers M.A. On the growth of lenticular martensite. Acta Metall., 28:757– 770, 1980. [78] Lokshin F.L. Primenenie teorii udarnykh voln k opisaniiu protsessa rosta kristallov martensita. In Nauchnye doklady vyshe´ı shkoly, number 1, pages 146–150. M.: Metallurgiia, 1969. [79] Crussard C. Application de theorie de ondes explosives a la croissance de la martensite. Compt. Rend., 240(24):2313–2315. [80] Rabinovich M.I. and Trubetskov D.I. Vvedenie v teoriiu kolebani´ı i voln. M.: Nauka, 1984. [81] Wasilewski R.J. On the nature of the martensitic transformation. Metall.Trans., 6A:1405–1418, 1975. [82] Kayser U. The activiation of the martensitic phase transformation in ferrous alloys by stimulated emission of phonons. J. Phys. F., 2:60–64, 1972. [83] Zvelto O. Fizika lazerov. M.: Mir, 1979. [84] Panin V.E., Egorushkin V.E., Khon Iu.A., and Elsukova T.F. Atomvakansionnye sostoianiia v kristallakh. Izv. vuzov SSSR. Ser. Fizika, (12):5–28, 1982. 198
[85] Zhang J. The nonequilibrium phase transition theory of martensitic transformation. J. Phys. F., 14(3):769–783, 1984. [86] Na´ı Dzh. Fizicheskie svo´ıctva kristallov. M.: Mir, 1967. [87] Za´ıman Dzh. Prinzipy teorii tverdogo tela. M.: Mir, 1974. [88] Kashchenko M.P. Lazernaia model’ martensitnogo prevrashcheniia v splavakh perekhodnykh metallov. In Martensitnye prevrashcheniia v metallakh i splavakh: Dokl. mezhdunar. konf. ,,ICOMAT77“, pages 137–141. Kiev: Naukova Dumka, 1979. [89] Kashchenko M.P. and Mints R.I. Mechanism of martensitic transformation due to the disequilibrium of the electronphonon system. JETP Lett., 26(6):309–310, 1977. [90] Kashchenko M.P. Sravnenie dvukh istochnikov neravnovesnosti ´elektronno´ı podsistemy pri uchete zatukhaniia ´elektronov. Izv. vuzov SSSR. Ser. Fizika, (3):113–114, 1982. [91] Afanas’ev A.M. and Kagan Iu. M. Ob osobennostiakh v zakone disper´ sii fononov, sviazannykh s ´elektronfononnym vzaimode´ıstviem. ZhETF, 43(10):1457–1463, 1962. [92] Bulaevski´ı L.N. Strukturnyi (pa´ıerlsovski´ı ) perekhod v kvaziodnomernykh sistemakh. UFN, 115:263–300, 1975. [93] Egorushkin V.E., Kulkov S.N., and Kulkova S.E. Electronic structure and the theory of phase transformation in NiMn. Physics, 123:61–68, 1983. [94] Kulikov N.I. and Tugushev V.V. Volny spinovo´ı plotnosti i zonny´ı antiferromagnetizm v metallakh. UFN, 144(4):643–680, 1984. [95] Gor’kov L.P. Ob osobennostiakh ´elektronnogo spektra soedineni´ı so struk´ turo´ı βW. Pis’ma v ZhETF, 20(8):571–574, 1974. [96] Gor’kov L.P. and Dorokhov O.N. Sverkhprovodiashchie svo´ıstva i strukturny´ı ´ perekhod v soenineniiakh s reshetko´ı A15. ZhETF, 71(5(11)):1934–1950, 1976. [97] Vonsovski´ı S.V., Iziumov Iu.A., and Kurmaev Z.Z. Sverkhprovodimost’ perekhodnykh metallov, ikh splavov i soedineni´ı. M.: Nauka, 1977. [98] L´eks M. Fluktuatsii i kogerentnye iavleniia. M.: Mir, 1975. [99] Kashchenko M.P. and Mints P.I. Kolebatel’nye analogi deformatsii be´ına i morfoogiia martensita v tverdykh pastvorakh sistem γ (FeNi). FTT, 19(2):329–334, 1977. 199
´ [100] Erenre´ıkh G. and Shvarts L. Elektronnaia struktura splavov. M.: Mir, 1976. [101] Vediaev A.V. Metod kogerentnogo potentsiala v teorii neuporiadochennykh splavov. TMF, 31(3):392–404, 1977. ´ [102] Egorushkin V.E. and Kul’ment’ev A.I. Elektronnaia struktura splavov perekhodnykh metallov s proizvol’nym dal’nim poriadkom. Izv. vuzov SSSR. Ser. fizika, (12):29–49, 1982. [103] Kallue´ı D. Teoriia ´ energetichesko´ı zonno´ı struktury. M.: Mir, 1969. [104] Slater J.C. and Koster G.F. Simplified L C A O method for potential problem. Phys. Rev., 94:1498–1512, 1954. [105] Dzhons G. Teoriia zon Brilliu´ ena i ´ elektronnye sostoianiia v kristallakh. M.: Mir, 1968. [106] Wood I.H. Energy bands in iron via the augmented plane wave method. Phys. Rev., 126:517–527, 1962. [107] Bagayoko D. and Callaway J. Lattice  parameter dependence of ferromagnetism in bcc and fcc iron. Phys. Rev.B., 28:5419–5422, 1983. [108] Zornberg E.I. Band structure and fermi surface of ferromagnetic nickel. Phys. Rev.B., 1:244–251, 1970. [109] Connolly J.W.D. Energy bands in ferromagnetic nickel. 159:415–418, 1967.
Phys. Rev.,
[110] Jarlborg T. and Freeman A.J. Selfconsistent semirelativistic energy band structure of fcc and tetragonal Ni metals. J. Magn. Magn. Mater, 22(1):6– 13, 1980. [111] Snow E.C. and Waber J.T. The APW energy bands of the body centered and face centered cubic modifications of the 3dtransition metals. Acta Metall., 17:623–635, 1969. [112] Roy D.M. and Pettifor D.G. Stoner theory support for the twostate hypothesis for iron. J.Phys.F., 7:183–187, 1977. ´ [113] Samsonov G.B., Priadko I.F., and Priadko L.F. Elektronnaia lokalizatsiia v tverdom tele. M.: Nauka, 1976. [114] Liakutkin A.V., Grigorovich V.K., and Ivakhnenko I.S. Issledovanie fazovykh perekhodov chistogo zheleza metodom magnitno´ı vospriimchivosti. DAN SSSR, 257(2):398–400, 1981. 200
[115] Liakutkin A.V. Vozmozhnost’ izomorfnogo okhlazhdeniia chistogo zheleza posle kristallizatsii iz rasplava. FMM, 54(1):129–136, 1982. [116] Wilkinson M.K. and Shull C.G. Neutron diffraction studies on iron at high temperatures. Phys. Rev., 103:516–524, 1956. [117] Brown P.J. and et al. Ferromagnetic correlations in both the α and γphases of paramagnetic iron. J. Magn. Magn. Mater, 30:335–339, 1983. [118] Grebennikov V.I., Prokop’ev Iu.I., Sokolov O.B., and Turov E.A. Metod lokal’nykh fluktuatsi´ı v teorii magnetizma perekhodnykh metallov. FMM, 52(4):679–694, 1981. [119] Tauer K.J. and Weiss R.J. Unusual magnetic structure of facecentered cubic Fe. Bull. Amer. Phys. Soc., 6:125, 1961. [120] Kaufman L., Clougherty E.V., and Weiss R.J. The lattice stability of metals  III iron. Acta Metal., 11:323–335, 1963. [121] Poulsen U.K., Kollart J., and Andersen O.K. Magnetic and cohesive properties from canonical bands. J. Phys., 6(9):241–247, 1976. [122] K¨ ubler J. Magnetic moments of ferromagnetic and antiferromagnetic bcc and fcc iron. Phys. Lett., 81A(1):81–83, 1981. ´ [123] Kulikov N.I. Elektronnaia struktura perekhodnykh metallov pod davleniem. Izv. vuzov SSSR. Ser. Fizika, (12):50–62, 1982. ´ ıshinski´ı E.R. Dva ´elektronnykh sostoianiia atomov zheleza v ego gtsk i [124] E´ otsk modifikatsiiakh. Dep. v VINITI, (number 1082), 1984. [125] Keller J., Fritz J., and Garritz A. Cluster method multiple scattering calculation of density of states of liquid transition metals, rare earth metals and their alloys. J. de Phys., 35(5):379–385, 1974. [126] Kondorski´ı E.I. Zonnaia teoriia magnetizma. Part I. Mosk.unta, 1976.
M.: Izdvo
[127] Krenkell A. and Wong K. Poverkhnost’ Fermi. M.: Atomizdat, 1978. [128] Kashchenko M.P. Interpretation of some characteristic morphological indicators of martensite of systems FeNi, FeC using the phonon maser model. Phys.Met. Metall., 58(5):24–31, 1984. [129] Vereshchagin V.P. and Kashchenko M.P. Optimal’naia struktura zonnogo spektra ´elektronov v modeli fononnogo mazera. Dostizheniia v oblasti metallovedeniia i termichesko´ı obrabotki metallov. Tez. zonal’no´ı konf. (IX Ural’sko´ı shkoly metallovedov  termistov). Sverdlovsk: Int fiziki metallov UNTs AN SSSR, pages 93–95, 1985. 201
[130] Vereshchagin V.P. and Kashchenko M.P. Prnciples of selection of pairs of electronic states which are potentially active in phonon generation. Phys.Met. Metall., 61(2):23–30, 1986. [131] Khanin Ia.I. Kvantovaia radiofizika. M.: Sov. radio, 1975. [132] Khaken G. and Va´ıdlikh V. Kvantovaia teoriia lazera. In Kvantovye fluktuatsii izlucheniia lazera, pages 143–205. M.: Mir, 1974. [133] Khaken G. Sinergetika. M.: Mir, 1980. [134] Makomber Dzh. Dinamika spektroskopicheskikh perekhodov. M.: Mir, 1979. [135] Khaken G. Statistika lazernogo izlucheniia s tochki zreniia teorii fazovykh perekhodov. In Spektroskopiia opticheskogo smeshcheniia i korrelliatsiia fotonov, pages 493–517. M.: Mir, 1978. [136] Taker Dzh. and R´empton V. Giperzvuk v fizike tverdogo tela. M.: Mir, 1975. ` [137] Teploprovodnost’ tverdykh tel. Spravochnik. M.: Energoatomizdat, 1984. [138] Gantmakher V.F. and Levinson I.B. Rasseianie nositele´ı toka v metallakh i poluprovodnikakh. M.: Nauka, 1984. [139] Agranat M.B., Ashitkov S.I., Granovski´ı A.B., and Rukman G.I. Vzaimode´ıstvie pikosekundnykh lazernykh impul’sov s ´elektronno´ı spinovo´ı i ´ fononno´ı podsistemami nikelia. ZhETF, 86(4):1376–1379, 1984. [140] Kashchenko M.P. and Mints R.I. Mikroskopicheski´ı mekhanizm marten´ sitnogo prevrashcheniia v sisteme FeNi. ZhETF, 75(6(12)):2280–2289, 1978. [141] Kashchenko M.P. Usloviia generatsii voln, sopostavliaemykh deformatsii Be´ına. FMM, 49(5):937–946, 1980. [142] Vereshchagin V.P. and Kashchenko M.P. Vydelenie markovskogo priblizheniia v metode neravnovesnogo statisticheskogo operatora. Fizicheskie metody issledovaniia tverdogo tela. Sverdlovsk, (3):57–67, 1979. [143] Vereshchagin V.P. and Kashchenko M.P. Markovskaia forma neravnovesnogo statisticheskogo operatora dlia sistem so slabym vzaimode´ıstviem. TMF, 42(1):133–138, 1980. [144] Vereshchagin V.P. and Kashchenko M.P. Postroenie kineticheskikh uravneni´ı dlia neravnovesnykh kvantovykh sistem. Sverdlovsk. Rukopic’ predstavlena Ural. lecotekh. intom. Dep. v VINITI 2 avg. 1979, No. 289379, 1979. 202
[145] Vereshchagin V.P. and Kashchenko M.P. Kineticheskie uravneniia dlia sistemy vzaimode´ıstvuiushchikh ´ elektronov i fononov. Sverdlovsk. Rukopic’ predstavlena Ural. lecotekh. intom. Dep. v VINITI 7 dek. 1979, No. 417779, 1979. [146] Vereshchagin V.P. and Kashchenko M.P. Prostranstvennolokal’nye kineticheskie uravneniia dlia ´ elektronov i fononov. Usloviia generatsii uprugikh voln. Sverdlovsk. Rukopic’ predstavlena Ural.lecotekh. intom. Dep. v VINITI 5 avg. 1980, No. 345580, 1980. [147] Vereshchagin V.P. Osobennosti neravnovesno´ı dinamiki sistemy vzaimode´ıstvuiushchikh ´ elektronov i fononov v tverdykh telakh:. Diss. ... kand. fiz.mat. nauk. Sverdlovsk: Ural. politekhn. int, 1980. [148] Zubarev D.N. Neravnovesnaia statisticheskaia termodinamika. M.: Nauka, 1971. [149] Kalashnikov V.P. Metod neravnovesnogo statisticheskogo operatora i ego prilozhenie k kinetike paramagnitnykh iavleni´ı v provodiashchikh kristallakh. Diss.... dokt. fiz.mat. nauk. Sverdlovsk: Int fiziki metallov UNTs AN SSSR, 1971. [150] Zubarev D.N. and Kalashnikov V.P. Teoriia vozmushcheni´ı i integral’nye uravneniia dlia neravnovesnykh statisticheskikh operatorov. TMF, 5(3):406– 416, 1970. [151] Pustovo´ıt V.I. Vzaimode´ıstvie ´elektronnykh potokov s uprugimi volnami reshetki. UFN, 97(2):257–306, 1969. [152] BonchBruevich V.L. and Kalashnikov S.G. Fizika poluprovodnikov. M.: Nauka, 1977. [153] Zheru I.I. Nizkochastotnye rezonansy ´ eksitonov i primesnykh tsentrov. Kishinev: Shtiintsa, 1976. [154] Kopvillem U.Kh. and Saburova R.V. Para´ elektricheski´ı rezonans. M.: Nauka, 1982. [155] Andreev A.V., Emel’ianov V.I., and Il’inski´ı Iu.A. Kollektivnoe spontannoe izluchenie (sverkhizluchenie Dike). UFN, 131(4):653–694, 1980. [156] Bogachev I.N. and Egolaev V.F. Struktura i svo´ıstva zhelezomargantsevykh splavov. M.: Metallurgiia, 1973. [157] Zyrianov P.S. and Klinger M.I. Kvantovaia teoriia iavleni´ı ´ elektronnogo perenosa v kristallicheskikh poluprovodnikakh. M.: Nauka, 1976. 203
[158] Weiss R.J. and Marotta A.S. Spindependence of the resistivity of magnetic metals. J. Phys. Chem. Sol., 9:302–309, 1959. [159] Vonsovski´ı S.V. Magnetizm. M.: Nauka, 1971. [160] Auslender M.I. and Kalashnikov V.P. Proizvodiashchi´ı funktsional dlia neravnovesno´ı sistemy ´elektronov i fononov. TMF, 25(3):370–381, 1975. [161] Khe´ıne V., Cohen M., and U´e´ır D. Teoriia psevdopotentsiala. M.: Mir, 1973. [162] Mirzaev D.A., Morozov O.P., and Shte´ınberg M.M. O sviazi prevrashcheni´ı v zheleze i ego splavakh. FMM, 36(3):560–568, 1973. [163] Shte´ınberg M.M., Mirzaev D.A., and Ponomareva T.N. Gamma al’fa prevrashchenie pri okhlazhdenii splavov zhelezomarganets. FMM, 43(1):166– 172, 1977. [164] Mirzaev D.A., Shte´ınberg M.M., Ponomareva T.N., and i dr. Fasovye γ → α prevrashcheniia v binarnykh splavakh zheleza s med’iu, kobal’tom, ruteniem i platino´ı. FMM, 51(2):364–375, 1981. [165] Mirzaev D.A., Shte´ınberg M.M., Ponomareva T.N., and Schastlivtsev V.M. Vliianie skorosti okhlazhdeniia na polozhenie martensitnykh tochek. Uglerodistye stali. FMM, 47(1):125–135, 1981. [166] Mirzaev D.A., Shte´ınberg M.M., Ponomareva T.N., and Schastlivtsev V.M. Vliianie skorosti okhlazhdeniia na polozhenie martensitno´ı tochki II. Legirovannye stali. FMM, 47(5):986–992, 1979. [167] Gudenaf D. Magnetizm i khimicheskaia sviaz. M.: Metallurgiia, 1968. ´ [168] Akhiezer A.I. Obshchaia fizika. Elektricheskie i magnitnye iavleniia: spravochnoe posobie. Kiev: Nauk. dumka, 1981. [169] Be´ılin V.M., Ze´ınalov T.I., and Rogel’b´erg I.L. Ob opredelenii vremeni ´elektronfononno´ı relaksatsii v nikele i ego splavakh. Mekhanizmy relaksatsionnykh iavleni´ı v tverdykh telakh. Kaunas: Kaunas.politekh. int, pages 44–46, 1974. [170] Vnukovski´ı N.I. Izluchatel’nye kharakteristiki khromistykh splavov: Avtoref. Diss. ... kand. fiz.mat. nauk. Sverdlovsk: Ural. politekhn. int, 1982. [171] Noskov M.M. Opticheskie i magnetoopticheskie svo´ıstva metallov. Sverdlovsk: UNTs AN SSSR, 1983. [172] Shirokovski´ı V.P., Kirillova M.M., and Shilkova N.A. Anomaliia opticheskogo ´ pogloshcheniia v zheleze. ZhETF, 82(3):784–792, 1982. 204
[173] Bolotin G.A., Noskov M.M., and Sasovskaia I.I. Mezhzonnoe opticheskoe pogloshchenie v ferromagnitnom kobal’te. Sviaz’ s plotnost’iu sostoiani´ı. FMM, 35(4):699–705, 1973. [174] Kaufman L. and Cohen M. The martensitic transformation in the ironnickel system. Trans. AIME, 206:1393–1401, 1956. [175] Sasovskaia I.I., Noskov M.M., and Men’shikov A.Z. Opticheskie i rentgenovskie spektry splava zheleza s 30% nikelia v gtsk i otsk strukturnykh sostoianiiakh. FMM, 27(2):272–279, 1969. [176] Bendic W. and Pepperhoff W. Temperature dependence of the electrical resistivity of fcc iron alloys. J. Phys. F. Metal. Phys., 8(12):2535–2544, 1978. [177] Kidin I.N., Shtremel’ M.A., and Andreev Iu.G. Elektrosoprotivlenie uglerodistogo martensita. FMM, 28(5):874–878, 1969. [178] Andreev Iu.G. Issledovanie svo´ıstv uglerodistogo martensita: Diss. ... kand. tekh. nauk. M.: MISiS, 1969. [179] Kekalo I.B. Fizicheskie svo´ıstva metallov i splavov. M.: MISiS, 1979. [180] Krivoglaz M.A. Difraktsiia rentgenovskikh luche´ı i ne´ıtronov v neideal’nykh kristallakh. Kiev: Nauk. dumka, 1983. [181] Nakamura Y. The invar problem. I E E E Trans. Magn., MAG.12:278– 291, 1976. [182] Tanji Y. and Nakamura Y. Steinemann anomalous elastic properties of FeNi (fcc) alloys and their invar. Physica, B 119:109–114, 1983. ´ [183] Kharrison U. Elektronnaia struktura i svo´ıstva tverdykh tel, volume 2. M.: Mir, 1983. [184] Kamenetskaia D.S., Piletskaia I.B., and Shiriaev V.I. Zhelezo vysoko´ı stepeni chistoty. M.: Metallurgiia, 1978. [185] Za´ıman Dzh. Modeli besporiadka. M.: Mir, 1982. [186] Gel’d P.V., Dovgopol S.P., Dovgopol M.G., and Radovskij I.Z. Magnitnaia vospriimchivost’ i struktura blizhnego poriadka zhelezouglerodistykh rasplavov. DAN SSSR, 236(4):853–856, 1977. [187] Kalinovich D.F., Kovenski´ı I.I., and Smolin M.D. Sostoianie ugleroda, rastvorennogo v γzheleze. Izv. AN SSSR. Metally, (4):105–107, 1974. 205
[188] Mirzaev D.A., Ponomareva T.N., and Shte´ınberg M.M. O stupeniakh prevrashcheniia v splavakh zheleza, vyiavliaiushchikhsia pri uvelichenii skorosti okhlazhdeniia do 4.105 grad/sek. In Mezhdunar. konf.,,Martensitnye prevrashcheniia“.Tez.dokl. Kiev, pages 142–143, 1977. [189] Kashchenko M.P. Soglasovanie kontsentratsionno´ı zavisimosti temperatur martensitnykh prevrashcheni´ı v sistemakh FeNi, FeMn s usloviiami generatsii v modeli fononnogo mazera. FMM, 50(3):671–672, 1980. ` ıshinski´ı E.R. Determination of the optimum tem[190] Kashchenko M.P. and E´ perature for fonon generation by nonequilibrium ´electrons in binary alloys of iron. Phys.Met. Metall., 56(4):47–54, 1983. ` ıshinski´ı E.R. Magnitnye i magnitoob“emnye svo´ıstva Fe i FeNi [191] E´ splavov v modeli vydelennykh sostoiani´ı atomov zheleza: Diss. ... kand. fiz.mat. nauk. Sverdlovsk: Ural. politekhn. int, 1984. [192] Shriffer Dzh. Teoriia sverkhprovodimosti. M.: Nauka, 1970. [193] Fedorov F.I. Teoriia uprugikh voln v kristallakh. M.: Nauka, 1965. [194] Novikov I.I. Defekty kristrallicheskogo stroeniia metallov. M.: Metallurgiia, 1975. [195] Marder A.R. and Krauss G. The formation of lowcarbon martensite in FeC alloys. Trans. Quart., 62(4):957–964, 1969. [196] Schastlivtsev V.M. Strukturnye osobennosti martensita v konstruktsionnykh staliakh. FMM, 33(2):326–334, 1972. ´ [197] Schastlivtsev V.M. Elektronnomikroskopicheskoe issledovanie struktury martensita konstruktsionnykh stale´ı. FMM, 38(4):326–334, 1974. [198] Schastlivtsev V.M., Koptseva N.V., and Artemova T.V. ´ Elektronnomikroskopicheskoe issledovanie struktury martensita v malouglerodistykh splavakh zheleza. FMM, 41(6):1251–1260, 1976. [199] Izotov V.I. Morfologiia i kristallogeometriia reechnogo (massivnogo) martensita. FMM, 34(1):123–132, 1972. [200] Izotov V.I. Struktura zakalenno´ı konstruktsionno´ı stali. Sostoianie peregreva. FMM, 39(4):801–814, 1975. ´ [201] Eterashvili T.V., Spaccki´ı M.N., Utevski´ı L.M., and Tulikov G.N. Razvitie plastichesko´ı deformatsii paketnogo martensita. FMM, 46(4):772–780, 1978. 206
´ [202] Eterashvili T.V., Utevski´ıL.M., and Spaccki´ı M.N. Struktura paketnogo martensita i lokalizatsiia ostatochnogo austenita v konstruktsionnykh staliakh. FMM, 48(4):807–815, 1979. [203] Andreev Iu.G., Devchenko L.N., Shelekhov E.V., and Shtremel’ M.A. Upakovka kristallov martensita v psevdomonokristalle. DAN SSSR, 237(3):574–576, 1977. [204] Andreev Iu.G., Devchenko L.N., Zarkova E.I., and Shtremel’ M.A. Kristallogeometriia martensitnogo sdviga v krupnom pakete. FMM, 56(4):783–790, 1983. [205] Sandvic B.P.I. and Wayman C.M. Electron microscopy studies of martensitic. J. Phys. (Fr.), 43(12):557–562, 1982. [206] Urusovskaia A.A. Mekhanicheskie svo´ıstva kristallov. In Sovremennaia kristallografiia, volume 4, pages 47–152. 1981. [207] Georgieva I.Ia. and Nikitina I.I. Izotermicheskoe i atermicheskoe martensitnye prevrashcheniia. MiTOM, (5):68–72, 1972. [208] Men’shikov A.Z. O vliianii magnitnogo sostoianiia austenita na kharakter martensitnogo prevrashcheniia. FMM, 40(4):853–856, 1975. [209] Zolotarevski´ı I.V., Snezhno´ı V.L., and She´ıko L.M. O magnitostriktsii paraprotsessa austenitnykh splavov vblizi martensitno´ı tochki. FMM, 47(6):1312–1313, 1979. [210] Zolotarevski´ı I.V., Kosenko N.S., and Krivoglaz M.A. Vliianie magnitostriktsii na sdvig tochki martensitnogo prevrashcheniia v sil’nom magnitnom pole. Metallofizika, 1(2):17–22, 1979. [211] Belov K.P. Uprugie, teplovye i ´ elektricheskie iavleniia v ferromagnitnykh metallakh. M.L.: GITTL, 1951. [212] Romashev L.N. Vliianie magnitnogo sostoianiia γfazy stale´ı na (γ → α) – martensitnoe prevrashchenie pod de´ıstviem magnitnogo polia. In Fazovye prevrashcheniia i struktrura metallov i splavov, pages 32–39. Sverdlovsk : UNTs AN SSSR, 1982. [213] Zolotarevski´ı I.V., Snezhno´ı V.L., Georgieva I.Ia., and Matiushenko L.A. Magnitostriktsiia austenita zhelezonikel’margantsevykh splavov, obladaiushchikh dvo´ıno´ı kinetiko´ı martensitnykh prevrashcheni´ı. FMM, 51(3):669–672, 1981. [214] Zolotarevski´ı I.V., Snezhno´ı V.L., and She´ıko L.M. Magnitostriktsiia austenita zhelezonikel’margantsevykh splavov i martensitnoe prevrashchenie pod de´ıstviem sil’nogo magnitnogo polia. FMM, 55(3):548–553, 1983. 207
´ [215] Zavadski´ı E.A. and Val’kov V.I. Magnitnye fazovye perekhody. Kiev: Naukova dumka, 1980. ` ıshinski´ı E.R. and Kashchenko M.P. Izmenenie skorosti zvuka za schet per[216] E´ eraspredeleniia ´elektronov pri magnitnom fazovom prevrashchenii. ZhTF, 51(11):2396–2398, 1981. ` ıshinski´ı E.R. and Kashchenko M.P. Izmenenie skorosti zvuka za schet per[217] E´ eraspredeleniia ´elektronov v slabykh kollektivizirovannykh ferromagnetikakh, imeiushchikh pik v plotnosti sostoiani´ı d´elektronov. Tez. dokl. XV Vsesoiuz. konf. po fizike magnitnykh iavleni´ı. Perm’: UNTs AN SSSR. Part I, pages 34–35, 1981. [218] Crangle J. and Hallam G.C. The magnetization of face centered cubic and body centered cubic iron + nickel alloys. Proc. Roy. Soc., A. 272:119–132, 1963. [219] Tikadzumi S. Fizika ferromagnetisma. Magnitnye svo´ıstva veshchestva. M.: Mir, 1983. [220] Zakharov A.I. Vliianie temperatury na rentgenovski´ı foto´elektronny´ı spektr ` valentnykh ´elektronov splava FeNi invarnogo sostava. Pis’ma v ZhETF, 24:276–278, 1976. [221] Zakharov A.I. and Narmonev A.G. Temperaturnye izmeneniia v rentgenovskikh foto´elektronnykh spektrakh valentnykh i ostovnykh ´elektronov splava FeNi invarnogo sostava. Metallofizika, 4:113–115, 1982. ´ [222] Vertkhe´ım G. Effekt Messbau´ era. M.: Mir, 1966. [223] Iurchikov E.E. Issledovanie metodom IaGR magnitnogo i strukturnogo sostoiania FeNi splavov: Avtoref. diss. ... kand. fiz.mat. nauk. Sverdlovsk: Int fiziki metallov UNTs AN SSSR, 1971. [224] Hesse J., M¨ uller J.B., Wiechmann B., and Ullrich H. Local magnetization of Fe atoms in FeNi alloys. J. Magn.Magn.Mater., 1518. Part 3:1195–1196, 1980. [225] Nakamura Y. The invar problem. IEEE Trans.Magn., MAG12:278–291, 1976. [226] Hasegawa H. and Kanamori J. An application of the coherent potential approximation to ferromagnetic alloys. J. Phys. Soc. Jap., 31:382–393, 1971. [227] Men’shikov A.Z. and Shestakov V.A. Magnitnye neodnorodnosti v invarnykh zhelesonikelevykh splavakh. FMM, 43(4):722–733, 1977. 208
[228] Goman’kov V.I., Mokhov B.N., and Nogin N.I. Kontsentratsionnye ferroantiferromagnitnye perekhody v sistemakh na osnove Fe. ZhETF, 77(2(8)):630–639, 1979. [229] Kuz’min N.N. and Men’shikov A.Z. Nizkotemperaturnoe kriticheskoe rasseianie ne´ıtronov v splavakh zhelezonikel’ i nikel’marganets. FMM, 49(2):433–437, 1980. [230] Sidorov S.K. and Doroshenko A.V. O magnitno´ı strukture splavov NiFe, imeiushchykh granetsentrirovannuiu kubicheskuiu reshetku. FMM, 19(5):786–788, 1965. [231] Iziumov Iu.A. and Medvedev M.V. Teoriia magnitouporiadochennykh kristallov s primesiami. M.: Nauka, 1970. [232] Kondorski´ı E.I. O prichinakh osobennoste´ı fizicheskikh svo´ıstv invarnykh splavov. ZhETF, 37:1819–1820, 1959. [233] Hatherly M., Hirakawa K., Lowde R.D., and et al. Spin wave energies and exchange parameters in ironnickel alloys. Proc. Phys. Soc., 84:55–62, 1964. [234] Dubinin S.F., Teploukhov S.G., and Sidorov S.K. Ne´ıtrondifraktsionnye ´effekty iskazheni´ı struktury splava Ni – 67,7 at.% Fe v magnitouporiadochennom sostoianii. FMM, 55(6):1160–1164, 1983. [235] Dubinin S.F., Teploukhov S.G., and Sidorov S.K. Utochnenie parametrov sverkhstruktury FeNi invarov. FMM, 59(6):1158–1164, 1985. [236] Dubinin S.F., Teploukhov S.G., Evtukh A.A., Koliadin V.P., Skorobogatov V.P., and Sidorov S.K. Atomnaia i magnitnaia sverkhstruktura ostatochnogo austenita v splave Ni – 66,8 at.% Fe s nezavershennym γ−α prevrashcheniem. FMM, 59(6):1165–1176, 1985. [237] Dubinin S.F., Izyumov Yu.A., Sidorov S.K., Syromyatnikov V.N., and Teploukhov S.G. The role of the incommensurable atomic structure in the mechanism of the martensite transformation in the invar alloys. Phys.stat. sol. (a), 67(1):75–82, 1981. [238] Dubinin S.F., Teploukhov S.G., Izyumov Yu.A., Syromyatnikov V.N., and Sidorov S.K. O simmetri´ıno´ı sviazi faz pri martensitnom prevrashchenii invarnykh FeNi splavov. FMM, 50(6):1276–1284, 1980. [239] Bukhalenkov V.V. Izmenenie ´elektronno´ı struktury splavov FeNi s GTsK reshetko´ı pri magnitnom fazovom perekhode. FMM, 55(4):826–829, 1983. [240] Bukhalenkov V.V. Isseldovanie magnitnogo i strukturnogo fazovykh perekhodov v FeNi splavakh metodom IaGR: Diss. ... kand. fiz.mat. nauk. Sverdlovsk: Ural. politekhn. inst, 1983. 209
[241] Bernshte´ın M.L. Termomagnitnaia obrabotka stali. M.: Metallurgiia, 1968. [242] Ermolenko A.S., Men’shikov A.Z., and Malinen P.A. Vozniknovenie odnoocno´ı magnitno´ı anizotropii pri martensitnom prevrashchenii v magnitnom pole. FMM, 26(1):76–80, 1968. [243] Blatt F. Fizika ´ elektronno´ı provodimosti v tverdykh telakh. M.:Mir, 1971. [244] Leont’ev A.A., Schastlivtsev V.M., and Romashev L.N. Gabitus i orientatsiia kristallov martensita, obrazuiushchikhsia pod de´ıstviem magnitnogo polia. FMM, 58(5):950–957, 1984. [245] Varlimont Kh. and Dile´ı L. Martensitnye prevrashcheniia v splavakh na osnove medi, serebra i zolota. M.:Nauka, 1980. [246] Kashchenko M.P. Opisanie gabitusnykh ploskoste´ı (hh1) v volnovykh modeliakh rosta splavov na osnove medi, zolota i zheleza. Izv. vuzov SSSR. Ser. Fizika, (3):41–43, 1982. [247] Kashchenko M.P. Opisanie gabitusnykh ploskoste´ı v volnovykh modeliakh rosta martensita. gabitusy (225), (557), (925). Izv. vuzov SSSR. Ser. Fizika, (2):7–9, 1982. [248] Kashchenko M.P. The habit planes (hh1) description in wave models of the martensite growth for Cu, Au and Febased alloys. Abstract bulletin ICOMAT82, Belgium, page 23, 1982. [249] Marri Dzh. Neline´ınye differentsial’nye uravneniia v biologii. Lektsii o modeliakh. M.:Mir, 1983. [250] Iakhno V.G. Avtovolnovye protsessy v odnomernykh relaksatsionnykh sistemakh. Avtovolnovye protsessy v sistemakh s diffuzie´ı. Gor’ki´ı: Int prikladno´ı fiziki AN SSSR, pages 46–76, 1981. [251] Patashinski´ı A.Z. and Pokrovski´ı V.L. Fluktuatsionnaia teoriia fazovykh perekhodov. M.:Nauka, 1982. [252] Missol V. Poverkhnostnaia ´ energiia razdela faz v metallakh. M.:Metallurgiia, 1978. [253] Iakhno V.G. O raschete skorosti voln v vozbudimo´ı srede. 21(3):547–550, 1984.
Biofizika,
[254] Gilmor R. Prikladnaia teoriia katastrof. Kn. 1. M.: Mir, 1984. 210
[255] Liubov B.Ia. and Ro´ıtburd A.L. Temperaturnye usloviia na poverkhnosti rastushchego martensitnogo kristalla. DAN SSSR, 131(4):809–812, 1960. [256] Lykov A.V. Teoriia teploprovodnosti. M.: Vysshaia shkola, 1967. [257] Likhachev A.A. and Koval’ Iu.N. O vozmozhnosti primeneniia fenomenologichesko´ı teorii Landau dlia opisaniia martensitnykh prevrashcheni´ı. Kiev: Institut metallofiziki AN USSR, 1983. [258] Fizicheskaia akustika. T. 7/ Pod red. Mazona, U.M. M.: Mir, 1974. [259] Bobrov V.S. and Lebedkin M.A. Nabliudenie ´elektricheskikh ´effektov pri ´ nizkotemperaturnom dvo´ınikovanii niobiia. Pis’ma v ZhETF, 38(7):334– 336, 1983. [260] Likhachev V.A. Kooperativnaia plastichnost’, obuslovlennaia dvizheniem granits razorientatsii i granits razdela faz. Izv. vuzov SSSR. Ser.Fizika, (6):83–102, 1982. [261] Kashchenko M.P. and Vereshchagin V.P. Dvizhenie granitsy martensitnogo kristalla kak avtovolnovo´ı protsess. Dostizheniia v oblasti metallovedeniia i termichesko´ı obrabotki metallov. Tez. zonal’no´ı konf. (IX Ural’sko´ı shkoly metallovedovtermistov). Perm’: Permski´ı politekhn. int, pages 4–5, 1985. [262] Kashchenko M.P. and Vereshchagin V.P. Migration of the boundary of a martensite crystal in the phonon maser mode. Phys.Met. Metall, 60(5):18– 26, 1985. [263] Kashchenko M.P. and Vereshchagin V.P. Skorost’ dvizheniia granitsy martensitnogo kristalla v volnovykh modeliakh rosta. Vsesoiuz. nauch. konf.,,Sverkhuprugost’, ´ effekt pamiati formy i ikh primenenie v novo´ı tekhnike“: Tez. dokl. Tomsk: Isdvo Tom. unta, pages 11–12, 1985. [264] Kashchenko M.P. and Vereshchagin V.P. Usloviia statsionarnogo dvizheniia granitsy martenstinogo kristalla v modeli fononnogo mazera. Vsesoiuz. nauch. konf.,,Sverkhuprugost’, ´ effekt pamiati formy i ikh primenenie v novo´ı tekhnike“: Tez. dokl. Tomsk: Isdvo Tom. unta, pages 54–55, 1985. ´ [265] Pa´ıns D. Elementarnye vozbuzhdeniia v tverdykh telakh. M.: Mir, 1965. [266] Kashchenko M.P. and Vereshchagin V.P. Tsentry zarozhdeniia i volnovye skhemy rosta martensita v splavakh zheleza. Izv. vuzov SSSR. Ser. Fizika, (8):16–20, 1989. 211
[267] Kashchenko M.P. and Vereshchagin V.P. Uchet uprugogo polia priamoline´ıno´ı dislokatsii v ramkakh volnovogo opisaniia rosta martensita. Izv. vuzov SSSR. Ser. Fizika, (8):20–23, 1989. [268] Vereshchagin V.P., Kashchenko S.M., and Kashchenko M.P. Uchet osobennoste´ı uprugogo polia dislokatsionnogo tsentra zarozhdeniia v volnovo´ı modeli rosta kristalla αmartensita v splavakh zheleza. Novye metody v fizike i mekhanike deformiruemogo tverdogo tela. Ch. 1. Tomsk: Izdvo Tomskogo unta, pages 136–143, 1990. [269] Vereshchagin V.P. and Kashchenko M.P. Dislokatsionnye tsentry zarozhdeniia αmartensita i orientatsionnye sootnosheniia pri γ −α prevrashcheniia v splavakh zheleza. FTT, 33(5):1605–1607, 1991. [270] Vereshchagin V.P., Kashchenko S.M., and Kashchenko M.P. Dislokatsionnye tsentry zarozhdeniia αmartensita v splavakh zheleza. Izv. vuzov SSSR. Ser. Fizika, (9):79–83, 1991. [271] Vereshchagin V.P., Kashchenko S.M., and Kashchenko M.P. Volnovaia priroda zarozhdenia i rosta αmartensita v splavakh zheleza. Sil’no vozbuzhdennye sostoianiia v kristallakh. Sbornik trudov Tomskogo IFPM. Tomsk: Izdvo Tomskogo nauch. tsentra SO AN SSSR, pages 75–89, 1991. [272] Vereshchagin V.P. and Kashchenko M.P. Obobshchenie volnovo´ı modeli rosta kristalla αmartensita v splavakh zheleza. Prognozirovanie mekhanicheskogo povedeniia materialov. Novgorod, pages 1–5, 1991. [273] Kashchenko M.P., Letuchev V.V., Konovalov S.V., and Neskoromny´ı S.V. Novy´ı podkhod k napravlennomu formirovaniiu struktury αmartensita v splavakh na osnove zheleza. Mekhanika prochnosti materialov s novymi funktsional’nymi svo’stvami. Rubezhnoe, pages 232–233, 1990. [274] Kashchenko M.P., Letuchev V.V., Konovalov S.V., and Neskoromny´ı S.V. Physical imitation of αmartensite nucleation. Phys.Met. Metall., 73(1):48–49, 1992. [275] Panin V.E., Griniaev Iu.V., Elsukova T.F., and Ivanchin A.G. Strukturnye urovni deformatsii tverdykh tel. Izv. vuzov SSSR. Ser. Fizika, (6):5–27, 1982. [276] Egorushkin V.E., Kul’ment’ev A.I., and Panin V.E. K probleme peremenno´ı valentnosti. DAN SSSR, 276(5):1104–1106, 1984. [277] Vediaev A.V., Granovski´ı A.B., Kondorski´ı E.I., and Kotel’nikova O.A. K teorii kineticheskikh iavleni´ı neuporiadochennykh splavov v priblizhenii kogerentnogo potentsiala. FTT, 20(1):166–170, 1978. 212
Epilogue The author is sure that readers, who have reached up to the end of the monography, have understood that the mechanism controlling the spontaneous growth of martensite crystals (at cooling or heating) is connected with process of elastic waves generation by nonequilibrium 3d electrons (see also [1, 2]). It is selfevident that the content of the monography is not exhausted by exposition of this process as the severe fathoming of the martensitic transformation mechanism in iron alloys needs the knowledge of solidstate physics in full. Really, the nucleation process exposition of martensite is guessing the knowledge of the elastic fields created by flaws (in particular by dislocations). It is necessary to understand, on the one hand, features of an energyband structure in transition metals, and on the other hand, the essence of the kinetic phenomenons in them to explain the generation mechanism of waves. It is necessary to take into account that not only pure metals must be discussed, but also alloys (in a wide range of concentrations and temperatures); not only paramagnetic state, but also the ferromagnetic state; not only linear, but also nonlinear waves with interior dynamic structure of a wavefront, etc. The explanations covering the physical essence of solved problems and distinctive role of the martensitic transformation γ − α in iron alloys among structural transformations in solids (as an example of phase transition with extremely high speed of growth) ensure worth of the given book for broad enough audience of specialists. The author has closely overlooked the monography once again and has convinced yourself that there is no need to make any essential changes in the text holding its topical nature (set of fine misprints have been eliminated at editing of translation). It is worth noting that research directions marked in the monography have received the progress during last decade. 1. Dislocation nucleation centres were established for the martensitic crystals with all types of habit planes [3]. It has allowed to interpret the processes of forming of typical ensembles of the martensitic crystals (see for example [4–6]). 2. The formation of fine twin structure has been described as the consequence 213
of the coordinated propagation of relatively shortwave and longwave atomic displacements (see [7–9]). 3. Calculations for the dislocation loops have been shown that their elastic fields (possessing the greater inhomogeneity in comparison with fields of the infinite rectilinear dislocations) create the such compact regions that the nucleation within them leads to observed distributions of habit planes. Hence the distribution of habit planes gives the additional information for reconstruction of the nucleation process via morphological indications [10– 12]. 4. The concept of the crystons was found convenient and constructive for description of the lattice losing a stability during propagation of the process controlling the martensite growth [6]. This concept was originally used for interpretation of shear band formation (see for example [13–17]). 5. The cryston model has been extended to exposition of strain martensite. In this case the crystons (the shear carriers of superdislocation type) are direct carriers of threshold strain (see [18, 19]). Thus there is clear enough fathoming of physical mechanisms for all alternatives of the γ − α martensitic transformation in iron based alloys. It is significant that concepts of the heterogeneous nucleation and the strain controlling the crystal growth (the last is localized in the frontal region of the growing crystal) are the universal for the exposition of martensite crystal formation. However the dynamic nature of controlling processes, as well as mechanisms of their energy support, essentially discriminate. For case of the cooling martensite this is the controlling wave process that is supported in the maser regime by nonequilibrium electrons due to the generation of energy in transforming phase. For case of the strain martensite this is the processes of the crystons propagation that are supported in basic by energy of exterior stresses. The author is sincerely grateful to mister U. KayserHerold and madam J. Gerlts. The translation that has been carried out by them, adequately transmits the content of the monography in Russian.
214
Bibliography for epilogue [1] Kashchenko M.P. and Letuchev V.V. and Konovalov S.V. and Neskoromnyi S.V. Wave mechanism of growth and novel technique for initiation of the martensite nucleation. Phys.Met. Metall., 76(3):300–308, 1993. [2] Letuchev V.V. and Konovalov S.V. and Kashchenko M.P. Dynamical Lattice State at the Initial Stage of Martensitic Transformation and Possibilities of its Physical Realization. Journal de Physique IV, Colloque C2, 5:53–58, 1995. [3] Letuchev V.V. and Vereshchagin V.P.and Alexina I.V. and Kashchenko M.P. Conception of New Phase DislocationBased Nucleation at Reconstructive Martensitic Transformations. Journal de Physique IV, Colloque C8, 5:151–156, 1995. [4] Kashchenko M.P. and Konovalov S.V. and Yablonskaya T.N. Dislocation Centers in αMartensite Formation and Dual Couplings of ThinlyLaminated Martensite Crystals. Russian Physics Journal, 37(6):567–570, 1994. [5] Kashchenko M.P. and Konovalov S.V. and Yablonskaya T.N. Dislocation Centers for Nucleation of αMartensite and Pairwise Joining of Martensite Crystals with Habits {hhl}. Russian Physics Journal, 37(4):363–366, 1994. [6] Kashchenko M.P. and Letuchev V.V. and Konovalov S.V. and Yablonskaya T.N. Model of packet martensite formation. Phys.Met. Metall., 83(3):237– 242, 1997. [7] Kashchenko M.P. and Chashchina V.G. Dinamicheskii mekhanizm dvoinikovaniia martensitnigo kristalla. Mekhanizmy deformatsii i razrusheniia perspektivnykh materialov. Sb. trudov XXXV seminara ”Aktual’nye problemy prochnosti”. Part I. Pskov: PPI SPbGTU, pages 14–19, 1999. [8] Kashchenko M.P. and Chashchina V.G. Vliianie neodnorodnosti fronta upravliaushchego volnovogo protsessa na raspredelenie dvoinikov prevrashchenia v kristallakh martesita s gabitusami tipa (259)  (3 10 15). Fizika 215
protsessov deformatsii i razrushenia i prognozirovanie mekhanicheskogo povedenia materialov: trudy XXXVI mezhdunarodnogo seminara ”Aktual’nye problemy prochnosti v 2 chastiakh”. Ch.I, Vitebsk, VGTU, pages 8186, 2000. [9] Kashchenko M.P. and Chashchina V.G. Vliianie neodnorodnosti fronta upravliaushchego volnovogo protsessa na raspredelenie dvoinikov prevrashchenia v kristallakh martesita s gabitusami tipa (225). Nauchnye trudy IV mezhdunarodnogo seminara ”Aktual’nye problemy prochnosti v 2 t.” T.I, Velikii Novgorod, NGU, pages 156158, 2000. [10] Kashchenko M.P. and Nefedov A.V. and Vereshchagin V.P. and Letuchev V.V. Nucleation of α martensite crystals with (hhl) habits in elastic fields of dislocation loops. Phys.Met. Metall., 85(4):392–402, 1998. [11] Dzhemilev K.N. and Kashchenko M.P. and Nefedov A.V. Vlianie tochechnykh defektov na uprugie polia dislokatsionnykh tsentrov zarozhdenia martensita. Fizika protsessov deformatsii i razrushenia i prognozirovanie mekhanicheskogo povedenia materialov: trudy XXXVI mezdunarodnogo seminara ”Aktual’nye problemy prochnosti v 2 chastiakh”. Ch.II, Vitebsk, VGTU, pages 506511, 2000. [12] Dzhemilev K.N. and Kashchenko M.P. and Nefedov A.V. Vlianie tochechnykh defektov na uprugie polia prizmaticheskikh dislokatsionnykh petel’. Nauchnye trudy IV mezdunarodnogo seminara ”Aktual’nye problemy prochnosti v 2 t.”. T.I, Velikii Novgorod, NGU, pages 195199, 2000. [13] Kashchenko M.P. and Letuchev V.V. and Teplyakova L.A. and Yablonskaya T.N. A model of formation of macroshear bands and straininduced martensite with (hhl) boundaries. Phys.Met. Metall., 82(4):329–336, 1996. [14] Kashchenko M.P. and Teplyakova L.A. and Sokolova O.A. and Konovalov S.V. Formations of planar shear bands with {123} boundaries in fcc single crystals. Phys.Met. Metall., 86(1):27–30, 1998. [15] Kashchenko M.P. and Teplyakova L.A. and Dzhemilev K.N. and Chashchina V.G. Conditions for the generation of crystons and the interpretation of the σ −ε curve for Ni3 Fe single crystals crystals. Phys.Met. Metall., 88(3):223– 227, 1999. [16] Kashchenko M.P. and Chashchina V.G. and Semenovih A.G. The mechanism of formation of the shear bands with orientations of boundaries {hhl} in cubic crystals. In Advances in mechanical behaviour, plasticity and damage. Proceedings of EUROMAT 2000, V.I., pages 305–310, Amsterdam: Elsevier science Ltd., 2000. 216
[17] Kashchenko M.P. and Chashchina V.G. and Semenovih A.G. Kristonnyi mekhanizm formirovania α′ martensita deformatsii v prisutstvii martensita napriazhenia. Voprosy materialovedenia, 1(29):253–259, 2002. [18] Kashchenko M.P. and Chashchina V.G. and Semenovih A.G. Kristonnaia model’ formirovania α′ martensita deformatsii v splavakh na osnove zheleza. Fizicheskaia mezomekhanika, 6(3):95–122, 2003. [19] Kashchenko M.P. and Chashchina V.G. and Semenovih A.G. Cryston model of strain induced martensite. J. Phys. IV France, 112:147–150, 2003.
217
Kashchenko M.P.”The wave model of martensite growth for the γ − α transformation of ironbased alloys”. 2005
Summary Kashchenko Mikhail Petrovich, professor (Holder of Physics Chair, Urals State Forest Engineering University), doctor of physicalmathematical sciences. The sphere of his scientific interests: physics of solids, highexcited states of solids, martensitic transformations, synergetics. This book is the first monograph in the scientific literature, dedicated to the γ −α transformation in ironbased alloys, in which the dynamical approach is used for the explanation of the martensite growth stage. The rapid growth of a martensite crystal is considered as a selforganized process controlled by the quasilongitudinal lattice displacement waves (DW). The regime of the DW initial excitation is rigid. DW have the frequencies ∼ 1010 sec−1 from the hypersound band and the amplitudes providing the level of deformation ∼ 10−3 . The conditions that are necessary for the generation of DW by nonequilibrium delectrons are analyzed. A wide range of questions (from peculiarities of the electronic spectrum to macroscopic morphological indicators), connected with the physical interpretation of the γ − α martensitic transformation in ironbased alloys, is discussed. The short review of results having fundamental meaning for the creation of a physical model describing the martensite nucleation process is given in the monograph’s conclusion. It is shown, that processes of the heterogeneous nucleation and wave growth have the genetic connection to the γ − α martensitic transformation.
218